DK2159_half 10/6/05 1:26 PM Page 1
Adhesion Measurement Methods Theory and Practice
DK2159_title 10/6/05 1:59 PM Pag...

Author:
Lacombe R.

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

DK2159_half 10/6/05 1:26 PM Page 1

Adhesion Measurement Methods Theory and Practice

DK2159_title 10/6/05 1:59 PM Page 1

Adhesion Measurement Methods Theory and Practice Robert Lacombe

Boca Raton London New York

A CRC title, part of the Taylor & Francis imprint, a member of the Taylor & Francis Group, the academic division of T&F Informa plc.

Preface This volume has arisen out of a short course on adhesion measurement methods given in conjunction with a series of symposia on surface related aspects of materials science technology. The conference Web site* caught the attention of John Corrigan, who at that time was an acquisition editor for Marcel Dekker. As I had long been contemplating writing a volume on adhesion measurement to use as supporting material for a short course on adhesion measurement, John did not have to work very hard to convince me that it would be a good idea to write a volume on this topic. In addition, John and I felt that such a volume would fill an important gap in the engineering science literature because there was no single text devoted to adhesion measurement technology notwithstanding the fact that an enormous body of literature existed on the subject in scientific journals and edited volumes. Having thus decided to engage in the project, I concluded that the main purpose of the volume would be to provide a useful reference work and handbook for the practicing engineer/scientist who has a need to confront problems of adhesion either in support of manufacturing operations or in the development of new products. Thus, this book is meant to be used and kept handy for any and all of the following purposes: 1. As a monograph/reference work to be used either for self-study or to become aware of what has been done in the realm of developing methods and useful tools for measuring the adhesion of coatings and thin films. 2. As supplementary reading material for courses on materials science, mechanics of materials, or engineering design of laminate structures at the advanced undergraduate or graduate level. 3. As a handbook for looking up useful information and formulae on adhesionrelated matters, such as driving force formulae for various modes of delamination, methods for estimating stress buildup, and material property data in support of “back-of-the-envelope” calculations. 4. As an introductory reference work for accessing the vast scientific and engineering literature on adhesion measurement. A substantial bibliography of some 40 key reference works plus over 500 articles and books is organized topicwise to provide a convenient introduction to the veritable ocean of information available in the literature. The contents of the book are organized into seven chapters and five appendices in the following order: Chapter 1 gives a brief introduction to the subject, including * Those interested in surface-related phenomena such as adhesion, cleaning, corrosion, and the like can go the conference Web site at www.mstconf.com; there you will find the programs and abstract listings of some 24 previous symposia on these topics, as well as up-to-date information on current and future symposia.

an attempt to define the term adhesion for the purpose of providing a definition that is both accurate and useful in practice. Chapter 2 provides an overview of the most common adhesion measurement methods plus a few exotic methods to round out the mix. From the point of view of this work, adhesion measurement techniques fall into one of the three following categories: qualitative, semiquantitative, and fully quantitative techniques. Each of the methods discussed has its uses and drawbacks, and the intent is to make this as clear as possible. Something akin to a Consumer Reports format is adopted to help the reader interested in selecting a method with which to address current adhesion problems. Anyone just getting involved with adhesion-related issues should find this chapter helpful. Chapter 3 lays the foundation required to step up to the problem of implementing fully quantitative adhesion measurement methods. To do this, however, one has to confront headlong the thermal-mechanical behavior of the materials with which one is dealing. This comes about from the simple fact that all adhesion measurement methods in some way or another apply an external load to the structure tested and then draw conclusions based on the observed deformations or mechanical reaction forces observed. The most general formalism available for dealing with this type of behavior is the continuum theory of solids, which is treated in some detail in this chapter. Inescapably, the level of mathematical treatment rises considerably over that given in Chapter 2. Every attempt is made to avoid excessive rigor and abstract formalism, which does more to flaunt the level of erudition as opposed to shedding light on the technical matters at hand. Thus, those who subscribe to the International Journal of Solid Structures will most likely find the mathematical level quite pedestrian, whereas members of the laity could find the discussion fairly heavy sledding. This should in no way, however, prevent anyone from using the results presented in succeeding chapters to practical advantage. Chapter 4 deals with the discipline of fracture mechanics, which draws directly on all the supporting material presented in Chapter 3. Fracture mechanics is the ultimate organizing tool for performing fully quantitative adhesion measurements. It provides the concepts of stress intensity factor and strain energy release rate, which are two of the most useful quantitative measures of adhesion strength. Thus, from the point of view of fracture mechanics, a delamination is nothing more than a particular kind of crack occurring at an interface in a bimaterial structure. Chapter 5 attempts to draw all of the above material together and make it seem more coherent and relevant by providing several specific and detailed examples of adhesion measurement in action. Thus, extensive examples of the peel test, the scratch test, and the pull test are presented. It is hoped that the reader will gain significant insight and intuition into how adhesion testing is carried out in practice and perhaps find some answers to specific problems of interest. Chapter 6 deals with the problem of measuring the residual or intrinsic stress in a coating or other laminate structure. Whoever reads through the previous three chapters will quickly realize that residual stress is one of the key factors governing the delamination behavior of coatings and laminates and is a critical parameter in most fracture mechanics formulae for stress intensity factors and strain energy release rates. Thus, a fairly comprehensive overview of most of the useful stress

measurement methods is provided. Use of one or more of these methods can be considered as providing an indispensable foundation for developing effective adhesion measurement procedures. Chapter 7 concludes with more examples taken from the author’s direct experience in wrestling with adhesion problems in the microelectronics industry. Silicon chips and ceramic multichip modules used to package these chips into useful devices give rise to a welter of adhesion-related problems because the number of interfaces involved is so varied and extensive that most structures can be looked at as one extensive interface. The presentation here is informal and intended to provide insight and intuition as to how adhesion problems and adhesion measurement happen in the “real world.” Several appendices are provided to make the volume more useful as a day-today handbook and handy reference for looking up simple formulae and material property data for performing back-of-the-envelope type calculations. Rudimentary calculations for estimating the stress expected in a coating or the driving force for delamination can be very helpful for making decisions regarding which processes or materials one should employ for fabricating a specific device. Appendix A provides an overview of vector and tensor calculus for those with a need to brush up on the topic both regarding performing elementary calculations and in understanding more fully the mathematical developments in Chapters 3 and 4. Appendix B gives a quick overview of the most useful aspects of strength of materials theory, which essentially amounts to computing all the ways a beam can bend. This is important material because bending beams figure heavily in many adhesion measurement schemes and stress measurement experiments. Appendix C gives an extended table of material property data required for nearly all the formulae in Appendices B and D. This type of data tends to be scattered far and wide in a variety of texts and reference works, which by Murphy’s second law are never at hand when most needed. Thus, having these data located next to the formulae that require them should prove convenient. Appendix D provides a list of the most useful formulae from fracture mechanics that can be applied to the most common failure modes observed in coatings and laminates. Finally, a two-part bibliography is given that should prove handy in obtaining useful references from the vast technical literature. In closing, I would like to state that this is very much a work in progress. It makes no attempt at being fully comprehensive or definitive in any sense. Rather, the goal is to provide a volume extensive enough to be useful but not so vast as to be more of a burden than a help. In this regard, it is clear that much of relevance had to be left out. It is hoped that future editions will correct this problem to some extent. I invite any and all constructive criticisms and suggestions to correct errors or improve the presentation. I am most readily reached at the e-mail address given below and will give due attention to any and all who respond. Finally, this work would not be complete without giving recognition to my longtime friend, colleague, and co-worker Dr. Kashmiri Lal Mittal (Kash to his friends). Kash has certainly been a key inspiration in completing this work. A cursory look at the references will make it clear that his contributions to the adhesion literature have been monumental. In addition to editing the Journal of Adhesion Science and Technology, he has published 81 (and counting) edited volumes dealing either

directly or indirectly with problems of surface science and adhesion. His many comments and corrections to this work have been indispensable. My thanks go also to John Corrigan, who gave the initial impetus that got this project going. Many thanks, John, wherever you are. Robert H. Lacombe MST Conferences, LLC 3 Hammer Drive Hopewell Junction, NY 12533-6124 E-mail: [email protected]

The Author Robert Lacombe, Ph.D., received his doctoral degree in macromolecular science from Case Western Reserve University and was a postdoctoral fellow at the University of Massachusetts, working on problems of polymer solution thermodynamics. Following his stint in academia, he was an IBM physicist for 20 years and worked on problems relating to thin film wiring technology for both semiconductor chips and multichip modules. After IBM, he worked for an independent consulting firm on hybrid nonintrusive inspection and evaluation techniques, as well as problems of materials compatibility of both semiconductor and microelectronic packaging devices. He is an expert in the area of stress buildup in laminate structures and using the techniques of fracture mechanics in solving problems of delamination and cracking in composite devices. He has been a leader in the areas of materials characterization and published some of the first mechanical response data on monolayer nanostructures in the early 1980s. In addition, he pioneered innovative uses of largescale computation using finite element methods and applied this expertise directly to problems affecting product development and manufacturing. Dr. Lacombe is Chairman of MST Conferences and has organized over 20 international symposia covering the topics of adhesion and other surface-related phenomena since 1998. He is credited with over 40 publications and patents. Dr. Lacombe is a leading innovator in the field of subsurface inspection methods dealing with flaws in structural parts of air, auto, marine, and aerospace vehicles. As part of his activities with MST Conferences, he teaches a semiannual course on adhesion measurement methods in conjunction with the symposia.

Table of Contents Chapter 1

Introduction ..........................................................................................1

1.1 1.2

Overview ..........................................................................................................1 What Is Adhesion and Can It Be Measured?..................................................2 1.2.1 Definition A: Criteria for a Truly Useful Definition of the Term Adhesion...............................................................................................3 1.2.2 Definition B: Adhesion ........................................................................5 1.3 Comments on Nomenclature and Usage .........................................................5 References..................................................................................................................6

Chapter 2 2.1 2.2

2.3

2.4

2.5

2.6

2.7

Overview of Most Common Adhesion Measurement Methods .........7

Preamble...........................................................................................................7 Peel Test ...........................................................................................................8 2.2.1 Introduction ..........................................................................................8 2.2.2 Advantages of the Peel Test ..............................................................10 2.2.3 Disadvantages of the Peel Test ..........................................................10 2.2.4 Summary and Recommendations ......................................................11 Tape Peel Test ................................................................................................11 2.3.1 Introduction ........................................................................................11 2.3.2 Advantages of the Tape Peel Test......................................................12 2.3.3 Disadvantages of the Tape Peel Test .................................................14 2.3.4 Summary and Recommendations ......................................................14 Pull Test..........................................................................................................14 2.4.1 Introduction ........................................................................................14 2.4.2 Advantages of the Pull Test ...............................................................15 2.4.3 Disadvantages of the Pull Test ..........................................................16 2.4.4 Summary and Recommendations ......................................................17 Indentation Debonding Test...........................................................................17 2.5.1 Introduction ........................................................................................17 2.5.2 Advantages of the Indentation Debonding Test ................................19 2.5.3 Disadvantages of the Indentation Debonding Test............................20 2.5.4 Summary and Recommendations ......................................................20 Scratch Test ....................................................................................................20 2.6.1 Introduction ........................................................................................20 2.6.2 Advantages of the Scratch Test .........................................................26 2.6.3 Disadvantages of the Scratch Test .....................................................27 2.6.4 Summary and Recommendations ......................................................27 Blister Test .....................................................................................................27

2.7.1 Introduction ........................................................................................27 2.7.2 Advantages of the Blister Test...........................................................31 2.7.3 Disadvantages of the Blister Test ......................................................31 2.7.4 Summary and Recommendations ......................................................32 2.8 Beam-Bending Tests ......................................................................................32 2.8.1 Introduction ........................................................................................32 2.8.2 Three-Point Bend Test .......................................................................32 2.8.3 Four-Point Bend Test .........................................................................34 2.8.4 Standard Double Cantilevered Beam Test.........................................35 2.8.5 Tapered Double Cantilevered Beam Test ..........................................37 2.8.6 Double-Cleavage Drilled Compression Test .....................................39 2.8.7 Brazil Nut Test ...................................................................................40 2.8.8 Wedge Test .........................................................................................41 2.8.9 Topple Beam Test...............................................................................42 2.8.10 Advantages of Beam-Bending Tests..................................................43 2.8.11 Disadvantages of Beam-Bending Tests .............................................43 2.8.12 Summary and Recommendations ......................................................44 2.9 Self-Loading Tests .........................................................................................44 2.9.1 Circle Cut Test ...................................................................................44 2.9.2 Modified Edge Liftoff Test ................................................................46 2.9.3 Microstrip Test ...................................................................................47 2.9.4 Advantages of Self-Loading Tests.....................................................48 2.9.5 Disadvantages of Self-Loading Tests ................................................48 2.9.6 Summary and Recommendations ......................................................49 2.10 More Exotic Adhesion Measurement Methods .............................................49 2.10.1 Laser Spallation: Early Work.............................................................49 2.10.2 Later Refined Experiments ................................................................51 2.10.3 Laser-Induced Decohesion Spectroscopy Experiment ......................54 2.10.4 Advantages of Laser Spallation Tests................................................55 2.10.5 Disadvantages of Laser Spallation Test.............................................55 2.10.6 Summary and Recommendations ......................................................56 2.11 Electromagnetic Test ......................................................................................56 2.11.1 Advantages of the Electromagnetic Test ...........................................60 2.11.2 Disadvantages of the Electromagnetic Test.......................................60 2.11.3 Summary and Recommendations ......................................................60 2.12 Nondestructive Tests ......................................................................................60 2.12.1 Dynamic Modulus Test ......................................................................61 2.12.2 Advantages of the Dynamic Modulus Test .......................................63 2.12.3 Disdvantages of the Dynamic Modulus Test.....................................65 2.12.4 Summary and Recommendations ......................................................65 2.13 Surface Acoustic Waves Test .........................................................................65 2.13.1 Advantages of the Surface Acoustic Waves Test ..............................68 2.13.2 Disadvantages of the Surface Acoustic Waves Test ..........................68 2.13.3 Summary and Recommendations ......................................................69 Notes ........................................................................................................................69

Chapter 3

Theoretical Foundations of Quantitative Adhesion Measurement Methods ..............................................................................................75

3.1

Introduction to Continuum Theory................................................................75 3.1.1 Concept of Stress in Solids................................................................77 3.1.2 Special Stress States and Stress Conditions......................................83 3.1.2.1 Principal Stresses ................................................................83 3.1.2.2 St. Venant’s Principle..........................................................84 3.1.2.3 Two-Dimensional Stress States ..........................................85 3.1.3 Equation of Motion in Solids ............................................................86 3.1.4 Deformation and Strain......................................................................89 3.1.5 Constitutive Relations or Connecting the Stress to the Strain..........93 3.1.5.1 General Behavior ................................................................93 3.1.5.2 Homogeneous Isotropic Materials......................................96 3.2 Examples ........................................................................................................99 3.2.1 Simple Deformations .........................................................................99 3.3 Solving the Field Equations.........................................................................106 3.3.1 Uniaxial Tension ..............................................................................106 3.3.2 Biaxial Tension.................................................................................108 3.3.3 Triaxial Stress Case..........................................................................110 3.4 Application to Simple Beams ......................................................................112 3.5 General Methods for Solving Field Equations of Elasticity.......................130 3.5.1 Displacement Formulation ...............................................................131 3.5.2 Stress Formulation ...........................................................................132 3.5.3 Mixed Formulation...........................................................................133 3.6 Numerical Methods......................................................................................134 3.6.1 Introduction ......................................................................................134 3.7 Detailed Stress Behavior of a Flexible Coating on a Rigid Disk...............135 3.8 Strain Energy Principles ..............................................................................138 3.9 The Marvelous Mysterious J Integral..........................................................146 3.10 Summary ......................................................................................................151 Notes ......................................................................................................................152 Chapter 4 4.1

4.2

Elementary Fracture Mechanics of Solids: Application to Problems of Adhesion......................................................................155

Introduction ..................................................................................................155 4.1.1 Introductory Concepts......................................................................155 4.1.1.1 Strain Energy Approach ...................................................159 4.1.1.2 Stress Intensity Factor Approach......................................161 Fracture Mechanics as Applied to Problems of Adhesion..........................163 4.2.1 Elementary Computational Methods ...............................................163 4.2.1.1 Basic Model of Thin Coating on Rigid Disk...................163 4.2.2 Decohesion Number Approach of Suo and Hutchinson .................174 4.2.2.1 The Decohesion Number..................................................179 4.2.3 Back-of-the-Envelope Calculations .................................................180

4.2.3.1 Polyimide on Glass-Ceramic............................................181 4.2.3.2 Nickel on Glass.................................................................183 4.3 Summary ......................................................................................................185 Notes ......................................................................................................................185 Chapter 5

Applied Adhesion Testing................................................................187

5.1

The Peel Test................................................................................................187 5.1.1 Sample Preparation ..........................................................................188 5.1.2 Test Equipment ................................................................................189 5.1.3 Peel Testing in Action......................................................................190 5.1.4 Advanced Peel Testing.....................................................................193 5.1.4.1 Thermodynamics of the Peel Test ....................................194 5.1.4.2 Deformation Calorimetry..................................................194 5.2 Fully Quantitative Peel Testing....................................................................198 5.2.1 Earliest Work, Elastic Analysis........................................................198 5.2.2 Elastic-Plastic Analysis ....................................................................210 5.2.2.1 Theory of Elastic-Plastic Peeling for Soft Metals ...........213 5.2.3 Full Elastic-Plastic Analysis ............................................................217 5.2.3.1 General Equations for Deformation of Peel Strip ...........217 5.2.3.2 Basic Goal.........................................................................217 5.2.3.3 Analysis Strategy and Assumptions .................................218 5.2.3.4 Equations of the Elastica ..................................................218 5.2.3.5 Case 1: Elastic Peeling .....................................................225 5.2.3.6 Case 2: Elastic-Plastic Peeling/Unloading .......................226 5.2.3.7 Case 3: Elastic-Plastic Loading and Unloading...............227 5.3 The Scratch/Cut Test....................................................................................231 5.3.1 The Cut Test.....................................................................................233 5.3.2 Simplified Analytical Model for Cut Test .......................................237 5.4 The Pull Test ................................................................................................242 5.5 Summary ......................................................................................................245 Notes ......................................................................................................................246 Chapter 6 6.1 6.2

Adhesion Aspects of Coating and Thin Film Stresses....................249

Introduction ..................................................................................................249 General Measurement Methods for Thin Films and Coatings ...................251 6.2.1 Cantilevered Beam Method .............................................................251 6.2.2 Variations on Bending Beam Approach ..........................................257 6.2.3 Optical Measurement of Deflection.................................................257 6.2.3.1 Microscopy .......................................................................257 6.2.3.2 Laser Beam Deflection .....................................................258 6.2.3.3 Laser Interferometry .........................................................258 6.2.3.4 Capacitive Measurement of Deflection ............................259 6.2.3.5 Stress Measurement by Vibrational Resonance ...............260 6.2.3.6 Holography of Suspended Membrane..............................265

6.2.4 6.2.5

X-ray Measurements ........................................................................269 Ultrasonics........................................................................................272 6.2.5.1 Through-Thickness Stress Measurement .........................279 6.2.5.2 Surface Stress Measurement Using Skimming Longitudinal Waves ..........................................................279 6.2.5.3 Rayleigh Wave Method ....................................................280 6.2.5.4 Surface-Skimming SH Waves ..........................................280 6.2.6 Photoelasticity ..................................................................................280 6.2.7 Strain Relief Methods ......................................................................294 6.2.8 Magnetics .........................................................................................297 6.2.8.1 Barkhausen Noise .............................................................297 6.2.8.2 Magnetostriction Approach ..............................................299 6.2.9 Raman Spectroscopy........................................................................299 6.2.10 Miscellaneous Methods....................................................................301 6.2.10.1 Stress Pattern Analysis by Thermal Emission .................301 6.2.10.2 Photoelastic Coating Technique .......................................302 6.2.10.3 Brittle Lacquer Method ....................................................302 6.3 Summary ......................................................................................................303 Notes ......................................................................................................................303 Chapter 7

Case Studies from the Field ............................................................309

7.1 A Study in Adhesion Sensitivity to Contamination ....................................310 7.2 Case of the Improperly Cured Film ............................................................317 7.3 Case of the Stressed Pin ..............................................................................325 7.4 Stability Maps ..............................................................................................333 7.5 Summary ......................................................................................................334 Notes ......................................................................................................................335 Appendix A Vectors and Vector Calculus..........................................................337 A.1 Introduction ..................................................................................................337 A.2 Elementary Definitions of Scalars, Vectors, and Tensors ...........................339 A.2.1 Simple Scalars..................................................................................339 A.2.2 Vectors ..............................................................................................339 A.2.2.1 Vector Operations .............................................................340 A.2.2.2 Tensor Operations .............................................................342 A.2.2.3 Special Tensors and Operations .......................................344 A.2.2.4 Tensor/Matrix Multiplication............................................347 A.2.2.5 Product of a Matrix with a Vector ...................................349 A.2.2.6 Tensor/Matrix Scalar Product...........................................350 A.2.2.7 Assorted Special Arrays and Operations..........................350 A.3 Vector Calculus ............................................................................................354 A.3.1 Fundamental Operations of Vector Calculus ...................................355 A.3.1.1 The Gradient Operator......................................................355 A.3.1.2 The Divergence Operator .................................................356

A.3.1.3 The Curl Operator ............................................................357 A.3.1.4 The Gradient of a Vector ..................................................359 A.3.2 Basic Theorems of Vector Calculus.................................................360 A.3.2.1 Divergence Theorem.........................................................360 A.3.2.2 Stokes Theorem ................................................................361 Notes ......................................................................................................................367 Appendix B Notes on Elementary Strength of Materials (SOM) Theory ........369 B.1 Basic Concepts.............................................................................................370 B.1.1 Notion of Static Equilibrium ...........................................................370 B.1.2 Equations for Bending of Simple Beams........................................372 Appendix C Material Property Data for Selected Substances ..........................377 C.1 Useful Formulae...........................................................................................378 Notes ......................................................................................................................381 Appendix D Driving Force Formulae for a Variety of Laminate Structures ....383 Notes ......................................................................................................................389 Appendix E Selected References and Commentary on Adhesion Measurement and Film Stress Literature ......................................391 E.1 E.2

E.3 E.4 E.5

General References ......................................................................................391 Selected References on Adhesion Measurement Methods .........................392 E.2.1 Blister Test .......................................................................................392 E.2.2 Scratch Test ......................................................................................393 E.2.3 Indentation Debonding Test.............................................................394 E.2.4 Scotch Tape Test ..............................................................................395 E.2.5 Laser Spallation................................................................................395 E.2.6 Selected References on Mechanics of Peel Test .............................395 E.2.7 Nondestructive Methods ..................................................................396 Selected References on Stresses in Laminate Structures and Coatings .....396 Selected References on Fracture Mechanics as Related to Problems of Adhesion of Films and Coatings .................................................................397 Selected References on Stresses in Solids ..................................................397

Appendix F General Adhesion Measurement References ................................399 F.1 F.2 F.3 F.4 F.5 F.6

Review Articles ............................................................................................399 General Adhesion Papers .............................................................................400 Acoustic Emission/Ultrasonic Methods.......................................................401 Bend Test......................................................................................................402 Blister Test ...................................................................................................403 Double Cantilevered Beam Test ..................................................................405

F.7 F.8 F.9 F.10 F.11 F.12 F.13 F.14 F.15 F.16 F.17 F.18 F.19 F.20 F.21 F.22 F.23 F.24 F.25 F.26

Centrifugal Loading Test .............................................................................405 Electromagnetic Test ....................................................................................406 Fracture Mechanics Studies .........................................................................406 Indentation Test ............................................................................................408 Internal Friction............................................................................................409 Impact Methods............................................................................................409 Lap Shear Test..............................................................................................409 Laser/Electron Spallation.............................................................................411 Miscellaneous Methods................................................................................411 Peel Test .......................................................................................................414 Pull Test........................................................................................................420 Pullout Test...................................................................................................422 Push Out Test ...............................................................................................423 Residual Stress Self-Loading Test ...............................................................423 Scratch Test ..................................................................................................424 Tape Test ......................................................................................................426 Theoretical Studies.......................................................................................427 Thermal Methods .........................................................................................428 Topple Beam Method...................................................................................428 Wedge Test ...................................................................................................428

Index ......................................................................................................................429

1

Introduction

Can you measure it? Can you express it in figures? Can you make a model of it? If not, your theory is apt to be based more upon imagination than upon knowledge. Lord Kelvin

1.1 OVERVIEW The science of adhesion has the curious distinction of being at one and the same time both a “sticky” subject and a “slippery” one. The sticky aspect is obvious and needs no further comment; it is the slippery aspect that will draw much of our attention in this volume. The essential problem arises from the fact that adhesion is a basic property of surfaces, and according to the famous physicist Wolfgang Pauli: “God created matter; surfaces were invented by devil.” Surfaces are indeed devilish entities, especially for those who seek a quantitative understanding of their behavior. This arises from the fact that, for nearly all macroscopic objects, the surface area forms a very small portion of the bulk, is further subject to highly asymmetric forces, and is strongly prone to contamination and a large variety of defects. All of this makes it very tricky to characterize the nature of a real surface. For instance, one can have a glass surface that, for all practical purposes, appears to be absolutely clean, but the presence of even a monolayer of contaminant can change its behavior from water wettable to hydrophobic. This in turn has dramatic consequences if one is trying to get a particular coating to adhere to the glass. From a practical point of view, obtaining good adhesion in a manufacturing process requires very serious attention to the state of cleanliness of the surface to which something must be bonded. Furthermore, simply cleaning the surface may not be enough because contaminants may intrude from the ambient atmosphere. A notorious example of this arises in brazing processes where, for instance, one is trying to adhere a metal cap to a ceramic substrate using a solder formulation. Every precaution can be taken to ensure that the mating surfaces are scrupulously clean, but a contaminant such as silicone oil can condense onto the mating surfaces in question, preventing proper wetting of the solder and thus causing a defective joint to be formed. In many instances, silicone oil may be used for a variety of purposes in neighboring sections of a manufacturing plant. A common heating/ventilation system can then carry microscopic amounts of the volatile liquid throughout the entire plant, and because only a monolayer of coverage is enough to disrupt the wetting properties of a surface, the consequences can be catastrophic for the brazing process. Such problems can and do happen rather more frequently than one might imagine in the world of industrial processing, which emphasizes the slippery aspect of adhesion phenomena.

1

Introduction

3

One of the earliest overviews of this issue was given by Mittal,1 and we take his discussion as a starting point. The basic argument comes down to what one takes as the definition of adhesion. Now, from a commonsense point of view, one would like to think that adhesion is a simple matter of how well two different materials tend to stick together, and that adhesion measurement is some indication of the force required to separate them. Although this approach may suffice for the person in the street, it runs into serious difficulty when one tries to arrive at a more scientific definition of adhesion that can be useful for engineering purposes. A truly useful definition of the term adhesion needs to have the properties as given in definition A.

1.2.1 DEFINITION A: CRITERIA OF THE TERM ADHESION

FOR A

TRULY USEFUL DEFINITION

If we say that X is the adhesion of material A to material B, then it should have the following characteristics: 1. X has the same meaning for all practitioners who would stick A to B. 2. X is unambiguously measurable by one or more commonly understood methods. 3. Knowing X allows the practitioner to predict the loading conditions that will cause material A to delaminate from material B. Many would agree that the above is certainly a worthy definition of the term adhesion, but it unfortunately runs into a number of difficulties in practice because of the slippery aspects of the science of adhesion discussed in this chapter. In particular, the following types of problems are likely to arise in practice: •

Problem 1: Universality of the Definition Regarding Selection of Materials to be Adhered and Nature of Active Practitioners — Definition A runs into a variety of problems regarding the universality condition mentioned as characteristic 1. Let us assume that material A is a coating material to be applied to a thick rigid substrate comprised of material B. For simplicity, we assume that these materials are universally available to practitioners P1 and P2 in reasonably pure form. However, practitioner P1 wants to coat A onto B as a thin film less than 1 μm thick, whereas practitioner P2 wants to coat A onto B as a thick coating more than 25 μm thick. All other conditions are equal. Let us also assume that our practitioners are equally scrupulous in cleaning the substrate material B, and it is reported that A adheres well to B. Nonetheless, it can easily happen that practitioner P1 will find good adhesion of A to B whereas P2 will experience delamination. Among a wide variety of problems that can occur, one of the most common is the presence of thin film stresses. If the two practitioners use different techniques to coat A onto B, then the two coatings can develop different material morphologies, which can lead to substantially different stress levels in the two coatings. The more highly stressed coating will be much more likely to delaminate than the other.

2

Adhesion Measurement Methods: Theory and Practice

The scope of problems alluded to here makes the science of adhesion a very broad one that covers the range of disciplines from surface characterization to strength of materials. Indeed, many volumes have been written on the subject. However, the focus here is on one key aspect of the study of adhesion phenomena: the science of adhesion measurement. The basic goal is twofold. First, this volume is to serve as a manual for the relatively uninitiated worker in either academia or industry who has a practical need to perform adhesion measurements either as part of an experimental program or possibly as part of some quality control procedure. A broad range of well-known experimental techniques are reviewed and critiqued regarding their respective strengths and weaknesses. References are given both to the technical literature and to applicable commercial instrumentation. Emphasis is given to those methods that supply at least a semiquantitative estimate of adhesion strength and can be implemented in any laboratory with minimum expenditure of resources. Thus, the practical user can look to this volume as a ready guide and resource for getting a handle on personal adhesion measurement needs. The second goal of this work is to provide a more fundamental understanding of the adhesion measurement process and its consequences regarding the design and manufacture of structures that have a critical dependence on the adhesion of disparate material layers. The multilevel wiring layers in microelectronic structures immediately come to mind as an appropriate paradigm. Such systems often involve the buildup of material stresses that, to be effectively handled, require an understanding of continuum theory and fracture mechanics. Thus, a substantial section of this volume is devoted to the elements of continuum theory and fracture mechanics most relevant to the problem of adhesion measurement. It should be mentioned also that the topics of material behavior and fracture mechanics are of great concern even for the practical individual mainly concerned with subduing a specific adhesion problem that is plaguing a particular manufacturing process. The point is that, if material stresses get high enough, no amount of adhesion improvement will solve the problem of device failure. If the interface proves to be too strong, then the delamination failure simply proceeds as a fracture crack in the bulk material. Solving such problems unavoidably requires understanding and control of the material stresses. Again, microelectronic structures provide a prime example in which such situations can arise. In response to this type of dilemma, an entire section of this work treats the topic of stability maps, which provide a means of navigating through such problems. This is a topic of significant interest for both the practical user as well as anyone interested in the more fundamental and theoretical aspects of adhesion measurement and control.

1.2 WHAT IS ADHESION AND CAN IT BE MEASURED? There has been considerable debate in the technical literature concerning the question of what adhesion is and if it can be measured, and it is certainly not the intent here to expound further on what has been discussed many times. However, to provide a certain measure of perspective and to establish a defensible position on this matter, it is worthwhile at least to discuss this problem briefly.

4

Adhesion Measurement Methods: Theory and Practice

•

•

Furthermore, even assuming that the two practitioners used identical coating techniques, practitioner P2 will be much more likely to experience delamination because of the thicker coating as, for a given level of film stress, the driving force for edge delamination will scale linearly with film thickness. A second problem that can occur is that the two coatings may be subjected to different loading conditions when in use. For example, practitioner P1’s coating may see predominantly shear loads, whereas that of practitioner P2 experiences predominantly tensile loads. Because most coatings tend to resist shear delamination (commonly referred to as mode II) much better than tensile delamination (commonly referred to as mode I), practitioner P2 will be much more likely to experience delamination problems than his counterpart P1. Thus, definition A falls short regarding the universality criterion in that it may give good results for those putting down thin coatings and poor results for those trying to make thick coatings. Problem 2: Definition A Enables the Use of Simple and Unambiguous Measurement Procedures — From the point of view of the practical practitioner, the use of simple and unambiguous measurement procedures is quite likely the most important property desired in any truly usable definition of the term adhesion. However, the two qualifications of simple and unambiguous tend to be mutually contradictory in that a truly simple test is not likely to be unambiguous because, for the sake of simplicity, a number of important details will be either omitted or glossed over. The truly unambiguous test will specify in great detail the conditions of sample preparation, including cleaning procedures, control of material properties, precise specification of loading conditions, and control of the ambient environment. Observing all of these caveats will tend to undermine the goal of achieving simplicity. Clearly, any truly usable definition of adhesion will have to seek an appropriate balance between these two criteria. Problem 3: Definition A Has True Predictive Power — It is at once clear that the property that definition A has true predictive power is at odds with characteristic 2 because to obtain a truly predictive measure of adhesion, clearly the utmost attention must be given to all the details that will ensure an unambiguous result. This will sacrifice the goal of achieving simplicity. In addition, to be truly predictive the measurements have to be fully quantitative and consistent with detailed calculations. This implies at minimum the use of fracture mechanics methods and continuum theory of materials.

So where does this leave us? It is clear that although definition A is what we would like to have for a definition of the term “Adhesion”, it is clearly unworkable in the real world. In this volume, therefore, we back off somewhat from definition A and revert to definition B. However, before we frame definition B, we reflect on just what we are after vis-à-vis what is practicably obtainable. As this volume is primarily intended for those who have a practical need to perform adhesion measurements in support of the need to fabricate useful structures, our definition focuses on the need to be readily measurable. This puts the property of simplicity in the forefront as

Introduction

5

complex measurement procedures have a relatively low probability of implementation in a manufacturing process in which time and resource expenditure are carefully regulated commodities. In addition, our working definition has to be hierarchal because there are different levels of quantitativeness that can be specified depending specifically on the end use of the adhesion measurement. Thus, we frame definition B:

1.2.2 DEFINITION B: ADHESION We say the adhesion of material A to material B is such and such based on the following criteria: 1. The adhesion of A to B is a relative figure of merit indicating the tendency of A to stick or bind to B derived from an observation or measurement that can be entirely qualitative, semiquantitative, or fully quantitative. 2. The precise meaning of the term is entirely dependent on the details of the measurement technique employed and the experimental and environmental conditions under which the measurement was made. This leads to a hierarchy of definitions. Thus, qualitatively we might say A has good adhesion to B based on the observation that A was never observed to separate from B under a variety of common loading conditions. A semiquantitative statement of the adhesion of a coating of material A onto a substrate of material B might indicate that 2% of the coating was removed during a “Scotch tape” test. Finally, a fully quantitative statement might conclude that the adhesion strength of A to B is 10 J/m2 based on a double-cantilever beam experiment carried out at 50°C under 40% relative humidity.

1.3 COMMENTS ON NOMENCLATURE AND USAGE Definition B can be considered as defining the practical adhesion of one material to another. As defined, it is clearly measurable and has definite significance within the context of the specific measurement technique employed. This definition stands in contradistinction to the term fundamental adhesion, which would imply the work required for separation of material A from B assuming they were joined across a perfect mathematical plane and that the separation avoided any tearing out of either material. The fundamental adhesion of one material to another is an important theoretical concept and is clearly definable in principle. The problem for our purposes is that the fundamental adhesion is exceedingly difficult, if not impossible, to measure under most conditions and even if measured is not likely to be of any immediate use. At this point, we simply recognize that practical adhesion is some complex function of fundamental adhesion that we fortunately do not need to know under most circumstances. Furthermore, we recognize that the fundamental adhesion between two materials can be modified by physicochemical means and is a powerful tool for modifying practical adhesion. For the most part, however, this topic is beyond the scope of this volume. At this point, a number of comments on usage are in order. We have defined the noun adhesion from definition B, and we largely follow common dictionary usage

6

Adhesion Measurement Methods: Theory and Practice

and use the term adhere as the verb form. Also, when a coating separates from its substrate we use the term delamination. In the mechanics literature, one sometimes comes across the term decohesion. A coating is said to decohere from its substrate. The genesis of this term arises from the fact that the locus of failure lies in the substrate material a few microns below the true interface. Thus, it makes sense to talk about cohesive failure. One can also say the coating delaminated from the surface because that is the net effect, and failure occurred so close to the interface that, given the analytical tools at hand, the cohesive nature of the failure could not be detected. In all cases, one has to rely on the context of the measurements and observations to decide which term is most appropriate.

References 1. Mittal, K.L. Adhesion Measurement: Recent Progress, Unsolved Problems, and Prospects, in Adhesion Measurement of Thin Films, Thick Films, and Bulk Coatings, ASTM STP-640 (K.L. Mittal, Ed.), American Society for Testing and Materials, Philadelphia, PA, 1978, pp. 5–17.

2

Overview of Most Common Adhesion Measurement Methods

No experiment is so dumb that it should not be tried. Attributed to Walther Gerlach in reply to Max Born’s comments that his work on magnetic fields with strong spatial gradients would not be worthwhile. This work turned out to be pivotal to the success of the now-famous Stern-Gerlach experiment, which demonstrated spatial quantization for the first time and has been one of the experimental linchpins for quantum theory ever since.1

2.1 PREAMBLE This chapter overviews some of the most commonly used, and consequently the most useful, adhesion measurement methods. The approach follows that of a Consumer Reports-type examination in which both the strengths and the weaknesses of each technique are examined, and specific recommendations are made as to which methods are most suitable for which applications. Definition B of the term “adhesion” as presented in the Chapter 1 is assumed throughout. In addition, the discussion is guided by the following criteria for the “ideal” adhesion test: •

•

•

Quantitative: Gives numerical data that can be unambiguously interpreted. Data analysis straightforward and clear. Ease of sample preparation: Samples quickly and easily prepared with readily available equipment. If sample preparation is too complex, the test will not likely be implemented. Results relevant to real world: Final data must have relevance to final use conditions.

It should be made clear from the outset that none of the techniques described below meets all of the above criteria for the ideal adhesion test. However, each of these tests provides useful and reliable data when applied in a conscientious manner. Finally, it should be stated that this survey in no way covers all of the adhesion measurement methods reported in the literature. Mittal2 informally counted over 300 reported methods as of early 1994. Most of the reported methods, however, are essentially variations on one of the techniques described in what follows.

7

8

Adhesion Measurement Methods: Theory and Practice

Adhesion measurement methods can be divided into two broad categories: destructive or nondestructive. The overwhelming majority fall into the destructive class, by which a loading force is applied to the coating in some specified manner and the resulting damage subsequently observed. Nondestructive methods typically apply a pulse of energy to the coating/substrate system and then try to identify a specific portion of the energy that can be assigned to losses occurring because of mechanisms operating only at the interface. Inferences are then made regarding the bonding strength between the coating and the substrate.

2.2 PEEL TEST 2.2.1 INTRODUCTION Within the realm of destructive adhesion tests, there are two major classes: those dealing with relatively soft flexible coatings and those dealing with hard brittle coatings. By far the most common test for flexible coatings is the peel test. Anyone who has removed wallpaper from an old house already has considerable practical experience with the basic rudiments of this test. When dealing with polymer-based paints, for example, the peel test readily suggests itself as the preferred experiment for testing the adhesion of the coating. Such coatings on curing and drying tend to build up a significant level of internal stress, which increases dramatically near the edge of the coating. If the level of adhesion between the coating and the substrate is not sufficient, then the coating will delaminate and peel back. The now-released coating can be grasped with a tweezer, and an ersatz peel test is performed. Thus, the peel test automatically suggests itself as an adhesion test for flexible paint coatings. The main task for the experimenter is to standardize and quantify the peel test experiment so that the results can be used either to establish a quantitative ranking among the coatings tested or to set a numerical specification for adhesion strength that can be subsequently used as a quality control standard. The problem of quantifying the test is readily solved by the use of an appropriate tensile test apparatus in conjunction with suitable hardware for applying the peel force load and maintaining the required peel angle. Figure 2.1 exhibits a number of common configurations. Figure 2.1a illustrates the common 90° peel test; it is the favored test for flexible coatings on rigid substrates. This is by far the most prevalent and most thoroughly studied of all the peel tests. Figure 2.1b illustrates the 180° version of Figure 2.1a. This configuration offers advantages when space is cramped; Chapter 5 presents this scenario for the peel test performed in a calorimeter. It is also clear that the peel test can be performed at any angle between 0 and 180°. For most practical purposes, there is little need to consider angles other than 90 or 180° unless there are geometric constraints imposed by the sample or test apparatus. From an analytical point of view, however, varying the peel angle can provide information on the effect of mode mixity on peel strength. When performing a peel test, the interfacial region is subjected to both tensile (mode I) and shear (mode II) loads. The ratio of these two loading types is loosely referred to as the loading mode mixity. The importance of knowing the mode mixity

Overview of Most Common Adhesion Measurement Methods

F

F

(a) 90 degree peel test

T

(c) Climbing drum test

9

(b) 180 degree peel test

F

F

(d) T peel test

FIGURE 2.1 Four standard peel test configurations: (a) 90˚ peel test, the most commonly used configuration; (b) 180˚ test preferred when available space precludes the 90˚ test; (c) climbing drum or peel roller test, which has the advantage of controlling the radius of curvature of the peel strip; (d) T-peel test, preferred when testing adhesion of two flexible strips. A symmetric peel is obtained when identical strips are separated. Can also be used in a nonsymmetric configuration in which the two strips are not identical.

stems from the fact that the apparent adhesion strength of many coatings is sensitive to the mode mixity. For example, glues tend to be much stronger in shear than in tension, which implies that they will exhibit much higher adhesion strength in a predominantly mode II test as opposed to a mode I test. A very common example of this phenomenon is exhibited by Velcro fasteners. When loaded in shear, the Velcro fastener exhibits a very tenacious grip. However, when pulled at a right angle (i.e., tensile or mode I loading) the fastener readily separates. Figure 2.1c illustrates the climbing drum test used in testing the adhesion of rubbers in the tire industry. One advantage of this version is that the radius of curvature of the peeling film is fixed by the drum radius, which simplifies later numerical analysis of the data. Finally, the T-peel test shown in Figure 2.1d can be used to test the adhesion between two flexible films.

10

2.2.2 ADVANTAGES

Adhesion Measurement Methods: Theory and Practice OF THE

PEEL TEST

The peel test in its many configurations meets many of the criteria of the ideal adhesion test. Sample preparation is typically reasonably simple and straightforward. This single fact more than anything else accounts for the overall popularity of this test. Also, the peel force gives a semiquantitative measure of the coating adhesion to the substrate, which can be readily used for ranking or quality control purposes. A further advantage of this test is the fact that the rate of delamination and the locus of failure can be controlled fairly precisely. This stems from the fact that a very high stress concentration exists at the point where the coating just lifts off the substrate. This tends to narrowly focus the failure region very close to the geometric interface between coating and substrate, which is the region of most interest in any adhesion test. Because the rate of delamination can be precisely controlled by the test equipment, studies of the rate dependence of adhesion strength can be easily carried out. This can be very important when studying coatings that exhibit a strong molecular relaxation behavior (i.e., glass transition and related phenomena) near the test temperature. Finally, the peel test readily lends itself to use under conditions of controlled temperature and environment (for example, temperature and humidity conditions).

2.2.3 DISADVANTAGES

OF THE

PEEL TEST

As noted, the peel test works quite well when used as a method for ranking the adhesion of a coating when the substrate has been subjected to a number of different surface treatments. However, when trying to ascertain whether the coating will survive a given set of end-use conditions, several problems arise. The main issue is the fact that the peel test subjects the coating to very high strain levels near the peel bend, which most coatings never see under common end-use conditions. The strain in the coating at the peel bend can easily approach 25% or higher, whereas real coatings delaminate under nearly strain-free conditions. Thus, the load state imposed by the peel test does not reasonably approximate the load conditions that cause failure in the field; therefore, conclusions arrived at on the basis of peel testing can be highly misleading when trying to anticipate the actual service behavior of a particular coating. A particularly illuminating example of how far off you can be was given by Farris and Goldfarb.3 These authors tested the adhesion of polyimide films to aluminum and demonstrated apparent peel strength adhesion values in the range of 500 to 900 J/m2. However, the same coatings self-delaminated at an adhesion strength of 23 J/m2 when the coating thickness was increased to 120 μm. Thus, it is clear that peel test results can present highly misleading estimates of the actual adhesion strength of a coating when subjected to realistic end-use conditions. Further limitations of the peel test stem from the fact that it is applicable only to tough flexible coatings. Attempts have been made to circumvent this limitation by applying peelable backing coatings on top of the coating to be tested and then peeling the composite laminate. One major problem with this approach is the fact that the locus of failure at the peel front can become unstable. The delamination front can wander between the backing layer and the test coating or between the coating under test and the substrate, making interpretation of the results unclear.

Overview of Most Common Adhesion Measurement Methods

11

A number of other drawbacks and limitations apply to the peel test, including difficulty in initiating a peel strip for coatings with strong adhesion and controlling sample-to-sample variability. These problems can typically be dealt with by developing appropriate experimental techniques.

2.2.4 SUMMARY

AND

RECOMMENDATIONS

The peel test is quite likely the method of choice when dealing with tough, flexible coatings on rigid substrates as it meets many of the criteria of the ideal adhesion test. First and foremost is the consideration of sample preparation. In this regard, it is typically quite straightforward to fabricate convenient-size coupons of the substrate material and apply the coating of interest to them. Suitable care should be taken to clean the substrate and apply the adhesion promoters of interest. Further technical details, such as providing a release layer so that the peel strip can be easily initiated, should not be overlooked. Last, care should be exercised in interpreting the final data. Peel test data can be reliable for ranking the effectiveness of adhesion promoters or for quality control measurements. As noted, one should not rely on peel test measurements as a guide to performance of the coating under end-use conditions because the load state imposed by the peel test does not generally reproduce actual load conditions in the field. A detailed example of a successful implementation of the peel test for studying the adhesion of high-temperature coatings to silicon substrates is given in Chapter 5.

2.3 TAPE PEEL TEST 2.3.1 INTRODUCTION The tape peel test is a rough-and-ready variant of the standard peel test. Its main advantage is ease of sample preparation. The predominant disadvantage is that the results of the test will tend to be qualitative only. Attempts at systematizing the test, however, have given semiquantitative results. In a typical application, a strip of specially fabricated tape is applied to the coating to be tested in a predefined manner. The main concern is to be as consistent as possible to achieve reproducible results. The tape is subsequently peeled off in a prescribed fashion, and the test surface is then inspected for whatever resulting damage that may have occurred. At the purely qualitative level, the experiment gives a “go/no go” type of result. indicating whether the adhesion of the coating is acceptable. A number of techniques have been invented to give a semiquantitative result by quantifying the level of partial damage that may have happened to the coating. An example of this for the case of ink coatings is discussed in Section 2.3.2. The main problem with obtaining truly quantitative results with the tape peel test is that one now has to deal with four different materials: the substrate, the coating, the tape adhesive, and the tape backing material. Satas and Egan4 reported the effect of the backing layer and the adhesive layer on the peel strength of pressuresensitive tapes. Their data showed that, depending on the tape backing material, the peel force can vary by as much as a factor of 2 for a given layer thickness.

12

Adhesion Measurement Methods: Theory and Practice

In a separate study Aubrey et al.5 investigated the effect of adhesive molecular weight, adhesive layer thickness, backing film thickness, peel rate, and peel angle on the peel strength of polyester backing polyacrylate adhesive pressure-sensitive tapes. They demonstrated that all of these factors have a significant effect on the measured peel force. In particular, the peel force showed dramatic dependence on peel rate with three fundamentally different modes of peeling. At low rates, the peel force is controlled by flow of the tape adhesive and is strongly rate dependent. At high rates, little viscous deformation occurs, and the peel force is largely rate independent. At intermediate peel rates, the peel force exhibits cyclic instability driven by alternate storage and dissipation of elastic energy. The net result is a type of “stick-slip” peeling. Thus, without even considering the coating and substrate properties, we already have a considerable degree of complexity introduced just by the properties of the tape alone. If we now introduce further degrees of freedom arising from the mechanical response of the coating and substrate, we see that the problem of deriving a truly quantitative analysis of the tape peel test rapidly becomes prohibitive.

2.3.2 ADVANTAGES

OF THE

TAPE PEEL TEST

Despite the difficulties mentioned in obtaining quantitative results with the tape peel test, it can still be a useful and effective measurement method in certain applications. This is best illustrated by the study of ink coatings by Calder et al.6 These authors succinctly summarized the case for using the tape peel test in a cogent manner7: There is a body of experience in the industry that confirms that the tape test is a reasonable predictor of how the ink will remain in place, intact on the substrate under many actual use conditions. The test is fast and can be performed at press side. It is obviously important to know rather quickly whether an ink has adequate adhesion when the film is being printed at 600 ft/min.

In their experiments on ink coatings, the authors applied the subject ink coating to the relevant paper or foil substrate. Tapes were applied to the ink coating after a specified drying time and removed rapidly by a 90° peel test. The degree of adhesion of the ink coating is then rapidly evaluated using a light spectrophotometer and is reported as percentage coating removal as compared to a standard untested sample. Appropriate calibration methods are used to ensure repeatability. Figure 2.2 illustrates some representative data from this type of experiment. The solid line shows the apparent adhesion versus time for an ink with a relatively “soft” binder matrix, and the dashed line illustrates the same behavior for an ink with a “hard” binder matrix. The data clearly reveal that the soft binder gives an ink with stronger adhesion at short times (lower percentage coating removal), and that both ink types level off to substantially the same adhesion level at longer times. This is the type of information that can be of practical use in the printing industry, in which different printing techniques have different requirements for ink adhesion.

Overview of Most Common Adhesion Measurement Methods

13

Tape Peel Data on Two Separate Ink Types (Data replotted from Calder et al., Ref 6) Soft Binder

Hard Binder

% Coating Removal

100

75

50

25

0

0

10

20

30

Drying Time (minutes)

FIGURE 2.2 Tape peel test data on printing ink. The relative adhesion strength is measured by the amount of light that can pass through the ink/paper layer after the tape is peeled off. The ordinate gives the percentage of light passing through the sample as a percentage referred to an appropriate standard. The abscissa represents the drying time. A high value indicates more light passing through and thus poorer adhesion of the ink. A low value indicates little ink removal and thus good adhesion. The solid line represents an ink using a “soft” binder system and the dashed line a “hard” binder system. The data clearly show that the soft binder gives better adhesion at short times than the hard one, and that both systems behave much the same at long drying times.

A different type of application of the tape peel test in the photographic film industry was given by Grace et al.8 These investigators used the tape peel test in conjunction with a time-resolved salt bath technique for investigating the adhesion of silver coatings to poly(ethylene terephthalate) (PET) films. In the salt bath test, silver-coated PET films were immersed in a salt bath, and the time required for the silver to lift off was noted. These results were then correlated with standard tape peel testing in a manner similar to that mentioned above. The essential result of this investigation was the demonstration that the salt bath test was able to better discriminate different levels of adhesion of the silver coatings than the tape peel test alone. The tape test basically gave a good/not good type of result, whereas coatings tested in the salt bath would survive for different lengths of time, thus giving a more continuous scale of adhesion performance. In particular, coatings that the tape peel test indicated were good were shown to delaminate at intermediate times in the salt bath test. However, films shown to be poor by the tape peel test were also poor by the salt bath test. Thus, the tape peel test supported the salt bath experiments but did not give the same degree of resolution of adhesion strength.

14

Adhesion Measurement Methods: Theory and Practice

2.3.3 DISADVANTAGES

OF THE

TAPE PEEL TEST

As pointed out, the tape peel test at best can give a semiquantitative estimate of the adhesion of a coating. The results of the test tend to be confounded by the mechanical response and other failure modes of the tape backing and the tape adhesive as well as similar behavior of the coating and the substrate material. With so many potential complicating factors, the interpretation of tape peel test data is very difficult if more than a simple qualitative estimate of adhesion strength is required. The use of calibration methods and reference samples is mandatory to ensure a reasonable level of repeatability.

2.3.4 SUMMARY

AND

RECOMMENDATIONS

Although the tape peel test is limited to a qualitative or at best semiquantitative evaluation of adhesion, it has a number of advantages that make it attractive in specific applications. In particular, in situations for which a simple rapid test is required, such as for testing printing inks, or for which a straightforward go/no go evaluation is sufficient, this test may be perfectly adequate. In some cases, it may be the only reasonable test available. However, great caution is recommended in evaluating tape peel data. and the results should not be overinterpreted in terms of trying to understand the fundamental adhesion of a coating because a large number of confounding factors come into play with this test.

2.4 PULL TEST 2.4.1 INTRODUCTION As with the peel test, the pull test is a general method for assessing both qualitatively and semiquantitatively the adhesion of coatings to a variety of substrates. Also, as with the peel test, it enjoys a number of advantages and suffers from several disadvantages. The advantages include the following: •

• •

Applicable to a wide variety of coatings and substrates including • brittle coatings • flexible coatings Gives both qualitative and semiquantitative results Relatively easy sample preparation

The disadvantages of this method include • • • •

Difficult data analysis, especially for quantitative measurements Rapid uncontrollable failure mode Wide scatter in data Need for bonding adhesive or solder

An excellent evaluation of the pull test as applied to paint coatings was given by Sickfeld.9 This author investigated two basic pull test configurations, as illustrated in Figure 2.3. The symmetric configuration is preferable for testing coatings on

Overview of Most Common Adhesion Measurement Methods

15

Asymmetric pulloﬀ specimen

Symmetric pulloﬀ specimen Coating Substrate

Substrate

(a)

(b)

FIGURE 2.3 Schematic of two pull test configurations. The symmetric configuration is preferred when the substrate is thin or flexible. The asymmetric mode is preferred when the substrate is thick or very rigid. Note: Glue/adhesive layer not shown.

relatively thin flexible substrates, whereas the asymmetric sample is preferred for thick rigid substrates. Similar to the tape peel test, the pull test involves two additional materials besides the coating and substrate under investigation. The test stud itself is fabricated out of a high-modulus metal or ceramic material and for the case of paint coatings can be considered almost perfectly rigid. This is not the case for testing stiff brittle coatings such as diamond or ceramics; in these cases, the stud material must be carefully figured into the analysis. In addition, an adhesive is required to attach the test stud to the coating under test. For paint coatings, this is typically an epoxy glue, and its properties will always enter the analysis. After the test stud is appropriately cemented to the coating under test, it is pulled off under controlled conditions using a tensile test apparatus. A number of complications now enter the picture as follows: •

•

• •

Unless the load is applied very carefully, there can be an off-axis component that can impose a bending moment to the sample in addition to the tensile load. Even assuming pure tensile loading, any real sample will not be uniformly bonded, and the applied stress field will seek out any defects or bonding weaknesses. Failure will be initiated at the weakest point in the structure and propagate at acoustic velocities to complete separation. Failure can occur either adhesively at any of the three sample interfaces or cohesively in any of the four bulk materials. Mixed-mode interfacial and cohesive fracture is the most common failure mode.

Given the list of complexities, it should come as no surprise that typical pull test data show a wide range of variation. Multiple tests must be run at any given condition, and data-censoring techniques should be applied to ferret out unwanted failure modes.

2.4.2 ADVANTAGES

OF THE

PULL TEST

The main advantage of the pull test is its wide-ranging applicability to all manner of coatings, from relatively soft flexible polymer coatings to hard brittle coatings

16

Adhesion Measurement Methods: Theory and Practice

such as diamond. In addition, as pointed out by Sickfeld,9 there are two types of information that can be obtained from this test. The first is qualitative, deriving from an analysis of the resulting pull off fracture surface. Some idea of the integrity of the coating can be obtained by noting whether failure tends to be mainly cohesive in the coating itself or interfacial between the coating and the substrate. In particular, Sickfeld was able to study the effect of moisture and solvent immersion on the failure mode of paint coatings. For the case of immersion of the coating in water, subsequent pull testing showed nearly interfacial failure between the coating and substrate. On the other hand, coatings immersed in gasoline or oil demonstrated a mixed interfacial/cohesive type of failure. This type of data can be very valuable when evaluating a particular coating for use under particular service conditions. A second advantage is the quantitative information derived from the pull test. It has been hypothesized that, in most cases, the failure mode in a given pull test experiment is determined by a preexisting distribution of flaws in the sample. Thus, as discussed in the preceding section, the applied stress field seeks out the largest, most vulnerable flaw in the sample. Failure initiates at this point, and the initial flaw rapidly propagates at acoustic velocities to ultimate separation of the pull stud and the sample surface. In effect, it is assumed that all samples will have some kind of inherent flaw distribution no matter how carefully they were prepared, and the stress field deriving from the pull test will inevitably find the most vulnerable flaw; failure will initiate and propagate from that point. It has further been found that Weibull statistics are very effective in analyzing this type of data. Pawel and McHargue10 used the pull test to analyze the adhesion of iron films to sapphire substrates. These investigators ion implanted both nickel and chromium impurities at the interface between an iron film and sapphire substrate. Subsequent pull testing and Weibull analysis unequivocally demonstrated that the chromium interlayer substantially improved the adhesion of the iron film over the untreated and nickel-treated cases. Finally, there are situations that are perfectly disposed toward the pull test, such as evaluating the durability of pins on a microelectronic packaging substrate. For large mainframe machines, such substrates can carry over 100 silicon chips and require over 1000 pins to distribute power and signal data to a supporting carrier board. The reliability of these pins is critical to the proper function and performance of the total chip/substrate assembly, and each pin must meet very stringent reliability and performance criteria. The pull test is the natural performance evaluation procedure for this application. Coupled with the appropriate Weibull analysis, the pull test provides a crucial engineering and quality control tool for the design and fabrication of such structures.

2.4.3 DISADVANTAGES

OF THE

PULL TEST

One of the main disadvantages of the pull test is the wide variability in typical test data. This problem has been documented most cogently by Alam et al.11 These investigators attempted to evaluate the adhesion of chemical vapor deposition (CVD) diamond coatings to tungsten substrates. Because of a variety of conditions affecting their sample preparation, including nonuniformity of film thickness, diamond quality,

Overview of Most Common Adhesion Measurement Methods

17

film cohesion, and surface preparation, they observed considerable variability in their pull test data. In the authors’ own words: “The measured adhesion values showed larger variations from point to point across the sample surface and from identically prepared samples than variations as a function of the film processing parameters.” Thus, the data derived from pull testing in this case were mainly qualitative. Every form of sample failure was observed, including clean interfacial delamination, partial delamination with partial film cohesive failure, cohesive failure in the epoxy adhesive coupled with delamination of the epoxy from the coating, and pure cohesive failure of the diamond coating. With such a wide range of failure modes, it was no wonder that the data showed a high degree of variability. With the use of statistical analysis, however, the authors were able to show that substrate preparation, gas flow, and gas pressure were the most important processing parameters.

2.4.4 SUMMARY

AND

RECOMMENDATIONS

In conclusion, it is clear that the pull test can be an effective tool for evaluating both the qualitative and semiquantitative durabilities of a wide variety of coatings. The main advantage of this technique is its versatility and applicability to a wide range of coating/substrate systems. It can be applied to both soft flexible coatings as well as hard brittle ones. Pull test equipment is commercially available and can be set up in any laboratory with a tensile testing apparatus. The use of advanced statistical analysis such as Weibull analysis can be helpful in providing semiquantitative information concerning the durability of various coatings. The wide variation in typical pull test data remains one of the main weaknesses of this technique. Multiple tests must be done on a given sample coupled with statistical analysis to obtain reliable quantitative data. However, there are a number of specific instances, such as pin testing on microelectronic substrates, for which the advantages of pull testing make it the most natural choice for reliability testing.

2.5 INDENTATION DEBONDING TEST 2.5.1 INTRODUCTION Figure 2.4 shows a schematic representation of the indentation test. In this test, an indenter with a hemispherical point (i.e., with a tip radius that is on the order of the thickness of the coating tested) is thrust into the coating under carefully controlled conditions. The dominant effect of this maneuver is to greatly compress the coating material directly under the indenting tip. Surprisingly, however, a concomitant delamination of the coating can also occur starting at the edge of the indenter and extending for a distance that can be several times the indenter tip radius. An early example of the use of this technique for testing the adhesion of epoxy to copper in circuit boards was given by Engel and Pedroza.12 These investigators worked with epoxy coatings in the range from 25 to 300 μm on copper metal substrates. Using an indenter tip of approximately 0.2-mm radius, they observed peripheral delamination around the central indentation out to a radius of up to 2 mm. One simple way of understanding the mechanics of what is happening is given in Figure 2.5. As the indenter penetrates the epoxy coating, material is extruded to

18

Adhesion Measurement Methods: Theory and Practice

F

FIGURE 2.4 Idealized representation of the indentation debonding test. An indenter with a spherical tip is pressed into the coating under carefully controlled loading conditions. A high compressive stress is developed under the indenter; however, depending on the elastic/plastic response of the substrate, a tensile field is developed at the periphery that can cause the coating to delaminate.

Indenter radius

Delamination radius

Compressive indenter stress

Normal lever stress

Pileup pivot

FIGURE 2.5 Simplified description of indentation debonding test. The coating is treated as a simple beam setup. The compressive force of the indenter loads the left ligament of the beam while also pushing underlying material to the periphery, where it piles up and forms a pivot. Material to the right of the pivot point experiences normal tension because of the lever effect of the coating acting as a simple beam.

the periphery of the indenter, causing a pileup at the edge. In this case, the underlying copper material is also pushed to the indenter edge because copper is a highly plastic material, which also contributes to the pileup of material. The excess mound of both epoxy and copper at the edge of the depression can be thought of as forming a sort of pivot for the epoxy coating to act in the fashion of a simple lever, as shown in Figure 2.5. The epoxy film will have significant rigidity on the length scale of 1 mm, so the normal stress generated by this levering effect can be quite significant and lead to delamination if the coating adhesion is not sufficient. A further contributing mechanism is the shear stress generated by the extrusion of the epoxy material from under the indenter. Thus, a combination of flow shear stress coupled with normal lever stress can operate to delaminate the coating starting at the indenter edge. Engel and Pedroza13 also used a simple plate model of the coating to estimate the radial

Overview of Most Common Adhesion Measurement Methods

19

strain in the coating and referred to this as the peel strain. Such a strain can be an energy source for driving the indentation delamination. A far more rigorous analysis of the stresses driving the delamination process in the indentation test was given by Jayachandran et al.14 These authors treated the case of a poly(methylmethacrylate) polymer coating on a rigid substrate. Having access to extensive data characterizing the constitutive behavior of the poly(methylmethacrylate), they were able to carry out highly detailed numerical studies of the indentation process using the finite element method, including full details of large deformation and viscoplastic strain phenomena. Because these authors assumed a perfectly rigid substrate, their results cannot be compared directly to those of Engel and Pedroza. What was found is that there was indeed a massive shear flow and pileup of material created by the indenter all the way to the edge and beyond. However, because of the assumption of a rigid substrate, only a small tensile normal stress was predicted beyond the indenter edge. Thus, the normal stress in the epoxy/copper system is mostly caused by the pileup of the copper at the indenter edge, which forms a pivot on which the epoxy coating acts as depicted in Figure 2.5. The indentation debonding method has also been applied to hard refractory coatings, as demonstrated by the work of Weppelmann et al.15 These authors investigated the titanium nitride (TiN)/silicon system both theoretically and experimentally. Experimentally, they used a diamond indenter in conjunction with a digital interference microscope to follow the sample deformation precisely. Theoretically, they were able to develop a simple formula for the strain energy release rate for delamination caused by the radial strain induced by the indentation process. Using their experimental results, they were able to estimate an adhesion strength of approximately 1.2 J/m2 for the TiN/silicon system.

2.5.2 ADVANTAGES

OF THE INDENTATION

DEBONDING TEST

The indentation test has a number of clear advantages, which can be summarized as follows: • • • •

Applicable to a wide variety of coating/substrate systems Ease of sample preparation Both qualitative and quantitative results obtained Commercial equipment readily available

The indentation test is readily implemented both in the laboratory and on the production line for a wide variety of coatings. As mentioned, it has been applied to both soft flexible coatings on metals and hard brittle coatings on silicon. Engel and Pedroza12 commented on the use of this test for quality control in testing the adhesion of epoxy on copper in circuit boards. Other than preparing the coating, no special preparation of the test sample is necessary. The test is clearly applicable to a wide variety of substrates and has been applied to testing scratch-resistant coatings on curved plastic lenses. As mentioned, the indentation test can be analyzed to give quantitative results in addition to a simple qualitative estimate of the coating durability. Finally, commercial off-the-shelf equipment is readily available in the form

20

Adhesion Measurement Methods: Theory and Practice

of indentation test equipment and powerful microscopes with digital interferometers for evaluating both substrate damage and deformation.

2.5.3 DISADVANTAGES

OF THE INDENTATION

DEBONDING TEST

The main disadvantages of the indentation test can be summarized as follows: • •

Complex mode of loading involving large compressive stress and high shear strains Difficult quantitative analysis and poorly understood precise mechanism of delamination

The very high compressive load induced by the indentation test coupled with the high shear flow associated with soft coatings may make the relevance of the indentation test questionable for some coating systems. In particular, coatings subjected to large temperature swings may delaminate at edges or other discontinuities under loading conditions that are far different from those induced by the indentation test. A further drawback for hard coatings is the fact that, in addition to a large compressive stress, a very significant hoop stress is also generated by this test, which can lead to radial cracking in the sample substrate as well as the coating. Thus, multiple failure modes can greatly complicate the interpretation of the data when one is primarily interested in the coating adhesion.

2.5.4 SUMMARY

AND

RECOMMENDATIONS

The indentation debonding test clearly passes many of the criteria required for an ideal adhesion test. Primary among these are the ease of sample preparation and applicability to a wide variety of coating/substrate systems. Ready availability of commercial equipment makes this test a favorite in many industries that have to deal with quality control issues involving coatings. The main problem to be aware of is whether the loading conditions created by this test are reasonably close to those that the coating under test must endure in practice. In general, this is a very relevant test for coatings that must endure abrasive conditions and contact with potentially penetrating surfaces. Great care should be taken, however, if the coating in question will be subjected to large thermal strains that can be induced by large temperature gradients or thermal expansion mismatch between the coating and substrate.

2.6 SCRATCH TEST 2.6.1 INTRODUCTION Figure 2.6 gives a highly schematic representation of the scratch test, which can be thought of as an extension of the indentation test with the added feature that the indenter is translated along the sample surface as well as into the coating. An informative overview of the early history of this technique was given by Ahn et al.16 Apparently, Heavens17 and Heavens and Collins18 were the first to employ this

Overview of Most Common Adhesion Measurement Methods

21

Load

Stylus

Track direction Coating Substrate

FIGURE 2.6 Essentials of the scratch test. Loading conditions are similar to the indentation test in that the stylus pressure is ramped up according to some specified program; however, the stylus is simultaneously driven forward at a fixed rate.

technique to study the durability of metallic films evaporated onto glass. Subsequently, Benjamin and Weaver19 performed an elementary mechanics analysis of this method and derived the following simple formula for the shear force to be overcome by the scratch stylus: F=

AH ( R 2 − A 2) (2.1)

A=

W πH

where A R W H F

= Radius of stylus contact circle = Radius of stylus tip = Applied load normal to coating surface = Indentation hardness of substrate = Shearing force resisting lateral motion of stylus

The hope was that the load W required to remove the coating could be taken as a measure of the coating adhesion by relating it to the generated shear force given in Equation (2.1). However, a number of complications were noted by later workers,20 who discovered several difficulties, including the following: •

• •

Delamination of the coating can be observed even before the stylus removes all traces down to the substrate. In addition, the film can be thinned to the point at which it becomes translucent and cannot be removed. Complex material properties such as the elastoplastic behavior of the coating and substrate determine the nature of the scratch track. Multiple modes of failure are observed, including mechanical failure in the bulk of the coating or substrate in addition to interfacial delamination.

22

Adhesion Measurement Methods: Theory and Practice

Given the complications observed in the mechanically simpler indentation test, none of these remarks should come as any surprise. It should be clear that an experiment such as the scratch test that involves the penetration and dragging of a stylus through an adhered coating is going to give rise to a whole range of complex thermomechanical response behaviors, including viscoplastic flow, bulk fracture, and interfacial failure. The immediate upshot is that, as with all the other adhesion tests discussed, the scratch test will be at best a semiquantitative technique. However, this does not preclude the usefulness or effectiveness of this method for providing insight into the adhesion and durability of coatings in a variety of applications. In particular, Ahn et al.21 demonstrated that the scratch test can readily reveal poor adhesion in a coating because in this case lateral delamination of the coating can be observed to occur along the length of the scratch track. In an attempt to put the scratch test on firmer footing, Oroshnik and Croll22 came up with the concept of threshold adhesion failure (TAF). These investigators noticed that, in the thin aluminum films they were investigating, small patches of delamination could be observed in the scratch track well before the scratch stylus penetrated to the underlying substrate. It occurred to them that the load at which this patchy delamination occurred could be used as a measure of the coating adhesion. They proposed the following definition: Threshold Adhesion Failure occurs if, within the boundaries of a scratch and over its 1-cm path, removal of the film from its substrate can be detected by transmitted light with a microscope (×40 magnification) at even one spot, no matter how small.

This definition coincides well with Definition B (see Chapter 1) for adhesion and is certainly serviceable for the purposes at hand. Oroshnik and Croll described the method by which TAF is obtained for a given coating. The load on the stylus is increased incrementally as it moves over the sample surface up to the point at which spots of delamination are just detected. The load is then incrementally decreased until the delamination events just disappear, at which point the load is again increased to the point at which the delaminations again appear. This procedure of successively incrementing and decrementing the stylus load is repeated until the apparent threshold load for producing delaminations is reliably boxed in between upper and lower load conditions. Figure 2.7 shows a schematic of the type of data obtained from this procedure. Note from this figure how the data tend to settle at a fixed level of apparent adhesion strength. Oroshnik and Croll went on to discover that, even though using a given stylus, the TAF data were highly reproducible and consistent, no two stylus tips were identical, and each gave different TAF results. Using microscopic interferometry, these authors discovered that the stylus tips they were using were neither spherical nor with an unambiguous radius. In fact, data were presented showing measurements taken with different styli on a single film for which the TAF load differed by nearly a factor of 2. Furthermore, it was shown that the Benjamin and Weaver result for the shear force given by Equation (2.1) was not verified by the data, which was not surprising given the nonspherical nature of the stylus tips used. It is in fact well established that the most critical factor controlling the scratch test is the nature of

Overview of Most Common Adhesion Measurement Methods

23

Typical Threshold Adhesion Failure (TAF) Data 0.36 Micron Film of Aluminum on Vitreous Silica

Stylus Load (grams)

(Data replotted from Oroshnik and Croll, Ref. 22)

Scratch Coordinate X 10–3 (inches)

FIGURE 2.7 Typical threshhold adhesion data. Filled squares indicate load level at which delamination first appears while the load is increasing. Open squares indicate load level at which delamination first ceases while the stylus load is decreased. At the critical load for delamination, the load increasing and the load decreasing data should closely overlap.

the stylus tip. Different results will be obtained depending on the stylus material (steel, tungsten carbide, or diamond) and the precise topography of the tip region that first contacts the coating surface. Later investigators expanded on the scratch test not only to include more sophisticated instrumentation for controlling the load program of the stylus and advanced microscopy for observing the scratch track, but also to couple the scratch method with acoustic spectroscopy, by which the sound vibrations generated by the stylus are detected and recorded at the same time that the scratch track is formed. Typical of the more modern approach is the work of Vaughn et al.23 These investigators performed adhesion measurements on both copper and diamondlike carbon (DLC) films coated onto PET substrates. These experiments gave an ideal opportunity to evaluate the performance of the scratch test on two radically different types of coatings on the same substrate material. The highly plastic copper coatings gave completely unremarkable stylus load-versus-scratch length plots in which the load simply increases monotonically, with scratch length showing no particular discontinuities where the film began to delaminate. Further, these coatings gave no discernible acoustic signal at coating failure events such as delamination. By contrast, the rigid brittle DLC coatings showed a sharp drop in the stylus load versus scratch length curve at points where the DLC coating fractured in the typical “herringbone”style cracks that can appear in the scratch track because of the high tensile stress just behind the advancing stylus tip. Figure 2.8 shows a schematic representation of the type of data obtained from the DLC coatings.

24

Adhesion Measurement Methods: Theory and Practice

Typical Acoustic Emission Data from a Scratch Track on a Diamond Like Carbon Film on a Polymer Substrate

Acoustic Emission (arbitrary scale and units)

(Data replotted from Vaughn et al., Ref. 23)

2.7

3.0

3.4

3.8

4.2

Normal Load (N)

FIGURE 2.8 Correlation of acoustic emission data with microscopy of scratch track. Note that the appearance of a “herringbone” crack as the load increases coincides exactly with a local peak in the acoustic emission plot.

An innovative version of the scratch test was implemented by Sarin,24 who basically turned the experiment on its side and performed a microscratch test on a cross section of the coating substrate sample at 90° to the coating surface (Figure 2.9). The sample is sliced across a section of interest, and the edge is precisely polished by standard metallographic methods. The scratch test is then carried out in the standard manner only on a microscale because of the very narrow cross section under investigation. One advantage of this approach is that, under certain conditions the failure mode can be isolated at the coating/substrate interface, and the precise locus of failure is immediately apparent by direct microscopic investigation. Sarin, in fact, found that for a titanium carbide (TiC) film coated onto a silicon nitride/titanium carbide (Si3N4 + TiC) ceramic composite, he was indeed able to generate a crack along the coating/substrate interface, thus obtaining a true delamination failure mode. However, when the same type of experiment was performed on a TiC coating on tungsten carbide-cobalt (TC-Co) substrate, cracks were observed to start in the substrate and then propagate into the coating. Sarin’s findings illustrate what tends to be a general rule for all adhesion measurement methods in that any given method will be found to work well on a given specific sample system but will generally give unexpected results when the sample is changed even in a relatively minor way. Further attempts at quantifying the scratch test have been reviewed by Bull,25 who examined the scratch test as applied to a number of qualitatively different coating/substrate systems. This author basically found that the following criteria must be met to achieve a truly quantitative assessment of adhesion strength using the scratch test:

Overview of Most Common Adhesion Measurement Methods

25

90 degree micro-scratch test (Adapted from V. K. Sarin ref. 24) Coating

Scratch track Substrate Micro-indenter

FIGURE 2.9 Innovative variation of scratch test in which the sample is sectioned, and using a microindenter, the scratch track proceeds from within the sample substrate toward the coating/substrate interface at a 90° angle.

1. There must be a well-defined delamination mode present under the prevailing test conditions. 2. Knowledge of the sample stress state leading to delamination failure must be available either through direct measurement or calculation. With these conditions in mind, Bull examined a variety of coating/substrate systems that basically fell into the categories of hard and soft. Soft systems generally give rise to a high level of viscoplastic deformation, and clean failure modes may not be clearly observable. Hard systems, on the other hand, often exhibit brittle fracture in the substrate, the coating, or both. Combinations of soft and hard materials can give rise to all of the previously mentioned failure modes plus interfacial delamination. Table 2.1 gives a highly qualitative overview of the general trends. This table illustrates the general observation that the scratch test works best when at least one component of the coating/substrate system is a relatively hard material. On reflection this is intuitively reasonable. You clearly would not use the scratch test to quantify the adhesion of molasses to chewing gum.

TABLE 2.1 Qualitative Summary of Failure Modes in the Scratch Test as a Function of Coating/Substrate Hardness Substrate hardness ⇒ Coating hardness ⇓ Soft Medium Hard

Soft

Medium

Hard

Plastic deformation extrusion Plastic deformation extrusion Plastic deformation extrusion

Coating thinning scrape off Delamination

Coating thinning scrape off Delamination fracture

Delamination fracture

Delamination fracture

26

Adhesion Measurement Methods: Theory and Practice

However, Bull did illustrate two situations for which the scratch test gives promising results for hard coatings on hard substrates. The first case involves what can basically be called buckling spallation. For the system TiN on stainless steel, a thin coating of the TiN can be made to spall off the substrate. The scratch stylus creates a compressive stress ahead of itself because of the deformation of the substrate, which causes the coating to buckle. High tensile stresses in the coating cause the buckled coating to crack and then flake off. For thicker coatings, the bending required for buckling does not occur because the coating is too stiff. However, compressive shear cracks can form ahead of the indenter through the thickness of the coating. These cracks typically have sloping sides that can act as an inclined plane or wedge. The forward motion of the indenter can then drive the edge of the coating up the ramp created by the crack, causing the interface between the coating and substrate to separate, which leads to spalling of the coating. Bull referred to this mode of delamination as wedge spallation. Finally, even though the scratch test has proven most effective for hard brittle coatings, work by Bull et al. 26 showed that this test can also give valuable information concerning the adhesion and durability of polymer coatings such as epoxies. The application in this case was the evaluation of epoxy coatings for covering the inner hull of coal-carrying vessels. The epoxy is intended to protect the metal hull from abrasion by the coal and corrosion caused by the brackish marine environment. Lumps of coal settling against the inner hull have an abrasive effect; thus, the scratch test was deemed an appropriate method for evaluating the performance of the epoxy coatings. A number of different coating formulations were investigated, and all showed varying tendencies to either crack or delaminate under the action of the scratch stylus. One interesting failure mode arose because of the tensile load imposed on the coating behind the moving stylus. This would cause a through crack to form behind the stylus, which would then drag the coating along, opening up the crack and further buckling the coating in front in much the same manner as a rug buckles when pushed laterally at one of its edges. In addition, it was found that coatings with extender pigmentation tended to crack more readily than the unfilled coatings. However, the filler also retarded adhesion degradation as determined by aging studies. Thus, scratch testing can be used to determine the optimal tradeoff between coating toughness and adhesion by comparing scratch results on coatings with varying levels of extender pigmentation.

2.6.2 ADVANTAGES

OF THE

SCRATCH TEST

As with the indentation test, the main advantage of the scratch test lies in the relative ease of sample preparation. One simply prepares coupons of a convenient size out of the relevant coating and substrate materials in the same manner as on the manufacturing line or in the build shop. In addition, the newer commercially available equipment can be fitted with a number of auxiliary tools, such as microscopes, acoustic spectrometers, and surface-profiling attachments. Because the stylus can also act as an indenter, the coating hardness and elastic properties can be determined. Thus, a single instrument can give valuable information on surface topography, mechanical properties, and modes of deformation and delamination. Semiquantitative

Overview of Most Common Adhesion Measurement Methods

27

information can be obtained by recording the stylus load at failure; thus, scratch testing can be used to rank the durability of a series of coating formulations. In some cases, a fully quantitative estimate of the fracture energy of the coating/substrate interface can be obtained if care is taken to measure carefully all relevant mechanical properties and carry out the appropriate fracture mechanics calculations.

2.6.3 DISADVANTAGES

OF THE

SCRATCH TEST

There are two essential disadvantages to using the scratch test as an adhesion measurement tool: This test is essentially limited to hard brittle coatings even though some exceptions, such as brittle epoxy coatings, may be successfully investigated. The softer metals and most polymer coatings tend to viscoplastically flow and deform around the scratch stylus, causing mounding at the edges of the scratch track and pileup in front of the stylus. In addition, these coatings do not give a distinct acoustic signal at the failure point, thus negating the use of acoustic spectroscopy. Also, some coatings can be thinned to the point of optical transparency without achieving complete coating removal, thus complicating any attempt to assess adhesion strength. The second limitation arises from the fact that, as with the indentation test, the scratch test is mechanically complex. The act of pushing the stylus into the coating gives rise to very high stresses and deformations in both the coating and the substrate, thus bringing into play the full range of highly nonlinear viscoplastic material behaviors. The usual type of elastic mechanical calculations do not give quantitatively reliable results and can be used only for a more heuristic analysis of scratch test data. Also, the basic failure modes of the scratch test are only poorly understood, and experience gained on a given coating/substrate system may not be reliably carried over to a different one.

2.6.4 SUMMARY

AND

RECOMMENDATIONS

The scratch test is one of the most popular adhesion tests currently in use in both industry and academia. This stems largely from the great versatility of this technique for evaluation of a wide range of coating/substrate systems and the ready availability of commercial equipment that can perform a variety of functions, such as surface inspection, surface roughness measurements, and the evaluation of coating mechanical properties. For the case of hard brittle coatings, the scratch test is quite likely the best available technique for most situations. For softer coatings, this method may also be able to give useful results under certain conditions and can be used in a complementary manner with other techniques, such as the pull test.

2.7 BLISTER TEST 2.7.1 INTRODUCTION One constant complaint about all of the adhesion tests mentioned above is the fact that they involve a mechanically complex process with large deformations and strains giving rise to highly nonlinear viscoplastic response behavior by the coating/substrate system investigated. An immediate consequence of this is the fact that the analysis

28

Adhesion Measurement Methods: Theory and Practice

of these systems in terms of continuum and fracture mechanics concepts is exceedingly difficult, if not impossible. The blister test is an attempt to circumvent these difficulties by developing a blister in the coating in a well-defined manner that will propagate a delamination front between the coating and substrate in a controlled manner using only moderate deformations and strains. Dannenberg27 was apparently the first investigator to apply this technique to measure the adhesion of polymer coatings. Lai and Dillard28 gave an insightful account of the mechanics of several versions of this test. Figure 2.10 is a schematic representation of four different versions of this test mentioned by these authors. Figure 2.10a illustrates the standard blister test configuration. The main limitation of this version occurs when the coating ruptures before the coating can delaminate. This problem limits the standard blister test to coatings with either very high fracture toughness or relatively low adhesion to the underlying substrate. To circumvent this problem, Allen and Senturia29,30 devised the island blister test shown in Figure 2.10b. Because of the much smaller debond front presented by the inner island, the driving force for delamination is much greater here than at the much larger circumference at the outer radius. Thus, delamination can be made to occur at the inner island at a much lower applied pressure than would be required in the standard blister test. Four versions of the blister test Top view (a) Standard blister test

Side view

o P

(b) Island blister test

o P

(c) Peninsular blister test

o P

(d) Constrained blister test

o P

FIGURE 2.10 Four different configurations of the blister test: (a) The standard test involves applying hydrostatic pressure to the bottom of the coating, thus inducing a blister. The main drawback of this approach is that the coating may burst before significant delamination occurs. (b) The island blister test is one attempt to get around the coating bursting problem. In this configuration, the driving force for delamination is much higher on the central island than on the periphery. Thus, one is more likely to get delamination before the coating fails. (c) The peninsular test is a variation of the island test that also alleviates the coating failure problem while improving on the stability of the test. (d) For the constrained blister test, placing a transparent rigid cover over the blister allows control of the coating deformation while observing the delamination front.

Overview of Most Common Adhesion Measurement Methods

29

One problem with the island blister test is that it tends to be unstable. To overcome this difficulty, Dillard and Bao* conceived the peninsular blister test depicted in Figure 2.10c. This version of the blister test maintains the high driving force for delamination as in the island blister test while maintaining a more steady delamination front. Figure 2.10d shows the constrained blister test, which cleverly supplies a simple cover for the standard blister test to prevent the problem of film rupture. The earliest investigations of this technique were apparently carried out by Napolitano et al.31,32 and nearly simultaneously by Dillard33–35 and co-workers. Napolitano and coworkers32 managed to derive, using simple thermodynamic arguments, the following formula for the expanding area of the propagating blister: 2

βp h A(t ) = exp[ (t - t 0)] A(t 0) ph - γ

(2.2)

where A(t) p h γ β t0, t

= Blister area at time t = Applied pressure = Spacer height = Interfacial fracture energy = Dissipative coefficient = Initial and current time, respectively

Equation (2.2) was used to analyze constrained blister test data taken on a pressure-sensitive adhesive tape. The interfacial fracture energy was determined by noticing at what combination of spacer height h and applied pressure p the onset of delamination occurred. The interfacial fracture energy could then be computed from the following simple formula: γ = (hp)threshold

(2.3)

where it is to be noted that the pressure p in Equation (2.3) is that which just causes blister delamination to progress. The dissipative coefficient could then be obtained from data on blister area versus time. Plotting the log of both sides of Equation (2.2) yields a straight line with a slope that gives the parameter β, knowing γ from Equation (2.3). Liang et al.36 gave a very interesting application of the constrained blister test as applied to electropolymerized polymer coatings on copper substrates. They improved significantly on the work of Napolitano et al. by bringing to bear advanced image analysis methods implemented on a powerful modern workstation. With this advanced hardware and software, they were able to measure in real time the critical blister growth front parameters and thereby analyze their data using a fracture mechanics result for the strain energy release rate derived by Chang et al.37 given by the following formula: * “The Peninsula Blister Test — A High and Constant Release Rate Fracture Specimen for Adhesives,” D.A. Dillard and Y. Bao, Journal of Adhesion, 33, 253 (1991).

30

Adhesion Measurement Methods: Theory and Practice

Geometric parameters in constrained blister test (Refer to Eq. 2.4) a d h

P

FIGURE 2.11 Illustration of the configurational parameters for the constrained blister test appearing in Equation (2.4).

⎡ ⎛ d ⎞ ⎡⎛ d ⎞ ⎤ ⎛ ∂d ⎞ ⎤ G = ph ⎢1 − ⎜ ⎟ + ⎢⎜ ⎟ − 1 2 ⎥ ⎜ ⎟ ⎥ ⎢⎣ ⎝ 2a ⎠ ⎣⎝ 3a ⎠ ⎦ ⎝ ∂a ⎠ ⎥⎦

(2.4)

In this equation, G is the strain energy release rate, and p is the applied pressure; the dimensional parameters are explained in Figure 2.11. An elementary analysis of the island blister test was given by Allen and Senturia.38 By assuming that the coating can be treated as a membrane (i.e., it is so thin that it has no unsupported stiffness) and that the major component of the driving force is caused by residual stress, they came up with the following simple formula for the surface fracture energy of adhesion: 2

γa =

( pc a1) 32σ 0t

⎡ β2 - 1 ⎤ − 2⎥ ⎢ ⎢⎣ ln β ⎥⎦

2

(2.5)

where γa pc σ0 t β a1, a2

= = = = = =

Surface fracture energy Critical pressure for delamination propagation Residual film stress Film thickness a1/a2 Geometric parameters shown in Figure 2.12

Allen and Senturia also gave an interesting comparison between the island blister test and the standard version and demonstrated why the former gives a much higher delamination force on the inner island than the latter can achieve on the outer circumference of the suspended membrane.

Overview of Most Common Adhesion Measurement Methods

31

Geometric parameters of island blister test (Refer to Eq. 2.5)

Suspended membrane a2

a1 Bonded coating

FIGURE 2.12 Illustration of the configurational parameters for the island blister test appearing in Equation (2.5).

2.7.2 ADVANTAGES

OF THE

BLISTER TEST

As can be ascertained from the discussion, the blister test has a number of advantages; mainly, it is the first test discussed here that lends itself readily to a fully quantitative analysis based on fracture mechanics methods. This is mainly because this test imposes relatively low strains on the coating material, thus avoiding the complex nonlinear viscoplastic behavior that greatly complicates methods such as the peel test. However, like the peel test the blister test also concentrates the maximum stress at the delamination front, thus constraining the failure crack to be close to the coating/substrate interface of interest. Also, given the fact that a number of different versions are available, as shown in Figure 2.10, the user has great flexibility in testing coatings with varying levels of adhesion.

2.7.3 DISADVANTAGES

OF THE

BLISTER TEST

Whereas the blister test lends itself fairly readily to quantitative analysis, this advantage is purchased at the price of ease of sample preparation. It seems in the realm of adhesion testing that nothing comes free. If you gain an advantage in one quarter, then you pay for it in another. The main impediment comes with drilling the hole at the center of the blister through which the pressurizing gas enters. This can be accomplished in a number of ways, but the most popular is the use of etchants, which will erode the substrate material and not attack the coating. For coatings on silicon substrates, all the methods of microelectronic lithography are available to etch holes in the silicon and construct the various structures required for tests such as the island blister configuration. However, to use these methods a wafer fabrication facility must be available to carry out the involved series of steps required to construct the desired structures. This work also requires the use of very nasty etchants, such

32

Adhesion Measurement Methods: Theory and Practice

as buffered hydrofluoric acid. In addition, the blister test is limited to fairly flexible coatings, such as polymer-based paints and soft metals. Hard brittle coatings will tend to crack before forming a blister under the influence of the applied pressure. Finally, this test will have severe problems with coatings under high compressive stress because this will cause the coating to buckle as soon as it is lifted from the supporting substrate.

2.7.4 SUMMARY

AND

RECOMMENDATIONS

The blister test is most suitable when a fully quantitative analysis of the adhesion strength of a coating to a particular substrate is required. Great flexibility is available in the types of samples that can be used, and a number of investigators have provided detailed analyses that can be used to interpret the data in a fully quantitative manner. Also, the fact that delamination is achieved at low strain levels makes the results of the test much more relevant to coating adhesion than large strain-inducing methods such as the peel test. On the downside, however, sample preparation is far more cumbersome than for many other techniques. Thus, the blister test is not recommended when only qualitative or semiquantitative data are required because many other simpler methods are available.

2.8

BEAM-BENDING TESTS

2.8.1 INTRODUCTION There are a variety of tests for measuring adhesion that rely on the relatively simple mechanics of the elastic beam to simplify the required analysis for the stress intensity factors and the strain energy release rates that drive the delamination process. Precise definitions of these quantities are given in Chapter 4, which treats the methods of fracture mechanics in detail. The most attractive feature of beam-bending tests is that the stress field induced by the bending operation is comparatively simple and can thus be analyzed by elementary methods. Details of this type of analysis are given in Chapter 3, in which the fundamentals of continuum theory are discussed in some detail. Figure 2.13 illustrates several of the most popular adhesion tests that rely on the mechanics of a bending beam. The following sections discuss each in turn.

2.8.2 THREE-POINT BEND TEST A standard configuration for the three-point bend test is shown in Figure 2.13a. Using the three-point bend test, McDevitt and Baun39 carried out one of the earliest studies on metal-to-metal adhesive joints. These investigators found the curious result that apparently the three-point bend test was more sensitive to interfacial weaknesses than other tests they were performing such as the T-peel, the wedge test, and the lap shear test. Load-versus-deflection data were gathered on metal/adhesive/ metal sandwich samples as depicted schematically in Figure 2.14. The top curve in this figure represents a nonbonded sample in which a cured strip of adhesive was simply laid between two metal layers with no apparent bonding other than simple friction. This load-displacement curve thus serves as a baseline for a completely nonbonded

Overview of Most Common Adhesion Measurement Methods

Knife edge

Preset cut

33

Knife edge (e) Double cleavage drilled compression

(a) Three point bend

a

F Preset cut

F

F

(b) Four point bend

P (f ) Brazil nut

Knife edge P Adherend

(c) Standard double cantilevered beam

Knife edge

P

Adhesive

Adherend

(g) Wedgetest

P P (d) Tapered double cantilevered beam

F

Adherend Adhesive Adherend

(h) Topple beam test

P

FIGURE 2.13 Eight different adhesion tests that rely on the elastic bending properties of stiff beams.

joint. Figure 2.14b shows the case where the metal/uncured adhesive/metal sandwich was cured in an oven to achieve maximal bonding between all the layers. Note that this sample achieves a much higher load level before yielding. In addition, the authors attributed the break in the curve to failure at the metal/adhesive interface. With basic calibration data in hand for completely bonded and unbonded specimens, the authors were able to test bonded samples subjected to a variety of thermal and environmental stress conditions. Roche et al.40 investigated an interesting variation of the three-point bend test that is also sensitive to conditions at the adherate/substrate interface. The basic configuration is depicted in Figure 2.15. At a high enough load, the adherend will detach from the substrate starting from the edge and proceeding to the center, as shown in the figure. With the configuration shown in Figure 2.15, the stress distribution in the adherend can be monitored using the photoelastic setup shown in Figure 2.15b. In a typical experiment, the sample stiffness and stress distribution are monitored as the load is increased. An important piece of information is the load at which delamination of the adherend just begins. This number is sensitive to the detailed substrate preparation procedure before application of the adherend. It is clearly shown that this technique can be a powerful tool for investigating the effect of different surface preparation procedures and adhesive formulations on the adherend/ substrate adhesion strength. Making multiple identical samples also allows one to

34

Adhesion Measurement Methods: Theory and Practice

Load-displacement data for metal/adhesive/metal samples (Note: Time plotted in place of actual displacement. Adapted from McDevitt and Braun, ref. 39) 3000 Load (lb)

Non-bonded specimen 2000 1000

1

2

3

4 5 Time (min)

6

7

6

7

(a)

Load (lb)

4500

Bonded specimen

3000 1500

1

2

3

4 5 Time (min) (b)

FIGURE 2.14 Bending load versus time for three-layer sandwich samples using the threepoint bend test: (a) Poorly bonded sample shows essentially continuous load buildup, with increasing bending basically reflecting the stiffness of the most rigid layer. (b) Strongly bonded sample shows significantly higher load versus deflection behavior than the poorly bonded case, indicating strong coupling and mutual reinforcement between all the layers of the sample. In addition, a sharp drop in the load is detected when the adhesive joint between the layers fails.

study the effect of thermal cycling and other environmental stress factors on the durability of the bond.

2.8.3 FOUR-POINT BEND TEST The standard configuration for the four-point bend test is shown in Figure 2.13b. Figure 2.16 shows the typical failure modes of the coating/substrate system as the bending load is increased. Note that there are two basic failure modes for this experiment. In the first case, failure is by clean delamination of the coating from the substrate. It can also happen that after propagating a short distance an initial delamination will dive into the substrate, initiating a cohesive failure. Experiments and theory confirm that the crack will dive to some fixed depth below the interface and then propagate indefinitely parallel to the interface. The precise depth of penetration is determined by the elastic properties of the coating and the substrate. This

Overview of Most Common Adhesion Measurement Methods

35

Modiﬁed 3 point bend test (after Roche et al., ref. 40) F Typical failure path Substrate Adherend

(a) Side view

Substrate Adherend Light source

Detector Polarizer (b) End view

FIGURE 2.15 Variation of the three-point bend test in which the stress in the adherend is monitored by photo elastic measurement: (a) Side view showing most likely delamination path. (b) End view showing schematic of photoelastic measurement setup.

problem is treated in detail in Chapters 3 and 4, which cover the fundamentals of continuum theory and fracture mechanics required to understand this type of behavior. The four-point bend test is favored largely by those interested in obtaining fully quantitative information on the adhesion strength of coatings by taking advantage of the relatively simple beam mechanics involved in the fracture analysis of this problem. In particular, Evans and co-workers used this test extensively to study the adhesion of a variety of metals to alumina (Al2O3) substrates. This work has been summarized by Evans.41 A synopsis of their results is given in Table 2.2. The basic conclusion from this work was that interfaces that were clean and free from contamination were inherently tough and ductile. Failure occurred either by rupture of the ceramic or ductile fracture of the metal. Moisture was observed to cause stress corrosion effects that greatly weakened some of the interfaces.

2.8.4 STANDARD DOUBLE CANTILEVERED BEAM TEST Figure 2.13c depicts the simplest form of what is generically known as the double cantilevered beam test (the popular acronym is DCB test). One of the earlier reviews of this test was given by Bascom and co-workers42 as applied to the adhesion of metals to glass and ceramic materials. Bascom et al.43 also gave an overview of the

36

Adhesion Measurement Methods: Theory and Practice

F

Clean delamination

F

F

Delamination followed by substrate cracking

F

FIGURE 2.16 Schematic of basic failure modes of four-point bend test. A cut is first made in the coating down to the underlying substrate. A bending load is then gradually applied. The singular stress field at the edge of the cut eventually drives a delamination, which can turn into the substrate, giving rise to a crack that can later lead to spalling of the coating.

TABLE 2.2 Summary of Adhesion Strength of Various Metals to Alumina (Al2O3) Substrates Metal Nickel γ-Nickel (Cr) Gold Gold Aluminum Copper

Conditions

Range of Adhesion Strength (J/m2)

Comments

High humidity Dry air High humidity Dry air All conditions All conditions

4–8 >100 1.5–2.5 >200 >50 >150

Impurity segregation at interface Failure in metal or Al2O3 Impurity segregation at interface Failure in metal or Al2O3 Al2O3 rupture above 300 J/m2 Failure in metal or Al2O3

Note: Data summarized from work of A.G. Evans, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed., VSP, Utrecht, The Netherlands, 2001, p. 1.

application of this technique to the study of structural adhesives. These authors pointed out that one of the primary needs for the development of this technique was the evaluation of the strength and reliability of structural adhesives required to bond the new lightweight, high-performance composite materials required for the next generation of naval vessels, such as hovercraft and hydrofoils. One problem that became apparent right away is the fact that the structural adhesive materials considered showed significantly different strength properties when used as thin adhesive layers as opposed to bulk samples. The cantilevered beam configuration solved this problem with the added benefit of allowing for a relatively simple analysis of the

Overview of Most Common Adhesion Measurement Methods

37

data based on elementary beam mechanics. As shown in Figure 2.13c, the sample is prepared by carefully gluing together two identical beams of the substrate material of interest with a thin layer of the adhesive material under test. Great care must be taken regarding the surface preparation and cleaning of the beams and controlling the thickness and cure conditions of the adhesive. A spacer of some inert material such as Teflon is used at the ends of the sample to set the layer thickness and provide a well-controlled initial crack length. The sample is then mounted in a standard tensile testing apparatus in which the load-displacement behavior can be carefully determined. A fairly elementary fracture mechanics analysis based on standard beam mechanics and the classic Griffith failure criteria gives the following equation for the apparent fracture toughness of the adhesive bond:

γ Ic =

4 Fc2 ⎛ 2a 2 1 ⎞ + b 2 E ⎜⎝ h3 h ⎟⎠

(2.6)

where Fc = Critical minimum load required to initiate crack propagation γIc = Critical mode I fracture energy for crack propagation a = crack length E = Beam modulus h = Beam height b = Beam width To determine γIc, the load on the sample is ramped up until the preexisting crack just begins to propagate. This load is recorded as Fc, which then can be inserted into Equation (2.6) along with the other beam parameters to determine the critical fracture energy.

2.8.5 TAPERED DOUBLE CANTILEVERED BEAM TEST Equation (2.6) is problematic from the experimental point of view in that one has to control both the crack length and the applied load simultaneously to establish a stable constant value of γIc. This is because of the involved dependence of γIc on the beam height. Someone apparently noticed that if you tapered the beam height h such that the quantity (a2/h3 + 1/h) in Equation (2.6) remains constant, then one only has to worry about controlling the applied load. Thus, the equation describing the critical fracture energy for the tapered beam shown in Figure 2.13d can be written as

γ Ic =

4 Fc2 C b2E

⎛ 2a 2 1 ⎞ C = ⎜ 3 + ⎟ = constantt h⎠ ⎝ h

(2.7)

Adhesion Measurement Methods: Theory and Practice

Ideal case

Load

38

FC

Displacement (a)

Load

Real polymers F1 FA Displacement (b)

FIGURE 2.17 Typical load-versus-displacement data for the DCB experiment: (a) Hypothetical ideal case in which load increases up to the failure point and then propagates at a constant value determined by the fracture toughness of the adhesive joint; (b) real-world data in which the failure load oscillates between high and low values because of the strain rate sensitivity of most adhesives.

According to Equation (2.7), if we use a tapered beam with the beam height h adjusted so that the factor C in Equation (2.7) is constant, then the critical fracture energy will depend solely on the applied load at fracture. Thus, the output of the tensile test machine that generates load-versus-displacement data as the beam is pulled apart should look like the schematic plot given in Figure 2.17a. In this figure, we see the load ramping up in a linear fashion until the adhesive material gives way or starts to delaminate from either the top or bottom beam. At this point, assuming a uniform failure process, the load will stabilize at a constant level Fc, which can be substituted into Equation (2.7) to determine the critical fracture energy γIc. However, even assuming a uniform failure process, actual data tend to look more like Figure 2.17b, with a sequence of peaks and valleys instead of a steady plateau. The reason behind this behavior stems from the fact that the polymer materials that comprise the major part of the adhesive tend to exhibit strain rate-dependent failure behavior. What this amounts to in practice is that γIc tends to decrease as the crack propagates. Thus, referring to Figure 2.17b, the load increases to the level FI , at which point the crack starts to propagate. Now, as just mentioned, γIc and thus the resistance to crack propagation decreases, resulting in a lower load level to drive the crack. The lower load level, however, decreases the strain energy in the sample that is driving the crack. Eventually, the crack slows to the point at which it is completely arrested, which occurs at some load FA. At this point, the fracture resistance of the sample has returned to its zero strain rate value, and the load on the sample can now increase back to the level FI, at which the whole process can repeat. The upper value of γIc is referred to as the initiation energy and the lower value as the arrest energy.

Overview of Most Common Adhesion Measurement Methods

39

Beam

Beam

Adhesive

Adhesive

Beam

Beam

(a) Straight stable propagation

(b) Unstable wavy propagation

Beam

Beam

Adhesive

Adhesive

Beam

Beam

(c) Stable interface failure

(d) Bistable interface failure

FIGURE 2.18 Known modes of failure in a DCB specimen.

In practice, the range of behavior of DCB samples is even more complex than Figure 2.17 would suggest. Hutchinson and Suo44 reviewed the analysis of the DCB specimen and pointed out that there are at least four modes of crack propagation that have been identified (shown schematically in Figure 2.18). Each of these modes will have its own characteristic load-displacement behavior. Of particular relevance for adhesion measurement purposes is the stable interface failure mode shown in Figure 2.18c. It turns out that this mode can be selected for by using a nonsymmetric beam configuration in which one beam is stiffer than the other. In this way, the failure mode can be forced to be interfacial as opposed to cohesive in the adhesive. The DCB technique has seen extensive use in characterizing adhesive systems of all types. An entire volume could be dedicated to this activity alone. For the present purposes, however, just to give some idea of the range of values to be expected, Table 2.3 gives sample critical fracture energy data taken on a variety of polymer systems.

2.8.6 DOUBLE-CLEAVAGE DRILLED COMPRESSION TEST Figure 2.13e shows the double cleavage drilled compression (DCDC) sample, which is similar to the DCB sample in that an adhesive layer is sandwiched between two stiff beams. The main difference between the two techniques is in the mode of loading. As with the DCB sample, the DCDC sample is fabricated by gluing together two beams using an adhesive material and suitable spacers to achieve a desired uniform thickness of the adhesive layer and convenient initial crack regions. The sandwich sample is then drilled in the center symmetrically with respect to the initial crack region. The purpose of the hole is to provide a region of weakness that will

40

Adhesion Measurement Methods: Theory and Practice

TABLE 2.3 Representative Values of the Measured Critical Fracture Energies of Common Materials and Polymer Systems Material Inorganic glasses Unmodified epoxies, polyesters, and polyimides Poly(methylmethacrylate) Rubber-modified epoxies Aluminum/nylon/epoxy adhesive Metals

Critical Fracture Energy (J/m2) γIc < 10 70 < γIc 17,000

Note: Data retabulated from work of W.D. Bascom, R.L. Cottington, and C.O. Timmons, Naval Engineers Journal, 73 (August 1976).

buckle outward when the axial compressive load is applied as shown in Figure 2.13e. The outward buckling of the beam drives the interface crack in a predominantly mode I tensile opening fashion. Michalske and Fuller45 used this sample to investigate the fracture behavior of silicate glass. These authors pointed out the following advantages of using this test: 1. Use of compressive loading simplifies gripping and loading the sample and allows for more convenient use in corrosive environments, at high temperatures, and at high vacuum conditions. 2. A uniform stress intensity is maintained along the crack front. 3. Stable crack propagation is achieved along the midplane of sample. Evans46 pointed out that this sample has the further distinct advantage of decreasing strain energy release rate with increasing crack length. This property greatly simplifies the process of introducing a well-defined precrack before carrying out the adhesion measurement and allows for a more controlled experiment. This can be contrasted, for example, with the pull test, which gives rise to uncontrolled and unbounded crack propagation immediately after the onset of crack initiation.

2.8.7 BRAZIL NUT TEST Figure 2.13f gives a schematic representation of what has come to be known as the Brazil nut sample. This sample starts out as a section of a solid cylinder that is cut across a diameter and then glued back together with the material to be tested. Appropriate spacers are used to control both the bond spacing and the initial crack length. This rather implausible specimen has the advantage of controlling the mode mixity of the crack propagation by simply adjusting the angle of the bond line with respect to the direction of the applied compressive load. For instance, setting bond line at an angle to the applied compressive load as shown in Figure 2.13f results in

Overview of Most Common Adhesion Measurement Methods

41

a predominantly mode II shearing load. On the other hand, setting the bond line nearly parallel to the applied load gives loading conditions similar to the DCDC test, which is predominantly mode I tensile crack opening. This specimen clearly has a strong advantage when one is interested in testing the bond strength as a function of the mode of loading. The Brazil nut test has been in use for quite some time to test homogeneous solid specimens47 and was apparently first adapted to test interfacial toughness by Wang and Suo.48 An overview of this test has been given by Hutchinson and Suo.49 One of the interesting and useful features of this test is the fact that residual stresses within the adhesive layer do not contribute to the driving force for crack propagation. Thus, unlike standard tests such as peeling or the DCB method, one does not have to take into account residual stresses within the adhesive layer to compute the true surface fracture energy. This property combined with the ability to adjust the mode mixity of crack propagation easily make this test a favorite when carrying out fundamental studies on interface adhesion. An interesting study was done by Lee,50 who used the Brazil nut configuration to study the adhesion of epoxy molding compound to copper lead frame substrates. This study was prompted by the need in the microelectronics industry to understand the adhesion of these materials, which are important for packaging silicon chips. It turns out that although copper is an excellent conductor, it does tend to oxidize easily, and loss of adhesion between oxidized copper and the epoxy compound has been blamed for a loss of adhesion between the two materials that can give rise to a notorious form of blistering known as the popcorn effect. What happens is that moisture can aggregate at the delaminated interface and then form a blister when heated as would happen in a wire bond or die attach procedure. Lee was able to fabricate Brazil nut-type specimens of the epoxy/oxidized copper materials and then investigate the fracture toughness as a function of the mode mixity of the applied load. For mode I (predominantly tensile opening) loading, his data showed that the fracture toughness was very close to that measured for the same materials but using a DCB specimen geometry. However, when loading under conditions carrying a high shear component or mode II-type load, the measured fracture toughness was roughly twice that obtained for mode I conditions. This study clearly indicated the practical usefulness of the Brazil nut specimen because one can clearly be mislead about the adhesion strength when relying on only one mode of loading.

2.8.8 WEDGE TEST Figure 2.13g illustrates the wedge test, by which a sandwich laminate is loaded by simply forcing a wedge into one end of the laminate. This test has been used effectively in the aircraft industry to evaluate the durability of sandwich layers of thin aluminum sheets bonded with an adhesive. An interesting study carried out by the Boeing company was informatively reviewed by Pocius.51 The main advantage of the wedge test is the fact that many samples can be easily and cheaply fabricated and then subjected to any variety of environmental stress conditions to determine the durability of the bond. The success of this method has led to the formulation of

42

Adhesion Measurement Methods: Theory and Practice

American Society for Testing and Materials (ASTM) Standard D3762, which describes in detail sample preparation and testing procedures. By loading the sample using the simple insertion of a wedge at one end, a constant load can be applied at a level just below that required for crack propagation. The sample can now be placed in a hostile environment (e.g., high temperature or humidity), and the progress of any preexisting crack can then be monitored as a function of time. For a good bond, the crack should be short and primarily within the adhesive layer itself. A faulty bond is indicated when the crack is relatively long and propagating along the metal/adhesive interface. The wedge test has found fairly wide application for testing the durability of adhesives. Interesting examples include the work of Sharif et al.,52 who used the wedge specimen to test the effectiveness of model copolymer adhesives on glass. Davis et al.53 used the technique to test the effectiveness of plasma sprayed coatings on titanium and aluminum, and Meyler and Brescia54 used the technique to test a variety of waterborne adhesives on aluminum and aluminum-lithium surfaces. The main advantage of the wedge test lies in the ability to easily create a large number of samples that can be used for long-term environmental stress testing. Also, because the method is basically grounded in the mechanics of bending beams, it can be analyzed quantitatively using standard fracture mechanics analysis.55–58

2.8.9 TOPPLE BEAM TEST As a final example of an adhesion test based on the mechanics of a bending beam, we mention the topple beam test as shown schematically in Figure 2.13h. This test has much in common with the well-known pull test discussed in Section 2.4, with the crucial difference being the mode of loading the sample. All of the sample preparation procedures prescribed for the pull test apply equally to the topple beam experiment. This experiment in fact shares just about all the advantages and disadvantages encountered in the pull test. One advantage of the topple beam, however, is that the mode of loading is nearly pure bending, allowing for a simplified analysis. Apalak59 in particular carried out an extensive mechanics analysis of the topple beam geometry, including the effects of geometric nonlinearity caused by large rotation of the beam. Another distinct advantage of the topple beam over the pull test is the fact that, by applying a lateral load to the top of the beam, the problem of gripping the beam is relatively trivial compared to the pull test, which has to ensure proper gripping to avoid slippage. This can be a significant problem when using beams made of hard brittle materials. Finally, with the pull test one has to be careful to apply the tensile load exactly along the beam axis to avoid applying a bending moment to the beam, a problem that does not arise in the topple beam approach. An overview of this method was given by Butler,60 and an application to metal films was provided by Kikuchi et al.61 It might be added in closing that the topple beam test has much to recommend it for the adhesion of pins on ceramic substrates. As mentioned, the pin pull method is widely used for testing pin adhesion. However, when inserting a pin into a socket there is always a significant bending load present.

Overview of Most Common Adhesion Measurement Methods

43

From the point of view of reliability testing, one would prefer that the pin should bend as opposed to tearing off the pad. A bent pin can be straightened, but a tear-off failure can render an entire substrate useless. The topple beam experiment is clearly an efficient way to sort out these distinct behaviors in a population of pins attached to a rigid substrate.

2.8.10 ADVANTAGES

OF

BEAM-BENDING TESTS

It is clear that the main advantage of using any one of the tests described in the previous sections is that they all lend themselves relatively easily to quantitative analysis using the methodology of fracture mechanics, which is described in detail in Chapter 4. The mechanics of bending beams was one of the earliest and quite likely the most studied topic in the history of applied mechanics. An extensive body of literature exists that can be called on to supply stress/strain solutions for nearly any beam configuration that can be imagined. Thus, it is fairly straightforward to convert load-displacement data taken on any of the samples shown in Figure 2.13 into fracture toughness or surface fracture energy results that are directly relevant to the adhesion failure process investigated. This type of data is especially important as input to detailed fracture mechanics-based models, which attempt to predict the failure of structures based on geometry, material properties, and loading conditions. A second advantage of beam-based tests is the ability to fabricate a large number of samples relatively easily for testing under a variety of conditions.

2.8.11 DISADVANTAGES

OF

BEAM-BENDING TESTS

As always, we have to recognize that there are no ideal adhesion tests, and the beambending methods are no exception. The key advantage of having a simple geometry that is suitable for analysis leads to the main disadvantage of these tests, which is the very limited sample geometries that can be investigated. Ideally, someone manufacturing automobile fenders would like a test that could indicate how well the paint is adhering to the metal and that could be implemented on the manufacturing line to give real-time results on a wide variety of fender shapes. The beam-bending experiments clearly do not fit the bill here and are thus confined to use solely in the testing laboratory. The second most serious complaint that can be lodged against the beam-bending methods is whether they adequately simulate the stress/strain loading environment that real manufactured parts must endure. In particular, cases for which the main mode of failure is through internal stresses, such as those caused by thermal expansion mismatch strains, the delamination process is driven mainly by the elastic energy generated by the stresses. In such cases as when, for example, a highly stressed coating deadheres spontaneously from its substrate, the delamination process occurs under near-infinitesimal strain conditions. In all of the beam-bending tests, however, the delamination process is driven by external loading at substantial levels of deformation and strain. Although the level of deformation is nowhere near that generated by something like a peel test, nonetheless this calls into question the relevance of beam-bending data for such situations.

44

2.8.12 SUMMARY

Adhesion Measurement Methods: Theory and Practice AND

RECOMMENDATIONS

The main conclusion that arises out of all the above discussion is that the bending beam experiments are quite likely the methods of choice when fully quantitative data is required, such as for critical surface fracture energies or mode I and mode II fracture toughness data. The bending beam methods provide the most reasonable way of obtaining fracture and delamination data over the entire range of mode mixity for a wide range of adhesive/adherend combinations. Sample fabrication is demanding but not excessively so. Geometries such as the wedge test allow generation of many samples for testing under a wide range of environmental conditions while giving quantitative data without the need for elaborate test equipment. On the downside, it must be recognized that the beam-bending tests will find best application in the laboratory environment as opposed to the manufacturing line. This arises primarily from the highly restricted sample geometries involved plus the need for careful sample fabrication and nontrivial data analysis.

2.9 SELF-LOADING TESTS It is well known that the internal stress in a coating can cause it to delaminate spontaneously from the underlying substrate. This effect is commonly seen in old paint coatings on wood trim and other artifacts in which shrinkage stresses in the coating cause it to peel back from the edges and other internal defects. The idea that naturally suggests itself is to set up an adhesion measurement experiment in which the driving force for delamination is derived solely from well-controlled internal stresses in the coating to be tested. The task of the experimenter is then reduced to monitoring the propagation of the delamination front at a known fixed level of internal stress. A number of experiments along these lines are discussed next. One of the major advantages of this type of experiment is that the loading conditions closely resemble those that initiate failure in real coatings subjected to field conditions.

2.9.1 CIRCLE CUT TEST Figure 2.19 gives a schematic illustration of what is called the circle cut test. In this experiment, one has a coating on a substrate with a uniform biaxial stress σ0 that can be caused by any number of factors, such as deposition conditions, thermal expansion mismatch strains, shrinkage caused by solvent loss, and so on. At time zero, a circular cut is made somewhere in the interior away from any edge, giving rise to the situation shown in Figure 2.19. As explained in Chapter 4, the act of generating a sharp edge creates a stress singularity at the edge of the cut at the interface between the coating and the substrate. If the adhesion of the coating is relatively weak, then the coating will deadhere from the substrate, forming an annular ring of delaminated material as shown in Figure 2.19. The radius of the cut and the radius of the delaminated annular region are then measured by optical or other means, and this information can then be used along with knowledge of the stress level σ0 in the coating and its elastic properties to calculate the critical surface fracture energy according to the following formula:

Overview of Most Common Adhesion Measurement Methods

45

a R h σ0

σ0

FIGURE 2.19 Schematic of circle cut test. A circular hole of radius R is cut in a coating carrying an internal stress σ0. If the coating adhesion to the substrate is insufficient, then because of the stress singularity at the edge of the hole, the coating will delaminate out to a radius R + a. The driving force for delamination can be easily determined if one knows the elastic constants of the coating, the film stress, and the geometric parameters in the diagram.

Gc =

β= where R, h, and a σ0 E v Gc

= = = = =

⎤ hσ 20 ⎡ 2β 2⎥ 2⎞ E ⎢⎢ ⎛ ⎡a⎤ ⎥ ⎢ ⎜ 1 + β⎢ ⎥ ⎟ ⎥ ⎣ R ⎦ ⎟⎠ ⎥⎦ ⎢⎣ ⎜⎝

(2.8)

1− ν 1+ ν

Coating and cut dimensions as shown in Figure 2.19 Residual stress in coating Modulus of coating material Poisson’s ratio of coating critical strain energy release rate

A convenient feature of this test is the fact that, according to Equation (2.8), the size of the annular delamination region will always be constrained because the driving force Gc decreases as the size of the delaminated region increases. Thus, at some finite value a, the driving force for deadhesion will be too small to propagate the delamination any further, and the experimenter can make the appropriate measurements at leisure. Farris and Bauer62 used this method to study the adhesion of polyimide coatings. This approach has a number of distinct advantages, including: •

• •

Close simulation of the mechanism by which coatings tend to delaminate under field conditions of high stress, low strain, and mixed-mode conditions of tension and shear Relative ease of sample preparation Amenability to quantitative analysis

46

Adhesion Measurement Methods: Theory and Practice

The main drawback is that because the driving force for delamination relies solely on the internal film stresses, there may not be sufficient strain energy in the coating to initiate a delamination if the level of adhesion is too high. This fact tends to limit this test to coatings with weak adhesion.

2.9.2 MODIFIED EDGE LIFTOFF TEST In view of the limited applicability of the circular cut test to weakly adhering coatings, a related approach called MELT (modified edge liftoff test) has been explored by Hay et al.63 The main innovation in this approach is the use of a layer of material on top of the coating to be tested that will drive up the total internal stress and thus give sufficient driving force to delaminate any coating. A schematic representation of this test is given in Figure 2.20. As shown in the figure, complications can arise because of crack initiation in the substrate rather than the interface of interest. Hay and co-workers exercised this technique on a multilayer sandwich consisting of epoxy/dielectric layer/silicon nitride/native oxide/silicon. They sidestepped the substrate fracture problem by using a hydrofluoric acid solution to etch out a large initial crack in the silicon nitride layer. In addition, they polished the edge of the sample with fine sandpaper to eliminate any flaws left behind by the wafer dicing operation. A thick epoxy top layer between 150 and 200 μm provided the driving force for crack propagation caused by thermal expansion mismatch with the silicon substrate. Under these conditions, they observed clean delamination of the dielectric layer from the silicon nitride. These workers noticed an interesting property of their epoxy-loaded samples that seemed to contradict previous work that used chromium as a superlayer instead of epoxy. From the chromium work, it was noticed that the driving force for delamination depended on the size of the initial crack length and did not settle down to a constant value until the delamination length had reached at least 20 times the chromium layer thickness. With the epoxy-loaded samples, there was no apparent Stressed superlayer σ Sample coating Delamination Substrate

Substrate crack

FIGURE 2.20 Schematic of the modified edge liftoff test (MELT), which attempts to circumvent the limitation of the self-loading test to the case of relatively weak adhesion, as in the circular cut test shown in Figure 2.19. A top layer of material with known internal stress behavior is applied to increase the delamination driving force to any desired level. As can be expected, a number of complications can arise, including possible failure of the underlying substrate.

Overview of Most Common Adhesion Measurement Methods

47

dependence of the driving force for delamination on the initial crack size. A subsequent finite element analysis of the problem comparing the driving force for delamination for both the epoxy- and chromium-loaded systems indicated that indeed the behavior of the epoxy and chromium systems is very different. In the epoxy case, the driving force rises so sharply with crack length it nearly resembles a step function. In the chromium system, the driving force rises much more slowly and essentially follows the rule of 20 times the chromium thickness before leveling off to a steady state.

2.9.3 MICROSTRIP TEST The microstrip test is closely related to MELT in that the same principle of using a superlayer on top of the layer to be tested is employed to obtain a sufficient driving force for delamination. A schematic of the basic sample configuration is shown in Figure 2.21. The version of the test described here was carried out by Bagchi et al.64 and reviewed by Evans.65 What is shown in the figure are the various layers of the adhesion measurement test structure. The substrate may be a block of ceramic or glass or whatever the material of interest is. On top of the substrate, narrow parallel strips of a release layer material are first deposited. A typical release layer strip is visible in the uncoated regions separating the sample strips shown in Figure 2.21. Next, the coating is applied as a blanket layer. On top of that, the superlayer is deposited as a blanket coating. A good candidate for this material when testing thin metal films is chromium, which can develop internal stress levels up to 1 GPa. The blanket coatings are now etched into thin strips perpendicular to the release layer strips using photolithographic methods. Sample strips

Cut

Release layer

FIGURE 2.21 The microstrip test is yet another self-loading adhesion test that takes advantage of photolithographic methods to create a large number of test specimens on a single substrate. The figure shows a greatly enlarged view of three test strips. The horizontal stripe is a release layer material to which the coating has poor adhesion. After applying blanket coatings of the test film and the loading layer, a large number of test strips are then etched out using lithographic methods. A cut is then created in the strips in the region where they overlay the release layer. Because of the poor adhesion to the release layer, delamination is immediately initiated and will proceed to propagate into the strip. However, the nature of the driving force is such that delamination will always terminate before the strip is entirely peeled off the substrate. The length of remaining adhered ligament can then be used to compute the surface fracture energy.

48

Adhesion Measurement Methods: Theory and Practice

The adhesion test begins after a thin cut is made down the center of the release layer strip using either etching or milling techniques. As the adhesion at the release layer is very weak by design, a delamination is immediately initiated starting from the cut to the edge of the release layer. Depending on conditions, the delamination front will proceed past the edge of the release layer and into the interface between the sample coating and the substrate. If the delamination stops at the edge of the release layer, then clearly there is not enough strain energy in the chromium superlayer, and a thicker layer of chromium needs to be applied. At a sufficient thickness of the chromium layer, the delamination will proceed at the coating/substrate interface or possibly proceed as a subcrack in the substrate depending on how well adhered the coating is. Assuming that the delamination proceeds at the coating substrate interface, it will go for a certain distance and then arrest. In this test, all of the test strips are finite length, and the driving force for delamination decreases toward zero as the crack front nears the end of the strip. Therefore, the delamination front must arrest, and the length of the remaining ligament is therefore indicative of the adhesion between the coating and the substrate.

2.9.4 ADVANTAGES

OF

SELF-LOADING TESTS

Self-loading tests come very close to mimicking the conditions under which real coatings delaminate in terms of strain level and mode mixity; this is their main advantage as an adhesion test. This is especially true for microelectronic structures, for which intrinsic stress is one of the major causes of device failure. In addition, the self-loading tests lend themselves readily to quantitative analysis because the strain level at failure is typically quite low, and linear elastic theory suffices to carry out the required fracture mechanics evaluation of the strain energy release rate. When used to evaluate microelectronic devices, the test structures required to carry out the adhesion measurements can be fabricated using equipment nearly identical to that used in the production line. Thus, although sample preparation is fairly involved, it does not require resources beyond what should already be available in the existing manufacturing facility. Finally, the test structures can be integrated into the actual manufacturing process as diagnostic probe sites capable of giving near-real-time quality control and monitoring information on real manufacturing parts. Of all the adhesion tests discussed so far, the self-loading tests come the closest to an ideal adhesion measurement method.

2.9.5 DISADVANTAGES

OF

SELF-LOADING TESTS

The main disadvantage of the self-loading tests is the need to know the internal stress and mechanical properties of the coating to be tested. The problem of determining the internal stress in a coating is a rather large subject, and an entire chapter in this volume (Chapter 6) is devoted to just this problem. Further complications arise if the internal stress level is insufficient to cause delamination and one of the superlayer methods must be implemented, thus greatly increasing the work required for sample preparation. Finally, the trajectory of the delamination crack front may deviate from the interface into either the substrate or the coating, depending on conditions. This will significantly complicate the fracture mechanics analysis involved.

Overview of Most Common Adhesion Measurement Methods

49

In essence, the self-loading tests share the common problems of all fully quantitative tests in that they inevitably involve much more work than the simply qualitative or semiquantitative methods.*

2.9.6 SUMMARY

AND

RECOMMENDATIONS

The self-loading adhesion tests are most suitable when quantitative data is required to support numerical modeling simulations of the structures under fabrication. Multilevel wiring structures from the microelectronics industry are a prime example of an application that can benefit greatly from this type of test. Such structures are replete with interfaces between dissimilar materials that are subject to numerous manufacturing processes that can introduce high levels of internal stress. As a specific example, consider the use of organic insulators as dielectric layers in multilevel wiring schemes. Some of the most popular materials for this application are the polyimides. These materials are typically coated as a viscous liquid using either spin- or spray-coating methods. The resulting film must be cured at an elevated temperature, generally above 300°C to achieve the correct electrical and mechanical properties required. Cooling to room temperature will induce a large internal thermal expansion mismatch strain in the coating if the underlying substrate is either silicon or a ceramic material because most polyimide materials have thermal expansion coefficients 10 to 30 times larger than either silicon or most ceramics. An elementary calculation using the principles of continuum theory covered in Chapter 3 shows that the resulting stress level in the coating can come to nearly 50% of the yield stress of the polyimide itself. In such cases, appropriate stress modeling supported by fully quantitative adhesion data are required to carry out the type of engineering design analysis necessary to support the fabrication and manufacture of a useful device. The large amount of work involved in implementing the self-loading methods will quite likely limit them to this type of application.

2.10 MORE EXOTIC ADHESION MEASUREMENT METHODS 2.10.1 LASER SPALLATION: EARLY WORK Up to this point, the adhesion tests under discussion have been of a fairly prosaic nature in that the mode of loading has always been some kind of mechanical tension, compression, or shear applied by a mechanical test apparatus, by the residual stress in the coating, or by some applied superlayer material. For the laser spallation test, however, the loading conditions are rather exotic in that they involve highly transient shock waves induced by ultrafast laser pulses. In a typical test, a laser pulse with a fluence of 500,000 J/m2 is focused onto a 1-mm diameter spot for 30 nsec, which amounts to energy deposition at a power rate of 13 MW.

* As a general rule of thumb, when going from a qualitative test to a fully quantitative one, you can expect to work not only twice as hard to obtain acceptable results but more likely 10 times as hard. This almost seems to be some kind of thermodynamic theorem proved through difficult experience if not from any formal axiomatic demonstration.

50

Adhesion Measurement Methods: Theory and Practice

This test was apparently first discussed in the open literature by Vossen66 and Stephens and Vossen,67 who used it to investigate the adhesion of metals to glass. A typical experimental setup is shown in Figure 2.22. In the earlier experiments, an array of islands of the coating to be tested were evaporated onto a glass substrate. Small islands were used to avoid the effect of tearing of the film, which would occur during the spallation of a continuous metal film. The opposite side of the glass substrate was coated with an energy-absorbing layer such as titanium. During a standard experiment, a high-intensity, short-duration laser pulse is directed at the titanium layer on the back side of the sample. The effect on impact is literally explosive vaporizing of the titanium and blasting it off while simultaneously depositing a large amount of heat into the underlying glass in a very short time. The recoil of the blasted titanium combined with the rapid thermal expansion of the glass generates a compressive shock wave that propagates to the front side of the glass, where the islands of deposited metal are waiting. The compression wave is reflected at the front surface of the substrate as a tensile wave caused by the rapid tensile snap back of the substrate. The elastic snap back propagates across the substrate metal interface, providing the rapid tensile loading that ejects the metal islands off the substrate. To determine the adhesion strength of the coating, the energy of the laser pulse is ramped up systematically until coating failure is first observed. Depending on conditions, a variety of collateral damages can occur to both the substrate and the coating tested. Vossen pointed out in particular that brittle substrates tend to shatter. However, one experiment used islands of gold deposited on glass and clearly demonstrated clean delamination. Backing layer Laser

Substrate

Sample island Compressive shock wave

(a) Pulse initiation

Backing layer Laser

Substrate Detached sample ﬁlm Reﬂected tensile wave

(b) Reﬂected tensile wave

FIGURE 2.22 Laser spallation experiment: (a) A high-intensity laser pulse impinges on the back of the substrate, initiating a strong compressive stress pulse because of the rapid heating at the point of impingement; (b) the compressive pulse reflects off the coating/substrate interface, generating a strong tensile reflective wave, which can cause delamination of the coating.

Overview of Most Common Adhesion Measurement Methods

Absorbing layer Backing layer Nd: Yag-laser

51

Sample coating Mirror 1

Substrate

Beam splitter Mirror 2

Lens Compressive shock wave Computer

He-Ne laser Photodetector digitizer

FIGURE 2.23 Improved laser ablation experiment. The basic principle is the same as in Figure 2.22 with the following improvements: (1) A backing layer is added over the energyabsorbing layer to carry away excess thermal energy that would otherwise create a long tail on the induced compressive pulse, which significantly reduces the resolution of the method. (2) A laser Doppler interferometer is employed to monitor the displacement of the sample surface in real time as it deforms because of the impinging stress pulse. This allows for an independent determination of the critical stress level for delamination.

2.10.2 LATER REFINED EXPERIMENTS The early experiments on laser spallation demonstrated that the technique could be used to test the adhesion of coatings in a unique way. A number of problems hindered progress, however, including the use of expensive finicky equipment that required careful and time-consuming calibration procedures. In addition, a large thermal stress tail followed the main pulse and limited the resolution that could be achieved in stressing the coating substrate interface. Additional problems, such as fracture of brittle materials, excessive stress damping, and potential decomposition of viscoelastic media, essentially limited the method to testing refractory materials. Advances in technology and techniques, however, have greatly improved the laser spallation test, as discussed by Gupta et al.68 Figure 2.23 illustrates an improved version of the laser spallation experiment shown in Figure 2.22. The new features in this version of the laser spallation experiment include 1. Inclusion of an absorbing layer between the back side of the substrate and a backing layer. This approach allows the user to nearly eliminate the long thermal stress tail associated with the earlier approach by essentially ablating away the excess thermal energy into the backing layer instead of letting it diffuse into the substrate, where it induces a large thermal stress. This long-tail thermal stress can confound the data analysis, especially when dealing with very thin sample coatings.

52

Adhesion Measurement Methods: Theory and Practice

2. Use of a laser Doppler interferometer to monitor in real time the deformation and velocity of the sample coating during impact by the reflected tensile shock wave. Use of this equipment allows the user to quantitatively estimate the tensile stress at the interface that initiates film separation from the substrate. 3. Using the quantitative stress measurements taken from the interferometer data, one can further estimate an “intrinsic” surface fracture energy associated with the film delamination. 4. Use of a modified interferometer to deal with nonspecular reflection off rough surfaces. The main advantage of the new approach is the ability to use the velocity/displacement data taken by the interferometer to estimate the critical stress level at which coating spallation occurs. As with the old method, the laser power is increased incrementally until spallation is observed. Table 2.4 lists sample values for the critical stress for coating liftoff for several coating substrate systems. The strength values listed in Table 2.4 are similar to those that might be obtained in a pull test or other form of tensile test. The main difference is the dynamic nature of the tensile shock pulse, which hits the interface at a strain rate on the order of 107 sec−1. At such an enormous strain rate, we can expect the material response to be significantly different from what would occur in a standard pull test. In particular, viscoelastic effects should be “frozen out,” giving rise to nearly pure brittle fracture because most molecular relaxation behavior will be too slow to follow the rapid deformation pulse. Finally, by using a recently developed scaling relationship for the binding energy-versus-distance curves for metals, Gupta et al.69 were able to convert their

TABLE 2.4 Representative Values of the Interface Strength for Selected Coating Substrate Systems

Substrate Polyimide Copper Copper Silicon carbide Alumina/diamond composite Alumina/diamond composite

Coating

Interface Strength σmax (GPa)

Silicon Silicon nitride Pyrolytic graphite Pyrolytic graphite CVD diamond CVD diamond

0.46 0.041 0.015 3.4–7.48 1.61 1.41

Comments 5.3-μm polyimide 0.1-μm copper on nitrided silicon 2.1-μm SiC on 1.69mm disc 5% of 1-μm diamond particles 5% of 10-μm diamond particles

Note: Data retabulated from V. Gupta, J. Yuan, and A. Pronin, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed., VSP, Utrecht, The Netherlands, 1995, p. 367.

Overview of Most Common Adhesion Measurement Methods

53

interface strength data to fracture toughness values similar to that obtained in the bending beam tests. By using physical arguments based on the nature of metal-tometal interactions at the interface between different metals, these investigators derived the following relationship between their measured critical interface stress and what they called the intrinsic toughness or ideal work of interfacial separation Gco: σ 2max =

Gco Eo e 2h

(2.9)

where σmax = Critical interface strength as shown in Table 2.4 Eo = Modulus at interface Gco = Intrinsic interface toughness h = Unstressed separation distance between atoms e = Mathematical constant epsilon, which is the base of the natural logarithms = 2.71828183 The quantity σmax is measured directly by the laser spallation experiment, and representative values are shown in Table 2.4. The unstressed separation distance h can be determined by direct transmission electron microscopy measurements, and the interface modulus Eo is inferred from delamination experiments and from published data. With this data in hand, Equation (2.9) can be used to estimate the apparent critical surface fracture energy Gco. Values for selected systems are summarized in Table 2.5.

TABLE 2.5 Values of Critical Intrinsic Surface Fracture Energy from Laser Spallation Measurements Interface System Silicon carbide/pyrolytic carbon ribbon Silicon carbide/silicon Cleavage of (111) planes of silicon Niobium/Al2O3

Critical Surface Fracture Energy Gco (J/m2) 3 3.31 0.84 0.0009

Comments h = 0.9 nm from TEMEo = 107 GPa (average of two media) h = 0.5 nm; Eo = 115 GPa Stress pulse sent normal to (111) planes; h = 0.32 nm; E111 = 185 GPa Value considered faulty because of interface flaws; should be close to 0.69

Note: Data tabulated from V. Gupta, J. Yuan, and A. Pronin, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed., VSP, Utrecht, The Netherlands, 1995, p. 395.

54

Adhesion Measurement Methods: Theory and Practice

In evaluating the data in Table 2.4, one has to keep in mind that the coatings studied were delaminated from their substrates under extreme loading conditions (strain rates near 107 sec−1) for which material properties and viscoplastic deformation behavior in particular can be expected to differ significantly from those in effect for the more standard adhesion tests, such as the bending beam experiments discussed in this chapter. The authors of this work went so far as to suggest that the quantity they called Gco be called an intrinsic critical surface fracture energy in distinction to the usual Gc because many of the viscoplastic processes that contribute to Gc will be frozen out in the laser spallation experiment. In other words, the various atomic/molecular deformation processes that can contribute to the measurement of Gc are too slow to play a part in the laser spallation experiment.

2.10.3 LASER-INDUCED DECOHESION SPECTROSCOPY EXPERIMENT A variant of the laser spallation experiment goes under the acronym LIDS, which stands for laser-induced decohesion spectroscopy* has been discussed by Meth.70 A schematic of the LIDS experimental setup is shown in Figure 2.24. Strictly speaking, the LIDS experiment is not a spallation test as discussed above because the coating is not removed from the substrate; however, laser energy is used to deadhere the coating, which is sufficient qualification to be included. Referring to Figure 2.24, the basic experiment consists of directing an infrared laser beam onto the sample to be tested, which is a multilayer laminate composed of a substrate, an energyabsorbing layer, and a top coating. The absorption properties of the coating are such that the laser radiation passes through and is soaked up predominantly by the underlying absorbing layer, which rapidly decomposes, giving rise to a gas pressure that initiates blistering of the coating much as one would observe in the standard blister test. At a sufficient level of laser power, the blister will propagate into an annular debonded region that can be monitored by optical means. The curvature of the blister is monitored simultaneously by reflecting a second laser beam from a low-power He-Ne laser off the top of the blister. The reflected laser beam passes through a fixed aperture and then onto a photodetector, which measures the intensity of the light passing through the aperture. When no blister is present, a fixed and calibrated intensity of reflected light is measured. After blistering, the reflected light is spread out in proportion to the blister curvature; because the aperture is fixed, less light reaches the photodetector, and the measured intensity drops. Thus, the blister curvature can be inferred from the light intensity observed at the photodetector. Meth70 discussed the details of the calculation used to determine the curvature based on a Gaussian beam shape. With the size and curvature of the blister in hand plus knowledge of the elastic properties of the coating, the gas pressure causing the blister can be inferred through a classical continuum mechanics calculation that treats the blistered coating as a plate subjected to uniform pressure from below. Much of this analysis is already known from standard blister test theory, and full details are covered by Meth.70 By carefully observing the laser power required to * A more appropriate designation would be laser-induced deadhesion spectroscopy. Another problem is that this experiment has nothing to do with spectroscopy as it is commonly understood.

Overview of Most Common Adhesion Measurement Methods

55

Infra red laser He-Ne laser

Photodetector Aperture

Coating Absorbing layer

Substrate

FIGURE 2.24 LIDS experiment. Strictly speaking, this is not a laser ablation experiment but is close enough to warrant consideration here. A strong laser pulse is directed at the coating substrate interfaces. Gases created during the intense heat buildup create a blister in the coating, which can further delaminate as in the standard blister test. The curvature, and thus the size, of the blister is monitored by reflection of a weak laser beam off the top of the blister into a photodetector.

just initiate annular debonding of the blister, one can further apply standard blister test methods to determine the critical surface fracture energy for delamination.

2.10.4 ADVANTAGES

OF

LASER SPALLATION TESTS

The main advantage of the laser spallation test derives from the unique way in which the delamination load is applied to the coating under investigation. No gripping scheme is required, and the ultrahigh loading rate precludes many viscoelastic/ viscoplastic mechanisms, which tend to cloud the analysis of more conventional adhesion tests, such as the bending beam methods discussed in Section 2.8. Laser spallation may in fact be the only effective method for analyzing refractory systems such as the diamond-on-alumina samples. This technique is also amenable to full quantitative analysis because of the availability of advanced instrumentation such as the laser Doppler interferometer. The LIDS version of this test has the potential of application to a wide variety of surfaces, including actual parts from the manufacturing line, because the laser pulse and surface displacement measurement are applied directly to the top surface of the coating under study. The fact that this is a noncontact method that can be fully automated makes it possible to implement the LIDS experiment directly on the manufacturing line as a real-time quality control tool.

2.10.5 DISADVANTAGES

OF

LASER SPALLATION TEST

The same properties that give the laser spallation test its unique advantages also impart a number of its most important disadvantages. The most significant disadvantage derives from the ultrahigh strain rates involved. To perform the laser Doppler

56

Adhesion Measurement Methods: Theory and Practice

measurements required to gain quantitative information on the adhesion strength of the coating, one needs to measure stress pulses with rise times shorter than 5 nsec, which necessitates the use of 10- to 100-GHz transient digitizers. The photodetector for measuring the laser pulse should have a rise time of less than 200 psec, which will allow a measurement of interference fringes with a resolution on the order of 0.2 nsec. Needless to say, this is not the type of equipment likely to be found at a local hardware store. Thus, it is clear that this method is going to require expensive equipment that is not readily available. A second limitation of the laser spallation technique is the relatively difficult and limited sample configurations available. The need for special backing and absorbing layers will quite likely limit this method to use in the development laboratory only. Finally, the fact that ultrahigh strain rates are involved in removing the coating from the substrate complicates the problem of interpreting the resulting data in terms of typical field conditions.

2.10.6 SUMMARY

AND

RECOMMENDATIONS

The laser spallation adhesion test is one of the more exotic adhesion measurement methods and has some unique advantages to recommend it in certain situations. In particular, it may be the only method available to reasonably test highly refractory coatings that are either too brittle or too hard to be tested by more conventional methods. The instrumentation required for fully quantitative measurements is not commonly available but can be purchased from specialty vendors. This equipment is expensive, so the need for the required data must be sufficiently compelling. The LIDS version of this technique has a number of potentially useful applications given the fact that it is a noncontact method that can be fully automated. There is a definite prospect for use in real-time manufacturing quality control applications because it can be applied to very small test sites and requires no special sample preparation whatever. The only special requirement is the need to tailor the spotforming laser pulse to be absorbed preferentially by an existing underlayer of the coating to be tested.

2.11 ELECTROMAGNETIC TEST Another fascinating adhesion test method is the electromagnetic test, which utilizes the surprisingly large forces that can be developed by currents in a magnetic field. Figure 2.25 gives a schematic illustration of the basic configuration for lifting a metal line off of an insulating substrate. This figure shows a cross section of the metal line that is directed out of the page and carries a current I also directed out of the page. A magnetic field B is applied at a right angle to the flow of the current giving rise to a Lorentz force F acting perpendicular to the metal/substrate interface. For this configuration, the Lorentz force is given by the following formula from basic electromagnetic theory: F = Il × B

(2.10)

Overview of Most Common Adhesion Measurement Methods

57

W Metal line

I B

h

F

Insulating substrate

FIGURE 2.25 In the electromagnetic test, a current I flows in a metal test line in the presence of a perpendicular magnetic field. If the current and the magnetic field are sufficiently strong, then the line can be lifted off the substrate because of the induced Lorentz force.

where F I l B

= = = =

Lorentz force Current flowing in line Unit length vector in direction of current flow Magnetic field vector

The right-hand side of Equation (2.10) involves the vector cross product between the length vector l and the magnetic field B. For the geometry in Figure 2.25 with l and B mutually perpendicular, the cross product evaluates to lB, and the Lorentz force becomes F= IlB pointing normal to the substrate surface as shown. What is of primary interest, however, is the stress on the line, which is evaluated by dividing the force by the area A = lw, which gives the following very simple formula for the normal stress tending to lift the line off the substrate:

σn =

IB w

(2.11)

Equation (2.11) gives the normal stress on the metal line caused by the Lorentz force induced by the interaction of the current I with the magnetic field B where w is the width of the line. If we assume a magnetic field of 2 T (Tesla) and a current of 30 A (ampere) with a line width of 1 μm Equation (2.11) gives the substantial normal stress of 60 MPa. Referring to Table 2.4, we see that this stress level is more than sufficient to lift a copper coating off of a silicon nitride substrate as evaluated by the laser spallation method. However, those familiar with electromagnetics will immediately detect a potential problem in that 30 A is a substantial current to pass

58

Adhesion Measurement Methods: Theory and Practice

through a 1-μm wide line, or any metal wire for that matter, without vaporizing it. Therefore, we really need to investigate the temperature rise we can expect by performing this experiment. One way to keep from cooking the sample before delamination can be observed is to use very short current pulses on the order of 1 μsec. Making this assumption, the expected temperature rise in the line can be easily calculated from Fourier’s heat transfer equation given by Equation (3.36) and summarized in Table 3.1. Because we are talking about very short heating times, we can ignore diffusion effects and thus leave out the spatial derivatives (i.e., ∇2T) and work with the following simple relation, which will be valid for the short timescale under consideration: dT γ = dt ρc

(2.12)

Because all quantities on the right-hand side are constants, this equation readily integrates to give the following relation for the expected temperature rise: ΔT = T − T0 =

γt ρc

(2.13)

where ΔT γ ρ c

= Temperature rise above ambient in degrees centigrade = Heating rate per unit volume caused by joule heating (J/sec m3) = Density of metal (kg/m3) = Specific heat of metal [J/(kg degrees centigrade)]

The heating rate can be estimated from the joule heating caused by the electric current I. Elementary circuit theory tell us that this is given by the product I 2R, where I is the current, and R is the line resistance. The line resistance is further given in terms of the metal resistivity r by the simple formula R = rl/A, where r is the resistivity, l is the length of the line segment, and A is the cross-sectional area. Dividing the input power I 2R by the total volume of the line segment (lA) gives the heating rate per unit volume as γ = I 2r/A2. Inserting this expression into Equation (2.13) gives our final expression for the expected temperature rise in the line segment on application of a current I for a time duration t: 2

rt ΔT = I 2 ρcA

(2.14)

where I is the applied current, A is the line cross-sectional area, and all other quantities are as defined in Equation (2.13). It is illustrative to see what this equation predicts for our 30-A, 1-μsec pulse if applied to a copper line 1 μm wide and 10 μm high. For this case, the quantities in Equation (2.14) are

Overview of Most Common Adhesion Measurement Methods

I t r c ρ A

= = = = = =

59

30 A line current 10−6 sec current pulse duration 1.7 × 10−8 ohm-m 385 J/(kg degrees centigrade) 8960 kg/m3 10−11 m2

Plugging these numbers into Equation (2.14) gives the rather sobering estimate of a 4400 C temperature rise in the line. Thus, we are far more likely to vaporize the line rather than delaminate it. Early workers in the field facing this problem noticed that the killer factor in Equation (2.14) is the very small cross-sectional area that appears in the denominator squared. Krongelb71 in particular got around this problem by fabricating top-heavy lines, as shown in Figure 2.26. This line has close to 10 times the cross-sectional area of the one shown in Figure 2.19 while maintaining the same common interfacial area with the substrate. Thus, all quantities remain the same in Equation (2.14) except that the A2 term is 100 times larger than previously, which lowers the calculated temperature rise in the line to 44 C, which brings the whole experiment back down to Earth and within the realm of possibility. In actual samples fabricated by Krongelb, the top portion of the test line is not a nice rectangle as shown in Figure 2.26 but looks more like a semicircle. The principle remains the same, however; the top part of the line carries the heavy current load and prevents the metal line from vaporization before it can be lifted off by the Lorentz force. In addition to the work of Krongelb, Baranski and Nevin72 used a version of this test to measure the adhesion of aluminum to polyimide coatings, demonstrating the usefulness of this method for evaluating the adhesion of metal lines to organic as well as inorganic substrates.

10 microns Metal line

10 microns

Insulating substrate

FIGURE 2.26 Modified line structure for the electromagnetic adhesion test. A much larger cross-sectional area is created to avoid vaporizing the metal line before delamination can occur.

60

Adhesion Measurement Methods: Theory and Practice

2.11.1 ADVANTAGES

OF THE

ELECTROMAGNETIC TEST

Like the laser spallation test, the electromagnetic test has distinct advantages for certain special applications. The electromagnetic test is perhaps the only test available for investigating the adhesion of 1-μm wide metal lines under conditions closely resembling those of actual microelectronic devices. As with the laser spallation test, there is no problem with gripping the sample. In addition, the very high strain rates on the order of 106 sec−1 make it likely that viscoplastic effects will also be suppressed in this test. Finally, with the electromagnetic test there is the possibility of performing chipscale device testing on the manufacturing line because all of the equipment can be automated, and the sample preparation uses only well-developed lithography techniques that are compatible with standard device fabrication equipment.

2.11.2 DISADVANTAGES

OF THE

ELECTROMAGNETIC TEST

The most obvious disadvantage of the electromagnetic test is that it can be applied to conducting materials only, which essentially limits it to metals such as copper and aluminum. Even considering this limitation, the test still suffers from the constraint of requiring large currents and very high magnetic fields to achieve sufficient lifting force to induce delamination. Constraints of sample fabrication essentially limit the usefulness of this method to electronic devices, for which it has certain natural advantages. Finally, the instrumentation required for this test, although not particularly exotic, is not standard, and every setup is likely to be of the one-of-a-kind variety.

2.11.3 SUMMARY

AND

RECOMMENDATIONS

The overall evaluation of the electromagnetic test runs pretty much parallel to that for laser spallation. This is a test that has clear advantages in certain applications but is unlikely to find wide application because of the constraints and limitations mentioned. Availability of the required resources and the specific needs of the intended project will govern whether the electromagnetic test will be the bestavailable procedure for adhesion measurement in any given situation.

2.12 NONDESTRUCTIVE TESTS Whereas the concept of a nondestructive adhesion is something of an oxymoron in that it is difficult to believe a result that is supposed to tell you how strongly two materials are stuck together without actually measuring the force required to pull them apart, it is nonetheless a useful concept. The fundamental concept behind nondestructive adhesion tests is to measure some quantity that depends on how well two materials are joined at their common interface. The two tests discussed in this section depend on the following properties: • •

Ability to transmit strain/deformation across an interface Ability to transmit vibrations along an interface

The dynamic modulus test relies on the ability to transmit strain across an interface. For two perfectly bonded adherends, there is a boundary condition at their

Overview of Most Common Adhesion Measurement Methods

61

common interface that the local displacement field be continuous. If the adhesion is not perfect, then there should be some slippage, which can be detected by some type of measurement. The surface wave propagation test relies on the fact that the velocity of surface waves in an interfacial region will depend on how well adhered the separate layers are. These two measurement techniques are investigated in more detail next.

2.12.1 DYNAMIC MODULUS TEST The dynamic modulus test was used by Su et al.73 to investigate the adhesion of metals to glass. The basic experimental setup is based on an internal friction apparatus originally developed by Berry and Pritchet74 to study atomic relaxation phenomena in thin films. A schematic diagram of the apparatus involved is given in Figure 2.27. In a typical experiment, the apparatus in Figure 2.27 can be used to measure the internal friction and dynamic modulus of thin, reedlike specimens depicted in Figure 2.28. The reed is a thin, cantilevered beam, and usual dimensions are roughly 4.5 cm long by 0.5 cm wide by 50 μm thick. By applying a harmonic driving force to the tip of the reed using a frequency oscillator, the reed can be made to vibrate in one of its normal modes of vibration, the frequencies of which are given by the following formula: 2

fn=

αn d 2 l 3π

E ρ

n = 1, 2, 3…∞

(2.15)

where fn αn E ρ d l

= Frequency of the nth normal mode of vibration = Mode number associated with the nth normal mode of vibration = Young’s modulus of reed = Reed density = Reed thickness = Reed length

516000 Drive oscillator

Detect circuit

FIGURE 2.27 Vibrating reed experiment for measuring internal friction and dynamic modulus. A cantilevered beam is set into vibration by an oscillatory signal applied at the beam tip. On removing the applied field, the resulting damped vibration is monitored by a second set of electrodes near the base of the sample.

62

Adhesion Measurement Methods: Theory and Practice

Base End view

Reed Side view

FIGURE 2.28 Typical configuration of the reed sample used in the vibration reed experiment of Figure 2.27.

If the dimensions and density of the reed material are accurately known, then Equation (2.15) provides a precise way of determining the modulus of the reed material from the normal mode frequencies. For the experimental setup shown in Figure 2.27, the frequency of the drive oscillator is varied until it comes close to one of the normal mode frequencies. Because the output of the drive oscillator is capacitively coupled to the tip of the reed through two drive electrodes, the reed will start vibrating in the mode corresponding to the applied frequency, as given by Equation (2.15). The drive signal is then turned off, and the frequency of the nowdecaying signal is measured by the detection circuitry, which is capacitively coupled through detect electrodes near the base of the reed. The rate of damping is determined by the internal friction behavior of the reed material and is measured by observing the log decrement, which essentially is calculated from the number of vibration cycles before the amplitude of vibration reaches half of its initial value. A variation of the above experiment can be used to measure the modulus of a thin film deposited on top of an initially bare reed. This technique was used by Lacombe and Greenblatt75 to measure the modulus of 0.5-μm polystyrene films on top of a vitreous silica reed. The basis of this measurement is the fact that a thin coating on top of a bare reed will cause the frequency of the coated reed to be shifted with respect to the bare reed frequency by an amount given by the following formula: 2

⎛ fc⎞ 2t ⎡ 3E f ρ f ⎤ n − ⎥ ⎜ 0 ⎟ =1+ ⎢ d ⎢⎣ E s ρs ⎥⎦ ⎝ f n⎠ where fnc fn0 t d Ef Es

= Vibration frequency of the nth mode of coated reed = Vibration frequency of the nth mode of bare reed = Coating thickness = Bare reed thickness = Modulus of coating = Modulus of bare reed

(2.16)

Overview of Most Common Adhesion Measurement Methods

63

ρf = Coating density ρs = Bare reed density From Equation (2.16), we see that there are two effects causing the frequency shift of the coated reed. The modulus of the coating adds a stiffening term that causes the frequency to increase. The mass of the coating adds extra inertia, which decreases the vibration frequency as given by the negative term in the ratio of the densities. The derivation of Equation (2.16) assumes that the coating is perfectly bonded to the underlying reed substrate. Su et al.73 wondered how Equation (2.16) would be changed if the bonding between the coating and the substrate was not perfect. To investigate, they introduced a coupling parameter γ, which can vary between 0 and 1, with 0 indicating no adhesion and 1 perfect adhesion. In this case, Equation (2.16) becomes 2

2 ⎛ fc⎞ 2t ⎡ 3γ E f ρ f ⎤ n ⎢ = + − ⎥ 1 ⎜ 0⎟ d ⎢ Es ρs ⎦⎥ ⎝ f n⎠ ⎣

(2.17)

All of the quantities in Equation (2.17) are the same as those in Equation (2.16) with the exception of the coupling parameter. Su et al. used Equation (2.17) to investigate the adhesion of NiTi films to silicon substrates. A replot of their data is shown in Figure 2.29. Note that because of imperfect adhesion, the frequency of the coated reed shown in the bottom curve was less than that of the bare reed and the predicted behavior for perfect adhesion (middle and top curves, respectively). If the adhesion were perfect γ = 1, Equation (2.17) would predict that the modulus term on the right-hand side of Equation (2.17) should dominate, giving rise to an increased frequency, whereas the observed decrease makes it clear that imperfect coupling was the cause for the frequency decrease. The value of γ in this case was 0.7. Thus, γ2 is 0.14, therefore reducing the modulus term in Equation (2.17) by nearly an order of magnitude, which accounts for the dominance of the negative density terms. The dynamic modulus test in effect is measuring the efficiency with which bending strains are transferred across the substrate coating interface. Quite interestingly, Su et al. were able to measure γ as a function of coating thickness and annealing treatments, thereby performing a unique set of nondestructive adhesion measurements for the NiTi/Si system.

2.12.2 ADVANTAGES

OF THE

DYNAMIC MODULUS TEST

The main advantages of the dynamic modulus test are its nondestructive nature and the fact that it can be integrated into microelectronic devices as shown in Figure 2.30. Using standard lithography techniques, cantilevered reedlike structures can be fabricated for direct use in testing a variety of material coatings and thin films used in electronic fabrication processes. Further, using micromechanical electronic machine systems technology, the reed structures can be made very small, to the point at which they can be integrated seamlessly into production wafers for purposes of real-time monitoring of adhesion under manufacturing conditions.

64

Adhesion Measurement Methods: Theory and Practice

Square of reed frequency × 106 (Hz2)

5.4 5.3

Perfectly bonded ﬁlm/substrate

5.2

Bare substrate

5.1

Poor ﬁlm/substrate adhesion

5.0 –100

–50

50

100 150 Temperature deg. C

200

FIGURE 2.29 Square of resonant frequency versus temperature for a silicon reed. Middle curve: bare silicon reed. Bottom curve: reed coated with 2-μm thick NiTi film. Top curve: predicted frequency for coated reed according to Equation (2.17) assuming perfect adhesion, γ = 1. The fact that the data for the coated reed are lower than that of the bare substrate indicates poor adhesion for this coating. (Data adapted and replotted from Q. Su, S.Z. Hua, and M. Wuttig, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed., VSP, Utrecht, The Netherlands, 1995, p. 357.)

FIGURE 2.30 Cantilevered silicon reed etched out of a chip. Lithographic methods can be used to miniaturize this structure, making it possible to use it as a diagnostic test site on manufacturing wafers.

A second advantage of the dynamic modulus test arises from the fact that the sample specimen lends itself naturally to internal friction measurements as well as dynamic modulus measurements. Internal friction data can be very useful in monitoring

Overview of Most Common Adhesion Measurement Methods

65

defect structures and impurity migration along grain boundaries in metal films and is also a sensitive way to detect the glass transition and secondary relaxation processes in polymer coatings. Thus, the dynamic modulus test can be a very versatile technique not only for measuring the adhesion on thin films, but also as a potential diagnostic tool for monitoring a wide range of material relaxation phenomena in both metal and insulator films.

2.12.3 DISDVANTAGES

OF THE

DYNAMIC MODULUS TEST

The clearest disadvantage of the dynamic modulus test lies in the limited sample configuration and the difficulty of sample preparation. The reed samples must be fabricated to precise tolerances to yield accurate data. Also, the nondestructive nature of the test makes it difficult to relate to more standard tests. In particular, there is at present no known relationship between the coupling parameter γ and more conventional measures of adhesion strength, such as the critical fracture energy or the critical fracture stress intensity factor.

2.12.4 SUMMARY

AND

RECOMMENDATIONS

At this stage of its development, the dynamic modulus test will be most useful within the research-and-development laboratory for specialized applications of the adhesion of thin films to microelectronic substrate materials such as silicon and vitreous silica. The main advantages of the test stem from its nondestructive nature and its versatile capabilities as a method for evaluating both adhesion strength and the thermalmechanical properties of thin films through internal friction measurements. A significant drawback of the method is that there is as yet no way of relating the measured coupling parameter γ to more conventional adhesion strength quantities such as the critical surface fracture energy. It should be possible to establish an empirical correlation between these quantities through experiments by which the same coating substrate system is tested by both the dynamic modulus test and by one of the more conventional methods discussed in this chapter. This test has significant potential for use in the semiconductor industry, in which the performance of thin metal films is of great concern.

2.13 SURFACE ACOUSTIC WAVES TEST If you bang on the surface of a block of solid material, then you will send a variety of compression and transverse waves propagating throughout the medium. These waves will typically propagate throughout the entire structure, reflecting off of any boundaries or internal discontinuities. The entire field of ultrasonic inspection is based on a much more controlled version of this primitive experiment. Piezoelectric coupling or another controllable method is used to send very high frequency waves through the structure under carefully controlled conditions. For purposes of adhesion testing, there is a special class of waves that propagate only on the surface of the material; these are known as surface acoustic waves (SAWs). These waves can be induced by a number of methods, including piezoelectric coupling, and are sensitive to the surface conditions of the material.

66

Adhesion Measurement Methods: Theory and Practice

FIGURE 2.31 Schematic of a typical surface acoustic wave (SAW) experiment. The input transducer sends out a surface wave that travels through the coating/substrate interface before it is received by the detection transducer. Changes in the amplitude and velocity of the surface wave on passing through the coating/substrate interface can reveal useful information concerning coating/substrate interactions.

Figure 2.31 illustrates an experiment in which a SAW is generated by a transducer, made to propagate along an interface between a coating and substrate and is subsequently detected by another transducer on the opposite side of the coating. As the surface wave travels through the interface between the coating and the substrate, both its velocity and its amplitude are affected. The shift in velocity gives rise to dispersion effects that are detectable when several different frequencies are present, as would be the case for a wave pulse. Amplitude effects can be used to detect loss mechanisms that might be indicative of poor coupling between the coating and substrate. The SAW method was reviewed by Ollendorf et al.,76 who studied TiN films on steel and compared the SAW method to several other more standard techniques, including the scratch test and the four-point bend test. These investigators used the SAW method to determine the modulus of the TiN coatings and found the value so determined correlated well with adhesion measurements on the same films as determined by the four-point bend and scratch tests. The basic effect is quite similar to the dynamic modulus test. As was seen in the dynamic modulus test, propagation of the SAW through the interface depends on how efficiently transverse strains are transmitted from the substrate to the coating. Voids, regions of loose packing, and other surface imperfections clearly interfere with efficient transmission of strain at the interface and thus affect the apparent modulus measurement of the film as inferred by the SAW method. Because these defects also reduce the film adhesion, it is clear why there should be a correlation between the modulus measurement and the film adhesion. An extensive review of the use of SAWs to study the performance of adhesive joints was given by Rokhlin.77 In another application of the SAW method, Galipeau et al.78 studied the adhesion of polyimide films on quartz substrates. Their basic setup is shown schematically in Figure 2.32. Because the substrate used is quartz, which is a natural piezoelectric material, the input and detection transducers consist simply of interdigitated lines that are patterned on the substrate using standard photolithographic methods. An oscillating input applied to the electrodes of the transducer couples directly into the substrate, setting up an analogous mechanical surface wave. This wave travels as an

Overview of Most Common Adhesion Measurement Methods

67

FIGURE 2.32 Surface acoustic wave experiment for polyimide on quartz. Because quartz is a natural piezoelectric material, transducers can simply be fabricated by evaporating metal lines onto the quartz as shown. Electrical signals in the metal lines are then directly converted into mechanical vibrations in the quartz. In the single delay line experiment using one substrate, the propagated surface wave is compared to a reference signal generated by the input driver. The dual delay line experiment employs two samples in which everything is the same except for the preparation of the coating/substrate interface. The two signals are compared at the detection transducers.

SAW into the coating/substrate interface and out the other end, where it is detected by an identical transducer, which converts the mechanical SAW back into an electrical signal. Note that this differs from the method used by Ollendorf et al. in that these authors used a laser pulse to generate a pulsed wave with many harmonics, which would then show dispersion effects going through the coating/substrate interface. The setup in Figure 2.32 will generate a single harmonic that will not show dispersion. The velocity of this wave will however be affected by passing through the interface, and this is detected in one of two ways. In the first method, the input signal is compared to that of the detector transducer in what is called a single delay line experiment. The second method uses two delay lines to compare the signals from two coatings prepared differently and therefore with different levels of adhesion. Figure 2.33 illustrates some sample data replotted from results presented by Galipeau et al. The curve shows the phase delay incurred when the surface wave passed through the interface between a polyimide film and the quartz substrate as a function of ambient humidity. The negative phase delay is indicative of slowing of the wave. Thus, as the humidity increases, it seems to have a softening effect on the interface, slowing the wave more and more as the relative humidity increases. Because it is well known from standard adhesion tests that high humidity reduces the adhesion of polyimide, we can assume that the apparent softening of the interface region is also partly responsible for this effect. One can perform the same type of

68

Adhesion Measurement Methods: Theory and Practice

FIGURE 2.33 Typical data showing the effect of relative humidity on the passage of a surface acoustic wave through a polyimide/quartz interface. The negative phase delay is indicative of slowing of the wave, indicating that the moisture accumulated at the interface is having a “softening” effect, thereby slowing the signal.

experiment using the dual delay line method in which two polyimide films, one with an adhesion promoter such as a silane material and one without, are compared. The dual delay line test clearly shows that the SAW travels faster through the coating with the adhesion promoter, thus accounting for the higher adhesion observed when the adhesion promoter is present.

2.13.1 ADVANTAGES

OF THE

SURFACE ACOUSTIC WAVES TEST

The key advantages of the SAW method lie in its nondestructive character and the possibility that it can be applied in a manufacturing environment for online quality control purposes. In addition, the SAW method can be calibrated against standard destructive adhesion measurement experiments to provide quantitative results related to surface fracture energies.

2.13.2 DISADVANTAGES

OF THE

SURFACE ACOUSTIC WAVES TEST

The main disadvantage of the SAW approach is that it does not yield direct adhesion strength data and must be calibrated against one of the more standard tests. In addition, sample preparation is an important problem with this method because it is not always a trivial matter to couple the input and output transducers to the substrate. Unlike the quartz substrates, most materials do not have natural piezoelectric behavior; therefore, some other method of coupling the electrical signal to

Overview of Most Common Adhesion Measurement Methods

69

the substrate must be devised. Many times, this involves the use of a coupling fluid, which works but also complicates the experiment.

2.13.3 SUMMARY

AND

RECOMMENDATIONS

From the discussion, it is fairly clear that the SAW adhesion measurement has its greatest potential for use as a real-time quality control tool. Using the laser pulse method to generate the surface waves coupled with interferometry as a detector, this method could be used to inspect coatings rapidly and without contact.

Notes 1. For further details on this most fascinating story, a first-rate account is given in “Stern and Gerlach: How a Bad Cigar Helped Reorient Atomic Physics,” B. Friedrich and D. Herschbach, Physics Today, 53 (December 2003). 2. “Adhesion Measurement of Films and Coatings: A Commentary,” K.L. Mittal, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 1. 3. “An Experimental Partitioning of the Mechanical Energy Expended During Peel Testing,” R.J. Farris and J.L. Goldfarb, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 265. 4. “Peel Adhesion and Pressure Sensitive Tapes,” D. Satas and F. Egan, Adhesives Age, 22 (August 1966). 5. “Failure Mechanisms in Peeling of Pressure-Sensitive Adhesive Tape,” D.W. Aubrey, G.N. Welding, and T. Wong, Journal of Applied Polymer Science, 13, 2193 (1969). 6. “Quantifying the Tape Adhesion Test,” G.V. Calder, F.C. Hansen, and A. Parra, in Adhesion Aspects of Polymeric Coatings, K.L. Mittal, Ed. (Plenum Press, New York, 1983), p. 569. 7. Ibid., p. 570. 8. “Salt Bath Test for Assessing the Adhesion of Silver to Poly(ethylene terephthalate) Web,” J.M. Grace, V. Botticelle, D. R. Freeman, W. Kosel, and R.G. Spahn, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 423. 9. “Pull-off Test, an Internationally Standardized Method for Adhesion Testing — Assessment of the Relevance of Test Results,” J. Sickfeld, in Adhesion Aspects of Polymeric Coatings, K.L. Mittal, Ed. (Plenum Press, New York, 1983), p. 543. 10. “Analysis of Pull Tests for Determining the Effects of Ion Implantation on the Adhesion of Iron Films to Sapphire Substrates,” J.E. Pawel and C.J. McHargue, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 323. 11. “Measurement of the Adhesion of Diamond Films on Tungsten and Correlations with Processing Parameters,” M. Alam, D.E. Peebles, and J.A. Ohlhausen, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 331. 12. “Indentation-Debonding Test for Adhered Thin Polymer Layers,” P.A. Engel and G.C. Pedroza, in Adhesion Aspects of Polymeric Coatings, K.L. Mittal, Ed. (Plenum Press, New York, 1983), p. 583. 13. Ibid., p. 588.

70

Adhesion Measurement Methods: Theory and Practice 14. “Mechanics of the Indentation Test and Its Use to Assess the Adhesion of Polymeric Coatings,” R. Jayachandran, M.C. Boyce, and A.S. Argon, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 189. 15. “Observations and Simple Fracture Mechanics Analysis of Indentation Fracture Delamination of TiN Films on Silicon,” E.R. Weppelmann, X.-Z. Hu, and M.V. Swain, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 217. 16. “Hardness and Adhesion of Filmed Structures as Determined by the Scratch Technique,” J. Ahn, K.L. Mittal and R.H. MacQueen, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 134. 17. “Some Factors Influencing the Adhesion of Films Produced by Vacuum Evaporation,” O.S. Heavens, Journal of the Physics of Radium, 11, 355 (1950). 18. “L’epitaxie dans les Lames Polycrystallines,” O.S. Heavens and L.E. Collins, Journal of the Physics of Radium, 13, 658 (1952). 19. “Measurement of Adhesion of Thin Film,” P. Benjamin and C. Weaver, Proceedings of the Royal Society (London), 254A, 163 (1960). 20. “The Stylus or Scratch Method for Thin Film Adhesion Measurement: Some Observations and Comments,” D.W. Butler, C.J.H. Stoddard, and P.R. Stuart, Journal of Physics (D): Applied Physics, 3, 887 (1970). 21. Note 16, p. 150. 22. “Threshold Adhesion Failure: An Approach to Aluminum Thin-Film Adhesion Measurement Using the Stylus Method,” J. Oroshnik and W.K. Croll, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 158. 23. “Scratch Indentation, a Simple Adhesion Test Method for Thin Films on Polymeric Supports,” G.D. Vaughn, B.G. Frushour, and W.C. Dale, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 127. 24. “Micro-scratch Test for Adhesion Evaluation of Thin Films,” V.K. Sarin, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 175. 25. “Can the Scratch Adhesion Test Ever Be Quantitative?” S.J. Bull, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 107. 26. “Scratch Test Failure Modes and Performance of Organic Coatings for Marine Applications,” S.J. Bull, K. Horvathova, L.P. Gilbert, D. Mitchell, R.I. Davidson, and J.R. White, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 175. 27. “Measurement of Adhesion by a Blister Method,” H. Dannenberg, Journal of Applied Polymer Science, 5, 125 (1961). 28. “A Study of the Fracture Efficiency Parameter of Blister Tests for Films and Coatings,” Y.-H. Lai and D.A. Dillard, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 231. 29. “Analysis of Critical Debonding Pressures of Stressed Thin Films in the Blister Test,” M.G. Allen and S.D. Senturia, Journal of Adhesion, 25, 303 (1988). 30. M.G. Allen and S.D. Senturia, Journal of Adhesion, 29, 219 (1989). 31. M.J. Napolitano, A. Chudnovsky, and A. Moet, Proceedings of ACS, Division of Polymer Material Science and Engineering, 57, 755 (1987).

Overview of Most Common Adhesion Measurement Methods

71

32. “The Constrained Blister Test for the Energy of Interfacial Adhesion,” M.J. Napolitano, A. Chudnovsky, and A. Moet, Journal of Adhesion Science and Technology, 2, 311 (1988). 33. “The Constrained Blister — A Nearly Constant Strain Energy Release Rate Test for Adhesives,” Y.S. Chang, Y.H. Lai, and D.A. Dillard, Journal of Adhesion, 27, 197 (1989). 34. “An Elementary Plate Theory Prediction for Strain Energy Release Rate of the Constrained Blister Test,” Y.H. Lai and D.A. Dillard, Journal of Adhesion, 31, 177 (1990). 35. “Numerical Analysis of the Constrained Blister Test,” Y.H. Lai and D.A. Dillard, Journal of Adhesion, 33, 63 (1990). 36. “Adhesion (Fracture Energy) of Electropolymerized Poly(n-octyl maleimide-co-styrene) on Copper Substrates Using a Constrained Blister Test,” J.-L. Liang, J.P. Bell, and A. Mehta, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 249. 37. Note 33. 38. Note 29, p. 311. 39. “The Three Point Bend Test for Adhesive Joints,” N.T. McDevitt and W.L. Braun, in Adhesive Joints: Formation, Characteristics and Testing, K.L. Mittal, Ed. (Plenum Press, New York, 1984), p. 381. 40. “Practical Adhesion Measurement in Adhering Systems: A Phase Boundary Sensitive Test,” A.A. Roche, M.J. Romand, and F. Sidoroff, in Adhesive Joints: Formation, Characteristics and Testing, K.L. Mittal, Ed. (Plenum Press, New York, 1984), p. 19. 41. “Interface Adhesion: Measurement and Analysis,” A.G. Evans, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 1. 42. “Use of Fracture Mechanics Concepts in Testing of Film Adhesion,” W.D. Bascom, P.F. Becher, J.L. Bitner, and J.S. Murday, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 63. 43. “Fracture Design Criteria for Structural Adhesive Bonding — Promise and Problems,” W.D. Bascom, R.L. Cottington, and C.O. Timmons, Naval Engineers Journal, 73 (August 1976). 44. “Mixed Mode Cracking in Layered Materials,” J.W. Hutchinson and Z. Suo, Advances in Applied Mechanics, 29, 63 (1991). 45. “Closure and Repropagation of Healed Cracks in Silicate Glass,” T.A. Michalske and E.R. Fuller Jr., Journal of the American Ceramics Society, 68, 586 (1985). 46. Note 41, p. 3. 47. “Combined Mode Fracture via the Cracked Brazilian Disk Test,” C. Atkinson, R.E. Smelser, and J. Sanchez, International Journal of Fracture, 18, 279 (1982). 48. “Experimental Determination of Interfacial Toughness Using Brazil-Nut-Sandwich,” J.S. Wang and Z. Suo, Acta Met., 38, 1279 (1990). 49. Note 44, p. 120. 50. “Fracture Toughness Curves for Epoxy Molding Compound/Leadframe Interfaces,” H.-Y. Lee, Journal of Adhesion Science and Technology, 16, 565 (2002). 51. “Adhesion and Adhesives Technology,” A.V. Pocius (Carl Hanser Verlag, Munich, 2002), p. 186. 52. “The Role of Interfacial Interactions and Loss Function of Model Adhesives on Their Adhesion to Glass,” A Sharif, N. Mohammadi, M. Nekoomanesh, and Y. Jahani, Journal of Adhesion Science and Technology, 16, 33 (2002).

72

Adhesion Measurement Methods: Theory and Practice 53. “Plasma Sprayed Coatings as Surface Treatments of Aluminum and Titanium Adherends,” G.D. Davis, P.L. Whisnant, D.K. Shaffer, G.B. Groff, and J.D. Venables, Journal of Adhesion Science and Technology, 9, 527 (1995). 54. “Effectiveness of Water Borne Primers for Structural Adhesive Bonding of Aluminum and Aluminum-Lithium Surfaces,” K.L. Meyler and J.A. Brescia, Journal of Adhesion Science and Technology, 9, 81 (1995). 55. J. Cognard, Journal of Adhesion, 22, 97 (1987). 56. M.F. Kauninen, International Journal of Fracture, 9, 83 (1973). 57. H.R. Brown, Journal of Material Science, 25, 2791 (1990). 58. “Strength of Polystyrene Poly(Methyl Methacrylate) Interfaces,” K.L. Foster and R.P. Wool, Macromolecules, 24(6), 1397 (1991). 59. “On the Non-linear Elastic Stresses in an Adhesively Bonded T-Joint With Double Support,” M.K. Apalak, Journal of Adhesion Science and Technology, 16, 459 (2002). 60. “A Simple Film Adhesion Comparator,” D.W. Butler, Journal of Physics (E): Science of Instrumentation, 3, 979 (1970). 61. “Measurement of the Adhesion of Silver Films to Glass Substrates,” A. Kikuchi, S. Baba, and A. Kinbara, Thin Solid Films, 124, 343 (1985). 62. “A Self-Delamination Method of Measuring the Surface Energy of Adhesion of Coatings,” R.J. Farris and C.L. Bauer, Journal of Adhesion, 26, 293 (1988). 63. “Measurement of Interfacial Fracture Energy in Microelectronic Multifilm Applications,” J.C. Hay, E. Lininger, and X.H. Liu, in Adhesion Measurement of films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 205. 64. The relevant references are: “A New Procedure for Measuring the Decohesion Energy for Thin Ductile Films on Substrates,” A. Bagchi, G.E. Lucas, Z. Suo, and A.G. Evans, J. Mater. Res., 9(7), 1734 (1994); “Thin Film Decohesion and its Measurement,” A. Bagchi and A.G. Evans, Mat. Res. Soc. Symp. Proc., 383, 183 (1995); “The Mechanics and Physics of Thin Film Decohesion and its Measurement,” A. Bagchi and A.G. Evans, Interface Science, 3, 169 (1996). 65. “Interface Adhesion: Measurement and Analysis,” A.G. Evans, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 9. 66. “Measurement of Film-Substrate Bond Strength by Laser Spallation,” J.L. Vossen, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 122. 67. “Measurement of Interfacial Bond Strength by Laser Spallation,” A.W. Stephens and J.L. Vossen, Journal of Vacuum Science and Technology, 13, 38 (1976). 68. “Recent Developments in the Laser Spallation Technique to Measure the Interface Strength and Its Relationship to Interface Toughness With Applications to Metal/Ceramic, Ceramic/Ceramic and Ceramic/Polymer Interfaces,” V. Gupta, J. Yuan, and A. Pronin, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 367. 69. Ibid., p. 395. 70. “Effect of Primer Curing Conditions on Basecoat-Primer Adhesion — A LIDS Study,” J.S. Meth, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 255. 71. “Electromagnetic Tensile Adhesion Test Method,” S. Krongelb, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 107.

Overview of Most Common Adhesion Measurement Methods

73

72. “Adhesion of Aluminum Films on Polyimide by the Electromagnetic Tensile Test,” B.P. Baranski and J.H. Nevin, Journal of Electronic Material, 16, 39 (1987). 73. “Nondestructive Dynamic Evaluation of Thin NiTi Film Adhesion,” Q. Su, S.Z. Hua, and M. Wuttig, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 357. 74. “Vibrating Reed Internal Friction Apparatus for Films and Foils,” B.S. Berry and W.C. Pritchet, IBM Journal of Research and Development, 19, 334 (1975). 75. “Mechanical Properties of Thin Polyimide Films,” R.H. Lacombe and J. Greenblatt, in Polyimides, Vol. 2, K.L. Mittal, Ed. (Plenum, New York, 1984), p. 647 76. “Testing the Adhesion of Hard Coatings Including the Non-destructive Technique of Surface Acoustic Waves,” H. Ollendorf, T. Schülke, and D. Schneider, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 49. 77. “Adhesive Joint Characterization by Ultrasonic Surface and Interface Waves,” S.I. Rokhlin, in Adhesive Joints: Formation, Characterization and Testing, K.L. Mittal, Ed. (Plenum Press, New York, 1984), p. 307. 78. “Adhesion Studies of Polyimide Films Using a Surface Acoustic Wave Sensor,” D.W. Galipeau, J.F. Vetelino, and C. Feger, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 411.

3

Theoretical Foundations of Quantitative Adhesion Measurement Methods

Since the subject became popular with mathematicians about 150 years ago and I am afraid that a really formidable number of unreadable, incomprehensible books have been written about elasticity, and generations of students have endured agonies of boredom in lectures about materials and structures. In my opinion the mystique and mumbo-jumbo is overdone and often beside the point. It is true that the higher flights of elasticity are mathematical and very difficult—but then this sort of theory is probably only rarely used by successful engineering designers. What we find difficult about mathematics is the symbolic presentation of the subject by pedagogues with a taste for dogma, sadism and incomprehensible squiggles. J. E. Gordon, Structures or Why Things Don’t Fall Down

3.1 INTRODUCTION TO CONTINUUM THEORY Because every method for performing an adhesion measurement involves applying a force or load of some type to the coating/substrate system, considerations of stress, strain, and deformation must inevitably be confronted. Notwithstanding the comments of Prof. Gordon quoted above, this chapter attempts to provide a brief introduction to the subject of the continuum theory of solids and to the greatest extent possible tries to avoid technical jargon while at the same time bringing into sharper focus the essential mechanics that need to be understood to grasp the role stress plays in adhesion measurement. The main focus is on developing a sufficient level of understanding of the fundamental theory so that the reader will be able to follow subsequent analytical developments, have sufficient background to confront the technical literature, and be able to perform simple but useful calculations in a competent manner. The development of necessity will be limited in scope, but a number of references to the more lucid and useful literature are provided to give ample means for the interested reader to delve deeper into the subject. Continuum theory is a subject with foundations that were essentially completed by the end of the 19th century by such famous physicists and mathematicians as Navier, Poisson, Green, Cauchy, Hooke, Young, and a number of others. By the early 20th century, the fashion in physics had shifted dramatically to the thenemerging theory of quantum mechanics, which was required to understand the behavior of matter at the atomic level. Continuum theory was essentially relegated to the engineers and a small coterie of mathematicians who found significant challenges

75

76

Adhesion Measurement Methods: Theory and Practice

in the mathematics of the subject. Indeed, by the time I was carrying out my undergraduate and graduate studies in physics, the subject of the continuum theory of matter had all but dropped out of the curriculum in deference to more current topics, such as particle mechanics, electromagnetism, optics, and of course quantum theory. Part of the problem stems from the fact that continuum theory was viewed as only an approximation to the reality of matter and was in fact clearly wrong at the atomic level. However, even though it may only be an approximate description of material behavior it proved to be an extremely useful one and is in fact indispensable as a modern engineering design tool for everything from safety pins to the space shuttle. For present purposes, it is assumed that matter at the scale of tenths of micrometers to tens of meters is accurately described by the field equations of continuum theory. The presentation is carried out in four parts. Sections 3.1.1 through 3.1.3 define the concept of stress in a solid. Stress is something of a mystery to most people, especially those who are more comfortable thinking about forces. A force is a vector quantity requiring three components to be given for a complete specification, one for each of the three mutually orthogonal directions in space. Stress, however, is a tensor quantity requiring in general nine components for a full description. Why all the complication? Why mess around with something three times more complicated than simple forces that most people can understand and that should, in principle, be sufficient to describe the loads applied to any solid? The discussion in Part 1 will try to motivate and explain the rationale behind the concept of stress. Section 3.1.4 introduces the concepts of deformation and strain. This is a relatively straightforward development because nearly everyone has a fairly intuitive sense of deformation. If you apply a load to an object, it will deform by bending, twisting, or stretching in some manner. However, there are a number of subtle and nonintuitive aspects to this subject that need careful attention and are appropriately highlighted. Section 3.1.5 introduces constitutive relations. At this point, all of the kinematical relations for defining the stresses and deformations in solids are in place but a further essential ingredient is missing, what is called the constitutive relations. The basic role of the constitutive relations is to connect the stresses to the strains. They describe a fundamental material property of the solid under investigation. Different materials require different constitutive relations. Without a constitutive relation, you really do not know the material with which you are dealing, whether it is a piece of metal, a slab of glass, or an item of ceramic cookware. The simplest such relation is Hooke’s law for elastic solids, which in essence says that the stress is linearly proportional to the strain, with the constant of proportionality the elastic modulus, often referred to as Young’s modulus. All of this is covered in detail in Section 3.1.5. Finally, in Section 3.2 and following, all of these ingredients are put together to form what are known as the field equations of thermoelasticity. As an extra benefit, Fourier’s equation of heat transfer is thrown into the pot so that problems of thermal stress loading can be addressed. These are very important loads for many problems. The final confection of field equations forms one of the crowning achievements of 19th century theoretical physics, and these equations are rivaled only by Maxwell’s equations, which form the foundation of electromagnetic theory. Maxwell’s theory is truly phenomenal. It is valid over spatial and timescales of at least 15 orders of

Theoretical Foundations of Quantitative Adhesion Measurement Methods

77

magnitude and was relativistically correct at its inception. The only correction that had to be made was to allow for the quantum nature of matter. This gave rise to quantum electrodynamics as developed by Feynman, Schwinger, and Tomonaga. The field equations of thermoelasticity are not relativistically correct or valid at the atomic level. However, for a vast range of practical problems, they are as valid in the 21st century as they were in the 19th century. The errors committed by ignoring relativistic and quantum mechanical effects are well below the sensitivity of most practical measurements. The largest source of error in fact arises from not having truly correct constitutive relations for the material substances under investigation. The general field equations of thermoelasticity are, to put it mildly, exceedingly difficult to solve by paper-and-pencil methods. The common practice in engineering applications is to resort to powerful numerical methods such as finite element analysis or boundary element analysis. Given the enormous computational power of modern workstations, these methods are highly effective at generating useful numerical solutions to the field equations. Surprisingly, however, there are a number of nontrivial special cases that can be solved “on the back of an envelope.” These cases are discussed in some detail as they provide a number of useful computational formulae for estimating stresses in situations of practical interest and supply a handy set of tools for the user.

3.1.1 CONCEPT

OF

STRESS

IN

SOLIDS

As pointed out, nine numbers are required in general to specify the state of stress at a point in a solid. In most cases, certain symmetries apply, and only six numbers are needed, but this is still twice as many as are required to determine a force vector, which should amount to the same thing. The problem arises because, in a continuous medium such as a solid, the relevant quantity is not the force vector alone but the force acting on some element of area. The simplest example is the pressure in a pneumatic tire, which is always specified in pounds per square inch (psi) or Newtons per square meter (Pascal or Pa). The point is that, when speaking of a continuous lump of matter, forces are generally applied to some element of area that gives rise to the concept of a stress that is a force per unit area. The pressure in a tire is a very special stress state known as a hydrostatic stress. It is the same in all directions and thus specified by only one number. This comes about from the fluid nature of the compressed gas in the tire, which cannot support anything but a hydrostatic load. Fluids in general cannot support either tensile or shear loads and thus must be confined to some type of sealed container in which they can be loaded hydrostatically. Solids, on the other hand, support both types of loads, and the state of stress in a solid is sensitive to how it is supported and the details of the applied force field that will typically act on the surface. For large objects, there is also what is called body forces, which strictly speaking act only on a specific point in the body. Gravitational loading is the most important example. Each and every element of a solid has a mass, which is computed as the density times the volume of the element. Each such mass element is under a force loading because of the Earth‘s gravitational field. This gravitational loading will give rise to stresses in the solid at the surfaces where it is supported. Thus, again forces per unit area must be considered.

78

Adhesion Measurement Methods: Theory and Practice

dF n dA

z y e3

e2 e1

x

FIGURE 3.1 An element of surface dA subjected to a localized force dF. The complete description of dA requires specification of the unit normal vector n, which defines the orientation of dA in three dimensions. The vector element dA is given by the product (dA)n.

Figure 3.1 depicts a hypothetical solid surface with a small element of area shown under the influence of some applied force vector dF. The area element also has a vector character because it is characterized by both a magnitude dA and a unit vector n that is perpendicular to the tangent plane that contains the area element. The vector n is commonly referred to as the unit normal that characterizes the direction of the area element dA. Although one does not normally associate a direction with the notion of area, it is clearly important in continuum theory because every surface in three-dimensional space is oriented in some way, and specifying the unit normal is a precise and convenient way of describing this property. The force dF arises because of the action of the material in the immediate neighborhood of the area element dA. It can be of an intrinsic nature, such as forces arising from material defects such as voids, inclusions, or dislocations. Alternately, it can arise from loads applied to the surface of the material that are transmitted to the interior in a chainlike fashion from one volume element to another. In general, the genesis of the local force vector is quite complex and not obtainable by simple means. Fortunately, for present purposes only the existence of this force is required. At equilibrium, an equal and opposite force −dF operates on the other side of the area element dA. Together, these forces create a state of stress acting on dA. Because each separate element of surface will require a different unit normal, it is clear that to come up with a general definition of stress, which is force per unit area, two vector quantities will be involved; this is the reason behind the tensor nature of the stress field. The area element vector is defined in the obvious way as follows: dA = dA n

(3.1)

More useful for our purposes, however, is the inverse area element, which also has an obvious definition: dA −1 =

n dA

(3.2)

Theoretical Foundations of Quantitative Adhesion Measurement Methods

79

The vector dA−1 represents the surface element by assigning it a direction n and a magnitude (1/dA). The stress acting at the area element dA can now be defined in a straightforward manner: T = d FdA −1

(3.3)

Equation (3.3) now fits the bill for the required tensor quantity that has the magnitude of a force per unit area but points in two directions at the same time. One direction is that of dF; the other is the direction of the area unit normal n. Thus, Equation (3.3) reads that T is the stress at the location of the area element dA caused by the vector force dF acting on the area element dA−1 pointing in the direction n. T is a dyadic quantity because it is the composition of two vectors that generally act in separate directions and thus exist in a higher dimensional space than simple vectors. Tensors and dyadics are roughly mathematical equivalents and are often used interchangeably as a matter of convenience. One can imagine even more complex quantities such as triadics, tetradics, and so on that can act in three or more directions. Refer to Appendix A on mathematical foundations for a more detailed treatment of this subject. A more useful description of T is provided by referring both dF and dA−1 to some appropriate Cartesian coordinate system as depicted in Figure 3.1: dF = dF1e1 + dF2e 2 + dF3e3 (3.4)

⎛ e e e ⎞ dA −1 = ⎜ 1 + 2 + 3 ⎟ ⎝ dA1 dA2 dA3 ⎠

The area elements dA1, dA2, and dA3 are projections of the element dA onto the coordinate planes perpendicular to the respective unit vectors e1, e2, and e3 depicted in Figure 3.1. The stress tensor T now becomes:

(

)(

T = dF dA −1 = dF1e1 + dF2e 2 + dF3e3 dA1−1e1 + dA2−1e 2 + dA3−1e3

)

If we carry out all the implied multiplications and collect terms appropriately, we see that the stress tensor can be written as dF1 e e + dF 2 e e + dF 3 e e 1 1 2 1 3 1 dA1 dA1 dA1 T = dF1 e1e 2 + dF 2 e 2 e 2 + dF 3 e 3e 2 dA2 dA2 dA2 dF1 e e + dF 2 e e + dF 3 e e 2 3 3 3 1 3 dA3 dA3 dA3

(3.5)

80

Adhesion Measurement Methods: Theory and Practice

Following standard convention, we write the stress tensor T in terms of three traction vectors T1, T2, and T3: T = e1T1 + e2T2 + e3T3

(3.6)

where dF1 e + dF 2 e + dF 3 e T1 = 1 2 3 dA1 dA1 dA1 dF1 e + dF 2 e + dF 3 e T2 = 1 2 3 dA2 dA2 dA2 dF1 e + dF 2 e + dF 3 e T3 = 3 1 2 dA3 dA3 dA3 The main purpose in defining the traction vectors is that they are the most convenient quantities for defining surface loads on solid bodies. They are convenient vector quantities defined directly in terms of the applied forces while at the same time are genuine stress quantities with the dimension of force per unit area. Thus, if one solid body impinges on another, there is always some finite area of contact involved, and the applied load is distributed over this area. Therefore, the actual load is a force per some area or a traction vector as defined above. The equations can be greatly simplified by introducing the standard notation for the components of the stress tensor σij: T1 = σ11e1 + σ12e 2 + σ13e 3 T2 = σ 21e1 + σ 22e 2 + σ 23e 3

(3.7)

T3 = σ 31e1 + σ 32e 2 + σ 33e 3 By comparing Equations (3.6) and (3.7), it is immediately clear what the definitions of the stress components σij are. For example σ11 is the stress generated by dF1 acting on area element dA1, which points in the direction e1. Likewise, σ12 is the stress generated by dF2 acting on area element dA1 pointing in the direction e2. Note that σ12 is a shear component because the force acts perpendicular to the area unit normal as opposed to σ11, which is called a tensile component because it acts parallel to the area unit normal. Similar observations hold for the remaining components. Working with quantities such as the stress tensor is awkward, to say the least. Because of this, a number of different notations have been invented to try to make the situation more manageable. Those who like matrices have come up with the obvious matrix definition: ⎡ σ11 ⎢ σ = ⎢ σ 21 ⎢ σ 31 ⎣

σ12 σ 22 σ 32

σ13 ⎤ ⎥ σ 23 ⎥ σ 33 ⎥⎦

(3.8)

Theoretical Foundations of Quantitative Adhesion Measurement Methods

81

This notation is handy when dealing with matrix operations on vectors and is also easily programmed on computers. A second approach is to use what is called indicial notation, by which one always deals with the tensor components as indexed scalar quantities. This notation has a number of advantages and is a favorite of the theoreticians. Thus, the stress tensor is simply referred to as σij where it is understood that the indices i and j run over the values 1, 2, and 3. The main advantage of the indicial notation is the easy ability to generalize and expand the definitions to tensor quantities of higher dimension and rank. Thus, the indices can run from 1 to 4 if the problem requires working in a four-dimensional space time as is the case in relativity theory. In addition, higher rank quantities are easily generated by simply adding more indices. In elasticity theory, the elastic constants of the most general class of crystals are specified by the fourth-order elasticity tensor Cijkl, which has 81 elements. The matrix version of this quantity is most useful simply to display the elements on a page as opposed to performing formal manipulations. Einstein’s field equations from his general relativity theory involve tensor quantities that are truly extravagant to the point of being mind boggling and have no matrix counterparts. For the purposes of this section, a hybrid vector/tensor notation is adopted to provide a compact and general notation for introducing the field equations of elasticity. Refer to Appendix A for a more detailed treatment of vector and tensor notation and manipulation. The primary thrust of this discussion, however, is to develop the basic field equations of continuum theory in a reasonably transparent manner and show that they arise in a straightforward way from the simpler equations of Newtonian particle mechanics. To this point, we have established that the main quantities of interest are the components of the stress tensor as opposed to the simpler vector forces that act on the body in question. This arises because the vector forces inevitably act on surface elements when a solid is considered as a continuum as opposed to a collection of point particles; as Equation (3.3) demonstrates, this leads to the formation of a higher dyadic quantity called the stress tensor. The usefulness of the stress tensor formulation becomes apparent when the stress on some arbitrary surface is required and not just the special orthogonal surfaces of the coordinate planes. The stress on any surface whatever can be related to the components of the stress tensor given in some fixed reference system in the following manner. Figure 3.2 shows the traction vector Tn acting on some arbitrary area element dA with surface normal vector n that is not parallel to any of the surfaces dA1, dA2, or dA3 associated with the coordinate planes and therefore must intersect each in some fashion, forming a tetrahedron figure shown in Figure 3.2. Equilibrium requires that the vector sum of the forces acting on all the faces of the tetrahedron should add to zero; thus, Fn − F1 − F2 − F3 = 0

(3.9)

Using Equations (3.6) and (3.7), Equation (3.9) can be satisfied on a componentby-component basis by collecting all terms acting in the direction e1 and setting them to zero and proceeding similarly for the directions e2 and e3. The result is

82

Adhesion Measurement Methods: Theory and Practice

n.e3 = cos(θ) e3 e3

hn

θ

n

θ Tn

h3

T1

n T2

dA dA3 e2 b

e1 T3

FIGURE 3.2 A surface element within a solid (dA) having some arbitrary orientation n with respect to a fixed coordinate system characterized by the unit vectors e1, e2, and e3. The area element dA is subjected to a surface traction Tn that is not parallel to the surface normal vector n. T1, T2, and T3 are the components of Tn along the coordinate axes. The shaded area labeled dA3 is the projection of dA onto the e1, e2 plane and has unit normal e3. The inset shows that the element dA3 is related to dA by the simple formula dA3 = dAn.e3. A similar relation holds for the remaining projections dA1 and dA2 (not shown).

(T ) dA − σ (T ) dA − σ (T ) dA − σ

dA1 − σ 21dA2 − σ 31dA3 = 0

n 1

11

n 2

12

n 3

13

dA1 − σ 22dA2 − σ 32dA3 = 0

(3.10)

dA1 − σ 23dA2 − σ 33dA3 = 0

Equations (3.10) can be greatly simplified by noting that the area elements dA1, dA2, and dA3 are just the projections of the area element dA onto the main coordinate planes. This fact is demonstrated by the inset in Figure 3.2 for the case of area element dA3. The primary result is the following useful set of relations: dA1 = dA(n.e1 ) = dA cos θ1 = n1dA dA2 = dA(n.e 2 ) = dA cos θ2 = n2dA

(3.11)

dA3 = dA(n.e 3 ) = dA cos θ3 = n3dA where n1 = cos θ1, n2 = cos θ2, and n3 = cos θ3 are the common direction cosines for the normal vector n. By substituting Equations (3.11) into Equations (3.10), the common factor dA can be seen to drop out, and with some obvious rearrangement, the following result is achieved:

Theoretical Foundations of Quantitative Adhesion Measurement Methods

(T ) (T ) (T )

n 1

= σ11n1 + σ 21n2 + σ 31n3

n 2

= σ12n1 + σ 22n2 + σ 32n3

n 3

= σ13n1 + σ 23n2 + σ 33n3

83

(3.12)

These equations have a very convenient matrix representation: ⎡ σ11 ⎡ Tn , Tn , Tn ⎤ = ⎡ n1 , n2 , n3 ⎤ ⎢ σ 21 ⎣ ⎦⎢ 1 2 3⎦ ⎣ ⎢ σ 31 ⎣

( ) ( ) ( )

σ12 σ 22 σ 32

σ13 ⎤ ⎥ σ 23 ⎥ σ 33 ⎥⎦

(3.13)

Using compact matrix notation, Equation (3.13) can be written very succinctly as T = n⋅σ. Equation (3.13) demonstrates the utility of the stress tensor σ because once it is established in any particular convenient coordinate system, the tractions across any desired area element can be obtained by simple matrix operations knowing only σ and the components of the area normal n.

3.1.2 SPECIAL STRESS STATES

AND

STRESS CONDITIONS

3.1.2.1 Principal Stresses On contemplating Equation (3.13), the alert reader may wonder, given the fact that the stress tensor can be defined in any convenient coordinate system, whether there are particular coordinates in which the stress tensor assumes a particularly simple form. This question has an affirmative answer. Quite generally, at any particular point in any elastic solid there is a coordinate system in which the stress tensor has a simple diagonal form: ⎡σ I ⎢ σ=⎢0 ⎢0 ⎣

0 σ II 0

0 ⎤ ⎥ 0 ⎥ σ III ⎥⎦

(3.14)

Equation (3.14) is very nice indeed because diagonal matrices are much simpler to manipulate than the general case. The components σI, σII, and σIII are called the principal stress components and are typically arranged so that σI > σII > σIII. However, there is a very important string attached in that the special coordinate system in which the stress tensor assumes a diagonal form will in general vary from point to point in the solid. This takes much of the fun out of using the principal stress coordinates, but they are still quite useful nonetheless. Indeed, the largest component σI, called the maximum principal stress, is useful in fracture mechanics work because it represents the largest stress component that can exist at a particular point. Furthermore, the direction in which σI acts can give an important clue to the direction

84

Adhesion Measurement Methods: Theory and Practice

A

F σz = F/A z y

σx = σy = 0 x

F

FIGURE 3.3 Simplest uniaxial stress state for a slender tensile sample.

in which a potential crack will propagate. All of this is valid for homogeneous isotropic materials and is discussed in more detail in Chapter 4, dealing with the fracture mechanics of delamination processes. By far the simplest example of a principal stress state is the case of uniaxial tension shown in Figure 3.3. The principal axes are intuitively obvious for this case, and the stress tensor assumes the simplest possible form as follows: ⎡0 ⎢ σ = ⎢0 ⎢0 ⎣

0 0 0

0⎤ ⎥ 0⎥ σ z ⎥⎦

(3.15)

This is the form of the stress tensor that is assumed for all tensile testing experiments. 3.1.2.2 St. Venant’s Principle The uniaxial tension case provides a clear and simple example of a useful and general rule of stress analysis. The basic idea is most simply illustrated by Figure 3.4, which exhibits three entirely different ways of clamping a uniaxial tensile sample. The fact that the net load is identical for each sample means that they are “statically identical” in the parlance of engineering mechanics. Because of the different clamping configurations, however, the stress state near the top end will be widely different for each sample. But, because each sample is of identical cross section and each is loaded in a statically identical manner (i.e., the net load F is identical in each case), the state of stress far from the clamped region near the center of the sample will be identical in each case and is in fact given by F/A, the net force divided by the crosssectional area. This is a fundamental fact underlying all tensile testing experiments. The general principle highlights the fact that the action of surface tractions is

Theoretical Foundations of Quantitative Adhesion Measurement Methods

85

F F

Center pivot clamp

F

Straight edge clamp

Outrigger pivot clamp

FIGURE 3.4 St. Venant’s principle for three equally loaded but differently clamped tensile samples. The details of the stress field near the clamped edge will differ significantly for each sample; however, because each sample is equally loaded, the stress state far from the clamped edge will be identical for each sample. This is a consequence of the localized nature of the surface tractions imposed by the different clamping arrangements.

essentially local in that the fine details of the local stress state decay away as one proceeds away from the point of application. The stress state in the “far field” depends only on the net loading and the boundary conditions. Although this principle is most clearly illustrated by the uniaxial tension case, it holds for a very general class of solids in one, two, and three dimensions. The precise meaning of far away depends on the details of the problem, but for each case a characteristic length can be defined, and the definition of far away is typically a small multiple of this length. An example of particular relevance to this work is a coating on a rigid substrate. The characteristic length in this case can be taken as the coating thickness and far away typically turns out to be about five times this thickness. 3.1.2.3 Two-Dimensional Stress States 3.1.2.3.1 Plane Stress The case of plane stress is of particular interest in adhesion work because nearly all coatings are in a state of plane stress in which the stress component perpendicular to the coating surface is zero. This is typically taken to be the z direction, so the stress tensor assumes the following form: ⎡ σ xx ⎢ σ = ⎢ σ yx ⎢ 0 ⎣

σ xy σ yy 0

0⎤ ⎥ 0⎥ 0 ⎥⎦

(3.16)

86

Adhesion Measurement Methods: Theory and Practice

The case of a homogeneous isotropic coating on a rigid substrate is particularly simple and can be solved easily with pencil and paper. The shear components σxy and σyx are zero in this case, so the stress tensor is diagonal, and σxx and σyy are in fact principal stresses. 3.1.2.3.2 Plane Strain When dealing with a long rodlike sample of arbitrary cross section, the state of stress away from the ends is approximately two dimensional, and the stress tensor has the following form: ⎡ σ xx ⎢ σ = ⎢ σ yx ⎢ 0 ⎣

σ xy σ yy 0

0 ⎤ ⎥ 0 ⎥ σ zz ⎥⎦

(3.17)

where σzz = ν(σxx + σyy). The plane strain case is also very important from the point of view of adhesion testing because nearly all fracture mechanics tests on crack propagation are performed in a state of plane strain. More is said on this matter in Chapter 4. 3.1.2.3.3 Hydrostatic Stress A final simplified stress state of interest is that of hydrostatic compression or tension. The stress tensor in this case is as simple as it can be: ⎡1 ⎢ σ = σ ⎢0 ⎢0 ⎣

0 1 0

0⎤ ⎥ 0⎥ 1⎥⎦

(3.18)

The stress tensor is simply a scalar times the identity matrix and is thus effectively a scalar quantity. The pressure in a pneumatic tire is the simplest example of this stress state. The pressure in most fluids is similarly characterized. In solids, the scalar factor σ can be positive, indicating a state of hydrostatic tension. This can be achieved when the sample is constrained along each of the three coordinate axes and can lead to void formation at high stress levels. This is an important failure mode in some rubbers.

3.1.3 EQUATION

OF

MOTION

IN

SOLIDS

The whole purpose of the presentation up to this point has been to set the stage for the development of the basic equation of motion for an elastic body. Figure 3.5 shows a small element of material embedded within a larger object. The question is how this object responds to the forces acting on it. The answer is the same as the one given by Sir Isaac Newton in the 17th century in his second law of particle mechanics; that is, the mass of the object times the acceleration is equal to the net vector sum of all the forces acting on it. This is typically written as follows:

Theoretical Foundations of Quantitative Adhesion Measurement Methods

n

87

T

dV dA fb e3 e2

e1

FIGURE 3.5 An element of volume dV embedded in a larger solid. The surface element dA with unit normal n is acted on by a traction T. A body force fb acts on the entire volume element.

∑

Fi = m

i

d 2u dt 2

(3.19)

where m = mass of volume element u = displacement vector Equation (3.19) is the typical expression given in texts on classical particle mechanics, which treat all objects as point masses, ignoring their internal structure as continuous bodies. This treatment is quite adequate for problems in ballistics, for which the projectile can be treated as a point mass acted on by the Earth’s gravitational field and various frictional forces due to the Earth’s atmosphere. This treatment calculates the projectile trajectory and where will it land. If it is desired to know what will happen when the projectile hits another object, then the continuum nature of the missile cannot be ignored, and continuum theory must be applied. Equation (3.19) must be modified to reflect that the projectile is in fact an extended body. The discrete mass m is replaced by the density times a volume element, and the list of forces must now include surface tractions caused by the impacting surfaces as well as the usual external forces, such as gravity. The following relations must now be used: dm = ρdV F=

∫ f dV + F b

V

int

(3.20)

88

Adhesion Measurement Methods: Theory and Practice

where ρ = material density fb = body force/unit volume (gravitational, electromagnetic, etc.) Fint = total internal traction forces =

∫ TdA = ∫ σ.ndA A

A

In light of these new definitions, Newton’s second law as expressed in Equation (3.19) now becomes

∫

∫

fb dV + σ .ndA =

V

A

∫

ρ

V

d 2u dV dt 2

(3.21)

At this point, one of the truly marvelous bits of legerdemain from vector calculus, known as the divergence theorem, is invoked to transform the surface integral over the stress tensor into a volume integral. The theorem, called the Divergence Theorem, is general and essentially states that

∫ σ.n dA = ∫∇ • σ dV . A

V

Readers who need to brush up on vector calculus or would like more detailed references on the subject should refer to Appendix A. The main point in doing this is as follows: All the terms can now be gathered within the same volume integral, which is set equal to zero. Because the volume is essentially arbitrary (i.e., the equation must hold for all shapes), the only way the integral can be zero is if the integrand itself is identically zero, which then leads to the required differential relation. Applying these steps to Equation (3.21) gives

∫ V

∫

fb dV + σ.ndA = A

∫

ρ

V

d 2u dV dt 2

(rearrange + divergeence theorem)

∫ V

∫

∫

fb dV + ∇· σdV − ρ V

V

d 2u =0 dt 2

(collect terms under common volume integral)

∫ V

⎛ d 2u ⎞ ⎜ fb dV + ∇·σ − ρ dt 2 ⎟ dV = 0 ⎝ ⎠

Because the last volume integral must hold for objects of arbitrary shape, size, and loading condition, the integrand itself must be zero, which gives

Theoretical Foundations of Quantitative Adhesion Measurement Methods

fb + ∇ · σ − ρ

d 2u =0 dt 2

89

(3.22)

where ρ fb σ u

= = = =

material density (kg/m3) body force density (N/m3) stress tensor (N/m2) displacement field vector (m)

Equation (3.22) represents Newton’s second law as applied to a continuous solid. The main feature that differs from the standard particle mechanics version given by Equation (3.19) is the divergence of the stress tensor, which accounts for the action of the internal stresses acting within the body.

3.1.4 DEFORMATION

AND

STRAIN

With the basic equation for stresses now in hand, the discussion proceeds to the complementary topic of deformation and strain. When a stress is applied to any material object, there is a resulting deformation, so the key questions now become how deformation is defined and how it is related to the applied stress. To most readers, the idea of a deformation should seem quite obvious because nearly everyone has an intuitive feel for what deformation is. If you run your car into a rigid post, the resulting deformation of the fender is obvious, so it is somewhat surprising that the mathematical description arising from continuum theory is fairly recondite, giving rise to dense topics such as deformation gradients and invariant strain measures. The basic difficulties arise from the need for mathematical precision and the fact that the world is three dimensional. In one dimension, everything falls out quite naturally. The stress is proportional to the strain (Hooke’s law), and the strain is just the increment in length divided by the original length. However, when describing general three-dimensional deformations, these concepts simply do not pass muster, and one must resort to something more heavy duty. The basic approach of continuum theory, therefore, is to treat any object whatsoever as a vector field as shown in Figure 3.6. In this figure, the object labeled Bu (subscript u for undeformed) is described as a vector field that is a region of space labeled by a collection of vectors X = (X1, X2, X3). It is clear then that just about any object can be so defined in terms of its geometric shape. Other properties are also required but that comes later in Section 3.1.5. At this point, to be able to define deformations in three dimensions the geometric configuration must first be defined, and the vector field X does the job. The precise shape of the object is defined by also defining the boundary of Bu (commonly designated as ∂Bu), but that is not needed to obtain a general definition of the deformation of an object. Now, the mathematicians are perfect wizards at performing deformations through entities called mappings, which turn out to be vector fields themselves and that describe transformations between different vector spaces. The vector K(X) shown in Figure 3.6 is such a mapping. The figure shows that K(X) is just the original

90

Adhesion Measurement Methods: Theory and Practice

Pd Bd

Bu

u(X)

Pu

e3 l3

X

12

K(X)

x e2

e1 l1

FIGURE 3.6 Continuum description of the deformation of a body Bu.

position vector X plus a deformation vector u, which in general will depend on X. It should be noted at this point that the mapping K will take the entire space to which Bu belongs (described by basis vectors l1, l2, l3) into an entirely new space described by basis vectors e1, e2, and e3. Thus, the mapping K(X) can be thought of as taking the point X in the space described by l1, l2, and l3 into the point x in the space with basis vectors e1, e2, and e3 or x = K(X). It is also clear that the configuration of the body can be equally well described using either coordinate system because the mapping K(X) is assumed to be continuous with continuous derivatives and suitably well behaved so that its inverse K–1(X) exists and is equally well behaved. This is both a powerful and convenient feature of the continuum description of the deformation process and, unfortunately, also a source of much confusion, so a few words must be said regarding nomenclature for the description used. When using the l1, l2, l3 basis vectors, one is said to be employing the Lagrangian formulation, and if using the e1, e2, e3 basis, then the Eulerian description is in effect. The main reason for noting this is for those who consult the continuum mechanics literature. For present purposes, the deformations and strains will be relatively small, and in this case the Lagrangian and Eulerian descriptions turn out to be nearly identical. Getting back now to the general description of deformation and strain, the basic relation for the deformation u can be written by referring to Figure 3.6 as u(X) = K(X) − X

(3.23)

Equation (3.23) describes the overall deformation process, but for purposes of describing the internal strain in the body something must be said about the gradient of the deformation or how steeply the deformation separates contiguous points in the object under consideration. Thus, taking the gradient of both sides of Equation (3.23) leads to

Theoretical Foundations of Quantitative Adhesion Measurement Methods

91

∇u(X) = ∇K(X) − I or

(3.24)

∇u(X) = F − I The new tensor quantity F = ∇K is called the deformation gradient, and the tensor ∇u is called the displacement gradient. Equations (3.23) and (3.24) lay a foundation for defining general deformations, but what is needed now is a proper definition of strain. This is somewhat trickier than just defining deformations because a true strain will always give rise to a concomitant stress. The general deformation given by Equation (3.23) contains translations and rotations as well as stretches and twists. The pure translations and rotations clearly will not induce any kind of stress in an object as they are rigid deformations in which every part of the object moves in unison. Simply moving a glass from the table and inverting it on the dresser will not induce any kind of stress. It is the stretches and twists that actually cause material particles within the object to separate relative to each other and that give rise to strains that induce a level of stress in the object. Take a glass rod and either twist it or bend it, and you will induce a strain that will cause a stress. There is no unique way of defining the strain. However, one approach is to take the deformation gradient F and cobble together a formula that will flush out those parts of the deformation that are essentially rigid rotations or translations and leave only the bona fide stretches, compressions, and twists. One such definition is as follows: T D = 1 2 ⎡⎢ F F − I ⎤⎥ ⎣ ⎦

(3.25)

It can be shown using the polar decomposition theorem that the finite strain tensor D defined in Equation (3.25) fits the bill in terms of eliminating all rigid body motions from the general deformation formula given by Equation (3.23) and thus includes only those stretches, compressions, and twists that will give rise to a stress. Unfortunately, D turns out to be a rather difficult entity to deal with in general because of what are commonly known as nonlinear effects. These typically arise when relatively large deformations occur, such as when one pulls a bar of taffy to two times its original length. However, if the deformations are relatively small, as in the case of shrinkage strains in a paint coating, then another, simpler strain measure can be used, which is defined as follows: ε = 1 2[(∇u) + (∇u)T ]

(3.26)

The strain tensor ε is closely related to D, as can be shown by the following simple manipulations:

92

Adhesion Measurement Methods: Theory and Practice

T D = 1 2 ⎡⎢ FF − I ⎤⎥ ⎦ ⎣

where F = ∇u + I FT = (∇u)T + I Substituting the expressions for F and FT into the expression for D gives the following result: T

T

D = 1 2 [F F − I] = 1 2 [(∇u + I)((∇u) + I) − I] T

= 1 2 [∇u + (∇u) ] + 1 2 (∇u)(∇u) = ε + 1 2 (∇u)(∇u)

T

T

The final definitions for strain can be summarized as follows: T D = 1 2 ⎡⎢ F F − I ⎤⎥ ⎣ ⎦

Finite deformations

T ε = 1 2 ⎡∇u + ∇u ⎤ ⎢⎣ ⎥⎦

( )

Small strains only

(3.27)

T

( )( )

D = ε + 1 2 ∇u ∇u

Note that D and ε are nearly equal when ∇u is small, which is always the case for small strain problems in the theory of linear elasticity. One further issue has to be confronted before the development of a suitable strain measure can be considered completed. The basic problem comes down to this: If we know the displacement field u, then Equations (3.27) give perfectly good recipes for conjuring up the required strain fields. However, in many problems of practical interest one first computes the strains, and the question arises as to whether Equations (3.27) will be sufficient to determine the corresponding displacements. The question is a subtle and tricky one, and the answer is generally “No.” Equations (3.27) alone do not guarantee that the derived strains will correspond to acceptable displacements. It turns out that one further relation is required to ensure compatibility between a derived set of strains and the corresponding displacements as follows: ∇×∇×ε = 0

(3.28)

Equation (3.28) is known as the equation of compatibility for the strain field ε. A clear and convincing development of Equation (3.28) has been presented by Gurtin,1 who also gives an excellent, if somewhat high-powered, development of the general deformation/strain equations. The now-complete continuum description of the deformation and strain fields can be summarized as follows:

Theoretical Foundations of Quantitative Adhesion Measurement Methods

a) x = K(X)

(Deformation mapping)

b) u = K(X) − X

(Displacement vector)

c) F = ∇K

(Deformation gradient)

d) J = ∇u − I

(Displacement gradient)

T e) D = 1 2 ⎡⎢ F F − I ⎤⎥ ⎣ ⎦

(Finite strain tensor)

f) ε = 1 2 ⎡⎣∇u + (∇u)T ⎤⎦

(Infinitesimal strain tensor)

g) ∇ × ∇ × ε = 0

(Equation of compatibility)

93

(3.29)

h) D = ε + 1 2 (∇u)((∇u)T (relation between D, ε , and u) Equations (3.29) essentially complete the second step in the continuum mechanics program outlined on page 76, to describe and compute deformations and stresses in solid bodies. A few words on nomenclature are in order for those who will consult the general literature on the subject. The tensor quantity F FT is called the Green’s strain after George Green, the famous 19th century mathematician. All of what has been developed to this point has been worked out in the Lagrangian description as defined here (meaning in the l1, l2, l3 coordinate system). One can easily imagine that by using the Euler description a somewhat different tensor quantity can be conjured up that will be essentially equivalent to F FT but referred to different coordinates. Names such as Cauchy’s strain tensor or Euler’s (Almansi’s) strain tensor will pop up in various places, which tends to give rise to much confusion regarding which is which. The reader can take heart from the fact that all descriptions give the same result for the small strain tensor ε, and that this is the most commonly used strain measure in the practical engineering literature. This arises from the fact ∇ that when the strains are small, the quantity ∇u is small, and thus the term ∇u(∇ u)T in Equation (3.27) is of second order in a small quantity and can be neglected. In this case, ε and D become identical. Caution must be exercised, however. A common problem arises when someone using a finite element code, for instance, does not understand which strain measure is used. In particular, if ε is used and the problem involves a significant degree of rotation, major errors can creep into the calculation even though the actual strains may be low. This comes about because ε does not accurately account for large rotations as the general deformation measure D does.

3.1.5 CONSTITUTIVE RELATIONS TO THE STRAIN

OR

CONNECTING

THE

STRESS

3.1.5.1 General Behavior At this point, Steps 1 and 2 of the continuum mechanics presentation have been accomplished. General definitions of stress, deformation, and strain are now in place.

94

Adhesion Measurement Methods: Theory and Practice

What is clearly lacking, however, is a description of how these quantities are related in a real material. What is required is referred to as the constitutive relation or material law for substances of interest. In general, this is a very difficult topic and goes to the very heart of the thermodynamic nature of materials and how they respond to the myriad array of loads and deformations to which they can be subjected. Everything from the bending of a pencil to the gravitational collapse of a star requires a fundamental understanding of the constitutive behavior of the material in question. Many common materials show a complex range of behaviors when subjected to relatively modest loading conditions. Materials such as mayonnaise tend to deform more easily as the deformation rate increases (shear thinning). Contrary materials such as Silly Putty do just the opposite. You can easily deform this material with your fingers like a putty, but if you drop it on the floor, it will bounce like a rubber ball (shear thickening). This type of behavior is commonly called thixotropic, which is basically a way of saying we really do not know what is going on, so let us just give it a fancy name and move on. There exists a vast body of literature dealing with the constitutive behavior of a wide range of materials, ranging from rubber bands to desert soils. The topic can easily require an entire encyclopedia for anything approaching a definitive treatment. Fortunately, however, a wide range of useful applications deal with materials undergoing relatively small deformations* for which the constitutive relation between the stress and the strain is essentially linear. In this circumstance, there exists a general formulation of the constitutive relation that is useful and is dealt with reasonably easily. It should also be added that focusing on the linear behavior of materials has other merits in addition relative tractability. When attacking the general nonlinear behavior of a material, for instance, it is useful to look at a linear approximation first to see the nature of the error incurred. In addition, nearly all numerical algorithms for solving full nonlinear problems proceed by a sequence of linear approximations that, if handled correctly, will converge to the true nonlinear solution. The problem now is as follows: What is the most general linear relationship that can exist between the stress tensor σ ij and the strain tensor εij? Given the complex nature of the tensor quantities involved, it is no surprise that the answer is also complex, involving the elasticity tensor Cijkl, which was mentioned earlier, thus: 3

σ ij =

∑C

ε

ijkl kl

(3.30)

k ,l =1

Equation (3.30) expresses the most general linear relationship between two second-order tensors that can exist. The fact that a fourth-order tensor is required to make the connection is not surprising because after summing over the two indices k and l, which describe the components of the strain tensor ε, there have to be two indices left over (i and j in this case) to designate the corresponding component of * Beware that small deformations and strains do not necessarily imply small stresses. Most engineering materials, for instance, have a fairly high modulus, so that relatively small strains can give rise to stresses that cause permanent deformations or in some cases lead to fracture.

Theoretical Foundations of Quantitative Adhesion Measurement Methods

95

the stress tensor σ. Because the indices i, j, k, l run over the values 1, 2, 3, the elasticity tensor Cijkl can have a maximum of 81 (34) independent components. Fortunately, a number of physical symmetries come to the rescue, which cuts down this horrendous number considerably. In particular, because the tensor quantities σij and εij are symmetric*, they have at most 6 independent components. This means that Cijkl will have at most 36 (62) independent components. This is still an outlandish number, but luckily real materials have further symmetries that cut this number down still further. Cubic** crystals, for instance, which have many rotational and reflection symmetries, require only 3 independent elastic constants. Ultimately, for homogeneous isotropic materials with full spherical symmetry (amorphous glasses, for instance), the final number comes down to only two elastic constants. It is quite surprising*** that in most applications the assumption of a homogeneous isotropic material seems to work out reasonably well. Even materials such as metals, which are nominally crystalline, can be successfully treated as homogeneous isotropic materials. This stems in large part from the fact that in their final use condition most metals are polycrystalline in nature, which means that they are made up of zillions of very small crystals oriented in random directions. The net effect is that, when viewed over a macroscopically small but microscopically large**** region, the material appears to be homogeneous isotropic. The main types of situations in which one can get into trouble by assuming homogeneous isotropic behavior is when dealing with materials that are large single crystals, composites containing highly oriented fibers, or nonisotropic coatings. The most ubiquitous example of large single crystals is the silicon wafers used in the microelectronics industry. These are near-perfect cubic crystals, and it is important to know how the parent crystal was cut in order to know the mechanical behavior of the product wafer. For example, some laboratories perform wafer-bending experiments to assess the stress state of the wafer. Not knowing which crystal plane the wafer was cut along can lead to very serious errors in such experiments. In particular, it is highly desirable in such experiments to have wafers that have been cut along the (111) plane and thereby have in-plane isotropy; otherwise, one has to deal with a significant level of anisotropy to obtain accurate results. Circuit boards are another example of objects that exhibit a high level of anisotropy because of their composite nature. The common FR4 board material, for example, is made up of a mat of glass fibers embedded in an epoxy matrix. All the fibers lie in the plane of the board, thus giving rise to a large difference between in-plane and out-of-plane mechanical properties. A final example of anisotropy that is of significant concern to the coatings industry is polymer systems made up of stiff chains that tend to orient parallel to the surface on which they are deposited after drying or during the curing process. * The symmetry of the stress tensor arises from the constraint that conservation of angular momentum must hold as well as linear momentum, which is expressed in Equation (3.22). For a detailed derivation, refer to page 20 in the work of Gould.2 Also beware that there are formulations of continuum theory in which the stress and strain tensors are not symmetric. ** A derivation of how this comes about was given by Feynman, Note 8, Chapter 39. *** Or perhaps this is not so surprising given the general human proclivity toward indolence. **** This is what is commonly referred to as the coarse graining approximation.

96

Adhesion Measurement Methods: Theory and Practice

Coatings made from these polymers tend to be highly anisotropic with far different mechanical properties in the plane compared to out-of-plane behavior. This is commonly referred to as orthotropic behavior, and an example is given in Table 3.1. 3.1.5.2 Homogeneous Isotropic Materials It is no accident that the most popular constitutive relation is the one that deals with homogeneous isotropic materials that require only two elastic constants, namely, the Young’s modulus and Poisson’s ratio. It seems that people already regard it as a burden to deal with 2 elastic constants, not to mention 36. If you are working with a newly synthesized polymer, for example, and you browse the manufacturer’s data sheet, you will most likely find only two useful constitutive properties mentioned: the Young’s modulus and the thermal expansion coefficient. In fact, if you inquire about it, the people who made the material, primarily chemists, are most likely unaware of what a Poisson’s ratio is. However, the main reason why it is difficult to find good data on Poisson’s ratio is that it is much more difficult to measure than the Young’s modulus. This problem is discussed in more detail in Section 3.3.1, but now it is important to establish the constitutive relation for homogeneous isotropic materials. This can be done by essentially applying the constraints of spherical symmetry to Equation (3.30). An excellent discussion of the procedure has been given by Gould,2 and the result comes down to the following:

ε11 =

1⎡ σ11 − ν σ 22 + σ 33 ⎤⎦ + αΔT E⎣

ε 22 =

1⎡ σ 22 − ν σ11 + σ 33 ⎤⎦ + αΔT E⎣

(

(

) )

(3.31)

1 ε 33 = ⎡⎣ σ 33 − ν σ11 + σ 22 ⎤⎦ + αΔT E

(

ε12 =

)

σ12 σ σ ; ε 23 = 23 ; ε 31 = 31 2G 2G 2G

Equations (3.31) are the simplest three-dimensional expression of Hooke’s law. In fact, it is easy to see that by collapsing down to one dimension the familiar onedimensional version pops out. Thus, for a simple tensile specimen σ22 = σ33 = σ12 = σ23 = σ31 = 0, and the remaining equation for σ11 becomes σ11 = E ε11, which is the familiar standard form taught in elementary texts. All of this is very satisfying, but yet another essential ingredient is missing. Not only is the real world three dimensional, but also it is governed very strictly by the laws of thermodynamics, which state that everything exists at some finite temperature. Not only that, but also the temperature tends to vary substantially from moment to moment and place to place, giving rise to thermal gradients; these gradients can give rise to strains, which also induce stresses in ordinary objects. In fact, in many

Theoretical Foundations of Quantitative Adhesion Measurement Methods

97

practical situations thermal stresses can entirely dominate the stress distribution in an object. The equation governing the temperature distribution in a body under most conditions is derived from three separate equations, the first of which is in essence a statement of the conservation of energy. Let h be defined as the heat flux vector, which describes the flow of heat (disordered energy) across some small surface area dA in a body per unit time. The quantity h is a vector that will generally vary from point to point in the body. In any particular small volume within the body, heat may be passing through from neighboring volume elements, and there may also be some local heat source within the element generating heat at some rate γ (joules per cubic meter per unit time). Letting q denote the total amount of heat energy per unit volume within the volume at any given time, the conservation of energy requires that

∇·h + γ =

∂q ∂t

(3.32)

Equation (3.32) is commonly referred to as an equation of continuity for the heat flow within a material body. It says in essence that the rate at which heat builds up or drains out of any particular volume is the sum of two terms. The first ∇⋅h accounts for the net flow in from or out to neighboring volume elements. The second term γ accounts for local heat generation, which could be caused by radioactive decay processes or embedded wires. Equation (3.32) states that the time rate of change of heat buildup or loss in any particular volume element is the net sum of energy flow through the bounding surface plus any local contribution from embedded sources. The second equation comes directly from thermodynamics and the definition of the specific heat, that is, (3.33)

dq = ρcv dT or dq dT = ρcv dt dt

In this equation, ρ is the density, and cv is the specific heat (or heat capacity per unit volume) under conditions of constant volume.* Combining Equations (3.32) and (3.33) leads to

∇·h + γ = ρcv

∂T ∂t

* Note that there is also a cp or specific heat under conditions of constant pressure.

(3.34)

98

Adhesion Measurement Methods: Theory and Practice

The final equation is known as Fourier’s law of heat conduction. It is basically the simplest linear constitutive relation for heat flow in solids, relating the heat flux to the gradient of the temperature: h = −κ∇T

(3.35)

Equation (3.35) is simply the statement that when there are spatial variations in the temperature field described by ∇T there will be a concomitant heat flow designated by h, with the constant of proportionality κ known as the thermal conductivity. Combining Equation (3.35) with Equation (3.34) leads to κ∇ 2T + γ = ρcv

∂T ∂t

(3.36)

Using Equation (3.36) along with appropriate initial and boundary conditions, the temperature field in a body can be calculated. If thermal gradients are present or if the body is a composite of materials with different thermal expansion coefficients and is either heated or cooled uniformly, then thermal strains will arise, given by the following formula: ε T = αΔT

(3.37)

with α = (thermal expansion coefficient ΔT = (T – T0) (temperature difference) The parameter α is the thermal expansion coefficient characterizing the tendency of the body to expand or contract on heating. ΔT is the temperature excursion from the reference temperature T0, where the body is in a reference state generally taken to be a condition of zero stress. The thermal strain given by Equation (3.37) must be added to the constitutive relations defined in Equations (3.31) to give the following relations for a thermoelastic solid: ε11 =

1⎡ σ11 − ν σ 22 + σ 33 ⎤⎦ + αΔT E⎣

ε 22 =

1⎡ σ 22 − ν σ11 + σ 33 ⎤⎦ + αΔT E⎣

(

(

) )

(3.38)

1 ε 33 = ⎡⎣ σ 33 − ν σ11 + σ 22 ⎤⎦ + αΔT E

(

ε12 =

)

σ12 σ σ ; ε 23 = 23 ; ε 31 = 31 2G 2G 2G

Equations (3.38) represent the constitutive relations for a homogeneous isotropic material and thereby complete the continuum mechanics program by providing the

Theoretical Foundations of Quantitative Adhesion Measurement Methods

99

essential link between the stresses and the strains in the body. It should be noted that these equations are by no means the most general that can be formulated and are essentially valid in the realm of small strains and temperature excursions. However, they are valid for a wide variety of practical problems, and they form a foundation for considering more elaborate situations in which the assumptions of isotropy, small strains, and the like are not valid. The complete set of field equations for the thermoelastic behavior of a homogeneous isotropic solid are summarized in Table 3.1.

3.2 EXAMPLES Table 3.1 essentially summarizes what was known about the thermoelastic behavior of solids by the end of the 19th century. As such, they represent a cumulative intellectual triumph of that century. However, in addition to representing a purely transcendent accomplishment of the human intellect, the field equations catalogued in Table 3.1 are also amazingly useful tools for analyzing the behavior of solid materials that have found constant application in engineering problems since their derivation. The advent of nearly unlimited computing power represented by the now ubiquitous personal computer workstation has made these equations even more powerful as tools of analysis because previously unusable numerical algorithms can now be fruitfully brought to bear to provide accurate solutions to these equations in support of myriad design and development projects. This section presents a number of “back-of-the-envelope” type calculations designed to give some insight into the utility of the field equations listed in Table 3.1 and provide some feel for how they can be put to work in a number of practical situations. The examples presented, however, only scratch the surface of what can be done with pencil and paper. Indeed, all serious work involving these equations is done on powerful workstations using the exceedingly effective finite element and boundary element analysis schemes.

3.2.1 SIMPLE DEFORMATIONS Some feel for the meaning of the equations for deformation and strain given by Equations (3.29) can be gained by looking at a few simple examples. The simplest possible deformation is a rigid translation. The required deformation mapping comes directly from Equation (3.29a): Consider as a simplest case a rigid translation along the x1 axis, where the displacement vector is simply given by u = b = (b1, 0, 0). Another way to write this is to combine Equations (3.29a) and (3.29b) to obtain the relation x = X + b. Yet another way of looking at it is to write Equation (3.29a) out explicitly; that is, x = K(X) where x = (x1, x2, x3), X = (X1, X2, X3), and K(X) = (X1 + b1, X2, X3). To make things clearer, this can be set out componentwise as follows:

( ) = K (X ) = X = K (X ) = X

x1 = K1 X = X1 + b1 x2 x3

2

2

3

3

(3.39)

100

Adhesion Measurement Methods: Theory and Practice

TABLE 3.1 Collected Field Equations for Homogeneous Isotropic Thermoelastic Material Formula

Variable/Parameter Descriptions

Momentum balance

σ= Stress tensor (N/m2) u = Displacement vector (m) fb = Body force vector (N/m3) ρ = Material density (kg/m3)

Equation (3.22): Newton’s second law generalized for a continuum body

u = Displacement vector (m) I = Identity tensor F, D, J, and ε dimensionless

Equations (3.29): Basic definitions of deformation and strain fields; note that ε is reliable for small strains only

2

fb + ∇ ·σ σ−ρ

d u =0 dt 2

Deformation and strain fields a) Deformation mapping x = K(X) b) Displacement vector u = K(X) – X

Comments

c) Deformation gradient F = ∇K d) Displacement gradient J = ∇u – I e) Finite strain tensor D = 1/2[F FT – I] f) Infinitesimal strain tensor ε = 1/2[∇u + (∇u)T ] g) Equation of compatibility ∇×∇×ε=0 h) Relation between D, ε and u D = ε + 1/2(∇u)(∇u)T εij = Components of strain tensor ε Equations (3.38): Basic equations connecting the σi,j = Components of stress tensor 3) σ stresses to the strains; (N/m Stresses in terms of strains define the solid as a I = Identity matrix ⎞ E ⎛ νI material entity with tr ε = ε11 + ε22 + ε33 σ= ε + tr ε + E α Δ T I ⎟⎠ 1 + ν ⎜⎝ 1 − 2ν recognizable physical tr σ = σ11 + σ22 + σ33 properties; the material is ΔT = (T − T0) thermal excursion Strains in terms of stresses assumed to be (K) 1+ ν ν tr σ homogeneous and E = Young’s modulus (N/m3) ε= σ− I + αΔT I E E G = Shear modulus (N/m3) isotropic v = Poisson’s ratio Componentwise strains in terms of stresses α = Thermal expansion coefficient 1 (K−1) ε11 = ⎡⎣ σ11 − ν σ 22 + σ 33 ⎤⎦ + αΔT E G = E/[2(1 + v)] 1 ε 22 = ⎡⎣ σ 22 − ν σ11 + σ 33 ⎤⎦ + αΔT E Constitutive relations for thermoelastic homogeneous isotropic material

(

)

(

)

ε 33 =

1⎡ σ 33 − ν σ11 + σ 22 ⎤ + αΔT ⎦ E⎣

ε12 =

σ 23 ; σ13 σ12 ; ε 23 = ε13 = 2G 2G 2G

(

)

Theoretical Foundations of Quantitative Adhesion Measurement Methods

101

TABLE 3.1 (continued) Collected Field Equations for Homogeneous Isotropic Thermoelastic Material Formula

Variable/Parameter Descriptions

Comments

εij = Components of strain tensor ε Basic stress-strain relations for a σi,j = Components of stress tensor 3) σ nonisotropic coating for (N/m Componentwise strains in terms of stresses which the elastic ΔT = (T − T0) thermal excursion 1 behavior is dependent on (K) ⎡⎣ σ11 − ν12 σ 22 − ν13σ 33 ⎤⎦ + α1ΔT ε11 = E 11 direction; these relations E1, E1, E1 = Nonisotropic Young’s 3) form the next level of moduli (N/m 1 ⎡⎣ σ 22 − ν21σ11 − ν23σ 33 ⎤⎦ + α 2ΔT ε 22 = i, j = 1, 2, 3 = Nonisotropic complexity above v ij, E 22 Poisson’s ratios Equations (3.38); for the 1 ⎡⎣ σ 33 − ν31σ11 − ν32 σ 22 ⎤⎦ + α 3ΔT G12, G13, G23 = Nonisotropic shear case of in-plane isotropy, ε 33 = E 33 moduli (N/m3) the following constraints α , α , α = Nonisotropic thermal hold: 1 2 3 ν12 = ν 21 expansion coefficients (K−1) E 11 E 22 E11 = E22 = E; E33 = Ez Constitutive relations for thermoelastic homogeneous orthotropic material

ε12 =

σ12 σ σ ; ε13 = 13 ; ε 23 = 23 2G12 2G13 2G23

ν12 = ν21 = ν ν31 = ν13 = ν23 = ν32 = ν z G12 =

E 2(1 + ν)

G13 = G23 =

EEz ( E + Ez + 2 E ν z )

ν2 < 1 and ν2z

Adhesion Measurement Methods Theory and Practice

DK2159_title 10/6/05 1:59 PM Page 1

Adhesion Measurement Methods Theory and Practice Robert Lacombe

Boca Raton London New York

A CRC title, part of the Taylor & Francis imprint, a member of the Taylor & Francis Group, the academic division of T&F Informa plc.

Preface This volume has arisen out of a short course on adhesion measurement methods given in conjunction with a series of symposia on surface related aspects of materials science technology. The conference Web site* caught the attention of John Corrigan, who at that time was an acquisition editor for Marcel Dekker. As I had long been contemplating writing a volume on adhesion measurement to use as supporting material for a short course on adhesion measurement, John did not have to work very hard to convince me that it would be a good idea to write a volume on this topic. In addition, John and I felt that such a volume would fill an important gap in the engineering science literature because there was no single text devoted to adhesion measurement technology notwithstanding the fact that an enormous body of literature existed on the subject in scientific journals and edited volumes. Having thus decided to engage in the project, I concluded that the main purpose of the volume would be to provide a useful reference work and handbook for the practicing engineer/scientist who has a need to confront problems of adhesion either in support of manufacturing operations or in the development of new products. Thus, this book is meant to be used and kept handy for any and all of the following purposes: 1. As a monograph/reference work to be used either for self-study or to become aware of what has been done in the realm of developing methods and useful tools for measuring the adhesion of coatings and thin films. 2. As supplementary reading material for courses on materials science, mechanics of materials, or engineering design of laminate structures at the advanced undergraduate or graduate level. 3. As a handbook for looking up useful information and formulae on adhesionrelated matters, such as driving force formulae for various modes of delamination, methods for estimating stress buildup, and material property data in support of “back-of-the-envelope” calculations. 4. As an introductory reference work for accessing the vast scientific and engineering literature on adhesion measurement. A substantial bibliography of some 40 key reference works plus over 500 articles and books is organized topicwise to provide a convenient introduction to the veritable ocean of information available in the literature. The contents of the book are organized into seven chapters and five appendices in the following order: Chapter 1 gives a brief introduction to the subject, including * Those interested in surface-related phenomena such as adhesion, cleaning, corrosion, and the like can go the conference Web site at www.mstconf.com; there you will find the programs and abstract listings of some 24 previous symposia on these topics, as well as up-to-date information on current and future symposia.

an attempt to define the term adhesion for the purpose of providing a definition that is both accurate and useful in practice. Chapter 2 provides an overview of the most common adhesion measurement methods plus a few exotic methods to round out the mix. From the point of view of this work, adhesion measurement techniques fall into one of the three following categories: qualitative, semiquantitative, and fully quantitative techniques. Each of the methods discussed has its uses and drawbacks, and the intent is to make this as clear as possible. Something akin to a Consumer Reports format is adopted to help the reader interested in selecting a method with which to address current adhesion problems. Anyone just getting involved with adhesion-related issues should find this chapter helpful. Chapter 3 lays the foundation required to step up to the problem of implementing fully quantitative adhesion measurement methods. To do this, however, one has to confront headlong the thermal-mechanical behavior of the materials with which one is dealing. This comes about from the simple fact that all adhesion measurement methods in some way or another apply an external load to the structure tested and then draw conclusions based on the observed deformations or mechanical reaction forces observed. The most general formalism available for dealing with this type of behavior is the continuum theory of solids, which is treated in some detail in this chapter. Inescapably, the level of mathematical treatment rises considerably over that given in Chapter 2. Every attempt is made to avoid excessive rigor and abstract formalism, which does more to flaunt the level of erudition as opposed to shedding light on the technical matters at hand. Thus, those who subscribe to the International Journal of Solid Structures will most likely find the mathematical level quite pedestrian, whereas members of the laity could find the discussion fairly heavy sledding. This should in no way, however, prevent anyone from using the results presented in succeeding chapters to practical advantage. Chapter 4 deals with the discipline of fracture mechanics, which draws directly on all the supporting material presented in Chapter 3. Fracture mechanics is the ultimate organizing tool for performing fully quantitative adhesion measurements. It provides the concepts of stress intensity factor and strain energy release rate, which are two of the most useful quantitative measures of adhesion strength. Thus, from the point of view of fracture mechanics, a delamination is nothing more than a particular kind of crack occurring at an interface in a bimaterial structure. Chapter 5 attempts to draw all of the above material together and make it seem more coherent and relevant by providing several specific and detailed examples of adhesion measurement in action. Thus, extensive examples of the peel test, the scratch test, and the pull test are presented. It is hoped that the reader will gain significant insight and intuition into how adhesion testing is carried out in practice and perhaps find some answers to specific problems of interest. Chapter 6 deals with the problem of measuring the residual or intrinsic stress in a coating or other laminate structure. Whoever reads through the previous three chapters will quickly realize that residual stress is one of the key factors governing the delamination behavior of coatings and laminates and is a critical parameter in most fracture mechanics formulae for stress intensity factors and strain energy release rates. Thus, a fairly comprehensive overview of most of the useful stress

measurement methods is provided. Use of one or more of these methods can be considered as providing an indispensable foundation for developing effective adhesion measurement procedures. Chapter 7 concludes with more examples taken from the author’s direct experience in wrestling with adhesion problems in the microelectronics industry. Silicon chips and ceramic multichip modules used to package these chips into useful devices give rise to a welter of adhesion-related problems because the number of interfaces involved is so varied and extensive that most structures can be looked at as one extensive interface. The presentation here is informal and intended to provide insight and intuition as to how adhesion problems and adhesion measurement happen in the “real world.” Several appendices are provided to make the volume more useful as a day-today handbook and handy reference for looking up simple formulae and material property data for performing back-of-the-envelope type calculations. Rudimentary calculations for estimating the stress expected in a coating or the driving force for delamination can be very helpful for making decisions regarding which processes or materials one should employ for fabricating a specific device. Appendix A provides an overview of vector and tensor calculus for those with a need to brush up on the topic both regarding performing elementary calculations and in understanding more fully the mathematical developments in Chapters 3 and 4. Appendix B gives a quick overview of the most useful aspects of strength of materials theory, which essentially amounts to computing all the ways a beam can bend. This is important material because bending beams figure heavily in many adhesion measurement schemes and stress measurement experiments. Appendix C gives an extended table of material property data required for nearly all the formulae in Appendices B and D. This type of data tends to be scattered far and wide in a variety of texts and reference works, which by Murphy’s second law are never at hand when most needed. Thus, having these data located next to the formulae that require them should prove convenient. Appendix D provides a list of the most useful formulae from fracture mechanics that can be applied to the most common failure modes observed in coatings and laminates. Finally, a two-part bibliography is given that should prove handy in obtaining useful references from the vast technical literature. In closing, I would like to state that this is very much a work in progress. It makes no attempt at being fully comprehensive or definitive in any sense. Rather, the goal is to provide a volume extensive enough to be useful but not so vast as to be more of a burden than a help. In this regard, it is clear that much of relevance had to be left out. It is hoped that future editions will correct this problem to some extent. I invite any and all constructive criticisms and suggestions to correct errors or improve the presentation. I am most readily reached at the e-mail address given below and will give due attention to any and all who respond. Finally, this work would not be complete without giving recognition to my longtime friend, colleague, and co-worker Dr. Kashmiri Lal Mittal (Kash to his friends). Kash has certainly been a key inspiration in completing this work. A cursory look at the references will make it clear that his contributions to the adhesion literature have been monumental. In addition to editing the Journal of Adhesion Science and Technology, he has published 81 (and counting) edited volumes dealing either

directly or indirectly with problems of surface science and adhesion. His many comments and corrections to this work have been indispensable. My thanks go also to John Corrigan, who gave the initial impetus that got this project going. Many thanks, John, wherever you are. Robert H. Lacombe MST Conferences, LLC 3 Hammer Drive Hopewell Junction, NY 12533-6124 E-mail: [email protected]

The Author Robert Lacombe, Ph.D., received his doctoral degree in macromolecular science from Case Western Reserve University and was a postdoctoral fellow at the University of Massachusetts, working on problems of polymer solution thermodynamics. Following his stint in academia, he was an IBM physicist for 20 years and worked on problems relating to thin film wiring technology for both semiconductor chips and multichip modules. After IBM, he worked for an independent consulting firm on hybrid nonintrusive inspection and evaluation techniques, as well as problems of materials compatibility of both semiconductor and microelectronic packaging devices. He is an expert in the area of stress buildup in laminate structures and using the techniques of fracture mechanics in solving problems of delamination and cracking in composite devices. He has been a leader in the areas of materials characterization and published some of the first mechanical response data on monolayer nanostructures in the early 1980s. In addition, he pioneered innovative uses of largescale computation using finite element methods and applied this expertise directly to problems affecting product development and manufacturing. Dr. Lacombe is Chairman of MST Conferences and has organized over 20 international symposia covering the topics of adhesion and other surface-related phenomena since 1998. He is credited with over 40 publications and patents. Dr. Lacombe is a leading innovator in the field of subsurface inspection methods dealing with flaws in structural parts of air, auto, marine, and aerospace vehicles. As part of his activities with MST Conferences, he teaches a semiannual course on adhesion measurement methods in conjunction with the symposia.

Table of Contents Chapter 1

Introduction ..........................................................................................1

1.1 1.2

Overview ..........................................................................................................1 What Is Adhesion and Can It Be Measured?..................................................2 1.2.1 Definition A: Criteria for a Truly Useful Definition of the Term Adhesion...............................................................................................3 1.2.2 Definition B: Adhesion ........................................................................5 1.3 Comments on Nomenclature and Usage .........................................................5 References..................................................................................................................6

Chapter 2 2.1 2.2

2.3

2.4

2.5

2.6

2.7

Overview of Most Common Adhesion Measurement Methods .........7

Preamble...........................................................................................................7 Peel Test ...........................................................................................................8 2.2.1 Introduction ..........................................................................................8 2.2.2 Advantages of the Peel Test ..............................................................10 2.2.3 Disadvantages of the Peel Test ..........................................................10 2.2.4 Summary and Recommendations ......................................................11 Tape Peel Test ................................................................................................11 2.3.1 Introduction ........................................................................................11 2.3.2 Advantages of the Tape Peel Test......................................................12 2.3.3 Disadvantages of the Tape Peel Test .................................................14 2.3.4 Summary and Recommendations ......................................................14 Pull Test..........................................................................................................14 2.4.1 Introduction ........................................................................................14 2.4.2 Advantages of the Pull Test ...............................................................15 2.4.3 Disadvantages of the Pull Test ..........................................................16 2.4.4 Summary and Recommendations ......................................................17 Indentation Debonding Test...........................................................................17 2.5.1 Introduction ........................................................................................17 2.5.2 Advantages of the Indentation Debonding Test ................................19 2.5.3 Disadvantages of the Indentation Debonding Test............................20 2.5.4 Summary and Recommendations ......................................................20 Scratch Test ....................................................................................................20 2.6.1 Introduction ........................................................................................20 2.6.2 Advantages of the Scratch Test .........................................................26 2.6.3 Disadvantages of the Scratch Test .....................................................27 2.6.4 Summary and Recommendations ......................................................27 Blister Test .....................................................................................................27

2.7.1 Introduction ........................................................................................27 2.7.2 Advantages of the Blister Test...........................................................31 2.7.3 Disadvantages of the Blister Test ......................................................31 2.7.4 Summary and Recommendations ......................................................32 2.8 Beam-Bending Tests ......................................................................................32 2.8.1 Introduction ........................................................................................32 2.8.2 Three-Point Bend Test .......................................................................32 2.8.3 Four-Point Bend Test .........................................................................34 2.8.4 Standard Double Cantilevered Beam Test.........................................35 2.8.5 Tapered Double Cantilevered Beam Test ..........................................37 2.8.6 Double-Cleavage Drilled Compression Test .....................................39 2.8.7 Brazil Nut Test ...................................................................................40 2.8.8 Wedge Test .........................................................................................41 2.8.9 Topple Beam Test...............................................................................42 2.8.10 Advantages of Beam-Bending Tests..................................................43 2.8.11 Disadvantages of Beam-Bending Tests .............................................43 2.8.12 Summary and Recommendations ......................................................44 2.9 Self-Loading Tests .........................................................................................44 2.9.1 Circle Cut Test ...................................................................................44 2.9.2 Modified Edge Liftoff Test ................................................................46 2.9.3 Microstrip Test ...................................................................................47 2.9.4 Advantages of Self-Loading Tests.....................................................48 2.9.5 Disadvantages of Self-Loading Tests ................................................48 2.9.6 Summary and Recommendations ......................................................49 2.10 More Exotic Adhesion Measurement Methods .............................................49 2.10.1 Laser Spallation: Early Work.............................................................49 2.10.2 Later Refined Experiments ................................................................51 2.10.3 Laser-Induced Decohesion Spectroscopy Experiment ......................54 2.10.4 Advantages of Laser Spallation Tests................................................55 2.10.5 Disadvantages of Laser Spallation Test.............................................55 2.10.6 Summary and Recommendations ......................................................56 2.11 Electromagnetic Test ......................................................................................56 2.11.1 Advantages of the Electromagnetic Test ...........................................60 2.11.2 Disadvantages of the Electromagnetic Test.......................................60 2.11.3 Summary and Recommendations ......................................................60 2.12 Nondestructive Tests ......................................................................................60 2.12.1 Dynamic Modulus Test ......................................................................61 2.12.2 Advantages of the Dynamic Modulus Test .......................................63 2.12.3 Disdvantages of the Dynamic Modulus Test.....................................65 2.12.4 Summary and Recommendations ......................................................65 2.13 Surface Acoustic Waves Test .........................................................................65 2.13.1 Advantages of the Surface Acoustic Waves Test ..............................68 2.13.2 Disadvantages of the Surface Acoustic Waves Test ..........................68 2.13.3 Summary and Recommendations ......................................................69 Notes ........................................................................................................................69

Chapter 3

Theoretical Foundations of Quantitative Adhesion Measurement Methods ..............................................................................................75

3.1

Introduction to Continuum Theory................................................................75 3.1.1 Concept of Stress in Solids................................................................77 3.1.2 Special Stress States and Stress Conditions......................................83 3.1.2.1 Principal Stresses ................................................................83 3.1.2.2 St. Venant’s Principle..........................................................84 3.1.2.3 Two-Dimensional Stress States ..........................................85 3.1.3 Equation of Motion in Solids ............................................................86 3.1.4 Deformation and Strain......................................................................89 3.1.5 Constitutive Relations or Connecting the Stress to the Strain..........93 3.1.5.1 General Behavior ................................................................93 3.1.5.2 Homogeneous Isotropic Materials......................................96 3.2 Examples ........................................................................................................99 3.2.1 Simple Deformations .........................................................................99 3.3 Solving the Field Equations.........................................................................106 3.3.1 Uniaxial Tension ..............................................................................106 3.3.2 Biaxial Tension.................................................................................108 3.3.3 Triaxial Stress Case..........................................................................110 3.4 Application to Simple Beams ......................................................................112 3.5 General Methods for Solving Field Equations of Elasticity.......................130 3.5.1 Displacement Formulation ...............................................................131 3.5.2 Stress Formulation ...........................................................................132 3.5.3 Mixed Formulation...........................................................................133 3.6 Numerical Methods......................................................................................134 3.6.1 Introduction ......................................................................................134 3.7 Detailed Stress Behavior of a Flexible Coating on a Rigid Disk...............135 3.8 Strain Energy Principles ..............................................................................138 3.9 The Marvelous Mysterious J Integral..........................................................146 3.10 Summary ......................................................................................................151 Notes ......................................................................................................................152 Chapter 4 4.1

4.2

Elementary Fracture Mechanics of Solids: Application to Problems of Adhesion......................................................................155

Introduction ..................................................................................................155 4.1.1 Introductory Concepts......................................................................155 4.1.1.1 Strain Energy Approach ...................................................159 4.1.1.2 Stress Intensity Factor Approach......................................161 Fracture Mechanics as Applied to Problems of Adhesion..........................163 4.2.1 Elementary Computational Methods ...............................................163 4.2.1.1 Basic Model of Thin Coating on Rigid Disk...................163 4.2.2 Decohesion Number Approach of Suo and Hutchinson .................174 4.2.2.1 The Decohesion Number..................................................179 4.2.3 Back-of-the-Envelope Calculations .................................................180

4.2.3.1 Polyimide on Glass-Ceramic............................................181 4.2.3.2 Nickel on Glass.................................................................183 4.3 Summary ......................................................................................................185 Notes ......................................................................................................................185 Chapter 5

Applied Adhesion Testing................................................................187

5.1

The Peel Test................................................................................................187 5.1.1 Sample Preparation ..........................................................................188 5.1.2 Test Equipment ................................................................................189 5.1.3 Peel Testing in Action......................................................................190 5.1.4 Advanced Peel Testing.....................................................................193 5.1.4.1 Thermodynamics of the Peel Test ....................................194 5.1.4.2 Deformation Calorimetry..................................................194 5.2 Fully Quantitative Peel Testing....................................................................198 5.2.1 Earliest Work, Elastic Analysis........................................................198 5.2.2 Elastic-Plastic Analysis ....................................................................210 5.2.2.1 Theory of Elastic-Plastic Peeling for Soft Metals ...........213 5.2.3 Full Elastic-Plastic Analysis ............................................................217 5.2.3.1 General Equations for Deformation of Peel Strip ...........217 5.2.3.2 Basic Goal.........................................................................217 5.2.3.3 Analysis Strategy and Assumptions .................................218 5.2.3.4 Equations of the Elastica ..................................................218 5.2.3.5 Case 1: Elastic Peeling .....................................................225 5.2.3.6 Case 2: Elastic-Plastic Peeling/Unloading .......................226 5.2.3.7 Case 3: Elastic-Plastic Loading and Unloading...............227 5.3 The Scratch/Cut Test....................................................................................231 5.3.1 The Cut Test.....................................................................................233 5.3.2 Simplified Analytical Model for Cut Test .......................................237 5.4 The Pull Test ................................................................................................242 5.5 Summary ......................................................................................................245 Notes ......................................................................................................................246 Chapter 6 6.1 6.2

Adhesion Aspects of Coating and Thin Film Stresses....................249

Introduction ..................................................................................................249 General Measurement Methods for Thin Films and Coatings ...................251 6.2.1 Cantilevered Beam Method .............................................................251 6.2.2 Variations on Bending Beam Approach ..........................................257 6.2.3 Optical Measurement of Deflection.................................................257 6.2.3.1 Microscopy .......................................................................257 6.2.3.2 Laser Beam Deflection .....................................................258 6.2.3.3 Laser Interferometry .........................................................258 6.2.3.4 Capacitive Measurement of Deflection ............................259 6.2.3.5 Stress Measurement by Vibrational Resonance ...............260 6.2.3.6 Holography of Suspended Membrane..............................265

6.2.4 6.2.5

X-ray Measurements ........................................................................269 Ultrasonics........................................................................................272 6.2.5.1 Through-Thickness Stress Measurement .........................279 6.2.5.2 Surface Stress Measurement Using Skimming Longitudinal Waves ..........................................................279 6.2.5.3 Rayleigh Wave Method ....................................................280 6.2.5.4 Surface-Skimming SH Waves ..........................................280 6.2.6 Photoelasticity ..................................................................................280 6.2.7 Strain Relief Methods ......................................................................294 6.2.8 Magnetics .........................................................................................297 6.2.8.1 Barkhausen Noise .............................................................297 6.2.8.2 Magnetostriction Approach ..............................................299 6.2.9 Raman Spectroscopy........................................................................299 6.2.10 Miscellaneous Methods....................................................................301 6.2.10.1 Stress Pattern Analysis by Thermal Emission .................301 6.2.10.2 Photoelastic Coating Technique .......................................302 6.2.10.3 Brittle Lacquer Method ....................................................302 6.3 Summary ......................................................................................................303 Notes ......................................................................................................................303 Chapter 7

Case Studies from the Field ............................................................309

7.1 A Study in Adhesion Sensitivity to Contamination ....................................310 7.2 Case of the Improperly Cured Film ............................................................317 7.3 Case of the Stressed Pin ..............................................................................325 7.4 Stability Maps ..............................................................................................333 7.5 Summary ......................................................................................................334 Notes ......................................................................................................................335 Appendix A Vectors and Vector Calculus..........................................................337 A.1 Introduction ..................................................................................................337 A.2 Elementary Definitions of Scalars, Vectors, and Tensors ...........................339 A.2.1 Simple Scalars..................................................................................339 A.2.2 Vectors ..............................................................................................339 A.2.2.1 Vector Operations .............................................................340 A.2.2.2 Tensor Operations .............................................................342 A.2.2.3 Special Tensors and Operations .......................................344 A.2.2.4 Tensor/Matrix Multiplication............................................347 A.2.2.5 Product of a Matrix with a Vector ...................................349 A.2.2.6 Tensor/Matrix Scalar Product...........................................350 A.2.2.7 Assorted Special Arrays and Operations..........................350 A.3 Vector Calculus ............................................................................................354 A.3.1 Fundamental Operations of Vector Calculus ...................................355 A.3.1.1 The Gradient Operator......................................................355 A.3.1.2 The Divergence Operator .................................................356

A.3.1.3 The Curl Operator ............................................................357 A.3.1.4 The Gradient of a Vector ..................................................359 A.3.2 Basic Theorems of Vector Calculus.................................................360 A.3.2.1 Divergence Theorem.........................................................360 A.3.2.2 Stokes Theorem ................................................................361 Notes ......................................................................................................................367 Appendix B Notes on Elementary Strength of Materials (SOM) Theory ........369 B.1 Basic Concepts.............................................................................................370 B.1.1 Notion of Static Equilibrium ...........................................................370 B.1.2 Equations for Bending of Simple Beams........................................372 Appendix C Material Property Data for Selected Substances ..........................377 C.1 Useful Formulae...........................................................................................378 Notes ......................................................................................................................381 Appendix D Driving Force Formulae for a Variety of Laminate Structures ....383 Notes ......................................................................................................................389 Appendix E Selected References and Commentary on Adhesion Measurement and Film Stress Literature ......................................391 E.1 E.2

E.3 E.4 E.5

General References ......................................................................................391 Selected References on Adhesion Measurement Methods .........................392 E.2.1 Blister Test .......................................................................................392 E.2.2 Scratch Test ......................................................................................393 E.2.3 Indentation Debonding Test.............................................................394 E.2.4 Scotch Tape Test ..............................................................................395 E.2.5 Laser Spallation................................................................................395 E.2.6 Selected References on Mechanics of Peel Test .............................395 E.2.7 Nondestructive Methods ..................................................................396 Selected References on Stresses in Laminate Structures and Coatings .....396 Selected References on Fracture Mechanics as Related to Problems of Adhesion of Films and Coatings .................................................................397 Selected References on Stresses in Solids ..................................................397

Appendix F General Adhesion Measurement References ................................399 F.1 F.2 F.3 F.4 F.5 F.6

Review Articles ............................................................................................399 General Adhesion Papers .............................................................................400 Acoustic Emission/Ultrasonic Methods.......................................................401 Bend Test......................................................................................................402 Blister Test ...................................................................................................403 Double Cantilevered Beam Test ..................................................................405

F.7 F.8 F.9 F.10 F.11 F.12 F.13 F.14 F.15 F.16 F.17 F.18 F.19 F.20 F.21 F.22 F.23 F.24 F.25 F.26

Centrifugal Loading Test .............................................................................405 Electromagnetic Test ....................................................................................406 Fracture Mechanics Studies .........................................................................406 Indentation Test ............................................................................................408 Internal Friction............................................................................................409 Impact Methods............................................................................................409 Lap Shear Test..............................................................................................409 Laser/Electron Spallation.............................................................................411 Miscellaneous Methods................................................................................411 Peel Test .......................................................................................................414 Pull Test........................................................................................................420 Pullout Test...................................................................................................422 Push Out Test ...............................................................................................423 Residual Stress Self-Loading Test ...............................................................423 Scratch Test ..................................................................................................424 Tape Test ......................................................................................................426 Theoretical Studies.......................................................................................427 Thermal Methods .........................................................................................428 Topple Beam Method...................................................................................428 Wedge Test ...................................................................................................428

Index ......................................................................................................................429

1

Introduction

Can you measure it? Can you express it in figures? Can you make a model of it? If not, your theory is apt to be based more upon imagination than upon knowledge. Lord Kelvin

1.1 OVERVIEW The science of adhesion has the curious distinction of being at one and the same time both a “sticky” subject and a “slippery” one. The sticky aspect is obvious and needs no further comment; it is the slippery aspect that will draw much of our attention in this volume. The essential problem arises from the fact that adhesion is a basic property of surfaces, and according to the famous physicist Wolfgang Pauli: “God created matter; surfaces were invented by devil.” Surfaces are indeed devilish entities, especially for those who seek a quantitative understanding of their behavior. This arises from the fact that, for nearly all macroscopic objects, the surface area forms a very small portion of the bulk, is further subject to highly asymmetric forces, and is strongly prone to contamination and a large variety of defects. All of this makes it very tricky to characterize the nature of a real surface. For instance, one can have a glass surface that, for all practical purposes, appears to be absolutely clean, but the presence of even a monolayer of contaminant can change its behavior from water wettable to hydrophobic. This in turn has dramatic consequences if one is trying to get a particular coating to adhere to the glass. From a practical point of view, obtaining good adhesion in a manufacturing process requires very serious attention to the state of cleanliness of the surface to which something must be bonded. Furthermore, simply cleaning the surface may not be enough because contaminants may intrude from the ambient atmosphere. A notorious example of this arises in brazing processes where, for instance, one is trying to adhere a metal cap to a ceramic substrate using a solder formulation. Every precaution can be taken to ensure that the mating surfaces are scrupulously clean, but a contaminant such as silicone oil can condense onto the mating surfaces in question, preventing proper wetting of the solder and thus causing a defective joint to be formed. In many instances, silicone oil may be used for a variety of purposes in neighboring sections of a manufacturing plant. A common heating/ventilation system can then carry microscopic amounts of the volatile liquid throughout the entire plant, and because only a monolayer of coverage is enough to disrupt the wetting properties of a surface, the consequences can be catastrophic for the brazing process. Such problems can and do happen rather more frequently than one might imagine in the world of industrial processing, which emphasizes the slippery aspect of adhesion phenomena.

1

Introduction

3

One of the earliest overviews of this issue was given by Mittal,1 and we take his discussion as a starting point. The basic argument comes down to what one takes as the definition of adhesion. Now, from a commonsense point of view, one would like to think that adhesion is a simple matter of how well two different materials tend to stick together, and that adhesion measurement is some indication of the force required to separate them. Although this approach may suffice for the person in the street, it runs into serious difficulty when one tries to arrive at a more scientific definition of adhesion that can be useful for engineering purposes. A truly useful definition of the term adhesion needs to have the properties as given in definition A.

1.2.1 DEFINITION A: CRITERIA OF THE TERM ADHESION

FOR A

TRULY USEFUL DEFINITION

If we say that X is the adhesion of material A to material B, then it should have the following characteristics: 1. X has the same meaning for all practitioners who would stick A to B. 2. X is unambiguously measurable by one or more commonly understood methods. 3. Knowing X allows the practitioner to predict the loading conditions that will cause material A to delaminate from material B. Many would agree that the above is certainly a worthy definition of the term adhesion, but it unfortunately runs into a number of difficulties in practice because of the slippery aspects of the science of adhesion discussed in this chapter. In particular, the following types of problems are likely to arise in practice: •

Problem 1: Universality of the Definition Regarding Selection of Materials to be Adhered and Nature of Active Practitioners — Definition A runs into a variety of problems regarding the universality condition mentioned as characteristic 1. Let us assume that material A is a coating material to be applied to a thick rigid substrate comprised of material B. For simplicity, we assume that these materials are universally available to practitioners P1 and P2 in reasonably pure form. However, practitioner P1 wants to coat A onto B as a thin film less than 1 μm thick, whereas practitioner P2 wants to coat A onto B as a thick coating more than 25 μm thick. All other conditions are equal. Let us also assume that our practitioners are equally scrupulous in cleaning the substrate material B, and it is reported that A adheres well to B. Nonetheless, it can easily happen that practitioner P1 will find good adhesion of A to B whereas P2 will experience delamination. Among a wide variety of problems that can occur, one of the most common is the presence of thin film stresses. If the two practitioners use different techniques to coat A onto B, then the two coatings can develop different material morphologies, which can lead to substantially different stress levels in the two coatings. The more highly stressed coating will be much more likely to delaminate than the other.

2

Adhesion Measurement Methods: Theory and Practice

The scope of problems alluded to here makes the science of adhesion a very broad one that covers the range of disciplines from surface characterization to strength of materials. Indeed, many volumes have been written on the subject. However, the focus here is on one key aspect of the study of adhesion phenomena: the science of adhesion measurement. The basic goal is twofold. First, this volume is to serve as a manual for the relatively uninitiated worker in either academia or industry who has a practical need to perform adhesion measurements either as part of an experimental program or possibly as part of some quality control procedure. A broad range of well-known experimental techniques are reviewed and critiqued regarding their respective strengths and weaknesses. References are given both to the technical literature and to applicable commercial instrumentation. Emphasis is given to those methods that supply at least a semiquantitative estimate of adhesion strength and can be implemented in any laboratory with minimum expenditure of resources. Thus, the practical user can look to this volume as a ready guide and resource for getting a handle on personal adhesion measurement needs. The second goal of this work is to provide a more fundamental understanding of the adhesion measurement process and its consequences regarding the design and manufacture of structures that have a critical dependence on the adhesion of disparate material layers. The multilevel wiring layers in microelectronic structures immediately come to mind as an appropriate paradigm. Such systems often involve the buildup of material stresses that, to be effectively handled, require an understanding of continuum theory and fracture mechanics. Thus, a substantial section of this volume is devoted to the elements of continuum theory and fracture mechanics most relevant to the problem of adhesion measurement. It should be mentioned also that the topics of material behavior and fracture mechanics are of great concern even for the practical individual mainly concerned with subduing a specific adhesion problem that is plaguing a particular manufacturing process. The point is that, if material stresses get high enough, no amount of adhesion improvement will solve the problem of device failure. If the interface proves to be too strong, then the delamination failure simply proceeds as a fracture crack in the bulk material. Solving such problems unavoidably requires understanding and control of the material stresses. Again, microelectronic structures provide a prime example in which such situations can arise. In response to this type of dilemma, an entire section of this work treats the topic of stability maps, which provide a means of navigating through such problems. This is a topic of significant interest for both the practical user as well as anyone interested in the more fundamental and theoretical aspects of adhesion measurement and control.

1.2 WHAT IS ADHESION AND CAN IT BE MEASURED? There has been considerable debate in the technical literature concerning the question of what adhesion is and if it can be measured, and it is certainly not the intent here to expound further on what has been discussed many times. However, to provide a certain measure of perspective and to establish a defensible position on this matter, it is worthwhile at least to discuss this problem briefly.

4

Adhesion Measurement Methods: Theory and Practice

•

•

Furthermore, even assuming that the two practitioners used identical coating techniques, practitioner P2 will be much more likely to experience delamination because of the thicker coating as, for a given level of film stress, the driving force for edge delamination will scale linearly with film thickness. A second problem that can occur is that the two coatings may be subjected to different loading conditions when in use. For example, practitioner P1’s coating may see predominantly shear loads, whereas that of practitioner P2 experiences predominantly tensile loads. Because most coatings tend to resist shear delamination (commonly referred to as mode II) much better than tensile delamination (commonly referred to as mode I), practitioner P2 will be much more likely to experience delamination problems than his counterpart P1. Thus, definition A falls short regarding the universality criterion in that it may give good results for those putting down thin coatings and poor results for those trying to make thick coatings. Problem 2: Definition A Enables the Use of Simple and Unambiguous Measurement Procedures — From the point of view of the practical practitioner, the use of simple and unambiguous measurement procedures is quite likely the most important property desired in any truly usable definition of the term adhesion. However, the two qualifications of simple and unambiguous tend to be mutually contradictory in that a truly simple test is not likely to be unambiguous because, for the sake of simplicity, a number of important details will be either omitted or glossed over. The truly unambiguous test will specify in great detail the conditions of sample preparation, including cleaning procedures, control of material properties, precise specification of loading conditions, and control of the ambient environment. Observing all of these caveats will tend to undermine the goal of achieving simplicity. Clearly, any truly usable definition of adhesion will have to seek an appropriate balance between these two criteria. Problem 3: Definition A Has True Predictive Power — It is at once clear that the property that definition A has true predictive power is at odds with characteristic 2 because to obtain a truly predictive measure of adhesion, clearly the utmost attention must be given to all the details that will ensure an unambiguous result. This will sacrifice the goal of achieving simplicity. In addition, to be truly predictive the measurements have to be fully quantitative and consistent with detailed calculations. This implies at minimum the use of fracture mechanics methods and continuum theory of materials.

So where does this leave us? It is clear that although definition A is what we would like to have for a definition of the term “Adhesion”, it is clearly unworkable in the real world. In this volume, therefore, we back off somewhat from definition A and revert to definition B. However, before we frame definition B, we reflect on just what we are after vis-à-vis what is practicably obtainable. As this volume is primarily intended for those who have a practical need to perform adhesion measurements in support of the need to fabricate useful structures, our definition focuses on the need to be readily measurable. This puts the property of simplicity in the forefront as

Introduction

5

complex measurement procedures have a relatively low probability of implementation in a manufacturing process in which time and resource expenditure are carefully regulated commodities. In addition, our working definition has to be hierarchal because there are different levels of quantitativeness that can be specified depending specifically on the end use of the adhesion measurement. Thus, we frame definition B:

1.2.2 DEFINITION B: ADHESION We say the adhesion of material A to material B is such and such based on the following criteria: 1. The adhesion of A to B is a relative figure of merit indicating the tendency of A to stick or bind to B derived from an observation or measurement that can be entirely qualitative, semiquantitative, or fully quantitative. 2. The precise meaning of the term is entirely dependent on the details of the measurement technique employed and the experimental and environmental conditions under which the measurement was made. This leads to a hierarchy of definitions. Thus, qualitatively we might say A has good adhesion to B based on the observation that A was never observed to separate from B under a variety of common loading conditions. A semiquantitative statement of the adhesion of a coating of material A onto a substrate of material B might indicate that 2% of the coating was removed during a “Scotch tape” test. Finally, a fully quantitative statement might conclude that the adhesion strength of A to B is 10 J/m2 based on a double-cantilever beam experiment carried out at 50°C under 40% relative humidity.

1.3 COMMENTS ON NOMENCLATURE AND USAGE Definition B can be considered as defining the practical adhesion of one material to another. As defined, it is clearly measurable and has definite significance within the context of the specific measurement technique employed. This definition stands in contradistinction to the term fundamental adhesion, which would imply the work required for separation of material A from B assuming they were joined across a perfect mathematical plane and that the separation avoided any tearing out of either material. The fundamental adhesion of one material to another is an important theoretical concept and is clearly definable in principle. The problem for our purposes is that the fundamental adhesion is exceedingly difficult, if not impossible, to measure under most conditions and even if measured is not likely to be of any immediate use. At this point, we simply recognize that practical adhesion is some complex function of fundamental adhesion that we fortunately do not need to know under most circumstances. Furthermore, we recognize that the fundamental adhesion between two materials can be modified by physicochemical means and is a powerful tool for modifying practical adhesion. For the most part, however, this topic is beyond the scope of this volume. At this point, a number of comments on usage are in order. We have defined the noun adhesion from definition B, and we largely follow common dictionary usage

6

Adhesion Measurement Methods: Theory and Practice

and use the term adhere as the verb form. Also, when a coating separates from its substrate we use the term delamination. In the mechanics literature, one sometimes comes across the term decohesion. A coating is said to decohere from its substrate. The genesis of this term arises from the fact that the locus of failure lies in the substrate material a few microns below the true interface. Thus, it makes sense to talk about cohesive failure. One can also say the coating delaminated from the surface because that is the net effect, and failure occurred so close to the interface that, given the analytical tools at hand, the cohesive nature of the failure could not be detected. In all cases, one has to rely on the context of the measurements and observations to decide which term is most appropriate.

References 1. Mittal, K.L. Adhesion Measurement: Recent Progress, Unsolved Problems, and Prospects, in Adhesion Measurement of Thin Films, Thick Films, and Bulk Coatings, ASTM STP-640 (K.L. Mittal, Ed.), American Society for Testing and Materials, Philadelphia, PA, 1978, pp. 5–17.

2

Overview of Most Common Adhesion Measurement Methods

No experiment is so dumb that it should not be tried. Attributed to Walther Gerlach in reply to Max Born’s comments that his work on magnetic fields with strong spatial gradients would not be worthwhile. This work turned out to be pivotal to the success of the now-famous Stern-Gerlach experiment, which demonstrated spatial quantization for the first time and has been one of the experimental linchpins for quantum theory ever since.1

2.1 PREAMBLE This chapter overviews some of the most commonly used, and consequently the most useful, adhesion measurement methods. The approach follows that of a Consumer Reports-type examination in which both the strengths and the weaknesses of each technique are examined, and specific recommendations are made as to which methods are most suitable for which applications. Definition B of the term “adhesion” as presented in the Chapter 1 is assumed throughout. In addition, the discussion is guided by the following criteria for the “ideal” adhesion test: •

•

•

Quantitative: Gives numerical data that can be unambiguously interpreted. Data analysis straightforward and clear. Ease of sample preparation: Samples quickly and easily prepared with readily available equipment. If sample preparation is too complex, the test will not likely be implemented. Results relevant to real world: Final data must have relevance to final use conditions.

It should be made clear from the outset that none of the techniques described below meets all of the above criteria for the ideal adhesion test. However, each of these tests provides useful and reliable data when applied in a conscientious manner. Finally, it should be stated that this survey in no way covers all of the adhesion measurement methods reported in the literature. Mittal2 informally counted over 300 reported methods as of early 1994. Most of the reported methods, however, are essentially variations on one of the techniques described in what follows.

7

8

Adhesion Measurement Methods: Theory and Practice

Adhesion measurement methods can be divided into two broad categories: destructive or nondestructive. The overwhelming majority fall into the destructive class, by which a loading force is applied to the coating in some specified manner and the resulting damage subsequently observed. Nondestructive methods typically apply a pulse of energy to the coating/substrate system and then try to identify a specific portion of the energy that can be assigned to losses occurring because of mechanisms operating only at the interface. Inferences are then made regarding the bonding strength between the coating and the substrate.

2.2 PEEL TEST 2.2.1 INTRODUCTION Within the realm of destructive adhesion tests, there are two major classes: those dealing with relatively soft flexible coatings and those dealing with hard brittle coatings. By far the most common test for flexible coatings is the peel test. Anyone who has removed wallpaper from an old house already has considerable practical experience with the basic rudiments of this test. When dealing with polymer-based paints, for example, the peel test readily suggests itself as the preferred experiment for testing the adhesion of the coating. Such coatings on curing and drying tend to build up a significant level of internal stress, which increases dramatically near the edge of the coating. If the level of adhesion between the coating and the substrate is not sufficient, then the coating will delaminate and peel back. The now-released coating can be grasped with a tweezer, and an ersatz peel test is performed. Thus, the peel test automatically suggests itself as an adhesion test for flexible paint coatings. The main task for the experimenter is to standardize and quantify the peel test experiment so that the results can be used either to establish a quantitative ranking among the coatings tested or to set a numerical specification for adhesion strength that can be subsequently used as a quality control standard. The problem of quantifying the test is readily solved by the use of an appropriate tensile test apparatus in conjunction with suitable hardware for applying the peel force load and maintaining the required peel angle. Figure 2.1 exhibits a number of common configurations. Figure 2.1a illustrates the common 90° peel test; it is the favored test for flexible coatings on rigid substrates. This is by far the most prevalent and most thoroughly studied of all the peel tests. Figure 2.1b illustrates the 180° version of Figure 2.1a. This configuration offers advantages when space is cramped; Chapter 5 presents this scenario for the peel test performed in a calorimeter. It is also clear that the peel test can be performed at any angle between 0 and 180°. For most practical purposes, there is little need to consider angles other than 90 or 180° unless there are geometric constraints imposed by the sample or test apparatus. From an analytical point of view, however, varying the peel angle can provide information on the effect of mode mixity on peel strength. When performing a peel test, the interfacial region is subjected to both tensile (mode I) and shear (mode II) loads. The ratio of these two loading types is loosely referred to as the loading mode mixity. The importance of knowing the mode mixity

Overview of Most Common Adhesion Measurement Methods

F

F

(a) 90 degree peel test

T

(c) Climbing drum test

9

(b) 180 degree peel test

F

F

(d) T peel test

FIGURE 2.1 Four standard peel test configurations: (a) 90˚ peel test, the most commonly used configuration; (b) 180˚ test preferred when available space precludes the 90˚ test; (c) climbing drum or peel roller test, which has the advantage of controlling the radius of curvature of the peel strip; (d) T-peel test, preferred when testing adhesion of two flexible strips. A symmetric peel is obtained when identical strips are separated. Can also be used in a nonsymmetric configuration in which the two strips are not identical.

stems from the fact that the apparent adhesion strength of many coatings is sensitive to the mode mixity. For example, glues tend to be much stronger in shear than in tension, which implies that they will exhibit much higher adhesion strength in a predominantly mode II test as opposed to a mode I test. A very common example of this phenomenon is exhibited by Velcro fasteners. When loaded in shear, the Velcro fastener exhibits a very tenacious grip. However, when pulled at a right angle (i.e., tensile or mode I loading) the fastener readily separates. Figure 2.1c illustrates the climbing drum test used in testing the adhesion of rubbers in the tire industry. One advantage of this version is that the radius of curvature of the peeling film is fixed by the drum radius, which simplifies later numerical analysis of the data. Finally, the T-peel test shown in Figure 2.1d can be used to test the adhesion between two flexible films.

10

2.2.2 ADVANTAGES

Adhesion Measurement Methods: Theory and Practice OF THE

PEEL TEST

The peel test in its many configurations meets many of the criteria of the ideal adhesion test. Sample preparation is typically reasonably simple and straightforward. This single fact more than anything else accounts for the overall popularity of this test. Also, the peel force gives a semiquantitative measure of the coating adhesion to the substrate, which can be readily used for ranking or quality control purposes. A further advantage of this test is the fact that the rate of delamination and the locus of failure can be controlled fairly precisely. This stems from the fact that a very high stress concentration exists at the point where the coating just lifts off the substrate. This tends to narrowly focus the failure region very close to the geometric interface between coating and substrate, which is the region of most interest in any adhesion test. Because the rate of delamination can be precisely controlled by the test equipment, studies of the rate dependence of adhesion strength can be easily carried out. This can be very important when studying coatings that exhibit a strong molecular relaxation behavior (i.e., glass transition and related phenomena) near the test temperature. Finally, the peel test readily lends itself to use under conditions of controlled temperature and environment (for example, temperature and humidity conditions).

2.2.3 DISADVANTAGES

OF THE

PEEL TEST

As noted, the peel test works quite well when used as a method for ranking the adhesion of a coating when the substrate has been subjected to a number of different surface treatments. However, when trying to ascertain whether the coating will survive a given set of end-use conditions, several problems arise. The main issue is the fact that the peel test subjects the coating to very high strain levels near the peel bend, which most coatings never see under common end-use conditions. The strain in the coating at the peel bend can easily approach 25% or higher, whereas real coatings delaminate under nearly strain-free conditions. Thus, the load state imposed by the peel test does not reasonably approximate the load conditions that cause failure in the field; therefore, conclusions arrived at on the basis of peel testing can be highly misleading when trying to anticipate the actual service behavior of a particular coating. A particularly illuminating example of how far off you can be was given by Farris and Goldfarb.3 These authors tested the adhesion of polyimide films to aluminum and demonstrated apparent peel strength adhesion values in the range of 500 to 900 J/m2. However, the same coatings self-delaminated at an adhesion strength of 23 J/m2 when the coating thickness was increased to 120 μm. Thus, it is clear that peel test results can present highly misleading estimates of the actual adhesion strength of a coating when subjected to realistic end-use conditions. Further limitations of the peel test stem from the fact that it is applicable only to tough flexible coatings. Attempts have been made to circumvent this limitation by applying peelable backing coatings on top of the coating to be tested and then peeling the composite laminate. One major problem with this approach is the fact that the locus of failure at the peel front can become unstable. The delamination front can wander between the backing layer and the test coating or between the coating under test and the substrate, making interpretation of the results unclear.

Overview of Most Common Adhesion Measurement Methods

11

A number of other drawbacks and limitations apply to the peel test, including difficulty in initiating a peel strip for coatings with strong adhesion and controlling sample-to-sample variability. These problems can typically be dealt with by developing appropriate experimental techniques.

2.2.4 SUMMARY

AND

RECOMMENDATIONS

The peel test is quite likely the method of choice when dealing with tough, flexible coatings on rigid substrates as it meets many of the criteria of the ideal adhesion test. First and foremost is the consideration of sample preparation. In this regard, it is typically quite straightforward to fabricate convenient-size coupons of the substrate material and apply the coating of interest to them. Suitable care should be taken to clean the substrate and apply the adhesion promoters of interest. Further technical details, such as providing a release layer so that the peel strip can be easily initiated, should not be overlooked. Last, care should be exercised in interpreting the final data. Peel test data can be reliable for ranking the effectiveness of adhesion promoters or for quality control measurements. As noted, one should not rely on peel test measurements as a guide to performance of the coating under end-use conditions because the load state imposed by the peel test does not generally reproduce actual load conditions in the field. A detailed example of a successful implementation of the peel test for studying the adhesion of high-temperature coatings to silicon substrates is given in Chapter 5.

2.3 TAPE PEEL TEST 2.3.1 INTRODUCTION The tape peel test is a rough-and-ready variant of the standard peel test. Its main advantage is ease of sample preparation. The predominant disadvantage is that the results of the test will tend to be qualitative only. Attempts at systematizing the test, however, have given semiquantitative results. In a typical application, a strip of specially fabricated tape is applied to the coating to be tested in a predefined manner. The main concern is to be as consistent as possible to achieve reproducible results. The tape is subsequently peeled off in a prescribed fashion, and the test surface is then inspected for whatever resulting damage that may have occurred. At the purely qualitative level, the experiment gives a “go/no go” type of result. indicating whether the adhesion of the coating is acceptable. A number of techniques have been invented to give a semiquantitative result by quantifying the level of partial damage that may have happened to the coating. An example of this for the case of ink coatings is discussed in Section 2.3.2. The main problem with obtaining truly quantitative results with the tape peel test is that one now has to deal with four different materials: the substrate, the coating, the tape adhesive, and the tape backing material. Satas and Egan4 reported the effect of the backing layer and the adhesive layer on the peel strength of pressuresensitive tapes. Their data showed that, depending on the tape backing material, the peel force can vary by as much as a factor of 2 for a given layer thickness.

12

Adhesion Measurement Methods: Theory and Practice

In a separate study Aubrey et al.5 investigated the effect of adhesive molecular weight, adhesive layer thickness, backing film thickness, peel rate, and peel angle on the peel strength of polyester backing polyacrylate adhesive pressure-sensitive tapes. They demonstrated that all of these factors have a significant effect on the measured peel force. In particular, the peel force showed dramatic dependence on peel rate with three fundamentally different modes of peeling. At low rates, the peel force is controlled by flow of the tape adhesive and is strongly rate dependent. At high rates, little viscous deformation occurs, and the peel force is largely rate independent. At intermediate peel rates, the peel force exhibits cyclic instability driven by alternate storage and dissipation of elastic energy. The net result is a type of “stick-slip” peeling. Thus, without even considering the coating and substrate properties, we already have a considerable degree of complexity introduced just by the properties of the tape alone. If we now introduce further degrees of freedom arising from the mechanical response of the coating and substrate, we see that the problem of deriving a truly quantitative analysis of the tape peel test rapidly becomes prohibitive.

2.3.2 ADVANTAGES

OF THE

TAPE PEEL TEST

Despite the difficulties mentioned in obtaining quantitative results with the tape peel test, it can still be a useful and effective measurement method in certain applications. This is best illustrated by the study of ink coatings by Calder et al.6 These authors succinctly summarized the case for using the tape peel test in a cogent manner7: There is a body of experience in the industry that confirms that the tape test is a reasonable predictor of how the ink will remain in place, intact on the substrate under many actual use conditions. The test is fast and can be performed at press side. It is obviously important to know rather quickly whether an ink has adequate adhesion when the film is being printed at 600 ft/min.

In their experiments on ink coatings, the authors applied the subject ink coating to the relevant paper or foil substrate. Tapes were applied to the ink coating after a specified drying time and removed rapidly by a 90° peel test. The degree of adhesion of the ink coating is then rapidly evaluated using a light spectrophotometer and is reported as percentage coating removal as compared to a standard untested sample. Appropriate calibration methods are used to ensure repeatability. Figure 2.2 illustrates some representative data from this type of experiment. The solid line shows the apparent adhesion versus time for an ink with a relatively “soft” binder matrix, and the dashed line illustrates the same behavior for an ink with a “hard” binder matrix. The data clearly reveal that the soft binder gives an ink with stronger adhesion at short times (lower percentage coating removal), and that both ink types level off to substantially the same adhesion level at longer times. This is the type of information that can be of practical use in the printing industry, in which different printing techniques have different requirements for ink adhesion.

Overview of Most Common Adhesion Measurement Methods

13

Tape Peel Data on Two Separate Ink Types (Data replotted from Calder et al., Ref 6) Soft Binder

Hard Binder

% Coating Removal

100

75

50

25

0

0

10

20

30

Drying Time (minutes)

FIGURE 2.2 Tape peel test data on printing ink. The relative adhesion strength is measured by the amount of light that can pass through the ink/paper layer after the tape is peeled off. The ordinate gives the percentage of light passing through the sample as a percentage referred to an appropriate standard. The abscissa represents the drying time. A high value indicates more light passing through and thus poorer adhesion of the ink. A low value indicates little ink removal and thus good adhesion. The solid line represents an ink using a “soft” binder system and the dashed line a “hard” binder system. The data clearly show that the soft binder gives better adhesion at short times than the hard one, and that both systems behave much the same at long drying times.

A different type of application of the tape peel test in the photographic film industry was given by Grace et al.8 These investigators used the tape peel test in conjunction with a time-resolved salt bath technique for investigating the adhesion of silver coatings to poly(ethylene terephthalate) (PET) films. In the salt bath test, silver-coated PET films were immersed in a salt bath, and the time required for the silver to lift off was noted. These results were then correlated with standard tape peel testing in a manner similar to that mentioned above. The essential result of this investigation was the demonstration that the salt bath test was able to better discriminate different levels of adhesion of the silver coatings than the tape peel test alone. The tape test basically gave a good/not good type of result, whereas coatings tested in the salt bath would survive for different lengths of time, thus giving a more continuous scale of adhesion performance. In particular, coatings that the tape peel test indicated were good were shown to delaminate at intermediate times in the salt bath test. However, films shown to be poor by the tape peel test were also poor by the salt bath test. Thus, the tape peel test supported the salt bath experiments but did not give the same degree of resolution of adhesion strength.

14

Adhesion Measurement Methods: Theory and Practice

2.3.3 DISADVANTAGES

OF THE

TAPE PEEL TEST

As pointed out, the tape peel test at best can give a semiquantitative estimate of the adhesion of a coating. The results of the test tend to be confounded by the mechanical response and other failure modes of the tape backing and the tape adhesive as well as similar behavior of the coating and the substrate material. With so many potential complicating factors, the interpretation of tape peel test data is very difficult if more than a simple qualitative estimate of adhesion strength is required. The use of calibration methods and reference samples is mandatory to ensure a reasonable level of repeatability.

2.3.4 SUMMARY

AND

RECOMMENDATIONS

Although the tape peel test is limited to a qualitative or at best semiquantitative evaluation of adhesion, it has a number of advantages that make it attractive in specific applications. In particular, in situations for which a simple rapid test is required, such as for testing printing inks, or for which a straightforward go/no go evaluation is sufficient, this test may be perfectly adequate. In some cases, it may be the only reasonable test available. However, great caution is recommended in evaluating tape peel data. and the results should not be overinterpreted in terms of trying to understand the fundamental adhesion of a coating because a large number of confounding factors come into play with this test.

2.4 PULL TEST 2.4.1 INTRODUCTION As with the peel test, the pull test is a general method for assessing both qualitatively and semiquantitatively the adhesion of coatings to a variety of substrates. Also, as with the peel test, it enjoys a number of advantages and suffers from several disadvantages. The advantages include the following: •

• •

Applicable to a wide variety of coatings and substrates including • brittle coatings • flexible coatings Gives both qualitative and semiquantitative results Relatively easy sample preparation

The disadvantages of this method include • • • •

Difficult data analysis, especially for quantitative measurements Rapid uncontrollable failure mode Wide scatter in data Need for bonding adhesive or solder

An excellent evaluation of the pull test as applied to paint coatings was given by Sickfeld.9 This author investigated two basic pull test configurations, as illustrated in Figure 2.3. The symmetric configuration is preferable for testing coatings on

Overview of Most Common Adhesion Measurement Methods

15

Asymmetric pulloﬀ specimen

Symmetric pulloﬀ specimen Coating Substrate

Substrate

(a)

(b)

FIGURE 2.3 Schematic of two pull test configurations. The symmetric configuration is preferred when the substrate is thin or flexible. The asymmetric mode is preferred when the substrate is thick or very rigid. Note: Glue/adhesive layer not shown.

relatively thin flexible substrates, whereas the asymmetric sample is preferred for thick rigid substrates. Similar to the tape peel test, the pull test involves two additional materials besides the coating and substrate under investigation. The test stud itself is fabricated out of a high-modulus metal or ceramic material and for the case of paint coatings can be considered almost perfectly rigid. This is not the case for testing stiff brittle coatings such as diamond or ceramics; in these cases, the stud material must be carefully figured into the analysis. In addition, an adhesive is required to attach the test stud to the coating under test. For paint coatings, this is typically an epoxy glue, and its properties will always enter the analysis. After the test stud is appropriately cemented to the coating under test, it is pulled off under controlled conditions using a tensile test apparatus. A number of complications now enter the picture as follows: •

•

• •

Unless the load is applied very carefully, there can be an off-axis component that can impose a bending moment to the sample in addition to the tensile load. Even assuming pure tensile loading, any real sample will not be uniformly bonded, and the applied stress field will seek out any defects or bonding weaknesses. Failure will be initiated at the weakest point in the structure and propagate at acoustic velocities to complete separation. Failure can occur either adhesively at any of the three sample interfaces or cohesively in any of the four bulk materials. Mixed-mode interfacial and cohesive fracture is the most common failure mode.

Given the list of complexities, it should come as no surprise that typical pull test data show a wide range of variation. Multiple tests must be run at any given condition, and data-censoring techniques should be applied to ferret out unwanted failure modes.

2.4.2 ADVANTAGES

OF THE

PULL TEST

The main advantage of the pull test is its wide-ranging applicability to all manner of coatings, from relatively soft flexible polymer coatings to hard brittle coatings

16

Adhesion Measurement Methods: Theory and Practice

such as diamond. In addition, as pointed out by Sickfeld,9 there are two types of information that can be obtained from this test. The first is qualitative, deriving from an analysis of the resulting pull off fracture surface. Some idea of the integrity of the coating can be obtained by noting whether failure tends to be mainly cohesive in the coating itself or interfacial between the coating and the substrate. In particular, Sickfeld was able to study the effect of moisture and solvent immersion on the failure mode of paint coatings. For the case of immersion of the coating in water, subsequent pull testing showed nearly interfacial failure between the coating and substrate. On the other hand, coatings immersed in gasoline or oil demonstrated a mixed interfacial/cohesive type of failure. This type of data can be very valuable when evaluating a particular coating for use under particular service conditions. A second advantage is the quantitative information derived from the pull test. It has been hypothesized that, in most cases, the failure mode in a given pull test experiment is determined by a preexisting distribution of flaws in the sample. Thus, as discussed in the preceding section, the applied stress field seeks out the largest, most vulnerable flaw in the sample. Failure initiates at this point, and the initial flaw rapidly propagates at acoustic velocities to ultimate separation of the pull stud and the sample surface. In effect, it is assumed that all samples will have some kind of inherent flaw distribution no matter how carefully they were prepared, and the stress field deriving from the pull test will inevitably find the most vulnerable flaw; failure will initiate and propagate from that point. It has further been found that Weibull statistics are very effective in analyzing this type of data. Pawel and McHargue10 used the pull test to analyze the adhesion of iron films to sapphire substrates. These investigators ion implanted both nickel and chromium impurities at the interface between an iron film and sapphire substrate. Subsequent pull testing and Weibull analysis unequivocally demonstrated that the chromium interlayer substantially improved the adhesion of the iron film over the untreated and nickel-treated cases. Finally, there are situations that are perfectly disposed toward the pull test, such as evaluating the durability of pins on a microelectronic packaging substrate. For large mainframe machines, such substrates can carry over 100 silicon chips and require over 1000 pins to distribute power and signal data to a supporting carrier board. The reliability of these pins is critical to the proper function and performance of the total chip/substrate assembly, and each pin must meet very stringent reliability and performance criteria. The pull test is the natural performance evaluation procedure for this application. Coupled with the appropriate Weibull analysis, the pull test provides a crucial engineering and quality control tool for the design and fabrication of such structures.

2.4.3 DISADVANTAGES

OF THE

PULL TEST

One of the main disadvantages of the pull test is the wide variability in typical test data. This problem has been documented most cogently by Alam et al.11 These investigators attempted to evaluate the adhesion of chemical vapor deposition (CVD) diamond coatings to tungsten substrates. Because of a variety of conditions affecting their sample preparation, including nonuniformity of film thickness, diamond quality,

Overview of Most Common Adhesion Measurement Methods

17

film cohesion, and surface preparation, they observed considerable variability in their pull test data. In the authors’ own words: “The measured adhesion values showed larger variations from point to point across the sample surface and from identically prepared samples than variations as a function of the film processing parameters.” Thus, the data derived from pull testing in this case were mainly qualitative. Every form of sample failure was observed, including clean interfacial delamination, partial delamination with partial film cohesive failure, cohesive failure in the epoxy adhesive coupled with delamination of the epoxy from the coating, and pure cohesive failure of the diamond coating. With such a wide range of failure modes, it was no wonder that the data showed a high degree of variability. With the use of statistical analysis, however, the authors were able to show that substrate preparation, gas flow, and gas pressure were the most important processing parameters.

2.4.4 SUMMARY

AND

RECOMMENDATIONS

In conclusion, it is clear that the pull test can be an effective tool for evaluating both the qualitative and semiquantitative durabilities of a wide variety of coatings. The main advantage of this technique is its versatility and applicability to a wide range of coating/substrate systems. It can be applied to both soft flexible coatings as well as hard brittle ones. Pull test equipment is commercially available and can be set up in any laboratory with a tensile testing apparatus. The use of advanced statistical analysis such as Weibull analysis can be helpful in providing semiquantitative information concerning the durability of various coatings. The wide variation in typical pull test data remains one of the main weaknesses of this technique. Multiple tests must be done on a given sample coupled with statistical analysis to obtain reliable quantitative data. However, there are a number of specific instances, such as pin testing on microelectronic substrates, for which the advantages of pull testing make it the most natural choice for reliability testing.

2.5 INDENTATION DEBONDING TEST 2.5.1 INTRODUCTION Figure 2.4 shows a schematic representation of the indentation test. In this test, an indenter with a hemispherical point (i.e., with a tip radius that is on the order of the thickness of the coating tested) is thrust into the coating under carefully controlled conditions. The dominant effect of this maneuver is to greatly compress the coating material directly under the indenting tip. Surprisingly, however, a concomitant delamination of the coating can also occur starting at the edge of the indenter and extending for a distance that can be several times the indenter tip radius. An early example of the use of this technique for testing the adhesion of epoxy to copper in circuit boards was given by Engel and Pedroza.12 These investigators worked with epoxy coatings in the range from 25 to 300 μm on copper metal substrates. Using an indenter tip of approximately 0.2-mm radius, they observed peripheral delamination around the central indentation out to a radius of up to 2 mm. One simple way of understanding the mechanics of what is happening is given in Figure 2.5. As the indenter penetrates the epoxy coating, material is extruded to

18

Adhesion Measurement Methods: Theory and Practice

F

FIGURE 2.4 Idealized representation of the indentation debonding test. An indenter with a spherical tip is pressed into the coating under carefully controlled loading conditions. A high compressive stress is developed under the indenter; however, depending on the elastic/plastic response of the substrate, a tensile field is developed at the periphery that can cause the coating to delaminate.

Indenter radius

Delamination radius

Compressive indenter stress

Normal lever stress

Pileup pivot

FIGURE 2.5 Simplified description of indentation debonding test. The coating is treated as a simple beam setup. The compressive force of the indenter loads the left ligament of the beam while also pushing underlying material to the periphery, where it piles up and forms a pivot. Material to the right of the pivot point experiences normal tension because of the lever effect of the coating acting as a simple beam.

the periphery of the indenter, causing a pileup at the edge. In this case, the underlying copper material is also pushed to the indenter edge because copper is a highly plastic material, which also contributes to the pileup of material. The excess mound of both epoxy and copper at the edge of the depression can be thought of as forming a sort of pivot for the epoxy coating to act in the fashion of a simple lever, as shown in Figure 2.5. The epoxy film will have significant rigidity on the length scale of 1 mm, so the normal stress generated by this levering effect can be quite significant and lead to delamination if the coating adhesion is not sufficient. A further contributing mechanism is the shear stress generated by the extrusion of the epoxy material from under the indenter. Thus, a combination of flow shear stress coupled with normal lever stress can operate to delaminate the coating starting at the indenter edge. Engel and Pedroza13 also used a simple plate model of the coating to estimate the radial

Overview of Most Common Adhesion Measurement Methods

19

strain in the coating and referred to this as the peel strain. Such a strain can be an energy source for driving the indentation delamination. A far more rigorous analysis of the stresses driving the delamination process in the indentation test was given by Jayachandran et al.14 These authors treated the case of a poly(methylmethacrylate) polymer coating on a rigid substrate. Having access to extensive data characterizing the constitutive behavior of the poly(methylmethacrylate), they were able to carry out highly detailed numerical studies of the indentation process using the finite element method, including full details of large deformation and viscoplastic strain phenomena. Because these authors assumed a perfectly rigid substrate, their results cannot be compared directly to those of Engel and Pedroza. What was found is that there was indeed a massive shear flow and pileup of material created by the indenter all the way to the edge and beyond. However, because of the assumption of a rigid substrate, only a small tensile normal stress was predicted beyond the indenter edge. Thus, the normal stress in the epoxy/copper system is mostly caused by the pileup of the copper at the indenter edge, which forms a pivot on which the epoxy coating acts as depicted in Figure 2.5. The indentation debonding method has also been applied to hard refractory coatings, as demonstrated by the work of Weppelmann et al.15 These authors investigated the titanium nitride (TiN)/silicon system both theoretically and experimentally. Experimentally, they used a diamond indenter in conjunction with a digital interference microscope to follow the sample deformation precisely. Theoretically, they were able to develop a simple formula for the strain energy release rate for delamination caused by the radial strain induced by the indentation process. Using their experimental results, they were able to estimate an adhesion strength of approximately 1.2 J/m2 for the TiN/silicon system.

2.5.2 ADVANTAGES

OF THE INDENTATION

DEBONDING TEST

The indentation test has a number of clear advantages, which can be summarized as follows: • • • •

Applicable to a wide variety of coating/substrate systems Ease of sample preparation Both qualitative and quantitative results obtained Commercial equipment readily available

The indentation test is readily implemented both in the laboratory and on the production line for a wide variety of coatings. As mentioned, it has been applied to both soft flexible coatings on metals and hard brittle coatings on silicon. Engel and Pedroza12 commented on the use of this test for quality control in testing the adhesion of epoxy on copper in circuit boards. Other than preparing the coating, no special preparation of the test sample is necessary. The test is clearly applicable to a wide variety of substrates and has been applied to testing scratch-resistant coatings on curved plastic lenses. As mentioned, the indentation test can be analyzed to give quantitative results in addition to a simple qualitative estimate of the coating durability. Finally, commercial off-the-shelf equipment is readily available in the form

20

Adhesion Measurement Methods: Theory and Practice

of indentation test equipment and powerful microscopes with digital interferometers for evaluating both substrate damage and deformation.

2.5.3 DISADVANTAGES

OF THE INDENTATION

DEBONDING TEST

The main disadvantages of the indentation test can be summarized as follows: • •

Complex mode of loading involving large compressive stress and high shear strains Difficult quantitative analysis and poorly understood precise mechanism of delamination

The very high compressive load induced by the indentation test coupled with the high shear flow associated with soft coatings may make the relevance of the indentation test questionable for some coating systems. In particular, coatings subjected to large temperature swings may delaminate at edges or other discontinuities under loading conditions that are far different from those induced by the indentation test. A further drawback for hard coatings is the fact that, in addition to a large compressive stress, a very significant hoop stress is also generated by this test, which can lead to radial cracking in the sample substrate as well as the coating. Thus, multiple failure modes can greatly complicate the interpretation of the data when one is primarily interested in the coating adhesion.

2.5.4 SUMMARY

AND

RECOMMENDATIONS

The indentation debonding test clearly passes many of the criteria required for an ideal adhesion test. Primary among these are the ease of sample preparation and applicability to a wide variety of coating/substrate systems. Ready availability of commercial equipment makes this test a favorite in many industries that have to deal with quality control issues involving coatings. The main problem to be aware of is whether the loading conditions created by this test are reasonably close to those that the coating under test must endure in practice. In general, this is a very relevant test for coatings that must endure abrasive conditions and contact with potentially penetrating surfaces. Great care should be taken, however, if the coating in question will be subjected to large thermal strains that can be induced by large temperature gradients or thermal expansion mismatch between the coating and substrate.

2.6 SCRATCH TEST 2.6.1 INTRODUCTION Figure 2.6 gives a highly schematic representation of the scratch test, which can be thought of as an extension of the indentation test with the added feature that the indenter is translated along the sample surface as well as into the coating. An informative overview of the early history of this technique was given by Ahn et al.16 Apparently, Heavens17 and Heavens and Collins18 were the first to employ this

Overview of Most Common Adhesion Measurement Methods

21

Load

Stylus

Track direction Coating Substrate

FIGURE 2.6 Essentials of the scratch test. Loading conditions are similar to the indentation test in that the stylus pressure is ramped up according to some specified program; however, the stylus is simultaneously driven forward at a fixed rate.

technique to study the durability of metallic films evaporated onto glass. Subsequently, Benjamin and Weaver19 performed an elementary mechanics analysis of this method and derived the following simple formula for the shear force to be overcome by the scratch stylus: F=

AH ( R 2 − A 2) (2.1)

A=

W πH

where A R W H F

= Radius of stylus contact circle = Radius of stylus tip = Applied load normal to coating surface = Indentation hardness of substrate = Shearing force resisting lateral motion of stylus

The hope was that the load W required to remove the coating could be taken as a measure of the coating adhesion by relating it to the generated shear force given in Equation (2.1). However, a number of complications were noted by later workers,20 who discovered several difficulties, including the following: •

• •

Delamination of the coating can be observed even before the stylus removes all traces down to the substrate. In addition, the film can be thinned to the point at which it becomes translucent and cannot be removed. Complex material properties such as the elastoplastic behavior of the coating and substrate determine the nature of the scratch track. Multiple modes of failure are observed, including mechanical failure in the bulk of the coating or substrate in addition to interfacial delamination.

22

Adhesion Measurement Methods: Theory and Practice

Given the complications observed in the mechanically simpler indentation test, none of these remarks should come as any surprise. It should be clear that an experiment such as the scratch test that involves the penetration and dragging of a stylus through an adhered coating is going to give rise to a whole range of complex thermomechanical response behaviors, including viscoplastic flow, bulk fracture, and interfacial failure. The immediate upshot is that, as with all the other adhesion tests discussed, the scratch test will be at best a semiquantitative technique. However, this does not preclude the usefulness or effectiveness of this method for providing insight into the adhesion and durability of coatings in a variety of applications. In particular, Ahn et al.21 demonstrated that the scratch test can readily reveal poor adhesion in a coating because in this case lateral delamination of the coating can be observed to occur along the length of the scratch track. In an attempt to put the scratch test on firmer footing, Oroshnik and Croll22 came up with the concept of threshold adhesion failure (TAF). These investigators noticed that, in the thin aluminum films they were investigating, small patches of delamination could be observed in the scratch track well before the scratch stylus penetrated to the underlying substrate. It occurred to them that the load at which this patchy delamination occurred could be used as a measure of the coating adhesion. They proposed the following definition: Threshold Adhesion Failure occurs if, within the boundaries of a scratch and over its 1-cm path, removal of the film from its substrate can be detected by transmitted light with a microscope (×40 magnification) at even one spot, no matter how small.

This definition coincides well with Definition B (see Chapter 1) for adhesion and is certainly serviceable for the purposes at hand. Oroshnik and Croll described the method by which TAF is obtained for a given coating. The load on the stylus is increased incrementally as it moves over the sample surface up to the point at which spots of delamination are just detected. The load is then incrementally decreased until the delamination events just disappear, at which point the load is again increased to the point at which the delaminations again appear. This procedure of successively incrementing and decrementing the stylus load is repeated until the apparent threshold load for producing delaminations is reliably boxed in between upper and lower load conditions. Figure 2.7 shows a schematic of the type of data obtained from this procedure. Note from this figure how the data tend to settle at a fixed level of apparent adhesion strength. Oroshnik and Croll went on to discover that, even though using a given stylus, the TAF data were highly reproducible and consistent, no two stylus tips were identical, and each gave different TAF results. Using microscopic interferometry, these authors discovered that the stylus tips they were using were neither spherical nor with an unambiguous radius. In fact, data were presented showing measurements taken with different styli on a single film for which the TAF load differed by nearly a factor of 2. Furthermore, it was shown that the Benjamin and Weaver result for the shear force given by Equation (2.1) was not verified by the data, which was not surprising given the nonspherical nature of the stylus tips used. It is in fact well established that the most critical factor controlling the scratch test is the nature of

Overview of Most Common Adhesion Measurement Methods

23

Typical Threshold Adhesion Failure (TAF) Data 0.36 Micron Film of Aluminum on Vitreous Silica

Stylus Load (grams)

(Data replotted from Oroshnik and Croll, Ref. 22)

Scratch Coordinate X 10–3 (inches)

FIGURE 2.7 Typical threshhold adhesion data. Filled squares indicate load level at which delamination first appears while the load is increasing. Open squares indicate load level at which delamination first ceases while the stylus load is decreased. At the critical load for delamination, the load increasing and the load decreasing data should closely overlap.

the stylus tip. Different results will be obtained depending on the stylus material (steel, tungsten carbide, or diamond) and the precise topography of the tip region that first contacts the coating surface. Later investigators expanded on the scratch test not only to include more sophisticated instrumentation for controlling the load program of the stylus and advanced microscopy for observing the scratch track, but also to couple the scratch method with acoustic spectroscopy, by which the sound vibrations generated by the stylus are detected and recorded at the same time that the scratch track is formed. Typical of the more modern approach is the work of Vaughn et al.23 These investigators performed adhesion measurements on both copper and diamondlike carbon (DLC) films coated onto PET substrates. These experiments gave an ideal opportunity to evaluate the performance of the scratch test on two radically different types of coatings on the same substrate material. The highly plastic copper coatings gave completely unremarkable stylus load-versus-scratch length plots in which the load simply increases monotonically, with scratch length showing no particular discontinuities where the film began to delaminate. Further, these coatings gave no discernible acoustic signal at coating failure events such as delamination. By contrast, the rigid brittle DLC coatings showed a sharp drop in the stylus load versus scratch length curve at points where the DLC coating fractured in the typical “herringbone”style cracks that can appear in the scratch track because of the high tensile stress just behind the advancing stylus tip. Figure 2.8 shows a schematic representation of the type of data obtained from the DLC coatings.

24

Adhesion Measurement Methods: Theory and Practice

Typical Acoustic Emission Data from a Scratch Track on a Diamond Like Carbon Film on a Polymer Substrate

Acoustic Emission (arbitrary scale and units)

(Data replotted from Vaughn et al., Ref. 23)

2.7

3.0

3.4

3.8

4.2

Normal Load (N)

FIGURE 2.8 Correlation of acoustic emission data with microscopy of scratch track. Note that the appearance of a “herringbone” crack as the load increases coincides exactly with a local peak in the acoustic emission plot.

An innovative version of the scratch test was implemented by Sarin,24 who basically turned the experiment on its side and performed a microscratch test on a cross section of the coating substrate sample at 90° to the coating surface (Figure 2.9). The sample is sliced across a section of interest, and the edge is precisely polished by standard metallographic methods. The scratch test is then carried out in the standard manner only on a microscale because of the very narrow cross section under investigation. One advantage of this approach is that, under certain conditions the failure mode can be isolated at the coating/substrate interface, and the precise locus of failure is immediately apparent by direct microscopic investigation. Sarin, in fact, found that for a titanium carbide (TiC) film coated onto a silicon nitride/titanium carbide (Si3N4 + TiC) ceramic composite, he was indeed able to generate a crack along the coating/substrate interface, thus obtaining a true delamination failure mode. However, when the same type of experiment was performed on a TiC coating on tungsten carbide-cobalt (TC-Co) substrate, cracks were observed to start in the substrate and then propagate into the coating. Sarin’s findings illustrate what tends to be a general rule for all adhesion measurement methods in that any given method will be found to work well on a given specific sample system but will generally give unexpected results when the sample is changed even in a relatively minor way. Further attempts at quantifying the scratch test have been reviewed by Bull,25 who examined the scratch test as applied to a number of qualitatively different coating/substrate systems. This author basically found that the following criteria must be met to achieve a truly quantitative assessment of adhesion strength using the scratch test:

Overview of Most Common Adhesion Measurement Methods

25

90 degree micro-scratch test (Adapted from V. K. Sarin ref. 24) Coating

Scratch track Substrate Micro-indenter

FIGURE 2.9 Innovative variation of scratch test in which the sample is sectioned, and using a microindenter, the scratch track proceeds from within the sample substrate toward the coating/substrate interface at a 90° angle.

1. There must be a well-defined delamination mode present under the prevailing test conditions. 2. Knowledge of the sample stress state leading to delamination failure must be available either through direct measurement or calculation. With these conditions in mind, Bull examined a variety of coating/substrate systems that basically fell into the categories of hard and soft. Soft systems generally give rise to a high level of viscoplastic deformation, and clean failure modes may not be clearly observable. Hard systems, on the other hand, often exhibit brittle fracture in the substrate, the coating, or both. Combinations of soft and hard materials can give rise to all of the previously mentioned failure modes plus interfacial delamination. Table 2.1 gives a highly qualitative overview of the general trends. This table illustrates the general observation that the scratch test works best when at least one component of the coating/substrate system is a relatively hard material. On reflection this is intuitively reasonable. You clearly would not use the scratch test to quantify the adhesion of molasses to chewing gum.

TABLE 2.1 Qualitative Summary of Failure Modes in the Scratch Test as a Function of Coating/Substrate Hardness Substrate hardness ⇒ Coating hardness ⇓ Soft Medium Hard

Soft

Medium

Hard

Plastic deformation extrusion Plastic deformation extrusion Plastic deformation extrusion

Coating thinning scrape off Delamination

Coating thinning scrape off Delamination fracture

Delamination fracture

Delamination fracture

26

Adhesion Measurement Methods: Theory and Practice

However, Bull did illustrate two situations for which the scratch test gives promising results for hard coatings on hard substrates. The first case involves what can basically be called buckling spallation. For the system TiN on stainless steel, a thin coating of the TiN can be made to spall off the substrate. The scratch stylus creates a compressive stress ahead of itself because of the deformation of the substrate, which causes the coating to buckle. High tensile stresses in the coating cause the buckled coating to crack and then flake off. For thicker coatings, the bending required for buckling does not occur because the coating is too stiff. However, compressive shear cracks can form ahead of the indenter through the thickness of the coating. These cracks typically have sloping sides that can act as an inclined plane or wedge. The forward motion of the indenter can then drive the edge of the coating up the ramp created by the crack, causing the interface between the coating and substrate to separate, which leads to spalling of the coating. Bull referred to this mode of delamination as wedge spallation. Finally, even though the scratch test has proven most effective for hard brittle coatings, work by Bull et al. 26 showed that this test can also give valuable information concerning the adhesion and durability of polymer coatings such as epoxies. The application in this case was the evaluation of epoxy coatings for covering the inner hull of coal-carrying vessels. The epoxy is intended to protect the metal hull from abrasion by the coal and corrosion caused by the brackish marine environment. Lumps of coal settling against the inner hull have an abrasive effect; thus, the scratch test was deemed an appropriate method for evaluating the performance of the epoxy coatings. A number of different coating formulations were investigated, and all showed varying tendencies to either crack or delaminate under the action of the scratch stylus. One interesting failure mode arose because of the tensile load imposed on the coating behind the moving stylus. This would cause a through crack to form behind the stylus, which would then drag the coating along, opening up the crack and further buckling the coating in front in much the same manner as a rug buckles when pushed laterally at one of its edges. In addition, it was found that coatings with extender pigmentation tended to crack more readily than the unfilled coatings. However, the filler also retarded adhesion degradation as determined by aging studies. Thus, scratch testing can be used to determine the optimal tradeoff between coating toughness and adhesion by comparing scratch results on coatings with varying levels of extender pigmentation.

2.6.2 ADVANTAGES

OF THE

SCRATCH TEST

As with the indentation test, the main advantage of the scratch test lies in the relative ease of sample preparation. One simply prepares coupons of a convenient size out of the relevant coating and substrate materials in the same manner as on the manufacturing line or in the build shop. In addition, the newer commercially available equipment can be fitted with a number of auxiliary tools, such as microscopes, acoustic spectrometers, and surface-profiling attachments. Because the stylus can also act as an indenter, the coating hardness and elastic properties can be determined. Thus, a single instrument can give valuable information on surface topography, mechanical properties, and modes of deformation and delamination. Semiquantitative

Overview of Most Common Adhesion Measurement Methods

27

information can be obtained by recording the stylus load at failure; thus, scratch testing can be used to rank the durability of a series of coating formulations. In some cases, a fully quantitative estimate of the fracture energy of the coating/substrate interface can be obtained if care is taken to measure carefully all relevant mechanical properties and carry out the appropriate fracture mechanics calculations.

2.6.3 DISADVANTAGES

OF THE

SCRATCH TEST

There are two essential disadvantages to using the scratch test as an adhesion measurement tool: This test is essentially limited to hard brittle coatings even though some exceptions, such as brittle epoxy coatings, may be successfully investigated. The softer metals and most polymer coatings tend to viscoplastically flow and deform around the scratch stylus, causing mounding at the edges of the scratch track and pileup in front of the stylus. In addition, these coatings do not give a distinct acoustic signal at the failure point, thus negating the use of acoustic spectroscopy. Also, some coatings can be thinned to the point of optical transparency without achieving complete coating removal, thus complicating any attempt to assess adhesion strength. The second limitation arises from the fact that, as with the indentation test, the scratch test is mechanically complex. The act of pushing the stylus into the coating gives rise to very high stresses and deformations in both the coating and the substrate, thus bringing into play the full range of highly nonlinear viscoplastic material behaviors. The usual type of elastic mechanical calculations do not give quantitatively reliable results and can be used only for a more heuristic analysis of scratch test data. Also, the basic failure modes of the scratch test are only poorly understood, and experience gained on a given coating/substrate system may not be reliably carried over to a different one.

2.6.4 SUMMARY

AND

RECOMMENDATIONS

The scratch test is one of the most popular adhesion tests currently in use in both industry and academia. This stems largely from the great versatility of this technique for evaluation of a wide range of coating/substrate systems and the ready availability of commercial equipment that can perform a variety of functions, such as surface inspection, surface roughness measurements, and the evaluation of coating mechanical properties. For the case of hard brittle coatings, the scratch test is quite likely the best available technique for most situations. For softer coatings, this method may also be able to give useful results under certain conditions and can be used in a complementary manner with other techniques, such as the pull test.

2.7 BLISTER TEST 2.7.1 INTRODUCTION One constant complaint about all of the adhesion tests mentioned above is the fact that they involve a mechanically complex process with large deformations and strains giving rise to highly nonlinear viscoplastic response behavior by the coating/substrate system investigated. An immediate consequence of this is the fact that the analysis

28

Adhesion Measurement Methods: Theory and Practice

of these systems in terms of continuum and fracture mechanics concepts is exceedingly difficult, if not impossible. The blister test is an attempt to circumvent these difficulties by developing a blister in the coating in a well-defined manner that will propagate a delamination front between the coating and substrate in a controlled manner using only moderate deformations and strains. Dannenberg27 was apparently the first investigator to apply this technique to measure the adhesion of polymer coatings. Lai and Dillard28 gave an insightful account of the mechanics of several versions of this test. Figure 2.10 is a schematic representation of four different versions of this test mentioned by these authors. Figure 2.10a illustrates the standard blister test configuration. The main limitation of this version occurs when the coating ruptures before the coating can delaminate. This problem limits the standard blister test to coatings with either very high fracture toughness or relatively low adhesion to the underlying substrate. To circumvent this problem, Allen and Senturia29,30 devised the island blister test shown in Figure 2.10b. Because of the much smaller debond front presented by the inner island, the driving force for delamination is much greater here than at the much larger circumference at the outer radius. Thus, delamination can be made to occur at the inner island at a much lower applied pressure than would be required in the standard blister test. Four versions of the blister test Top view (a) Standard blister test

Side view

o P

(b) Island blister test

o P

(c) Peninsular blister test

o P

(d) Constrained blister test

o P

FIGURE 2.10 Four different configurations of the blister test: (a) The standard test involves applying hydrostatic pressure to the bottom of the coating, thus inducing a blister. The main drawback of this approach is that the coating may burst before significant delamination occurs. (b) The island blister test is one attempt to get around the coating bursting problem. In this configuration, the driving force for delamination is much higher on the central island than on the periphery. Thus, one is more likely to get delamination before the coating fails. (c) The peninsular test is a variation of the island test that also alleviates the coating failure problem while improving on the stability of the test. (d) For the constrained blister test, placing a transparent rigid cover over the blister allows control of the coating deformation while observing the delamination front.

Overview of Most Common Adhesion Measurement Methods

29

One problem with the island blister test is that it tends to be unstable. To overcome this difficulty, Dillard and Bao* conceived the peninsular blister test depicted in Figure 2.10c. This version of the blister test maintains the high driving force for delamination as in the island blister test while maintaining a more steady delamination front. Figure 2.10d shows the constrained blister test, which cleverly supplies a simple cover for the standard blister test to prevent the problem of film rupture. The earliest investigations of this technique were apparently carried out by Napolitano et al.31,32 and nearly simultaneously by Dillard33–35 and co-workers. Napolitano and coworkers32 managed to derive, using simple thermodynamic arguments, the following formula for the expanding area of the propagating blister: 2

βp h A(t ) = exp[ (t - t 0)] A(t 0) ph - γ

(2.2)

where A(t) p h γ β t0, t

= Blister area at time t = Applied pressure = Spacer height = Interfacial fracture energy = Dissipative coefficient = Initial and current time, respectively

Equation (2.2) was used to analyze constrained blister test data taken on a pressure-sensitive adhesive tape. The interfacial fracture energy was determined by noticing at what combination of spacer height h and applied pressure p the onset of delamination occurred. The interfacial fracture energy could then be computed from the following simple formula: γ = (hp)threshold

(2.3)

where it is to be noted that the pressure p in Equation (2.3) is that which just causes blister delamination to progress. The dissipative coefficient could then be obtained from data on blister area versus time. Plotting the log of both sides of Equation (2.2) yields a straight line with a slope that gives the parameter β, knowing γ from Equation (2.3). Liang et al.36 gave a very interesting application of the constrained blister test as applied to electropolymerized polymer coatings on copper substrates. They improved significantly on the work of Napolitano et al. by bringing to bear advanced image analysis methods implemented on a powerful modern workstation. With this advanced hardware and software, they were able to measure in real time the critical blister growth front parameters and thereby analyze their data using a fracture mechanics result for the strain energy release rate derived by Chang et al.37 given by the following formula: * “The Peninsula Blister Test — A High and Constant Release Rate Fracture Specimen for Adhesives,” D.A. Dillard and Y. Bao, Journal of Adhesion, 33, 253 (1991).

30

Adhesion Measurement Methods: Theory and Practice

Geometric parameters in constrained blister test (Refer to Eq. 2.4) a d h

P

FIGURE 2.11 Illustration of the configurational parameters for the constrained blister test appearing in Equation (2.4).

⎡ ⎛ d ⎞ ⎡⎛ d ⎞ ⎤ ⎛ ∂d ⎞ ⎤ G = ph ⎢1 − ⎜ ⎟ + ⎢⎜ ⎟ − 1 2 ⎥ ⎜ ⎟ ⎥ ⎢⎣ ⎝ 2a ⎠ ⎣⎝ 3a ⎠ ⎦ ⎝ ∂a ⎠ ⎥⎦

(2.4)

In this equation, G is the strain energy release rate, and p is the applied pressure; the dimensional parameters are explained in Figure 2.11. An elementary analysis of the island blister test was given by Allen and Senturia.38 By assuming that the coating can be treated as a membrane (i.e., it is so thin that it has no unsupported stiffness) and that the major component of the driving force is caused by residual stress, they came up with the following simple formula for the surface fracture energy of adhesion: 2

γa =

( pc a1) 32σ 0t

⎡ β2 - 1 ⎤ − 2⎥ ⎢ ⎢⎣ ln β ⎥⎦

2

(2.5)

where γa pc σ0 t β a1, a2

= = = = = =

Surface fracture energy Critical pressure for delamination propagation Residual film stress Film thickness a1/a2 Geometric parameters shown in Figure 2.12

Allen and Senturia also gave an interesting comparison between the island blister test and the standard version and demonstrated why the former gives a much higher delamination force on the inner island than the latter can achieve on the outer circumference of the suspended membrane.

Overview of Most Common Adhesion Measurement Methods

31

Geometric parameters of island blister test (Refer to Eq. 2.5)

Suspended membrane a2

a1 Bonded coating

FIGURE 2.12 Illustration of the configurational parameters for the island blister test appearing in Equation (2.5).

2.7.2 ADVANTAGES

OF THE

BLISTER TEST

As can be ascertained from the discussion, the blister test has a number of advantages; mainly, it is the first test discussed here that lends itself readily to a fully quantitative analysis based on fracture mechanics methods. This is mainly because this test imposes relatively low strains on the coating material, thus avoiding the complex nonlinear viscoplastic behavior that greatly complicates methods such as the peel test. However, like the peel test the blister test also concentrates the maximum stress at the delamination front, thus constraining the failure crack to be close to the coating/substrate interface of interest. Also, given the fact that a number of different versions are available, as shown in Figure 2.10, the user has great flexibility in testing coatings with varying levels of adhesion.

2.7.3 DISADVANTAGES

OF THE

BLISTER TEST

Whereas the blister test lends itself fairly readily to quantitative analysis, this advantage is purchased at the price of ease of sample preparation. It seems in the realm of adhesion testing that nothing comes free. If you gain an advantage in one quarter, then you pay for it in another. The main impediment comes with drilling the hole at the center of the blister through which the pressurizing gas enters. This can be accomplished in a number of ways, but the most popular is the use of etchants, which will erode the substrate material and not attack the coating. For coatings on silicon substrates, all the methods of microelectronic lithography are available to etch holes in the silicon and construct the various structures required for tests such as the island blister configuration. However, to use these methods a wafer fabrication facility must be available to carry out the involved series of steps required to construct the desired structures. This work also requires the use of very nasty etchants, such

32

Adhesion Measurement Methods: Theory and Practice

as buffered hydrofluoric acid. In addition, the blister test is limited to fairly flexible coatings, such as polymer-based paints and soft metals. Hard brittle coatings will tend to crack before forming a blister under the influence of the applied pressure. Finally, this test will have severe problems with coatings under high compressive stress because this will cause the coating to buckle as soon as it is lifted from the supporting substrate.

2.7.4 SUMMARY

AND

RECOMMENDATIONS

The blister test is most suitable when a fully quantitative analysis of the adhesion strength of a coating to a particular substrate is required. Great flexibility is available in the types of samples that can be used, and a number of investigators have provided detailed analyses that can be used to interpret the data in a fully quantitative manner. Also, the fact that delamination is achieved at low strain levels makes the results of the test much more relevant to coating adhesion than large strain-inducing methods such as the peel test. On the downside, however, sample preparation is far more cumbersome than for many other techniques. Thus, the blister test is not recommended when only qualitative or semiquantitative data are required because many other simpler methods are available.

2.8

BEAM-BENDING TESTS

2.8.1 INTRODUCTION There are a variety of tests for measuring adhesion that rely on the relatively simple mechanics of the elastic beam to simplify the required analysis for the stress intensity factors and the strain energy release rates that drive the delamination process. Precise definitions of these quantities are given in Chapter 4, which treats the methods of fracture mechanics in detail. The most attractive feature of beam-bending tests is that the stress field induced by the bending operation is comparatively simple and can thus be analyzed by elementary methods. Details of this type of analysis are given in Chapter 3, in which the fundamentals of continuum theory are discussed in some detail. Figure 2.13 illustrates several of the most popular adhesion tests that rely on the mechanics of a bending beam. The following sections discuss each in turn.

2.8.2 THREE-POINT BEND TEST A standard configuration for the three-point bend test is shown in Figure 2.13a. Using the three-point bend test, McDevitt and Baun39 carried out one of the earliest studies on metal-to-metal adhesive joints. These investigators found the curious result that apparently the three-point bend test was more sensitive to interfacial weaknesses than other tests they were performing such as the T-peel, the wedge test, and the lap shear test. Load-versus-deflection data were gathered on metal/adhesive/ metal sandwich samples as depicted schematically in Figure 2.14. The top curve in this figure represents a nonbonded sample in which a cured strip of adhesive was simply laid between two metal layers with no apparent bonding other than simple friction. This load-displacement curve thus serves as a baseline for a completely nonbonded

Overview of Most Common Adhesion Measurement Methods

Knife edge

Preset cut

33

Knife edge (e) Double cleavage drilled compression

(a) Three point bend

a

F Preset cut

F

F

(b) Four point bend

P (f ) Brazil nut

Knife edge P Adherend

(c) Standard double cantilevered beam

Knife edge

P

Adhesive

Adherend

(g) Wedgetest

P P (d) Tapered double cantilevered beam

F

Adherend Adhesive Adherend

(h) Topple beam test

P

FIGURE 2.13 Eight different adhesion tests that rely on the elastic bending properties of stiff beams.

joint. Figure 2.14b shows the case where the metal/uncured adhesive/metal sandwich was cured in an oven to achieve maximal bonding between all the layers. Note that this sample achieves a much higher load level before yielding. In addition, the authors attributed the break in the curve to failure at the metal/adhesive interface. With basic calibration data in hand for completely bonded and unbonded specimens, the authors were able to test bonded samples subjected to a variety of thermal and environmental stress conditions. Roche et al.40 investigated an interesting variation of the three-point bend test that is also sensitive to conditions at the adherate/substrate interface. The basic configuration is depicted in Figure 2.15. At a high enough load, the adherend will detach from the substrate starting from the edge and proceeding to the center, as shown in the figure. With the configuration shown in Figure 2.15, the stress distribution in the adherend can be monitored using the photoelastic setup shown in Figure 2.15b. In a typical experiment, the sample stiffness and stress distribution are monitored as the load is increased. An important piece of information is the load at which delamination of the adherend just begins. This number is sensitive to the detailed substrate preparation procedure before application of the adherend. It is clearly shown that this technique can be a powerful tool for investigating the effect of different surface preparation procedures and adhesive formulations on the adherend/ substrate adhesion strength. Making multiple identical samples also allows one to

34

Adhesion Measurement Methods: Theory and Practice

Load-displacement data for metal/adhesive/metal samples (Note: Time plotted in place of actual displacement. Adapted from McDevitt and Braun, ref. 39) 3000 Load (lb)

Non-bonded specimen 2000 1000

1

2

3

4 5 Time (min)

6

7

6

7

(a)

Load (lb)

4500

Bonded specimen

3000 1500

1

2

3

4 5 Time (min) (b)

FIGURE 2.14 Bending load versus time for three-layer sandwich samples using the threepoint bend test: (a) Poorly bonded sample shows essentially continuous load buildup, with increasing bending basically reflecting the stiffness of the most rigid layer. (b) Strongly bonded sample shows significantly higher load versus deflection behavior than the poorly bonded case, indicating strong coupling and mutual reinforcement between all the layers of the sample. In addition, a sharp drop in the load is detected when the adhesive joint between the layers fails.

study the effect of thermal cycling and other environmental stress factors on the durability of the bond.

2.8.3 FOUR-POINT BEND TEST The standard configuration for the four-point bend test is shown in Figure 2.13b. Figure 2.16 shows the typical failure modes of the coating/substrate system as the bending load is increased. Note that there are two basic failure modes for this experiment. In the first case, failure is by clean delamination of the coating from the substrate. It can also happen that after propagating a short distance an initial delamination will dive into the substrate, initiating a cohesive failure. Experiments and theory confirm that the crack will dive to some fixed depth below the interface and then propagate indefinitely parallel to the interface. The precise depth of penetration is determined by the elastic properties of the coating and the substrate. This

Overview of Most Common Adhesion Measurement Methods

35

Modiﬁed 3 point bend test (after Roche et al., ref. 40) F Typical failure path Substrate Adherend

(a) Side view

Substrate Adherend Light source

Detector Polarizer (b) End view

FIGURE 2.15 Variation of the three-point bend test in which the stress in the adherend is monitored by photo elastic measurement: (a) Side view showing most likely delamination path. (b) End view showing schematic of photoelastic measurement setup.

problem is treated in detail in Chapters 3 and 4, which cover the fundamentals of continuum theory and fracture mechanics required to understand this type of behavior. The four-point bend test is favored largely by those interested in obtaining fully quantitative information on the adhesion strength of coatings by taking advantage of the relatively simple beam mechanics involved in the fracture analysis of this problem. In particular, Evans and co-workers used this test extensively to study the adhesion of a variety of metals to alumina (Al2O3) substrates. This work has been summarized by Evans.41 A synopsis of their results is given in Table 2.2. The basic conclusion from this work was that interfaces that were clean and free from contamination were inherently tough and ductile. Failure occurred either by rupture of the ceramic or ductile fracture of the metal. Moisture was observed to cause stress corrosion effects that greatly weakened some of the interfaces.

2.8.4 STANDARD DOUBLE CANTILEVERED BEAM TEST Figure 2.13c depicts the simplest form of what is generically known as the double cantilevered beam test (the popular acronym is DCB test). One of the earlier reviews of this test was given by Bascom and co-workers42 as applied to the adhesion of metals to glass and ceramic materials. Bascom et al.43 also gave an overview of the

36

Adhesion Measurement Methods: Theory and Practice

F

Clean delamination

F

F

Delamination followed by substrate cracking

F

FIGURE 2.16 Schematic of basic failure modes of four-point bend test. A cut is first made in the coating down to the underlying substrate. A bending load is then gradually applied. The singular stress field at the edge of the cut eventually drives a delamination, which can turn into the substrate, giving rise to a crack that can later lead to spalling of the coating.

TABLE 2.2 Summary of Adhesion Strength of Various Metals to Alumina (Al2O3) Substrates Metal Nickel γ-Nickel (Cr) Gold Gold Aluminum Copper

Conditions

Range of Adhesion Strength (J/m2)

Comments

High humidity Dry air High humidity Dry air All conditions All conditions

4–8 >100 1.5–2.5 >200 >50 >150

Impurity segregation at interface Failure in metal or Al2O3 Impurity segregation at interface Failure in metal or Al2O3 Al2O3 rupture above 300 J/m2 Failure in metal or Al2O3

Note: Data summarized from work of A.G. Evans, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed., VSP, Utrecht, The Netherlands, 2001, p. 1.

application of this technique to the study of structural adhesives. These authors pointed out that one of the primary needs for the development of this technique was the evaluation of the strength and reliability of structural adhesives required to bond the new lightweight, high-performance composite materials required for the next generation of naval vessels, such as hovercraft and hydrofoils. One problem that became apparent right away is the fact that the structural adhesive materials considered showed significantly different strength properties when used as thin adhesive layers as opposed to bulk samples. The cantilevered beam configuration solved this problem with the added benefit of allowing for a relatively simple analysis of the

Overview of Most Common Adhesion Measurement Methods

37

data based on elementary beam mechanics. As shown in Figure 2.13c, the sample is prepared by carefully gluing together two identical beams of the substrate material of interest with a thin layer of the adhesive material under test. Great care must be taken regarding the surface preparation and cleaning of the beams and controlling the thickness and cure conditions of the adhesive. A spacer of some inert material such as Teflon is used at the ends of the sample to set the layer thickness and provide a well-controlled initial crack length. The sample is then mounted in a standard tensile testing apparatus in which the load-displacement behavior can be carefully determined. A fairly elementary fracture mechanics analysis based on standard beam mechanics and the classic Griffith failure criteria gives the following equation for the apparent fracture toughness of the adhesive bond:

γ Ic =

4 Fc2 ⎛ 2a 2 1 ⎞ + b 2 E ⎜⎝ h3 h ⎟⎠

(2.6)

where Fc = Critical minimum load required to initiate crack propagation γIc = Critical mode I fracture energy for crack propagation a = crack length E = Beam modulus h = Beam height b = Beam width To determine γIc, the load on the sample is ramped up until the preexisting crack just begins to propagate. This load is recorded as Fc, which then can be inserted into Equation (2.6) along with the other beam parameters to determine the critical fracture energy.

2.8.5 TAPERED DOUBLE CANTILEVERED BEAM TEST Equation (2.6) is problematic from the experimental point of view in that one has to control both the crack length and the applied load simultaneously to establish a stable constant value of γIc. This is because of the involved dependence of γIc on the beam height. Someone apparently noticed that if you tapered the beam height h such that the quantity (a2/h3 + 1/h) in Equation (2.6) remains constant, then one only has to worry about controlling the applied load. Thus, the equation describing the critical fracture energy for the tapered beam shown in Figure 2.13d can be written as

γ Ic =

4 Fc2 C b2E

⎛ 2a 2 1 ⎞ C = ⎜ 3 + ⎟ = constantt h⎠ ⎝ h

(2.7)

Adhesion Measurement Methods: Theory and Practice

Ideal case

Load

38

FC

Displacement (a)

Load

Real polymers F1 FA Displacement (b)

FIGURE 2.17 Typical load-versus-displacement data for the DCB experiment: (a) Hypothetical ideal case in which load increases up to the failure point and then propagates at a constant value determined by the fracture toughness of the adhesive joint; (b) real-world data in which the failure load oscillates between high and low values because of the strain rate sensitivity of most adhesives.

According to Equation (2.7), if we use a tapered beam with the beam height h adjusted so that the factor C in Equation (2.7) is constant, then the critical fracture energy will depend solely on the applied load at fracture. Thus, the output of the tensile test machine that generates load-versus-displacement data as the beam is pulled apart should look like the schematic plot given in Figure 2.17a. In this figure, we see the load ramping up in a linear fashion until the adhesive material gives way or starts to delaminate from either the top or bottom beam. At this point, assuming a uniform failure process, the load will stabilize at a constant level Fc, which can be substituted into Equation (2.7) to determine the critical fracture energy γIc. However, even assuming a uniform failure process, actual data tend to look more like Figure 2.17b, with a sequence of peaks and valleys instead of a steady plateau. The reason behind this behavior stems from the fact that the polymer materials that comprise the major part of the adhesive tend to exhibit strain rate-dependent failure behavior. What this amounts to in practice is that γIc tends to decrease as the crack propagates. Thus, referring to Figure 2.17b, the load increases to the level FI , at which point the crack starts to propagate. Now, as just mentioned, γIc and thus the resistance to crack propagation decreases, resulting in a lower load level to drive the crack. The lower load level, however, decreases the strain energy in the sample that is driving the crack. Eventually, the crack slows to the point at which it is completely arrested, which occurs at some load FA. At this point, the fracture resistance of the sample has returned to its zero strain rate value, and the load on the sample can now increase back to the level FI, at which the whole process can repeat. The upper value of γIc is referred to as the initiation energy and the lower value as the arrest energy.

Overview of Most Common Adhesion Measurement Methods

39

Beam

Beam

Adhesive

Adhesive

Beam

Beam

(a) Straight stable propagation

(b) Unstable wavy propagation

Beam

Beam

Adhesive

Adhesive

Beam

Beam

(c) Stable interface failure

(d) Bistable interface failure

FIGURE 2.18 Known modes of failure in a DCB specimen.

In practice, the range of behavior of DCB samples is even more complex than Figure 2.17 would suggest. Hutchinson and Suo44 reviewed the analysis of the DCB specimen and pointed out that there are at least four modes of crack propagation that have been identified (shown schematically in Figure 2.18). Each of these modes will have its own characteristic load-displacement behavior. Of particular relevance for adhesion measurement purposes is the stable interface failure mode shown in Figure 2.18c. It turns out that this mode can be selected for by using a nonsymmetric beam configuration in which one beam is stiffer than the other. In this way, the failure mode can be forced to be interfacial as opposed to cohesive in the adhesive. The DCB technique has seen extensive use in characterizing adhesive systems of all types. An entire volume could be dedicated to this activity alone. For the present purposes, however, just to give some idea of the range of values to be expected, Table 2.3 gives sample critical fracture energy data taken on a variety of polymer systems.

2.8.6 DOUBLE-CLEAVAGE DRILLED COMPRESSION TEST Figure 2.13e shows the double cleavage drilled compression (DCDC) sample, which is similar to the DCB sample in that an adhesive layer is sandwiched between two stiff beams. The main difference between the two techniques is in the mode of loading. As with the DCB sample, the DCDC sample is fabricated by gluing together two beams using an adhesive material and suitable spacers to achieve a desired uniform thickness of the adhesive layer and convenient initial crack regions. The sandwich sample is then drilled in the center symmetrically with respect to the initial crack region. The purpose of the hole is to provide a region of weakness that will

40

Adhesion Measurement Methods: Theory and Practice

TABLE 2.3 Representative Values of the Measured Critical Fracture Energies of Common Materials and Polymer Systems Material Inorganic glasses Unmodified epoxies, polyesters, and polyimides Poly(methylmethacrylate) Rubber-modified epoxies Aluminum/nylon/epoxy adhesive Metals

Critical Fracture Energy (J/m2) γIc < 10 70 < γIc 17,000

Note: Data retabulated from work of W.D. Bascom, R.L. Cottington, and C.O. Timmons, Naval Engineers Journal, 73 (August 1976).

buckle outward when the axial compressive load is applied as shown in Figure 2.13e. The outward buckling of the beam drives the interface crack in a predominantly mode I tensile opening fashion. Michalske and Fuller45 used this sample to investigate the fracture behavior of silicate glass. These authors pointed out the following advantages of using this test: 1. Use of compressive loading simplifies gripping and loading the sample and allows for more convenient use in corrosive environments, at high temperatures, and at high vacuum conditions. 2. A uniform stress intensity is maintained along the crack front. 3. Stable crack propagation is achieved along the midplane of sample. Evans46 pointed out that this sample has the further distinct advantage of decreasing strain energy release rate with increasing crack length. This property greatly simplifies the process of introducing a well-defined precrack before carrying out the adhesion measurement and allows for a more controlled experiment. This can be contrasted, for example, with the pull test, which gives rise to uncontrolled and unbounded crack propagation immediately after the onset of crack initiation.

2.8.7 BRAZIL NUT TEST Figure 2.13f gives a schematic representation of what has come to be known as the Brazil nut sample. This sample starts out as a section of a solid cylinder that is cut across a diameter and then glued back together with the material to be tested. Appropriate spacers are used to control both the bond spacing and the initial crack length. This rather implausible specimen has the advantage of controlling the mode mixity of the crack propagation by simply adjusting the angle of the bond line with respect to the direction of the applied compressive load. For instance, setting bond line at an angle to the applied compressive load as shown in Figure 2.13f results in

Overview of Most Common Adhesion Measurement Methods

41

a predominantly mode II shearing load. On the other hand, setting the bond line nearly parallel to the applied load gives loading conditions similar to the DCDC test, which is predominantly mode I tensile crack opening. This specimen clearly has a strong advantage when one is interested in testing the bond strength as a function of the mode of loading. The Brazil nut test has been in use for quite some time to test homogeneous solid specimens47 and was apparently first adapted to test interfacial toughness by Wang and Suo.48 An overview of this test has been given by Hutchinson and Suo.49 One of the interesting and useful features of this test is the fact that residual stresses within the adhesive layer do not contribute to the driving force for crack propagation. Thus, unlike standard tests such as peeling or the DCB method, one does not have to take into account residual stresses within the adhesive layer to compute the true surface fracture energy. This property combined with the ability to adjust the mode mixity of crack propagation easily make this test a favorite when carrying out fundamental studies on interface adhesion. An interesting study was done by Lee,50 who used the Brazil nut configuration to study the adhesion of epoxy molding compound to copper lead frame substrates. This study was prompted by the need in the microelectronics industry to understand the adhesion of these materials, which are important for packaging silicon chips. It turns out that although copper is an excellent conductor, it does tend to oxidize easily, and loss of adhesion between oxidized copper and the epoxy compound has been blamed for a loss of adhesion between the two materials that can give rise to a notorious form of blistering known as the popcorn effect. What happens is that moisture can aggregate at the delaminated interface and then form a blister when heated as would happen in a wire bond or die attach procedure. Lee was able to fabricate Brazil nut-type specimens of the epoxy/oxidized copper materials and then investigate the fracture toughness as a function of the mode mixity of the applied load. For mode I (predominantly tensile opening) loading, his data showed that the fracture toughness was very close to that measured for the same materials but using a DCB specimen geometry. However, when loading under conditions carrying a high shear component or mode II-type load, the measured fracture toughness was roughly twice that obtained for mode I conditions. This study clearly indicated the practical usefulness of the Brazil nut specimen because one can clearly be mislead about the adhesion strength when relying on only one mode of loading.

2.8.8 WEDGE TEST Figure 2.13g illustrates the wedge test, by which a sandwich laminate is loaded by simply forcing a wedge into one end of the laminate. This test has been used effectively in the aircraft industry to evaluate the durability of sandwich layers of thin aluminum sheets bonded with an adhesive. An interesting study carried out by the Boeing company was informatively reviewed by Pocius.51 The main advantage of the wedge test is the fact that many samples can be easily and cheaply fabricated and then subjected to any variety of environmental stress conditions to determine the durability of the bond. The success of this method has led to the formulation of

42

Adhesion Measurement Methods: Theory and Practice

American Society for Testing and Materials (ASTM) Standard D3762, which describes in detail sample preparation and testing procedures. By loading the sample using the simple insertion of a wedge at one end, a constant load can be applied at a level just below that required for crack propagation. The sample can now be placed in a hostile environment (e.g., high temperature or humidity), and the progress of any preexisting crack can then be monitored as a function of time. For a good bond, the crack should be short and primarily within the adhesive layer itself. A faulty bond is indicated when the crack is relatively long and propagating along the metal/adhesive interface. The wedge test has found fairly wide application for testing the durability of adhesives. Interesting examples include the work of Sharif et al.,52 who used the wedge specimen to test the effectiveness of model copolymer adhesives on glass. Davis et al.53 used the technique to test the effectiveness of plasma sprayed coatings on titanium and aluminum, and Meyler and Brescia54 used the technique to test a variety of waterborne adhesives on aluminum and aluminum-lithium surfaces. The main advantage of the wedge test lies in the ability to easily create a large number of samples that can be used for long-term environmental stress testing. Also, because the method is basically grounded in the mechanics of bending beams, it can be analyzed quantitatively using standard fracture mechanics analysis.55–58

2.8.9 TOPPLE BEAM TEST As a final example of an adhesion test based on the mechanics of a bending beam, we mention the topple beam test as shown schematically in Figure 2.13h. This test has much in common with the well-known pull test discussed in Section 2.4, with the crucial difference being the mode of loading the sample. All of the sample preparation procedures prescribed for the pull test apply equally to the topple beam experiment. This experiment in fact shares just about all the advantages and disadvantages encountered in the pull test. One advantage of the topple beam, however, is that the mode of loading is nearly pure bending, allowing for a simplified analysis. Apalak59 in particular carried out an extensive mechanics analysis of the topple beam geometry, including the effects of geometric nonlinearity caused by large rotation of the beam. Another distinct advantage of the topple beam over the pull test is the fact that, by applying a lateral load to the top of the beam, the problem of gripping the beam is relatively trivial compared to the pull test, which has to ensure proper gripping to avoid slippage. This can be a significant problem when using beams made of hard brittle materials. Finally, with the pull test one has to be careful to apply the tensile load exactly along the beam axis to avoid applying a bending moment to the beam, a problem that does not arise in the topple beam approach. An overview of this method was given by Butler,60 and an application to metal films was provided by Kikuchi et al.61 It might be added in closing that the topple beam test has much to recommend it for the adhesion of pins on ceramic substrates. As mentioned, the pin pull method is widely used for testing pin adhesion. However, when inserting a pin into a socket there is always a significant bending load present.

Overview of Most Common Adhesion Measurement Methods

43

From the point of view of reliability testing, one would prefer that the pin should bend as opposed to tearing off the pad. A bent pin can be straightened, but a tear-off failure can render an entire substrate useless. The topple beam experiment is clearly an efficient way to sort out these distinct behaviors in a population of pins attached to a rigid substrate.

2.8.10 ADVANTAGES

OF

BEAM-BENDING TESTS

It is clear that the main advantage of using any one of the tests described in the previous sections is that they all lend themselves relatively easily to quantitative analysis using the methodology of fracture mechanics, which is described in detail in Chapter 4. The mechanics of bending beams was one of the earliest and quite likely the most studied topic in the history of applied mechanics. An extensive body of literature exists that can be called on to supply stress/strain solutions for nearly any beam configuration that can be imagined. Thus, it is fairly straightforward to convert load-displacement data taken on any of the samples shown in Figure 2.13 into fracture toughness or surface fracture energy results that are directly relevant to the adhesion failure process investigated. This type of data is especially important as input to detailed fracture mechanics-based models, which attempt to predict the failure of structures based on geometry, material properties, and loading conditions. A second advantage of beam-based tests is the ability to fabricate a large number of samples relatively easily for testing under a variety of conditions.

2.8.11 DISADVANTAGES

OF

BEAM-BENDING TESTS

As always, we have to recognize that there are no ideal adhesion tests, and the beambending methods are no exception. The key advantage of having a simple geometry that is suitable for analysis leads to the main disadvantage of these tests, which is the very limited sample geometries that can be investigated. Ideally, someone manufacturing automobile fenders would like a test that could indicate how well the paint is adhering to the metal and that could be implemented on the manufacturing line to give real-time results on a wide variety of fender shapes. The beam-bending experiments clearly do not fit the bill here and are thus confined to use solely in the testing laboratory. The second most serious complaint that can be lodged against the beam-bending methods is whether they adequately simulate the stress/strain loading environment that real manufactured parts must endure. In particular, cases for which the main mode of failure is through internal stresses, such as those caused by thermal expansion mismatch strains, the delamination process is driven mainly by the elastic energy generated by the stresses. In such cases as when, for example, a highly stressed coating deadheres spontaneously from its substrate, the delamination process occurs under near-infinitesimal strain conditions. In all of the beam-bending tests, however, the delamination process is driven by external loading at substantial levels of deformation and strain. Although the level of deformation is nowhere near that generated by something like a peel test, nonetheless this calls into question the relevance of beam-bending data for such situations.

44

2.8.12 SUMMARY

Adhesion Measurement Methods: Theory and Practice AND

RECOMMENDATIONS

The main conclusion that arises out of all the above discussion is that the bending beam experiments are quite likely the methods of choice when fully quantitative data is required, such as for critical surface fracture energies or mode I and mode II fracture toughness data. The bending beam methods provide the most reasonable way of obtaining fracture and delamination data over the entire range of mode mixity for a wide range of adhesive/adherend combinations. Sample fabrication is demanding but not excessively so. Geometries such as the wedge test allow generation of many samples for testing under a wide range of environmental conditions while giving quantitative data without the need for elaborate test equipment. On the downside, it must be recognized that the beam-bending tests will find best application in the laboratory environment as opposed to the manufacturing line. This arises primarily from the highly restricted sample geometries involved plus the need for careful sample fabrication and nontrivial data analysis.

2.9 SELF-LOADING TESTS It is well known that the internal stress in a coating can cause it to delaminate spontaneously from the underlying substrate. This effect is commonly seen in old paint coatings on wood trim and other artifacts in which shrinkage stresses in the coating cause it to peel back from the edges and other internal defects. The idea that naturally suggests itself is to set up an adhesion measurement experiment in which the driving force for delamination is derived solely from well-controlled internal stresses in the coating to be tested. The task of the experimenter is then reduced to monitoring the propagation of the delamination front at a known fixed level of internal stress. A number of experiments along these lines are discussed next. One of the major advantages of this type of experiment is that the loading conditions closely resemble those that initiate failure in real coatings subjected to field conditions.

2.9.1 CIRCLE CUT TEST Figure 2.19 gives a schematic illustration of what is called the circle cut test. In this experiment, one has a coating on a substrate with a uniform biaxial stress σ0 that can be caused by any number of factors, such as deposition conditions, thermal expansion mismatch strains, shrinkage caused by solvent loss, and so on. At time zero, a circular cut is made somewhere in the interior away from any edge, giving rise to the situation shown in Figure 2.19. As explained in Chapter 4, the act of generating a sharp edge creates a stress singularity at the edge of the cut at the interface between the coating and the substrate. If the adhesion of the coating is relatively weak, then the coating will deadhere from the substrate, forming an annular ring of delaminated material as shown in Figure 2.19. The radius of the cut and the radius of the delaminated annular region are then measured by optical or other means, and this information can then be used along with knowledge of the stress level σ0 in the coating and its elastic properties to calculate the critical surface fracture energy according to the following formula:

Overview of Most Common Adhesion Measurement Methods

45

a R h σ0

σ0

FIGURE 2.19 Schematic of circle cut test. A circular hole of radius R is cut in a coating carrying an internal stress σ0. If the coating adhesion to the substrate is insufficient, then because of the stress singularity at the edge of the hole, the coating will delaminate out to a radius R + a. The driving force for delamination can be easily determined if one knows the elastic constants of the coating, the film stress, and the geometric parameters in the diagram.

Gc =

β= where R, h, and a σ0 E v Gc

= = = = =

⎤ hσ 20 ⎡ 2β 2⎥ 2⎞ E ⎢⎢ ⎛ ⎡a⎤ ⎥ ⎢ ⎜ 1 + β⎢ ⎥ ⎟ ⎥ ⎣ R ⎦ ⎟⎠ ⎥⎦ ⎢⎣ ⎜⎝

(2.8)

1− ν 1+ ν

Coating and cut dimensions as shown in Figure 2.19 Residual stress in coating Modulus of coating material Poisson’s ratio of coating critical strain energy release rate

A convenient feature of this test is the fact that, according to Equation (2.8), the size of the annular delamination region will always be constrained because the driving force Gc decreases as the size of the delaminated region increases. Thus, at some finite value a, the driving force for deadhesion will be too small to propagate the delamination any further, and the experimenter can make the appropriate measurements at leisure. Farris and Bauer62 used this method to study the adhesion of polyimide coatings. This approach has a number of distinct advantages, including: •

• •

Close simulation of the mechanism by which coatings tend to delaminate under field conditions of high stress, low strain, and mixed-mode conditions of tension and shear Relative ease of sample preparation Amenability to quantitative analysis

46

Adhesion Measurement Methods: Theory and Practice

The main drawback is that because the driving force for delamination relies solely on the internal film stresses, there may not be sufficient strain energy in the coating to initiate a delamination if the level of adhesion is too high. This fact tends to limit this test to coatings with weak adhesion.

2.9.2 MODIFIED EDGE LIFTOFF TEST In view of the limited applicability of the circular cut test to weakly adhering coatings, a related approach called MELT (modified edge liftoff test) has been explored by Hay et al.63 The main innovation in this approach is the use of a layer of material on top of the coating to be tested that will drive up the total internal stress and thus give sufficient driving force to delaminate any coating. A schematic representation of this test is given in Figure 2.20. As shown in the figure, complications can arise because of crack initiation in the substrate rather than the interface of interest. Hay and co-workers exercised this technique on a multilayer sandwich consisting of epoxy/dielectric layer/silicon nitride/native oxide/silicon. They sidestepped the substrate fracture problem by using a hydrofluoric acid solution to etch out a large initial crack in the silicon nitride layer. In addition, they polished the edge of the sample with fine sandpaper to eliminate any flaws left behind by the wafer dicing operation. A thick epoxy top layer between 150 and 200 μm provided the driving force for crack propagation caused by thermal expansion mismatch with the silicon substrate. Under these conditions, they observed clean delamination of the dielectric layer from the silicon nitride. These workers noticed an interesting property of their epoxy-loaded samples that seemed to contradict previous work that used chromium as a superlayer instead of epoxy. From the chromium work, it was noticed that the driving force for delamination depended on the size of the initial crack length and did not settle down to a constant value until the delamination length had reached at least 20 times the chromium layer thickness. With the epoxy-loaded samples, there was no apparent Stressed superlayer σ Sample coating Delamination Substrate

Substrate crack

FIGURE 2.20 Schematic of the modified edge liftoff test (MELT), which attempts to circumvent the limitation of the self-loading test to the case of relatively weak adhesion, as in the circular cut test shown in Figure 2.19. A top layer of material with known internal stress behavior is applied to increase the delamination driving force to any desired level. As can be expected, a number of complications can arise, including possible failure of the underlying substrate.

Overview of Most Common Adhesion Measurement Methods

47

dependence of the driving force for delamination on the initial crack size. A subsequent finite element analysis of the problem comparing the driving force for delamination for both the epoxy- and chromium-loaded systems indicated that indeed the behavior of the epoxy and chromium systems is very different. In the epoxy case, the driving force rises so sharply with crack length it nearly resembles a step function. In the chromium system, the driving force rises much more slowly and essentially follows the rule of 20 times the chromium thickness before leveling off to a steady state.

2.9.3 MICROSTRIP TEST The microstrip test is closely related to MELT in that the same principle of using a superlayer on top of the layer to be tested is employed to obtain a sufficient driving force for delamination. A schematic of the basic sample configuration is shown in Figure 2.21. The version of the test described here was carried out by Bagchi et al.64 and reviewed by Evans.65 What is shown in the figure are the various layers of the adhesion measurement test structure. The substrate may be a block of ceramic or glass or whatever the material of interest is. On top of the substrate, narrow parallel strips of a release layer material are first deposited. A typical release layer strip is visible in the uncoated regions separating the sample strips shown in Figure 2.21. Next, the coating is applied as a blanket layer. On top of that, the superlayer is deposited as a blanket coating. A good candidate for this material when testing thin metal films is chromium, which can develop internal stress levels up to 1 GPa. The blanket coatings are now etched into thin strips perpendicular to the release layer strips using photolithographic methods. Sample strips

Cut

Release layer

FIGURE 2.21 The microstrip test is yet another self-loading adhesion test that takes advantage of photolithographic methods to create a large number of test specimens on a single substrate. The figure shows a greatly enlarged view of three test strips. The horizontal stripe is a release layer material to which the coating has poor adhesion. After applying blanket coatings of the test film and the loading layer, a large number of test strips are then etched out using lithographic methods. A cut is then created in the strips in the region where they overlay the release layer. Because of the poor adhesion to the release layer, delamination is immediately initiated and will proceed to propagate into the strip. However, the nature of the driving force is such that delamination will always terminate before the strip is entirely peeled off the substrate. The length of remaining adhered ligament can then be used to compute the surface fracture energy.

48

Adhesion Measurement Methods: Theory and Practice

The adhesion test begins after a thin cut is made down the center of the release layer strip using either etching or milling techniques. As the adhesion at the release layer is very weak by design, a delamination is immediately initiated starting from the cut to the edge of the release layer. Depending on conditions, the delamination front will proceed past the edge of the release layer and into the interface between the sample coating and the substrate. If the delamination stops at the edge of the release layer, then clearly there is not enough strain energy in the chromium superlayer, and a thicker layer of chromium needs to be applied. At a sufficient thickness of the chromium layer, the delamination will proceed at the coating/substrate interface or possibly proceed as a subcrack in the substrate depending on how well adhered the coating is. Assuming that the delamination proceeds at the coating substrate interface, it will go for a certain distance and then arrest. In this test, all of the test strips are finite length, and the driving force for delamination decreases toward zero as the crack front nears the end of the strip. Therefore, the delamination front must arrest, and the length of the remaining ligament is therefore indicative of the adhesion between the coating and the substrate.

2.9.4 ADVANTAGES

OF

SELF-LOADING TESTS

Self-loading tests come very close to mimicking the conditions under which real coatings delaminate in terms of strain level and mode mixity; this is their main advantage as an adhesion test. This is especially true for microelectronic structures, for which intrinsic stress is one of the major causes of device failure. In addition, the self-loading tests lend themselves readily to quantitative analysis because the strain level at failure is typically quite low, and linear elastic theory suffices to carry out the required fracture mechanics evaluation of the strain energy release rate. When used to evaluate microelectronic devices, the test structures required to carry out the adhesion measurements can be fabricated using equipment nearly identical to that used in the production line. Thus, although sample preparation is fairly involved, it does not require resources beyond what should already be available in the existing manufacturing facility. Finally, the test structures can be integrated into the actual manufacturing process as diagnostic probe sites capable of giving near-real-time quality control and monitoring information on real manufacturing parts. Of all the adhesion tests discussed so far, the self-loading tests come the closest to an ideal adhesion measurement method.

2.9.5 DISADVANTAGES

OF

SELF-LOADING TESTS

The main disadvantage of the self-loading tests is the need to know the internal stress and mechanical properties of the coating to be tested. The problem of determining the internal stress in a coating is a rather large subject, and an entire chapter in this volume (Chapter 6) is devoted to just this problem. Further complications arise if the internal stress level is insufficient to cause delamination and one of the superlayer methods must be implemented, thus greatly increasing the work required for sample preparation. Finally, the trajectory of the delamination crack front may deviate from the interface into either the substrate or the coating, depending on conditions. This will significantly complicate the fracture mechanics analysis involved.

Overview of Most Common Adhesion Measurement Methods

49

In essence, the self-loading tests share the common problems of all fully quantitative tests in that they inevitably involve much more work than the simply qualitative or semiquantitative methods.*

2.9.6 SUMMARY

AND

RECOMMENDATIONS

The self-loading adhesion tests are most suitable when quantitative data is required to support numerical modeling simulations of the structures under fabrication. Multilevel wiring structures from the microelectronics industry are a prime example of an application that can benefit greatly from this type of test. Such structures are replete with interfaces between dissimilar materials that are subject to numerous manufacturing processes that can introduce high levels of internal stress. As a specific example, consider the use of organic insulators as dielectric layers in multilevel wiring schemes. Some of the most popular materials for this application are the polyimides. These materials are typically coated as a viscous liquid using either spin- or spray-coating methods. The resulting film must be cured at an elevated temperature, generally above 300°C to achieve the correct electrical and mechanical properties required. Cooling to room temperature will induce a large internal thermal expansion mismatch strain in the coating if the underlying substrate is either silicon or a ceramic material because most polyimide materials have thermal expansion coefficients 10 to 30 times larger than either silicon or most ceramics. An elementary calculation using the principles of continuum theory covered in Chapter 3 shows that the resulting stress level in the coating can come to nearly 50% of the yield stress of the polyimide itself. In such cases, appropriate stress modeling supported by fully quantitative adhesion data are required to carry out the type of engineering design analysis necessary to support the fabrication and manufacture of a useful device. The large amount of work involved in implementing the self-loading methods will quite likely limit them to this type of application.

2.10 MORE EXOTIC ADHESION MEASUREMENT METHODS 2.10.1 LASER SPALLATION: EARLY WORK Up to this point, the adhesion tests under discussion have been of a fairly prosaic nature in that the mode of loading has always been some kind of mechanical tension, compression, or shear applied by a mechanical test apparatus, by the residual stress in the coating, or by some applied superlayer material. For the laser spallation test, however, the loading conditions are rather exotic in that they involve highly transient shock waves induced by ultrafast laser pulses. In a typical test, a laser pulse with a fluence of 500,000 J/m2 is focused onto a 1-mm diameter spot for 30 nsec, which amounts to energy deposition at a power rate of 13 MW.

* As a general rule of thumb, when going from a qualitative test to a fully quantitative one, you can expect to work not only twice as hard to obtain acceptable results but more likely 10 times as hard. This almost seems to be some kind of thermodynamic theorem proved through difficult experience if not from any formal axiomatic demonstration.

50

Adhesion Measurement Methods: Theory and Practice

This test was apparently first discussed in the open literature by Vossen66 and Stephens and Vossen,67 who used it to investigate the adhesion of metals to glass. A typical experimental setup is shown in Figure 2.22. In the earlier experiments, an array of islands of the coating to be tested were evaporated onto a glass substrate. Small islands were used to avoid the effect of tearing of the film, which would occur during the spallation of a continuous metal film. The opposite side of the glass substrate was coated with an energy-absorbing layer such as titanium. During a standard experiment, a high-intensity, short-duration laser pulse is directed at the titanium layer on the back side of the sample. The effect on impact is literally explosive vaporizing of the titanium and blasting it off while simultaneously depositing a large amount of heat into the underlying glass in a very short time. The recoil of the blasted titanium combined with the rapid thermal expansion of the glass generates a compressive shock wave that propagates to the front side of the glass, where the islands of deposited metal are waiting. The compression wave is reflected at the front surface of the substrate as a tensile wave caused by the rapid tensile snap back of the substrate. The elastic snap back propagates across the substrate metal interface, providing the rapid tensile loading that ejects the metal islands off the substrate. To determine the adhesion strength of the coating, the energy of the laser pulse is ramped up systematically until coating failure is first observed. Depending on conditions, a variety of collateral damages can occur to both the substrate and the coating tested. Vossen pointed out in particular that brittle substrates tend to shatter. However, one experiment used islands of gold deposited on glass and clearly demonstrated clean delamination. Backing layer Laser

Substrate

Sample island Compressive shock wave

(a) Pulse initiation

Backing layer Laser

Substrate Detached sample ﬁlm Reﬂected tensile wave

(b) Reﬂected tensile wave

FIGURE 2.22 Laser spallation experiment: (a) A high-intensity laser pulse impinges on the back of the substrate, initiating a strong compressive stress pulse because of the rapid heating at the point of impingement; (b) the compressive pulse reflects off the coating/substrate interface, generating a strong tensile reflective wave, which can cause delamination of the coating.

Overview of Most Common Adhesion Measurement Methods

Absorbing layer Backing layer Nd: Yag-laser

51

Sample coating Mirror 1

Substrate

Beam splitter Mirror 2

Lens Compressive shock wave Computer

He-Ne laser Photodetector digitizer

FIGURE 2.23 Improved laser ablation experiment. The basic principle is the same as in Figure 2.22 with the following improvements: (1) A backing layer is added over the energyabsorbing layer to carry away excess thermal energy that would otherwise create a long tail on the induced compressive pulse, which significantly reduces the resolution of the method. (2) A laser Doppler interferometer is employed to monitor the displacement of the sample surface in real time as it deforms because of the impinging stress pulse. This allows for an independent determination of the critical stress level for delamination.

2.10.2 LATER REFINED EXPERIMENTS The early experiments on laser spallation demonstrated that the technique could be used to test the adhesion of coatings in a unique way. A number of problems hindered progress, however, including the use of expensive finicky equipment that required careful and time-consuming calibration procedures. In addition, a large thermal stress tail followed the main pulse and limited the resolution that could be achieved in stressing the coating substrate interface. Additional problems, such as fracture of brittle materials, excessive stress damping, and potential decomposition of viscoelastic media, essentially limited the method to testing refractory materials. Advances in technology and techniques, however, have greatly improved the laser spallation test, as discussed by Gupta et al.68 Figure 2.23 illustrates an improved version of the laser spallation experiment shown in Figure 2.22. The new features in this version of the laser spallation experiment include 1. Inclusion of an absorbing layer between the back side of the substrate and a backing layer. This approach allows the user to nearly eliminate the long thermal stress tail associated with the earlier approach by essentially ablating away the excess thermal energy into the backing layer instead of letting it diffuse into the substrate, where it induces a large thermal stress. This long-tail thermal stress can confound the data analysis, especially when dealing with very thin sample coatings.

52

Adhesion Measurement Methods: Theory and Practice

2. Use of a laser Doppler interferometer to monitor in real time the deformation and velocity of the sample coating during impact by the reflected tensile shock wave. Use of this equipment allows the user to quantitatively estimate the tensile stress at the interface that initiates film separation from the substrate. 3. Using the quantitative stress measurements taken from the interferometer data, one can further estimate an “intrinsic” surface fracture energy associated with the film delamination. 4. Use of a modified interferometer to deal with nonspecular reflection off rough surfaces. The main advantage of the new approach is the ability to use the velocity/displacement data taken by the interferometer to estimate the critical stress level at which coating spallation occurs. As with the old method, the laser power is increased incrementally until spallation is observed. Table 2.4 lists sample values for the critical stress for coating liftoff for several coating substrate systems. The strength values listed in Table 2.4 are similar to those that might be obtained in a pull test or other form of tensile test. The main difference is the dynamic nature of the tensile shock pulse, which hits the interface at a strain rate on the order of 107 sec−1. At such an enormous strain rate, we can expect the material response to be significantly different from what would occur in a standard pull test. In particular, viscoelastic effects should be “frozen out,” giving rise to nearly pure brittle fracture because most molecular relaxation behavior will be too slow to follow the rapid deformation pulse. Finally, by using a recently developed scaling relationship for the binding energy-versus-distance curves for metals, Gupta et al.69 were able to convert their

TABLE 2.4 Representative Values of the Interface Strength for Selected Coating Substrate Systems

Substrate Polyimide Copper Copper Silicon carbide Alumina/diamond composite Alumina/diamond composite

Coating

Interface Strength σmax (GPa)

Silicon Silicon nitride Pyrolytic graphite Pyrolytic graphite CVD diamond CVD diamond

0.46 0.041 0.015 3.4–7.48 1.61 1.41

Comments 5.3-μm polyimide 0.1-μm copper on nitrided silicon 2.1-μm SiC on 1.69mm disc 5% of 1-μm diamond particles 5% of 10-μm diamond particles

Note: Data retabulated from V. Gupta, J. Yuan, and A. Pronin, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed., VSP, Utrecht, The Netherlands, 1995, p. 367.

Overview of Most Common Adhesion Measurement Methods

53

interface strength data to fracture toughness values similar to that obtained in the bending beam tests. By using physical arguments based on the nature of metal-tometal interactions at the interface between different metals, these investigators derived the following relationship between their measured critical interface stress and what they called the intrinsic toughness or ideal work of interfacial separation Gco: σ 2max =

Gco Eo e 2h

(2.9)

where σmax = Critical interface strength as shown in Table 2.4 Eo = Modulus at interface Gco = Intrinsic interface toughness h = Unstressed separation distance between atoms e = Mathematical constant epsilon, which is the base of the natural logarithms = 2.71828183 The quantity σmax is measured directly by the laser spallation experiment, and representative values are shown in Table 2.4. The unstressed separation distance h can be determined by direct transmission electron microscopy measurements, and the interface modulus Eo is inferred from delamination experiments and from published data. With this data in hand, Equation (2.9) can be used to estimate the apparent critical surface fracture energy Gco. Values for selected systems are summarized in Table 2.5.

TABLE 2.5 Values of Critical Intrinsic Surface Fracture Energy from Laser Spallation Measurements Interface System Silicon carbide/pyrolytic carbon ribbon Silicon carbide/silicon Cleavage of (111) planes of silicon Niobium/Al2O3

Critical Surface Fracture Energy Gco (J/m2) 3 3.31 0.84 0.0009

Comments h = 0.9 nm from TEMEo = 107 GPa (average of two media) h = 0.5 nm; Eo = 115 GPa Stress pulse sent normal to (111) planes; h = 0.32 nm; E111 = 185 GPa Value considered faulty because of interface flaws; should be close to 0.69

Note: Data tabulated from V. Gupta, J. Yuan, and A. Pronin, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed., VSP, Utrecht, The Netherlands, 1995, p. 395.

54

Adhesion Measurement Methods: Theory and Practice

In evaluating the data in Table 2.4, one has to keep in mind that the coatings studied were delaminated from their substrates under extreme loading conditions (strain rates near 107 sec−1) for which material properties and viscoplastic deformation behavior in particular can be expected to differ significantly from those in effect for the more standard adhesion tests, such as the bending beam experiments discussed in this chapter. The authors of this work went so far as to suggest that the quantity they called Gco be called an intrinsic critical surface fracture energy in distinction to the usual Gc because many of the viscoplastic processes that contribute to Gc will be frozen out in the laser spallation experiment. In other words, the various atomic/molecular deformation processes that can contribute to the measurement of Gc are too slow to play a part in the laser spallation experiment.

2.10.3 LASER-INDUCED DECOHESION SPECTROSCOPY EXPERIMENT A variant of the laser spallation experiment goes under the acronym LIDS, which stands for laser-induced decohesion spectroscopy* has been discussed by Meth.70 A schematic of the LIDS experimental setup is shown in Figure 2.24. Strictly speaking, the LIDS experiment is not a spallation test as discussed above because the coating is not removed from the substrate; however, laser energy is used to deadhere the coating, which is sufficient qualification to be included. Referring to Figure 2.24, the basic experiment consists of directing an infrared laser beam onto the sample to be tested, which is a multilayer laminate composed of a substrate, an energyabsorbing layer, and a top coating. The absorption properties of the coating are such that the laser radiation passes through and is soaked up predominantly by the underlying absorbing layer, which rapidly decomposes, giving rise to a gas pressure that initiates blistering of the coating much as one would observe in the standard blister test. At a sufficient level of laser power, the blister will propagate into an annular debonded region that can be monitored by optical means. The curvature of the blister is monitored simultaneously by reflecting a second laser beam from a low-power He-Ne laser off the top of the blister. The reflected laser beam passes through a fixed aperture and then onto a photodetector, which measures the intensity of the light passing through the aperture. When no blister is present, a fixed and calibrated intensity of reflected light is measured. After blistering, the reflected light is spread out in proportion to the blister curvature; because the aperture is fixed, less light reaches the photodetector, and the measured intensity drops. Thus, the blister curvature can be inferred from the light intensity observed at the photodetector. Meth70 discussed the details of the calculation used to determine the curvature based on a Gaussian beam shape. With the size and curvature of the blister in hand plus knowledge of the elastic properties of the coating, the gas pressure causing the blister can be inferred through a classical continuum mechanics calculation that treats the blistered coating as a plate subjected to uniform pressure from below. Much of this analysis is already known from standard blister test theory, and full details are covered by Meth.70 By carefully observing the laser power required to * A more appropriate designation would be laser-induced deadhesion spectroscopy. Another problem is that this experiment has nothing to do with spectroscopy as it is commonly understood.

Overview of Most Common Adhesion Measurement Methods

55

Infra red laser He-Ne laser

Photodetector Aperture

Coating Absorbing layer

Substrate

FIGURE 2.24 LIDS experiment. Strictly speaking, this is not a laser ablation experiment but is close enough to warrant consideration here. A strong laser pulse is directed at the coating substrate interfaces. Gases created during the intense heat buildup create a blister in the coating, which can further delaminate as in the standard blister test. The curvature, and thus the size, of the blister is monitored by reflection of a weak laser beam off the top of the blister into a photodetector.

just initiate annular debonding of the blister, one can further apply standard blister test methods to determine the critical surface fracture energy for delamination.

2.10.4 ADVANTAGES

OF

LASER SPALLATION TESTS

The main advantage of the laser spallation test derives from the unique way in which the delamination load is applied to the coating under investigation. No gripping scheme is required, and the ultrahigh loading rate precludes many viscoelastic/ viscoplastic mechanisms, which tend to cloud the analysis of more conventional adhesion tests, such as the bending beam methods discussed in Section 2.8. Laser spallation may in fact be the only effective method for analyzing refractory systems such as the diamond-on-alumina samples. This technique is also amenable to full quantitative analysis because of the availability of advanced instrumentation such as the laser Doppler interferometer. The LIDS version of this test has the potential of application to a wide variety of surfaces, including actual parts from the manufacturing line, because the laser pulse and surface displacement measurement are applied directly to the top surface of the coating under study. The fact that this is a noncontact method that can be fully automated makes it possible to implement the LIDS experiment directly on the manufacturing line as a real-time quality control tool.

2.10.5 DISADVANTAGES

OF

LASER SPALLATION TEST

The same properties that give the laser spallation test its unique advantages also impart a number of its most important disadvantages. The most significant disadvantage derives from the ultrahigh strain rates involved. To perform the laser Doppler

56

Adhesion Measurement Methods: Theory and Practice

measurements required to gain quantitative information on the adhesion strength of the coating, one needs to measure stress pulses with rise times shorter than 5 nsec, which necessitates the use of 10- to 100-GHz transient digitizers. The photodetector for measuring the laser pulse should have a rise time of less than 200 psec, which will allow a measurement of interference fringes with a resolution on the order of 0.2 nsec. Needless to say, this is not the type of equipment likely to be found at a local hardware store. Thus, it is clear that this method is going to require expensive equipment that is not readily available. A second limitation of the laser spallation technique is the relatively difficult and limited sample configurations available. The need for special backing and absorbing layers will quite likely limit this method to use in the development laboratory only. Finally, the fact that ultrahigh strain rates are involved in removing the coating from the substrate complicates the problem of interpreting the resulting data in terms of typical field conditions.

2.10.6 SUMMARY

AND

RECOMMENDATIONS

The laser spallation adhesion test is one of the more exotic adhesion measurement methods and has some unique advantages to recommend it in certain situations. In particular, it may be the only method available to reasonably test highly refractory coatings that are either too brittle or too hard to be tested by more conventional methods. The instrumentation required for fully quantitative measurements is not commonly available but can be purchased from specialty vendors. This equipment is expensive, so the need for the required data must be sufficiently compelling. The LIDS version of this technique has a number of potentially useful applications given the fact that it is a noncontact method that can be fully automated. There is a definite prospect for use in real-time manufacturing quality control applications because it can be applied to very small test sites and requires no special sample preparation whatever. The only special requirement is the need to tailor the spotforming laser pulse to be absorbed preferentially by an existing underlayer of the coating to be tested.

2.11 ELECTROMAGNETIC TEST Another fascinating adhesion test method is the electromagnetic test, which utilizes the surprisingly large forces that can be developed by currents in a magnetic field. Figure 2.25 gives a schematic illustration of the basic configuration for lifting a metal line off of an insulating substrate. This figure shows a cross section of the metal line that is directed out of the page and carries a current I also directed out of the page. A magnetic field B is applied at a right angle to the flow of the current giving rise to a Lorentz force F acting perpendicular to the metal/substrate interface. For this configuration, the Lorentz force is given by the following formula from basic electromagnetic theory: F = Il × B

(2.10)

Overview of Most Common Adhesion Measurement Methods

57

W Metal line

I B

h

F

Insulating substrate

FIGURE 2.25 In the electromagnetic test, a current I flows in a metal test line in the presence of a perpendicular magnetic field. If the current and the magnetic field are sufficiently strong, then the line can be lifted off the substrate because of the induced Lorentz force.

where F I l B

= = = =

Lorentz force Current flowing in line Unit length vector in direction of current flow Magnetic field vector

The right-hand side of Equation (2.10) involves the vector cross product between the length vector l and the magnetic field B. For the geometry in Figure 2.25 with l and B mutually perpendicular, the cross product evaluates to lB, and the Lorentz force becomes F= IlB pointing normal to the substrate surface as shown. What is of primary interest, however, is the stress on the line, which is evaluated by dividing the force by the area A = lw, which gives the following very simple formula for the normal stress tending to lift the line off the substrate:

σn =

IB w

(2.11)

Equation (2.11) gives the normal stress on the metal line caused by the Lorentz force induced by the interaction of the current I with the magnetic field B where w is the width of the line. If we assume a magnetic field of 2 T (Tesla) and a current of 30 A (ampere) with a line width of 1 μm Equation (2.11) gives the substantial normal stress of 60 MPa. Referring to Table 2.4, we see that this stress level is more than sufficient to lift a copper coating off of a silicon nitride substrate as evaluated by the laser spallation method. However, those familiar with electromagnetics will immediately detect a potential problem in that 30 A is a substantial current to pass

58

Adhesion Measurement Methods: Theory and Practice

through a 1-μm wide line, or any metal wire for that matter, without vaporizing it. Therefore, we really need to investigate the temperature rise we can expect by performing this experiment. One way to keep from cooking the sample before delamination can be observed is to use very short current pulses on the order of 1 μsec. Making this assumption, the expected temperature rise in the line can be easily calculated from Fourier’s heat transfer equation given by Equation (3.36) and summarized in Table 3.1. Because we are talking about very short heating times, we can ignore diffusion effects and thus leave out the spatial derivatives (i.e., ∇2T) and work with the following simple relation, which will be valid for the short timescale under consideration: dT γ = dt ρc

(2.12)

Because all quantities on the right-hand side are constants, this equation readily integrates to give the following relation for the expected temperature rise: ΔT = T − T0 =

γt ρc

(2.13)

where ΔT γ ρ c

= Temperature rise above ambient in degrees centigrade = Heating rate per unit volume caused by joule heating (J/sec m3) = Density of metal (kg/m3) = Specific heat of metal [J/(kg degrees centigrade)]

The heating rate can be estimated from the joule heating caused by the electric current I. Elementary circuit theory tell us that this is given by the product I 2R, where I is the current, and R is the line resistance. The line resistance is further given in terms of the metal resistivity r by the simple formula R = rl/A, where r is the resistivity, l is the length of the line segment, and A is the cross-sectional area. Dividing the input power I 2R by the total volume of the line segment (lA) gives the heating rate per unit volume as γ = I 2r/A2. Inserting this expression into Equation (2.13) gives our final expression for the expected temperature rise in the line segment on application of a current I for a time duration t: 2

rt ΔT = I 2 ρcA

(2.14)

where I is the applied current, A is the line cross-sectional area, and all other quantities are as defined in Equation (2.13). It is illustrative to see what this equation predicts for our 30-A, 1-μsec pulse if applied to a copper line 1 μm wide and 10 μm high. For this case, the quantities in Equation (2.14) are

Overview of Most Common Adhesion Measurement Methods

I t r c ρ A

= = = = = =

59

30 A line current 10−6 sec current pulse duration 1.7 × 10−8 ohm-m 385 J/(kg degrees centigrade) 8960 kg/m3 10−11 m2

Plugging these numbers into Equation (2.14) gives the rather sobering estimate of a 4400 C temperature rise in the line. Thus, we are far more likely to vaporize the line rather than delaminate it. Early workers in the field facing this problem noticed that the killer factor in Equation (2.14) is the very small cross-sectional area that appears in the denominator squared. Krongelb71 in particular got around this problem by fabricating top-heavy lines, as shown in Figure 2.26. This line has close to 10 times the cross-sectional area of the one shown in Figure 2.19 while maintaining the same common interfacial area with the substrate. Thus, all quantities remain the same in Equation (2.14) except that the A2 term is 100 times larger than previously, which lowers the calculated temperature rise in the line to 44 C, which brings the whole experiment back down to Earth and within the realm of possibility. In actual samples fabricated by Krongelb, the top portion of the test line is not a nice rectangle as shown in Figure 2.26 but looks more like a semicircle. The principle remains the same, however; the top part of the line carries the heavy current load and prevents the metal line from vaporization before it can be lifted off by the Lorentz force. In addition to the work of Krongelb, Baranski and Nevin72 used a version of this test to measure the adhesion of aluminum to polyimide coatings, demonstrating the usefulness of this method for evaluating the adhesion of metal lines to organic as well as inorganic substrates.

10 microns Metal line

10 microns

Insulating substrate

FIGURE 2.26 Modified line structure for the electromagnetic adhesion test. A much larger cross-sectional area is created to avoid vaporizing the metal line before delamination can occur.

60

Adhesion Measurement Methods: Theory and Practice

2.11.1 ADVANTAGES

OF THE

ELECTROMAGNETIC TEST

Like the laser spallation test, the electromagnetic test has distinct advantages for certain special applications. The electromagnetic test is perhaps the only test available for investigating the adhesion of 1-μm wide metal lines under conditions closely resembling those of actual microelectronic devices. As with the laser spallation test, there is no problem with gripping the sample. In addition, the very high strain rates on the order of 106 sec−1 make it likely that viscoplastic effects will also be suppressed in this test. Finally, with the electromagnetic test there is the possibility of performing chipscale device testing on the manufacturing line because all of the equipment can be automated, and the sample preparation uses only well-developed lithography techniques that are compatible with standard device fabrication equipment.

2.11.2 DISADVANTAGES

OF THE

ELECTROMAGNETIC TEST

The most obvious disadvantage of the electromagnetic test is that it can be applied to conducting materials only, which essentially limits it to metals such as copper and aluminum. Even considering this limitation, the test still suffers from the constraint of requiring large currents and very high magnetic fields to achieve sufficient lifting force to induce delamination. Constraints of sample fabrication essentially limit the usefulness of this method to electronic devices, for which it has certain natural advantages. Finally, the instrumentation required for this test, although not particularly exotic, is not standard, and every setup is likely to be of the one-of-a-kind variety.

2.11.3 SUMMARY

AND

RECOMMENDATIONS

The overall evaluation of the electromagnetic test runs pretty much parallel to that for laser spallation. This is a test that has clear advantages in certain applications but is unlikely to find wide application because of the constraints and limitations mentioned. Availability of the required resources and the specific needs of the intended project will govern whether the electromagnetic test will be the bestavailable procedure for adhesion measurement in any given situation.

2.12 NONDESTRUCTIVE TESTS Whereas the concept of a nondestructive adhesion is something of an oxymoron in that it is difficult to believe a result that is supposed to tell you how strongly two materials are stuck together without actually measuring the force required to pull them apart, it is nonetheless a useful concept. The fundamental concept behind nondestructive adhesion tests is to measure some quantity that depends on how well two materials are joined at their common interface. The two tests discussed in this section depend on the following properties: • •

Ability to transmit strain/deformation across an interface Ability to transmit vibrations along an interface

The dynamic modulus test relies on the ability to transmit strain across an interface. For two perfectly bonded adherends, there is a boundary condition at their

Overview of Most Common Adhesion Measurement Methods

61

common interface that the local displacement field be continuous. If the adhesion is not perfect, then there should be some slippage, which can be detected by some type of measurement. The surface wave propagation test relies on the fact that the velocity of surface waves in an interfacial region will depend on how well adhered the separate layers are. These two measurement techniques are investigated in more detail next.

2.12.1 DYNAMIC MODULUS TEST The dynamic modulus test was used by Su et al.73 to investigate the adhesion of metals to glass. The basic experimental setup is based on an internal friction apparatus originally developed by Berry and Pritchet74 to study atomic relaxation phenomena in thin films. A schematic diagram of the apparatus involved is given in Figure 2.27. In a typical experiment, the apparatus in Figure 2.27 can be used to measure the internal friction and dynamic modulus of thin, reedlike specimens depicted in Figure 2.28. The reed is a thin, cantilevered beam, and usual dimensions are roughly 4.5 cm long by 0.5 cm wide by 50 μm thick. By applying a harmonic driving force to the tip of the reed using a frequency oscillator, the reed can be made to vibrate in one of its normal modes of vibration, the frequencies of which are given by the following formula: 2

fn=

αn d 2 l 3π

E ρ

n = 1, 2, 3…∞

(2.15)

where fn αn E ρ d l

= Frequency of the nth normal mode of vibration = Mode number associated with the nth normal mode of vibration = Young’s modulus of reed = Reed density = Reed thickness = Reed length

516000 Drive oscillator

Detect circuit

FIGURE 2.27 Vibrating reed experiment for measuring internal friction and dynamic modulus. A cantilevered beam is set into vibration by an oscillatory signal applied at the beam tip. On removing the applied field, the resulting damped vibration is monitored by a second set of electrodes near the base of the sample.

62

Adhesion Measurement Methods: Theory and Practice

Base End view

Reed Side view

FIGURE 2.28 Typical configuration of the reed sample used in the vibration reed experiment of Figure 2.27.

If the dimensions and density of the reed material are accurately known, then Equation (2.15) provides a precise way of determining the modulus of the reed material from the normal mode frequencies. For the experimental setup shown in Figure 2.27, the frequency of the drive oscillator is varied until it comes close to one of the normal mode frequencies. Because the output of the drive oscillator is capacitively coupled to the tip of the reed through two drive electrodes, the reed will start vibrating in the mode corresponding to the applied frequency, as given by Equation (2.15). The drive signal is then turned off, and the frequency of the nowdecaying signal is measured by the detection circuitry, which is capacitively coupled through detect electrodes near the base of the reed. The rate of damping is determined by the internal friction behavior of the reed material and is measured by observing the log decrement, which essentially is calculated from the number of vibration cycles before the amplitude of vibration reaches half of its initial value. A variation of the above experiment can be used to measure the modulus of a thin film deposited on top of an initially bare reed. This technique was used by Lacombe and Greenblatt75 to measure the modulus of 0.5-μm polystyrene films on top of a vitreous silica reed. The basis of this measurement is the fact that a thin coating on top of a bare reed will cause the frequency of the coated reed to be shifted with respect to the bare reed frequency by an amount given by the following formula: 2

⎛ fc⎞ 2t ⎡ 3E f ρ f ⎤ n − ⎥ ⎜ 0 ⎟ =1+ ⎢ d ⎢⎣ E s ρs ⎥⎦ ⎝ f n⎠ where fnc fn0 t d Ef Es

= Vibration frequency of the nth mode of coated reed = Vibration frequency of the nth mode of bare reed = Coating thickness = Bare reed thickness = Modulus of coating = Modulus of bare reed

(2.16)

Overview of Most Common Adhesion Measurement Methods

63

ρf = Coating density ρs = Bare reed density From Equation (2.16), we see that there are two effects causing the frequency shift of the coated reed. The modulus of the coating adds a stiffening term that causes the frequency to increase. The mass of the coating adds extra inertia, which decreases the vibration frequency as given by the negative term in the ratio of the densities. The derivation of Equation (2.16) assumes that the coating is perfectly bonded to the underlying reed substrate. Su et al.73 wondered how Equation (2.16) would be changed if the bonding between the coating and the substrate was not perfect. To investigate, they introduced a coupling parameter γ, which can vary between 0 and 1, with 0 indicating no adhesion and 1 perfect adhesion. In this case, Equation (2.16) becomes 2

2 ⎛ fc⎞ 2t ⎡ 3γ E f ρ f ⎤ n ⎢ = + − ⎥ 1 ⎜ 0⎟ d ⎢ Es ρs ⎦⎥ ⎝ f n⎠ ⎣

(2.17)

All of the quantities in Equation (2.17) are the same as those in Equation (2.16) with the exception of the coupling parameter. Su et al. used Equation (2.17) to investigate the adhesion of NiTi films to silicon substrates. A replot of their data is shown in Figure 2.29. Note that because of imperfect adhesion, the frequency of the coated reed shown in the bottom curve was less than that of the bare reed and the predicted behavior for perfect adhesion (middle and top curves, respectively). If the adhesion were perfect γ = 1, Equation (2.17) would predict that the modulus term on the right-hand side of Equation (2.17) should dominate, giving rise to an increased frequency, whereas the observed decrease makes it clear that imperfect coupling was the cause for the frequency decrease. The value of γ in this case was 0.7. Thus, γ2 is 0.14, therefore reducing the modulus term in Equation (2.17) by nearly an order of magnitude, which accounts for the dominance of the negative density terms. The dynamic modulus test in effect is measuring the efficiency with which bending strains are transferred across the substrate coating interface. Quite interestingly, Su et al. were able to measure γ as a function of coating thickness and annealing treatments, thereby performing a unique set of nondestructive adhesion measurements for the NiTi/Si system.

2.12.2 ADVANTAGES

OF THE

DYNAMIC MODULUS TEST

The main advantages of the dynamic modulus test are its nondestructive nature and the fact that it can be integrated into microelectronic devices as shown in Figure 2.30. Using standard lithography techniques, cantilevered reedlike structures can be fabricated for direct use in testing a variety of material coatings and thin films used in electronic fabrication processes. Further, using micromechanical electronic machine systems technology, the reed structures can be made very small, to the point at which they can be integrated seamlessly into production wafers for purposes of real-time monitoring of adhesion under manufacturing conditions.

64

Adhesion Measurement Methods: Theory and Practice

Square of reed frequency × 106 (Hz2)

5.4 5.3

Perfectly bonded ﬁlm/substrate

5.2

Bare substrate

5.1

Poor ﬁlm/substrate adhesion

5.0 –100

–50

50

100 150 Temperature deg. C

200

FIGURE 2.29 Square of resonant frequency versus temperature for a silicon reed. Middle curve: bare silicon reed. Bottom curve: reed coated with 2-μm thick NiTi film. Top curve: predicted frequency for coated reed according to Equation (2.17) assuming perfect adhesion, γ = 1. The fact that the data for the coated reed are lower than that of the bare substrate indicates poor adhesion for this coating. (Data adapted and replotted from Q. Su, S.Z. Hua, and M. Wuttig, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed., VSP, Utrecht, The Netherlands, 1995, p. 357.)

FIGURE 2.30 Cantilevered silicon reed etched out of a chip. Lithographic methods can be used to miniaturize this structure, making it possible to use it as a diagnostic test site on manufacturing wafers.

A second advantage of the dynamic modulus test arises from the fact that the sample specimen lends itself naturally to internal friction measurements as well as dynamic modulus measurements. Internal friction data can be very useful in monitoring

Overview of Most Common Adhesion Measurement Methods

65

defect structures and impurity migration along grain boundaries in metal films and is also a sensitive way to detect the glass transition and secondary relaxation processes in polymer coatings. Thus, the dynamic modulus test can be a very versatile technique not only for measuring the adhesion on thin films, but also as a potential diagnostic tool for monitoring a wide range of material relaxation phenomena in both metal and insulator films.

2.12.3 DISDVANTAGES

OF THE

DYNAMIC MODULUS TEST

The clearest disadvantage of the dynamic modulus test lies in the limited sample configuration and the difficulty of sample preparation. The reed samples must be fabricated to precise tolerances to yield accurate data. Also, the nondestructive nature of the test makes it difficult to relate to more standard tests. In particular, there is at present no known relationship between the coupling parameter γ and more conventional measures of adhesion strength, such as the critical fracture energy or the critical fracture stress intensity factor.

2.12.4 SUMMARY

AND

RECOMMENDATIONS

At this stage of its development, the dynamic modulus test will be most useful within the research-and-development laboratory for specialized applications of the adhesion of thin films to microelectronic substrate materials such as silicon and vitreous silica. The main advantages of the test stem from its nondestructive nature and its versatile capabilities as a method for evaluating both adhesion strength and the thermalmechanical properties of thin films through internal friction measurements. A significant drawback of the method is that there is as yet no way of relating the measured coupling parameter γ to more conventional adhesion strength quantities such as the critical surface fracture energy. It should be possible to establish an empirical correlation between these quantities through experiments by which the same coating substrate system is tested by both the dynamic modulus test and by one of the more conventional methods discussed in this chapter. This test has significant potential for use in the semiconductor industry, in which the performance of thin metal films is of great concern.

2.13 SURFACE ACOUSTIC WAVES TEST If you bang on the surface of a block of solid material, then you will send a variety of compression and transverse waves propagating throughout the medium. These waves will typically propagate throughout the entire structure, reflecting off of any boundaries or internal discontinuities. The entire field of ultrasonic inspection is based on a much more controlled version of this primitive experiment. Piezoelectric coupling or another controllable method is used to send very high frequency waves through the structure under carefully controlled conditions. For purposes of adhesion testing, there is a special class of waves that propagate only on the surface of the material; these are known as surface acoustic waves (SAWs). These waves can be induced by a number of methods, including piezoelectric coupling, and are sensitive to the surface conditions of the material.

66

Adhesion Measurement Methods: Theory and Practice

FIGURE 2.31 Schematic of a typical surface acoustic wave (SAW) experiment. The input transducer sends out a surface wave that travels through the coating/substrate interface before it is received by the detection transducer. Changes in the amplitude and velocity of the surface wave on passing through the coating/substrate interface can reveal useful information concerning coating/substrate interactions.

Figure 2.31 illustrates an experiment in which a SAW is generated by a transducer, made to propagate along an interface between a coating and substrate and is subsequently detected by another transducer on the opposite side of the coating. As the surface wave travels through the interface between the coating and the substrate, both its velocity and its amplitude are affected. The shift in velocity gives rise to dispersion effects that are detectable when several different frequencies are present, as would be the case for a wave pulse. Amplitude effects can be used to detect loss mechanisms that might be indicative of poor coupling between the coating and substrate. The SAW method was reviewed by Ollendorf et al.,76 who studied TiN films on steel and compared the SAW method to several other more standard techniques, including the scratch test and the four-point bend test. These investigators used the SAW method to determine the modulus of the TiN coatings and found the value so determined correlated well with adhesion measurements on the same films as determined by the four-point bend and scratch tests. The basic effect is quite similar to the dynamic modulus test. As was seen in the dynamic modulus test, propagation of the SAW through the interface depends on how efficiently transverse strains are transmitted from the substrate to the coating. Voids, regions of loose packing, and other surface imperfections clearly interfere with efficient transmission of strain at the interface and thus affect the apparent modulus measurement of the film as inferred by the SAW method. Because these defects also reduce the film adhesion, it is clear why there should be a correlation between the modulus measurement and the film adhesion. An extensive review of the use of SAWs to study the performance of adhesive joints was given by Rokhlin.77 In another application of the SAW method, Galipeau et al.78 studied the adhesion of polyimide films on quartz substrates. Their basic setup is shown schematically in Figure 2.32. Because the substrate used is quartz, which is a natural piezoelectric material, the input and detection transducers consist simply of interdigitated lines that are patterned on the substrate using standard photolithographic methods. An oscillating input applied to the electrodes of the transducer couples directly into the substrate, setting up an analogous mechanical surface wave. This wave travels as an

Overview of Most Common Adhesion Measurement Methods

67

FIGURE 2.32 Surface acoustic wave experiment for polyimide on quartz. Because quartz is a natural piezoelectric material, transducers can simply be fabricated by evaporating metal lines onto the quartz as shown. Electrical signals in the metal lines are then directly converted into mechanical vibrations in the quartz. In the single delay line experiment using one substrate, the propagated surface wave is compared to a reference signal generated by the input driver. The dual delay line experiment employs two samples in which everything is the same except for the preparation of the coating/substrate interface. The two signals are compared at the detection transducers.

SAW into the coating/substrate interface and out the other end, where it is detected by an identical transducer, which converts the mechanical SAW back into an electrical signal. Note that this differs from the method used by Ollendorf et al. in that these authors used a laser pulse to generate a pulsed wave with many harmonics, which would then show dispersion effects going through the coating/substrate interface. The setup in Figure 2.32 will generate a single harmonic that will not show dispersion. The velocity of this wave will however be affected by passing through the interface, and this is detected in one of two ways. In the first method, the input signal is compared to that of the detector transducer in what is called a single delay line experiment. The second method uses two delay lines to compare the signals from two coatings prepared differently and therefore with different levels of adhesion. Figure 2.33 illustrates some sample data replotted from results presented by Galipeau et al. The curve shows the phase delay incurred when the surface wave passed through the interface between a polyimide film and the quartz substrate as a function of ambient humidity. The negative phase delay is indicative of slowing of the wave. Thus, as the humidity increases, it seems to have a softening effect on the interface, slowing the wave more and more as the relative humidity increases. Because it is well known from standard adhesion tests that high humidity reduces the adhesion of polyimide, we can assume that the apparent softening of the interface region is also partly responsible for this effect. One can perform the same type of

68

Adhesion Measurement Methods: Theory and Practice

FIGURE 2.33 Typical data showing the effect of relative humidity on the passage of a surface acoustic wave through a polyimide/quartz interface. The negative phase delay is indicative of slowing of the wave, indicating that the moisture accumulated at the interface is having a “softening” effect, thereby slowing the signal.

experiment using the dual delay line method in which two polyimide films, one with an adhesion promoter such as a silane material and one without, are compared. The dual delay line test clearly shows that the SAW travels faster through the coating with the adhesion promoter, thus accounting for the higher adhesion observed when the adhesion promoter is present.

2.13.1 ADVANTAGES

OF THE

SURFACE ACOUSTIC WAVES TEST

The key advantages of the SAW method lie in its nondestructive character and the possibility that it can be applied in a manufacturing environment for online quality control purposes. In addition, the SAW method can be calibrated against standard destructive adhesion measurement experiments to provide quantitative results related to surface fracture energies.

2.13.2 DISADVANTAGES

OF THE

SURFACE ACOUSTIC WAVES TEST

The main disadvantage of the SAW approach is that it does not yield direct adhesion strength data and must be calibrated against one of the more standard tests. In addition, sample preparation is an important problem with this method because it is not always a trivial matter to couple the input and output transducers to the substrate. Unlike the quartz substrates, most materials do not have natural piezoelectric behavior; therefore, some other method of coupling the electrical signal to

Overview of Most Common Adhesion Measurement Methods

69

the substrate must be devised. Many times, this involves the use of a coupling fluid, which works but also complicates the experiment.

2.13.3 SUMMARY

AND

RECOMMENDATIONS

From the discussion, it is fairly clear that the SAW adhesion measurement has its greatest potential for use as a real-time quality control tool. Using the laser pulse method to generate the surface waves coupled with interferometry as a detector, this method could be used to inspect coatings rapidly and without contact.

Notes 1. For further details on this most fascinating story, a first-rate account is given in “Stern and Gerlach: How a Bad Cigar Helped Reorient Atomic Physics,” B. Friedrich and D. Herschbach, Physics Today, 53 (December 2003). 2. “Adhesion Measurement of Films and Coatings: A Commentary,” K.L. Mittal, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 1. 3. “An Experimental Partitioning of the Mechanical Energy Expended During Peel Testing,” R.J. Farris and J.L. Goldfarb, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 265. 4. “Peel Adhesion and Pressure Sensitive Tapes,” D. Satas and F. Egan, Adhesives Age, 22 (August 1966). 5. “Failure Mechanisms in Peeling of Pressure-Sensitive Adhesive Tape,” D.W. Aubrey, G.N. Welding, and T. Wong, Journal of Applied Polymer Science, 13, 2193 (1969). 6. “Quantifying the Tape Adhesion Test,” G.V. Calder, F.C. Hansen, and A. Parra, in Adhesion Aspects of Polymeric Coatings, K.L. Mittal, Ed. (Plenum Press, New York, 1983), p. 569. 7. Ibid., p. 570. 8. “Salt Bath Test for Assessing the Adhesion of Silver to Poly(ethylene terephthalate) Web,” J.M. Grace, V. Botticelle, D. R. Freeman, W. Kosel, and R.G. Spahn, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 423. 9. “Pull-off Test, an Internationally Standardized Method for Adhesion Testing — Assessment of the Relevance of Test Results,” J. Sickfeld, in Adhesion Aspects of Polymeric Coatings, K.L. Mittal, Ed. (Plenum Press, New York, 1983), p. 543. 10. “Analysis of Pull Tests for Determining the Effects of Ion Implantation on the Adhesion of Iron Films to Sapphire Substrates,” J.E. Pawel and C.J. McHargue, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 323. 11. “Measurement of the Adhesion of Diamond Films on Tungsten and Correlations with Processing Parameters,” M. Alam, D.E. Peebles, and J.A. Ohlhausen, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 331. 12. “Indentation-Debonding Test for Adhered Thin Polymer Layers,” P.A. Engel and G.C. Pedroza, in Adhesion Aspects of Polymeric Coatings, K.L. Mittal, Ed. (Plenum Press, New York, 1983), p. 583. 13. Ibid., p. 588.

70

Adhesion Measurement Methods: Theory and Practice 14. “Mechanics of the Indentation Test and Its Use to Assess the Adhesion of Polymeric Coatings,” R. Jayachandran, M.C. Boyce, and A.S. Argon, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 189. 15. “Observations and Simple Fracture Mechanics Analysis of Indentation Fracture Delamination of TiN Films on Silicon,” E.R. Weppelmann, X.-Z. Hu, and M.V. Swain, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 217. 16. “Hardness and Adhesion of Filmed Structures as Determined by the Scratch Technique,” J. Ahn, K.L. Mittal and R.H. MacQueen, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 134. 17. “Some Factors Influencing the Adhesion of Films Produced by Vacuum Evaporation,” O.S. Heavens, Journal of the Physics of Radium, 11, 355 (1950). 18. “L’epitaxie dans les Lames Polycrystallines,” O.S. Heavens and L.E. Collins, Journal of the Physics of Radium, 13, 658 (1952). 19. “Measurement of Adhesion of Thin Film,” P. Benjamin and C. Weaver, Proceedings of the Royal Society (London), 254A, 163 (1960). 20. “The Stylus or Scratch Method for Thin Film Adhesion Measurement: Some Observations and Comments,” D.W. Butler, C.J.H. Stoddard, and P.R. Stuart, Journal of Physics (D): Applied Physics, 3, 887 (1970). 21. Note 16, p. 150. 22. “Threshold Adhesion Failure: An Approach to Aluminum Thin-Film Adhesion Measurement Using the Stylus Method,” J. Oroshnik and W.K. Croll, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 158. 23. “Scratch Indentation, a Simple Adhesion Test Method for Thin Films on Polymeric Supports,” G.D. Vaughn, B.G. Frushour, and W.C. Dale, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 127. 24. “Micro-scratch Test for Adhesion Evaluation of Thin Films,” V.K. Sarin, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 175. 25. “Can the Scratch Adhesion Test Ever Be Quantitative?” S.J. Bull, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 107. 26. “Scratch Test Failure Modes and Performance of Organic Coatings for Marine Applications,” S.J. Bull, K. Horvathova, L.P. Gilbert, D. Mitchell, R.I. Davidson, and J.R. White, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 175. 27. “Measurement of Adhesion by a Blister Method,” H. Dannenberg, Journal of Applied Polymer Science, 5, 125 (1961). 28. “A Study of the Fracture Efficiency Parameter of Blister Tests for Films and Coatings,” Y.-H. Lai and D.A. Dillard, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 231. 29. “Analysis of Critical Debonding Pressures of Stressed Thin Films in the Blister Test,” M.G. Allen and S.D. Senturia, Journal of Adhesion, 25, 303 (1988). 30. M.G. Allen and S.D. Senturia, Journal of Adhesion, 29, 219 (1989). 31. M.J. Napolitano, A. Chudnovsky, and A. Moet, Proceedings of ACS, Division of Polymer Material Science and Engineering, 57, 755 (1987).

Overview of Most Common Adhesion Measurement Methods

71

32. “The Constrained Blister Test for the Energy of Interfacial Adhesion,” M.J. Napolitano, A. Chudnovsky, and A. Moet, Journal of Adhesion Science and Technology, 2, 311 (1988). 33. “The Constrained Blister — A Nearly Constant Strain Energy Release Rate Test for Adhesives,” Y.S. Chang, Y.H. Lai, and D.A. Dillard, Journal of Adhesion, 27, 197 (1989). 34. “An Elementary Plate Theory Prediction for Strain Energy Release Rate of the Constrained Blister Test,” Y.H. Lai and D.A. Dillard, Journal of Adhesion, 31, 177 (1990). 35. “Numerical Analysis of the Constrained Blister Test,” Y.H. Lai and D.A. Dillard, Journal of Adhesion, 33, 63 (1990). 36. “Adhesion (Fracture Energy) of Electropolymerized Poly(n-octyl maleimide-co-styrene) on Copper Substrates Using a Constrained Blister Test,” J.-L. Liang, J.P. Bell, and A. Mehta, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 249. 37. Note 33. 38. Note 29, p. 311. 39. “The Three Point Bend Test for Adhesive Joints,” N.T. McDevitt and W.L. Braun, in Adhesive Joints: Formation, Characteristics and Testing, K.L. Mittal, Ed. (Plenum Press, New York, 1984), p. 381. 40. “Practical Adhesion Measurement in Adhering Systems: A Phase Boundary Sensitive Test,” A.A. Roche, M.J. Romand, and F. Sidoroff, in Adhesive Joints: Formation, Characteristics and Testing, K.L. Mittal, Ed. (Plenum Press, New York, 1984), p. 19. 41. “Interface Adhesion: Measurement and Analysis,” A.G. Evans, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 1. 42. “Use of Fracture Mechanics Concepts in Testing of Film Adhesion,” W.D. Bascom, P.F. Becher, J.L. Bitner, and J.S. Murday, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 63. 43. “Fracture Design Criteria for Structural Adhesive Bonding — Promise and Problems,” W.D. Bascom, R.L. Cottington, and C.O. Timmons, Naval Engineers Journal, 73 (August 1976). 44. “Mixed Mode Cracking in Layered Materials,” J.W. Hutchinson and Z. Suo, Advances in Applied Mechanics, 29, 63 (1991). 45. “Closure and Repropagation of Healed Cracks in Silicate Glass,” T.A. Michalske and E.R. Fuller Jr., Journal of the American Ceramics Society, 68, 586 (1985). 46. Note 41, p. 3. 47. “Combined Mode Fracture via the Cracked Brazilian Disk Test,” C. Atkinson, R.E. Smelser, and J. Sanchez, International Journal of Fracture, 18, 279 (1982). 48. “Experimental Determination of Interfacial Toughness Using Brazil-Nut-Sandwich,” J.S. Wang and Z. Suo, Acta Met., 38, 1279 (1990). 49. Note 44, p. 120. 50. “Fracture Toughness Curves for Epoxy Molding Compound/Leadframe Interfaces,” H.-Y. Lee, Journal of Adhesion Science and Technology, 16, 565 (2002). 51. “Adhesion and Adhesives Technology,” A.V. Pocius (Carl Hanser Verlag, Munich, 2002), p. 186. 52. “The Role of Interfacial Interactions and Loss Function of Model Adhesives on Their Adhesion to Glass,” A Sharif, N. Mohammadi, M. Nekoomanesh, and Y. Jahani, Journal of Adhesion Science and Technology, 16, 33 (2002).

72

Adhesion Measurement Methods: Theory and Practice 53. “Plasma Sprayed Coatings as Surface Treatments of Aluminum and Titanium Adherends,” G.D. Davis, P.L. Whisnant, D.K. Shaffer, G.B. Groff, and J.D. Venables, Journal of Adhesion Science and Technology, 9, 527 (1995). 54. “Effectiveness of Water Borne Primers for Structural Adhesive Bonding of Aluminum and Aluminum-Lithium Surfaces,” K.L. Meyler and J.A. Brescia, Journal of Adhesion Science and Technology, 9, 81 (1995). 55. J. Cognard, Journal of Adhesion, 22, 97 (1987). 56. M.F. Kauninen, International Journal of Fracture, 9, 83 (1973). 57. H.R. Brown, Journal of Material Science, 25, 2791 (1990). 58. “Strength of Polystyrene Poly(Methyl Methacrylate) Interfaces,” K.L. Foster and R.P. Wool, Macromolecules, 24(6), 1397 (1991). 59. “On the Non-linear Elastic Stresses in an Adhesively Bonded T-Joint With Double Support,” M.K. Apalak, Journal of Adhesion Science and Technology, 16, 459 (2002). 60. “A Simple Film Adhesion Comparator,” D.W. Butler, Journal of Physics (E): Science of Instrumentation, 3, 979 (1970). 61. “Measurement of the Adhesion of Silver Films to Glass Substrates,” A. Kikuchi, S. Baba, and A. Kinbara, Thin Solid Films, 124, 343 (1985). 62. “A Self-Delamination Method of Measuring the Surface Energy of Adhesion of Coatings,” R.J. Farris and C.L. Bauer, Journal of Adhesion, 26, 293 (1988). 63. “Measurement of Interfacial Fracture Energy in Microelectronic Multifilm Applications,” J.C. Hay, E. Lininger, and X.H. Liu, in Adhesion Measurement of films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 205. 64. The relevant references are: “A New Procedure for Measuring the Decohesion Energy for Thin Ductile Films on Substrates,” A. Bagchi, G.E. Lucas, Z. Suo, and A.G. Evans, J. Mater. Res., 9(7), 1734 (1994); “Thin Film Decohesion and its Measurement,” A. Bagchi and A.G. Evans, Mat. Res. Soc. Symp. Proc., 383, 183 (1995); “The Mechanics and Physics of Thin Film Decohesion and its Measurement,” A. Bagchi and A.G. Evans, Interface Science, 3, 169 (1996). 65. “Interface Adhesion: Measurement and Analysis,” A.G. Evans, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 9. 66. “Measurement of Film-Substrate Bond Strength by Laser Spallation,” J.L. Vossen, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 122. 67. “Measurement of Interfacial Bond Strength by Laser Spallation,” A.W. Stephens and J.L. Vossen, Journal of Vacuum Science and Technology, 13, 38 (1976). 68. “Recent Developments in the Laser Spallation Technique to Measure the Interface Strength and Its Relationship to Interface Toughness With Applications to Metal/Ceramic, Ceramic/Ceramic and Ceramic/Polymer Interfaces,” V. Gupta, J. Yuan, and A. Pronin, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 367. 69. Ibid., p. 395. 70. “Effect of Primer Curing Conditions on Basecoat-Primer Adhesion — A LIDS Study,” J.S. Meth, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 255. 71. “Electromagnetic Tensile Adhesion Test Method,” S. Krongelb, in Adhesion Measurement of Thin Films, Thick Films and Bulk Coatings, ASTM STP 640, K.L. Mittal, Ed. (American Society for Testing and Materials, West Conshohocken, PA, 1978), p. 107.

Overview of Most Common Adhesion Measurement Methods

73

72. “Adhesion of Aluminum Films on Polyimide by the Electromagnetic Tensile Test,” B.P. Baranski and J.H. Nevin, Journal of Electronic Material, 16, 39 (1987). 73. “Nondestructive Dynamic Evaluation of Thin NiTi Film Adhesion,” Q. Su, S.Z. Hua, and M. Wuttig, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 357. 74. “Vibrating Reed Internal Friction Apparatus for Films and Foils,” B.S. Berry and W.C. Pritchet, IBM Journal of Research and Development, 19, 334 (1975). 75. “Mechanical Properties of Thin Polyimide Films,” R.H. Lacombe and J. Greenblatt, in Polyimides, Vol. 2, K.L. Mittal, Ed. (Plenum, New York, 1984), p. 647 76. “Testing the Adhesion of Hard Coatings Including the Non-destructive Technique of Surface Acoustic Waves,” H. Ollendorf, T. Schülke, and D. Schneider, in Adhesion Measurement of Films and Coatings, Vol. 2, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 2001), p. 49. 77. “Adhesive Joint Characterization by Ultrasonic Surface and Interface Waves,” S.I. Rokhlin, in Adhesive Joints: Formation, Characterization and Testing, K.L. Mittal, Ed. (Plenum Press, New York, 1984), p. 307. 78. “Adhesion Studies of Polyimide Films Using a Surface Acoustic Wave Sensor,” D.W. Galipeau, J.F. Vetelino, and C. Feger, in Adhesion Measurement of Films and Coatings, K.L. Mittal, Ed. (VSP, Utrecht, The Netherlands, 1995), p. 411.

3

Theoretical Foundations of Quantitative Adhesion Measurement Methods

Since the subject became popular with mathematicians about 150 years ago and I am afraid that a really formidable number of unreadable, incomprehensible books have been written about elasticity, and generations of students have endured agonies of boredom in lectures about materials and structures. In my opinion the mystique and mumbo-jumbo is overdone and often beside the point. It is true that the higher flights of elasticity are mathematical and very difficult—but then this sort of theory is probably only rarely used by successful engineering designers. What we find difficult about mathematics is the symbolic presentation of the subject by pedagogues with a taste for dogma, sadism and incomprehensible squiggles. J. E. Gordon, Structures or Why Things Don’t Fall Down

3.1 INTRODUCTION TO CONTINUUM THEORY Because every method for performing an adhesion measurement involves applying a force or load of some type to the coating/substrate system, considerations of stress, strain, and deformation must inevitably be confronted. Notwithstanding the comments of Prof. Gordon quoted above, this chapter attempts to provide a brief introduction to the subject of the continuum theory of solids and to the greatest extent possible tries to avoid technical jargon while at the same time bringing into sharper focus the essential mechanics that need to be understood to grasp the role stress plays in adhesion measurement. The main focus is on developing a sufficient level of understanding of the fundamental theory so that the reader will be able to follow subsequent analytical developments, have sufficient background to confront the technical literature, and be able to perform simple but useful calculations in a competent manner. The development of necessity will be limited in scope, but a number of references to the more lucid and useful literature are provided to give ample means for the interested reader to delve deeper into the subject. Continuum theory is a subject with foundations that were essentially completed by the end of the 19th century by such famous physicists and mathematicians as Navier, Poisson, Green, Cauchy, Hooke, Young, and a number of others. By the early 20th century, the fashion in physics had shifted dramatically to the thenemerging theory of quantum mechanics, which was required to understand the behavior of matter at the atomic level. Continuum theory was essentially relegated to the engineers and a small coterie of mathematicians who found significant challenges

75

76

Adhesion Measurement Methods: Theory and Practice

in the mathematics of the subject. Indeed, by the time I was carrying out my undergraduate and graduate studies in physics, the subject of the continuum theory of matter had all but dropped out of the curriculum in deference to more current topics, such as particle mechanics, electromagnetism, optics, and of course quantum theory. Part of the problem stems from the fact that continuum theory was viewed as only an approximation to the reality of matter and was in fact clearly wrong at the atomic level. However, even though it may only be an approximate description of material behavior it proved to be an extremely useful one and is in fact indispensable as a modern engineering design tool for everything from safety pins to the space shuttle. For present purposes, it is assumed that matter at the scale of tenths of micrometers to tens of meters is accurately described by the field equations of continuum theory. The presentation is carried out in four parts. Sections 3.1.1 through 3.1.3 define the concept of stress in a solid. Stress is something of a mystery to most people, especially those who are more comfortable thinking about forces. A force is a vector quantity requiring three components to be given for a complete specification, one for each of the three mutually orthogonal directions in space. Stress, however, is a tensor quantity requiring in general nine components for a full description. Why all the complication? Why mess around with something three times more complicated than simple forces that most people can understand and that should, in principle, be sufficient to describe the loads applied to any solid? The discussion in Part 1 will try to motivate and explain the rationale behind the concept of stress. Section 3.1.4 introduces the concepts of deformation and strain. This is a relatively straightforward development because nearly everyone has a fairly intuitive sense of deformation. If you apply a load to an object, it will deform by bending, twisting, or stretching in some manner. However, there are a number of subtle and nonintuitive aspects to this subject that need careful attention and are appropriately highlighted. Section 3.1.5 introduces constitutive relations. At this point, all of the kinematical relations for defining the stresses and deformations in solids are in place but a further essential ingredient is missing, what is called the constitutive relations. The basic role of the constitutive relations is to connect the stresses to the strains. They describe a fundamental material property of the solid under investigation. Different materials require different constitutive relations. Without a constitutive relation, you really do not know the material with which you are dealing, whether it is a piece of metal, a slab of glass, or an item of ceramic cookware. The simplest such relation is Hooke’s law for elastic solids, which in essence says that the stress is linearly proportional to the strain, with the constant of proportionality the elastic modulus, often referred to as Young’s modulus. All of this is covered in detail in Section 3.1.5. Finally, in Section 3.2 and following, all of these ingredients are put together to form what are known as the field equations of thermoelasticity. As an extra benefit, Fourier’s equation of heat transfer is thrown into the pot so that problems of thermal stress loading can be addressed. These are very important loads for many problems. The final confection of field equations forms one of the crowning achievements of 19th century theoretical physics, and these equations are rivaled only by Maxwell’s equations, which form the foundation of electromagnetic theory. Maxwell’s theory is truly phenomenal. It is valid over spatial and timescales of at least 15 orders of

Theoretical Foundations of Quantitative Adhesion Measurement Methods

77

magnitude and was relativistically correct at its inception. The only correction that had to be made was to allow for the quantum nature of matter. This gave rise to quantum electrodynamics as developed by Feynman, Schwinger, and Tomonaga. The field equations of thermoelasticity are not relativistically correct or valid at the atomic level. However, for a vast range of practical problems, they are as valid in the 21st century as they were in the 19th century. The errors committed by ignoring relativistic and quantum mechanical effects are well below the sensitivity of most practical measurements. The largest source of error in fact arises from not having truly correct constitutive relations for the material substances under investigation. The general field equations of thermoelasticity are, to put it mildly, exceedingly difficult to solve by paper-and-pencil methods. The common practice in engineering applications is to resort to powerful numerical methods such as finite element analysis or boundary element analysis. Given the enormous computational power of modern workstations, these methods are highly effective at generating useful numerical solutions to the field equations. Surprisingly, however, there are a number of nontrivial special cases that can be solved “on the back of an envelope.” These cases are discussed in some detail as they provide a number of useful computational formulae for estimating stresses in situations of practical interest and supply a handy set of tools for the user.

3.1.1 CONCEPT

OF

STRESS

IN

SOLIDS

As pointed out, nine numbers are required in general to specify the state of stress at a point in a solid. In most cases, certain symmetries apply, and only six numbers are needed, but this is still twice as many as are required to determine a force vector, which should amount to the same thing. The problem arises because, in a continuous medium such as a solid, the relevant quantity is not the force vector alone but the force acting on some element of area. The simplest example is the pressure in a pneumatic tire, which is always specified in pounds per square inch (psi) or Newtons per square meter (Pascal or Pa). The point is that, when speaking of a continuous lump of matter, forces are generally applied to some element of area that gives rise to the concept of a stress that is a force per unit area. The pressure in a tire is a very special stress state known as a hydrostatic stress. It is the same in all directions and thus specified by only one number. This comes about from the fluid nature of the compressed gas in the tire, which cannot support anything but a hydrostatic load. Fluids in general cannot support either tensile or shear loads and thus must be confined to some type of sealed container in which they can be loaded hydrostatically. Solids, on the other hand, support both types of loads, and the state of stress in a solid is sensitive to how it is supported and the details of the applied force field that will typically act on the surface. For large objects, there is also what is called body forces, which strictly speaking act only on a specific point in the body. Gravitational loading is the most important example. Each and every element of a solid has a mass, which is computed as the density times the volume of the element. Each such mass element is under a force loading because of the Earth‘s gravitational field. This gravitational loading will give rise to stresses in the solid at the surfaces where it is supported. Thus, again forces per unit area must be considered.

78

Adhesion Measurement Methods: Theory and Practice

dF n dA

z y e3

e2 e1

x

FIGURE 3.1 An element of surface dA subjected to a localized force dF. The complete description of dA requires specification of the unit normal vector n, which defines the orientation of dA in three dimensions. The vector element dA is given by the product (dA)n.

Figure 3.1 depicts a hypothetical solid surface with a small element of area shown under the influence of some applied force vector dF. The area element also has a vector character because it is characterized by both a magnitude dA and a unit vector n that is perpendicular to the tangent plane that contains the area element. The vector n is commonly referred to as the unit normal that characterizes the direction of the area element dA. Although one does not normally associate a direction with the notion of area, it is clearly important in continuum theory because every surface in three-dimensional space is oriented in some way, and specifying the unit normal is a precise and convenient way of describing this property. The force dF arises because of the action of the material in the immediate neighborhood of the area element dA. It can be of an intrinsic nature, such as forces arising from material defects such as voids, inclusions, or dislocations. Alternately, it can arise from loads applied to the surface of the material that are transmitted to the interior in a chainlike fashion from one volume element to another. In general, the genesis of the local force vector is quite complex and not obtainable by simple means. Fortunately, for present purposes only the existence of this force is required. At equilibrium, an equal and opposite force −dF operates on the other side of the area element dA. Together, these forces create a state of stress acting on dA. Because each separate element of surface will require a different unit normal, it is clear that to come up with a general definition of stress, which is force per unit area, two vector quantities will be involved; this is the reason behind the tensor nature of the stress field. The area element vector is defined in the obvious way as follows: dA = dA n

(3.1)

More useful for our purposes, however, is the inverse area element, which also has an obvious definition: dA −1 =

n dA

(3.2)

Theoretical Foundations of Quantitative Adhesion Measurement Methods

79

The vector dA−1 represents the surface element by assigning it a direction n and a magnitude (1/dA). The stress acting at the area element dA can now be defined in a straightforward manner: T = d FdA −1

(3.3)

Equation (3.3) now fits the bill for the required tensor quantity that has the magnitude of a force per unit area but points in two directions at the same time. One direction is that of dF; the other is the direction of the area unit normal n. Thus, Equation (3.3) reads that T is the stress at the location of the area element dA caused by the vector force dF acting on the area element dA−1 pointing in the direction n. T is a dyadic quantity because it is the composition of two vectors that generally act in separate directions and thus exist in a higher dimensional space than simple vectors. Tensors and dyadics are roughly mathematical equivalents and are often used interchangeably as a matter of convenience. One can imagine even more complex quantities such as triadics, tetradics, and so on that can act in three or more directions. Refer to Appendix A on mathematical foundations for a more detailed treatment of this subject. A more useful description of T is provided by referring both dF and dA−1 to some appropriate Cartesian coordinate system as depicted in Figure 3.1: dF = dF1e1 + dF2e 2 + dF3e3 (3.4)

⎛ e e e ⎞ dA −1 = ⎜ 1 + 2 + 3 ⎟ ⎝ dA1 dA2 dA3 ⎠

The area elements dA1, dA2, and dA3 are projections of the element dA onto the coordinate planes perpendicular to the respective unit vectors e1, e2, and e3 depicted in Figure 3.1. The stress tensor T now becomes:

(

)(

T = dF dA −1 = dF1e1 + dF2e 2 + dF3e3 dA1−1e1 + dA2−1e 2 + dA3−1e3

)

If we carry out all the implied multiplications and collect terms appropriately, we see that the stress tensor can be written as dF1 e e + dF 2 e e + dF 3 e e 1 1 2 1 3 1 dA1 dA1 dA1 T = dF1 e1e 2 + dF 2 e 2 e 2 + dF 3 e 3e 2 dA2 dA2 dA2 dF1 e e + dF 2 e e + dF 3 e e 2 3 3 3 1 3 dA3 dA3 dA3

(3.5)

80

Adhesion Measurement Methods: Theory and Practice

Following standard convention, we write the stress tensor T in terms of three traction vectors T1, T2, and T3: T = e1T1 + e2T2 + e3T3

(3.6)

where dF1 e + dF 2 e + dF 3 e T1 = 1 2 3 dA1 dA1 dA1 dF1 e + dF 2 e + dF 3 e T2 = 1 2 3 dA2 dA2 dA2 dF1 e + dF 2 e + dF 3 e T3 = 3 1 2 dA3 dA3 dA3 The main purpose in defining the traction vectors is that they are the most convenient quantities for defining surface loads on solid bodies. They are convenient vector quantities defined directly in terms of the applied forces while at the same time are genuine stress quantities with the dimension of force per unit area. Thus, if one solid body impinges on another, there is always some finite area of contact involved, and the applied load is distributed over this area. Therefore, the actual load is a force per some area or a traction vector as defined above. The equations can be greatly simplified by introducing the standard notation for the components of the stress tensor σij: T1 = σ11e1 + σ12e 2 + σ13e 3 T2 = σ 21e1 + σ 22e 2 + σ 23e 3

(3.7)

T3 = σ 31e1 + σ 32e 2 + σ 33e 3 By comparing Equations (3.6) and (3.7), it is immediately clear what the definitions of the stress components σij are. For example σ11 is the stress generated by dF1 acting on area element dA1, which points in the direction e1. Likewise, σ12 is the stress generated by dF2 acting on area element dA1 pointing in the direction e2. Note that σ12 is a shear component because the force acts perpendicular to the area unit normal as opposed to σ11, which is called a tensile component because it acts parallel to the area unit normal. Similar observations hold for the remaining components. Working with quantities such as the stress tensor is awkward, to say the least. Because of this, a number of different notations have been invented to try to make the situation more manageable. Those who like matrices have come up with the obvious matrix definition: ⎡ σ11 ⎢ σ = ⎢ σ 21 ⎢ σ 31 ⎣

σ12 σ 22 σ 32

σ13 ⎤ ⎥ σ 23 ⎥ σ 33 ⎥⎦

(3.8)

Theoretical Foundations of Quantitative Adhesion Measurement Methods

81

This notation is handy when dealing with matrix operations on vectors and is also easily programmed on computers. A second approach is to use what is called indicial notation, by which one always deals with the tensor components as indexed scalar quantities. This notation has a number of advantages and is a favorite of the theoreticians. Thus, the stress tensor is simply referred to as σij where it is understood that the indices i and j run over the values 1, 2, and 3. The main advantage of the indicial notation is the easy ability to generalize and expand the definitions to tensor quantities of higher dimension and rank. Thus, the indices can run from 1 to 4 if the problem requires working in a four-dimensional space time as is the case in relativity theory. In addition, higher rank quantities are easily generated by simply adding more indices. In elasticity theory, the elastic constants of the most general class of crystals are specified by the fourth-order elasticity tensor Cijkl, which has 81 elements. The matrix version of this quantity is most useful simply to display the elements on a page as opposed to performing formal manipulations. Einstein’s field equations from his general relativity theory involve tensor quantities that are truly extravagant to the point of being mind boggling and have no matrix counterparts. For the purposes of this section, a hybrid vector/tensor notation is adopted to provide a compact and general notation for introducing the field equations of elasticity. Refer to Appendix A for a more detailed treatment of vector and tensor notation and manipulation. The primary thrust of this discussion, however, is to develop the basic field equations of continuum theory in a reasonably transparent manner and show that they arise in a straightforward way from the simpler equations of Newtonian particle mechanics. To this point, we have established that the main quantities of interest are the components of the stress tensor as opposed to the simpler vector forces that act on the body in question. This arises because the vector forces inevitably act on surface elements when a solid is considered as a continuum as opposed to a collection of point particles; as Equation (3.3) demonstrates, this leads to the formation of a higher dyadic quantity called the stress tensor. The usefulness of the stress tensor formulation becomes apparent when the stress on some arbitrary surface is required and not just the special orthogonal surfaces of the coordinate planes. The stress on any surface whatever can be related to the components of the stress tensor given in some fixed reference system in the following manner. Figure 3.2 shows the traction vector Tn acting on some arbitrary area element dA with surface normal vector n that is not parallel to any of the surfaces dA1, dA2, or dA3 associated with the coordinate planes and therefore must intersect each in some fashion, forming a tetrahedron figure shown in Figure 3.2. Equilibrium requires that the vector sum of the forces acting on all the faces of the tetrahedron should add to zero; thus, Fn − F1 − F2 − F3 = 0

(3.9)

Using Equations (3.6) and (3.7), Equation (3.9) can be satisfied on a componentby-component basis by collecting all terms acting in the direction e1 and setting them to zero and proceeding similarly for the directions e2 and e3. The result is

82

Adhesion Measurement Methods: Theory and Practice

n.e3 = cos(θ) e3 e3

hn

θ

n

θ Tn

h3

T1

n T2

dA dA3 e2 b

e1 T3

FIGURE 3.2 A surface element within a solid (dA) having some arbitrary orientation n with respect to a fixed coordinate system characterized by the unit vectors e1, e2, and e3. The area element dA is subjected to a surface traction Tn that is not parallel to the surface normal vector n. T1, T2, and T3 are the components of Tn along the coordinate axes. The shaded area labeled dA3 is the projection of dA onto the e1, e2 plane and has unit normal e3. The inset shows that the element dA3 is related to dA by the simple formula dA3 = dAn.e3. A similar relation holds for the remaining projections dA1 and dA2 (not shown).

(T ) dA − σ (T ) dA − σ (T ) dA − σ

dA1 − σ 21dA2 − σ 31dA3 = 0

n 1

11

n 2

12

n 3

13

dA1 − σ 22dA2 − σ 32dA3 = 0

(3.10)

dA1 − σ 23dA2 − σ 33dA3 = 0

Equations (3.10) can be greatly simplified by noting that the area elements dA1, dA2, and dA3 are just the projections of the area element dA onto the main coordinate planes. This fact is demonstrated by the inset in Figure 3.2 for the case of area element dA3. The primary result is the following useful set of relations: dA1 = dA(n.e1 ) = dA cos θ1 = n1dA dA2 = dA(n.e 2 ) = dA cos θ2 = n2dA

(3.11)

dA3 = dA(n.e 3 ) = dA cos θ3 = n3dA where n1 = cos θ1, n2 = cos θ2, and n3 = cos θ3 are the common direction cosines for the normal vector n. By substituting Equations (3.11) into Equations (3.10), the common factor dA can be seen to drop out, and with some obvious rearrangement, the following result is achieved:

Theoretical Foundations of Quantitative Adhesion Measurement Methods

(T ) (T ) (T )

n 1

= σ11n1 + σ 21n2 + σ 31n3

n 2

= σ12n1 + σ 22n2 + σ 32n3

n 3

= σ13n1 + σ 23n2 + σ 33n3

83

(3.12)

These equations have a very convenient matrix representation: ⎡ σ11 ⎡ Tn , Tn , Tn ⎤ = ⎡ n1 , n2 , n3 ⎤ ⎢ σ 21 ⎣ ⎦⎢ 1 2 3⎦ ⎣ ⎢ σ 31 ⎣

( ) ( ) ( )

σ12 σ 22 σ 32

σ13 ⎤ ⎥ σ 23 ⎥ σ 33 ⎥⎦

(3.13)

Using compact matrix notation, Equation (3.13) can be written very succinctly as T = n⋅σ. Equation (3.13) demonstrates the utility of the stress tensor σ because once it is established in any particular convenient coordinate system, the tractions across any desired area element can be obtained by simple matrix operations knowing only σ and the components of the area normal n.

3.1.2 SPECIAL STRESS STATES

AND

STRESS CONDITIONS

3.1.2.1 Principal Stresses On contemplating Equation (3.13), the alert reader may wonder, given the fact that the stress tensor can be defined in any convenient coordinate system, whether there are particular coordinates in which the stress tensor assumes a particularly simple form. This question has an affirmative answer. Quite generally, at any particular point in any elastic solid there is a coordinate system in which the stress tensor has a simple diagonal form: ⎡σ I ⎢ σ=⎢0 ⎢0 ⎣

0 σ II 0

0 ⎤ ⎥ 0 ⎥ σ III ⎥⎦

(3.14)

Equation (3.14) is very nice indeed because diagonal matrices are much simpler to manipulate than the general case. The components σI, σII, and σIII are called the principal stress components and are typically arranged so that σI > σII > σIII. However, there is a very important string attached in that the special coordinate system in which the stress tensor assumes a diagonal form will in general vary from point to point in the solid. This takes much of the fun out of using the principal stress coordinates, but they are still quite useful nonetheless. Indeed, the largest component σI, called the maximum principal stress, is useful in fracture mechanics work because it represents the largest stress component that can exist at a particular point. Furthermore, the direction in which σI acts can give an important clue to the direction

84

Adhesion Measurement Methods: Theory and Practice

A

F σz = F/A z y

σx = σy = 0 x

F

FIGURE 3.3 Simplest uniaxial stress state for a slender tensile sample.

in which a potential crack will propagate. All of this is valid for homogeneous isotropic materials and is discussed in more detail in Chapter 4, dealing with the fracture mechanics of delamination processes. By far the simplest example of a principal stress state is the case of uniaxial tension shown in Figure 3.3. The principal axes are intuitively obvious for this case, and the stress tensor assumes the simplest possible form as follows: ⎡0 ⎢ σ = ⎢0 ⎢0 ⎣

0 0 0

0⎤ ⎥ 0⎥ σ z ⎥⎦

(3.15)

This is the form of the stress tensor that is assumed for all tensile testing experiments. 3.1.2.2 St. Venant’s Principle The uniaxial tension case provides a clear and simple example of a useful and general rule of stress analysis. The basic idea is most simply illustrated by Figure 3.4, which exhibits three entirely different ways of clamping a uniaxial tensile sample. The fact that the net load is identical for each sample means that they are “statically identical” in the parlance of engineering mechanics. Because of the different clamping configurations, however, the stress state near the top end will be widely different for each sample. But, because each sample is of identical cross section and each is loaded in a statically identical manner (i.e., the net load F is identical in each case), the state of stress far from the clamped region near the center of the sample will be identical in each case and is in fact given by F/A, the net force divided by the crosssectional area. This is a fundamental fact underlying all tensile testing experiments. The general principle highlights the fact that the action of surface tractions is

Theoretical Foundations of Quantitative Adhesion Measurement Methods

85

F F

Center pivot clamp

F

Straight edge clamp

Outrigger pivot clamp

FIGURE 3.4 St. Venant’s principle for three equally loaded but differently clamped tensile samples. The details of the stress field near the clamped edge will differ significantly for each sample; however, because each sample is equally loaded, the stress state far from the clamped edge will be identical for each sample. This is a consequence of the localized nature of the surface tractions imposed by the different clamping arrangements.

essentially local in that the fine details of the local stress state decay away as one proceeds away from the point of application. The stress state in the “far field” depends only on the net loading and the boundary conditions. Although this principle is most clearly illustrated by the uniaxial tension case, it holds for a very general class of solids in one, two, and three dimensions. The precise meaning of far away depends on the details of the problem, but for each case a characteristic length can be defined, and the definition of far away is typically a small multiple of this length. An example of particular relevance to this work is a coating on a rigid substrate. The characteristic length in this case can be taken as the coating thickness and far away typically turns out to be about five times this thickness. 3.1.2.3 Two-Dimensional Stress States 3.1.2.3.1 Plane Stress The case of plane stress is of particular interest in adhesion work because nearly all coatings are in a state of plane stress in which the stress component perpendicular to the coating surface is zero. This is typically taken to be the z direction, so the stress tensor assumes the following form: ⎡ σ xx ⎢ σ = ⎢ σ yx ⎢ 0 ⎣

σ xy σ yy 0

0⎤ ⎥ 0⎥ 0 ⎥⎦

(3.16)

86

Adhesion Measurement Methods: Theory and Practice

The case of a homogeneous isotropic coating on a rigid substrate is particularly simple and can be solved easily with pencil and paper. The shear components σxy and σyx are zero in this case, so the stress tensor is diagonal, and σxx and σyy are in fact principal stresses. 3.1.2.3.2 Plane Strain When dealing with a long rodlike sample of arbitrary cross section, the state of stress away from the ends is approximately two dimensional, and the stress tensor has the following form: ⎡ σ xx ⎢ σ = ⎢ σ yx ⎢ 0 ⎣

σ xy σ yy 0

0 ⎤ ⎥ 0 ⎥ σ zz ⎥⎦

(3.17)

where σzz = ν(σxx + σyy). The plane strain case is also very important from the point of view of adhesion testing because nearly all fracture mechanics tests on crack propagation are performed in a state of plane strain. More is said on this matter in Chapter 4. 3.1.2.3.3 Hydrostatic Stress A final simplified stress state of interest is that of hydrostatic compression or tension. The stress tensor in this case is as simple as it can be: ⎡1 ⎢ σ = σ ⎢0 ⎢0 ⎣

0 1 0

0⎤ ⎥ 0⎥ 1⎥⎦

(3.18)

The stress tensor is simply a scalar times the identity matrix and is thus effectively a scalar quantity. The pressure in a pneumatic tire is the simplest example of this stress state. The pressure in most fluids is similarly characterized. In solids, the scalar factor σ can be positive, indicating a state of hydrostatic tension. This can be achieved when the sample is constrained along each of the three coordinate axes and can lead to void formation at high stress levels. This is an important failure mode in some rubbers.

3.1.3 EQUATION

OF

MOTION

IN

SOLIDS

The whole purpose of the presentation up to this point has been to set the stage for the development of the basic equation of motion for an elastic body. Figure 3.5 shows a small element of material embedded within a larger object. The question is how this object responds to the forces acting on it. The answer is the same as the one given by Sir Isaac Newton in the 17th century in his second law of particle mechanics; that is, the mass of the object times the acceleration is equal to the net vector sum of all the forces acting on it. This is typically written as follows:

Theoretical Foundations of Quantitative Adhesion Measurement Methods

n

87

T

dV dA fb e3 e2

e1

FIGURE 3.5 An element of volume dV embedded in a larger solid. The surface element dA with unit normal n is acted on by a traction T. A body force fb acts on the entire volume element.

∑

Fi = m

i

d 2u dt 2

(3.19)

where m = mass of volume element u = displacement vector Equation (3.19) is the typical expression given in texts on classical particle mechanics, which treat all objects as point masses, ignoring their internal structure as continuous bodies. This treatment is quite adequate for problems in ballistics, for which the projectile can be treated as a point mass acted on by the Earth’s gravitational field and various frictional forces due to the Earth’s atmosphere. This treatment calculates the projectile trajectory and where will it land. If it is desired to know what will happen when the projectile hits another object, then the continuum nature of the missile cannot be ignored, and continuum theory must be applied. Equation (3.19) must be modified to reflect that the projectile is in fact an extended body. The discrete mass m is replaced by the density times a volume element, and the list of forces must now include surface tractions caused by the impacting surfaces as well as the usual external forces, such as gravity. The following relations must now be used: dm = ρdV F=

∫ f dV + F b

V

int

(3.20)

88

Adhesion Measurement Methods: Theory and Practice

where ρ = material density fb = body force/unit volume (gravitational, electromagnetic, etc.) Fint = total internal traction forces =

∫ TdA = ∫ σ.ndA A

A

In light of these new definitions, Newton’s second law as expressed in Equation (3.19) now becomes

∫

∫

fb dV + σ .ndA =

V

A

∫

ρ

V

d 2u dV dt 2

(3.21)

At this point, one of the truly marvelous bits of legerdemain from vector calculus, known as the divergence theorem, is invoked to transform the surface integral over the stress tensor into a volume integral. The theorem, called the Divergence Theorem, is general and essentially states that

∫ σ.n dA = ∫∇ • σ dV . A

V

Readers who need to brush up on vector calculus or would like more detailed references on the subject should refer to Appendix A. The main point in doing this is as follows: All the terms can now be gathered within the same volume integral, which is set equal to zero. Because the volume is essentially arbitrary (i.e., the equation must hold for all shapes), the only way the integral can be zero is if the integrand itself is identically zero, which then leads to the required differential relation. Applying these steps to Equation (3.21) gives

∫ V

∫

fb dV + σ.ndA = A

∫

ρ

V

d 2u dV dt 2

(rearrange + divergeence theorem)

∫ V

∫

∫

fb dV + ∇· σdV − ρ V

V

d 2u =0 dt 2

(collect terms under common volume integral)

∫ V

⎛ d 2u ⎞ ⎜ fb dV + ∇·σ − ρ dt 2 ⎟ dV = 0 ⎝ ⎠

Because the last volume integral must hold for objects of arbitrary shape, size, and loading condition, the integrand itself must be zero, which gives

Theoretical Foundations of Quantitative Adhesion Measurement Methods

fb + ∇ · σ − ρ

d 2u =0 dt 2

89

(3.22)

where ρ fb σ u

= = = =

material density (kg/m3) body force density (N/m3) stress tensor (N/m2) displacement field vector (m)

Equation (3.22) represents Newton’s second law as applied to a continuous solid. The main feature that differs from the standard particle mechanics version given by Equation (3.19) is the divergence of the stress tensor, which accounts for the action of the internal stresses acting within the body.

3.1.4 DEFORMATION

AND

STRAIN

With the basic equation for stresses now in hand, the discussion proceeds to the complementary topic of deformation and strain. When a stress is applied to any material object, there is a resulting deformation, so the key questions now become how deformation is defined and how it is related to the applied stress. To most readers, the idea of a deformation should seem quite obvious because nearly everyone has an intuitive feel for what deformation is. If you run your car into a rigid post, the resulting deformation of the fender is obvious, so it is somewhat surprising that the mathematical description arising from continuum theory is fairly recondite, giving rise to dense topics such as deformation gradients and invariant strain measures. The basic difficulties arise from the need for mathematical precision and the fact that the world is three dimensional. In one dimension, everything falls out quite naturally. The stress is proportional to the strain (Hooke’s law), and the strain is just the increment in length divided by the original length. However, when describing general three-dimensional deformations, these concepts simply do not pass muster, and one must resort to something more heavy duty. The basic approach of continuum theory, therefore, is to treat any object whatsoever as a vector field as shown in Figure 3.6. In this figure, the object labeled Bu (subscript u for undeformed) is described as a vector field that is a region of space labeled by a collection of vectors X = (X1, X2, X3). It is clear then that just about any object can be so defined in terms of its geometric shape. Other properties are also required but that comes later in Section 3.1.5. At this point, to be able to define deformations in three dimensions the geometric configuration must first be defined, and the vector field X does the job. The precise shape of the object is defined by also defining the boundary of Bu (commonly designated as ∂Bu), but that is not needed to obtain a general definition of the deformation of an object. Now, the mathematicians are perfect wizards at performing deformations through entities called mappings, which turn out to be vector fields themselves and that describe transformations between different vector spaces. The vector K(X) shown in Figure 3.6 is such a mapping. The figure shows that K(X) is just the original

90

Adhesion Measurement Methods: Theory and Practice

Pd Bd

Bu

u(X)

Pu

e3 l3

X

12

K(X)

x e2

e1 l1

FIGURE 3.6 Continuum description of the deformation of a body Bu.

position vector X plus a deformation vector u, which in general will depend on X. It should be noted at this point that the mapping K will take the entire space to which Bu belongs (described by basis vectors l1, l2, l3) into an entirely new space described by basis vectors e1, e2, and e3. Thus, the mapping K(X) can be thought of as taking the point X in the space described by l1, l2, and l3 into the point x in the space with basis vectors e1, e2, and e3 or x = K(X). It is also clear that the configuration of the body can be equally well described using either coordinate system because the mapping K(X) is assumed to be continuous with continuous derivatives and suitably well behaved so that its inverse K–1(X) exists and is equally well behaved. This is both a powerful and convenient feature of the continuum description of the deformation process and, unfortunately, also a source of much confusion, so a few words must be said regarding nomenclature for the description used. When using the l1, l2, l3 basis vectors, one is said to be employing the Lagrangian formulation, and if using the e1, e2, e3 basis, then the Eulerian description is in effect. The main reason for noting this is for those who consult the continuum mechanics literature. For present purposes, the deformations and strains will be relatively small, and in this case the Lagrangian and Eulerian descriptions turn out to be nearly identical. Getting back now to the general description of deformation and strain, the basic relation for the deformation u can be written by referring to Figure 3.6 as u(X) = K(X) − X

(3.23)

Equation (3.23) describes the overall deformation process, but for purposes of describing the internal strain in the body something must be said about the gradient of the deformation or how steeply the deformation separates contiguous points in the object under consideration. Thus, taking the gradient of both sides of Equation (3.23) leads to

Theoretical Foundations of Quantitative Adhesion Measurement Methods

91

∇u(X) = ∇K(X) − I or

(3.24)

∇u(X) = F − I The new tensor quantity F = ∇K is called the deformation gradient, and the tensor ∇u is called the displacement gradient. Equations (3.23) and (3.24) lay a foundation for defining general deformations, but what is needed now is a proper definition of strain. This is somewhat trickier than just defining deformations because a true strain will always give rise to a concomitant stress. The general deformation given by Equation (3.23) contains translations and rotations as well as stretches and twists. The pure translations and rotations clearly will not induce any kind of stress in an object as they are rigid deformations in which every part of the object moves in unison. Simply moving a glass from the table and inverting it on the dresser will not induce any kind of stress. It is the stretches and twists that actually cause material particles within the object to separate relative to each other and that give rise to strains that induce a level of stress in the object. Take a glass rod and either twist it or bend it, and you will induce a strain that will cause a stress. There is no unique way of defining the strain. However, one approach is to take the deformation gradient F and cobble together a formula that will flush out those parts of the deformation that are essentially rigid rotations or translations and leave only the bona fide stretches, compressions, and twists. One such definition is as follows: T D = 1 2 ⎡⎢ F F − I ⎤⎥ ⎣ ⎦

(3.25)

It can be shown using the polar decomposition theorem that the finite strain tensor D defined in Equation (3.25) fits the bill in terms of eliminating all rigid body motions from the general deformation formula given by Equation (3.23) and thus includes only those stretches, compressions, and twists that will give rise to a stress. Unfortunately, D turns out to be a rather difficult entity to deal with in general because of what are commonly known as nonlinear effects. These typically arise when relatively large deformations occur, such as when one pulls a bar of taffy to two times its original length. However, if the deformations are relatively small, as in the case of shrinkage strains in a paint coating, then another, simpler strain measure can be used, which is defined as follows: ε = 1 2[(∇u) + (∇u)T ]

(3.26)

The strain tensor ε is closely related to D, as can be shown by the following simple manipulations:

92

Adhesion Measurement Methods: Theory and Practice

T D = 1 2 ⎡⎢ FF − I ⎤⎥ ⎦ ⎣

where F = ∇u + I FT = (∇u)T + I Substituting the expressions for F and FT into the expression for D gives the following result: T

T

D = 1 2 [F F − I] = 1 2 [(∇u + I)((∇u) + I) − I] T

= 1 2 [∇u + (∇u) ] + 1 2 (∇u)(∇u) = ε + 1 2 (∇u)(∇u)

T

T

The final definitions for strain can be summarized as follows: T D = 1 2 ⎡⎢ F F − I ⎤⎥ ⎣ ⎦

Finite deformations

T ε = 1 2 ⎡∇u + ∇u ⎤ ⎢⎣ ⎥⎦

( )

Small strains only

(3.27)

T

( )( )

D = ε + 1 2 ∇u ∇u

Note that D and ε are nearly equal when ∇u is small, which is always the case for small strain problems in the theory of linear elasticity. One further issue has to be confronted before the development of a suitable strain measure can be considered completed. The basic problem comes down to this: If we know the displacement field u, then Equations (3.27) give perfectly good recipes for conjuring up the required strain fields. However, in many problems of practical interest one first computes the strains, and the question arises as to whether Equations (3.27) will be sufficient to determine the corresponding displacements. The question is a subtle and tricky one, and the answer is generally “No.” Equations (3.27) alone do not guarantee that the derived strains will correspond to acceptable displacements. It turns out that one further relation is required to ensure compatibility between a derived set of strains and the corresponding displacements as follows: ∇×∇×ε = 0

(3.28)

Equation (3.28) is known as the equation of compatibility for the strain field ε. A clear and convincing development of Equation (3.28) has been presented by Gurtin,1 who also gives an excellent, if somewhat high-powered, development of the general deformation/strain equations. The now-complete continuum description of the deformation and strain fields can be summarized as follows:

Theoretical Foundations of Quantitative Adhesion Measurement Methods

a) x = K(X)

(Deformation mapping)

b) u = K(X) − X

(Displacement vector)

c) F = ∇K

(Deformation gradient)

d) J = ∇u − I

(Displacement gradient)

T e) D = 1 2 ⎡⎢ F F − I ⎤⎥ ⎣ ⎦

(Finite strain tensor)

f) ε = 1 2 ⎡⎣∇u + (∇u)T ⎤⎦

(Infinitesimal strain tensor)

g) ∇ × ∇ × ε = 0

(Equation of compatibility)

93

(3.29)

h) D = ε + 1 2 (∇u)((∇u)T (relation between D, ε , and u) Equations (3.29) essentially complete the second step in the continuum mechanics program outlined on page 76, to describe and compute deformations and stresses in solid bodies. A few words on nomenclature are in order for those who will consult the general literature on the subject. The tensor quantity F FT is called the Green’s strain after George Green, the famous 19th century mathematician. All of what has been developed to this point has been worked out in the Lagrangian description as defined here (meaning in the l1, l2, l3 coordinate system). One can easily imagine that by using the Euler description a somewhat different tensor quantity can be conjured up that will be essentially equivalent to F FT but referred to different coordinates. Names such as Cauchy’s strain tensor or Euler’s (Almansi’s) strain tensor will pop up in various places, which tends to give rise to much confusion regarding which is which. The reader can take heart from the fact that all descriptions give the same result for the small strain tensor ε, and that this is the most commonly used strain measure in the practical engineering literature. This arises from the fact ∇ that when the strains are small, the quantity ∇u is small, and thus the term ∇u(∇ u)T in Equation (3.27) is of second order in a small quantity and can be neglected. In this case, ε and D become identical. Caution must be exercised, however. A common problem arises when someone using a finite element code, for instance, does not understand which strain measure is used. In particular, if ε is used and the problem involves a significant degree of rotation, major errors can creep into the calculation even though the actual strains may be low. This comes about because ε does not accurately account for large rotations as the general deformation measure D does.

3.1.5 CONSTITUTIVE RELATIONS TO THE STRAIN

OR

CONNECTING

THE

STRESS

3.1.5.1 General Behavior At this point, Steps 1 and 2 of the continuum mechanics presentation have been accomplished. General definitions of stress, deformation, and strain are now in place.

94

Adhesion Measurement Methods: Theory and Practice

What is clearly lacking, however, is a description of how these quantities are related in a real material. What is required is referred to as the constitutive relation or material law for substances of interest. In general, this is a very difficult topic and goes to the very heart of the thermodynamic nature of materials and how they respond to the myriad array of loads and deformations to which they can be subjected. Everything from the bending of a pencil to the gravitational collapse of a star requires a fundamental understanding of the constitutive behavior of the material in question. Many common materials show a complex range of behaviors when subjected to relatively modest loading conditions. Materials such as mayonnaise tend to deform more easily as the deformation rate increases (shear thinning). Contrary materials such as Silly Putty do just the opposite. You can easily deform this material with your fingers like a putty, but if you drop it on the floor, it will bounce like a rubber ball (shear thickening). This type of behavior is commonly called thixotropic, which is basically a way of saying we really do not know what is going on, so let us just give it a fancy name and move on. There exists a vast body of literature dealing with the constitutive behavior of a wide range of materials, ranging from rubber bands to desert soils. The topic can easily require an entire encyclopedia for anything approaching a definitive treatment. Fortunately, however, a wide range of useful applications deal with materials undergoing relatively small deformations* for which the constitutive relation between the stress and the strain is essentially linear. In this circumstance, there exists a general formulation of the constitutive relation that is useful and is dealt with reasonably easily. It should also be added that focusing on the linear behavior of materials has other merits in addition relative tractability. When attacking the general nonlinear behavior of a material, for instance, it is useful to look at a linear approximation first to see the nature of the error incurred. In addition, nearly all numerical algorithms for solving full nonlinear problems proceed by a sequence of linear approximations that, if handled correctly, will converge to the true nonlinear solution. The problem now is as follows: What is the most general linear relationship that can exist between the stress tensor σ ij and the strain tensor εij? Given the complex nature of the tensor quantities involved, it is no surprise that the answer is also complex, involving the elasticity tensor Cijkl, which was mentioned earlier, thus: 3

σ ij =

∑C

ε

ijkl kl

(3.30)

k ,l =1

Equation (3.30) expresses the most general linear relationship between two second-order tensors that can exist. The fact that a fourth-order tensor is required to make the connection is not surprising because after summing over the two indices k and l, which describe the components of the strain tensor ε, there have to be two indices left over (i and j in this case) to designate the corresponding component of * Beware that small deformations and strains do not necessarily imply small stresses. Most engineering materials, for instance, have a fairly high modulus, so that relatively small strains can give rise to stresses that cause permanent deformations or in some cases lead to fracture.

Theoretical Foundations of Quantitative Adhesion Measurement Methods

95

the stress tensor σ. Because the indices i, j, k, l run over the values 1, 2, 3, the elasticity tensor Cijkl can have a maximum of 81 (34) independent components. Fortunately, a number of physical symmetries come to the rescue, which cuts down this horrendous number considerably. In particular, because the tensor quantities σij and εij are symmetric*, they have at most 6 independent components. This means that Cijkl will have at most 36 (62) independent components. This is still an outlandish number, but luckily real materials have further symmetries that cut this number down still further. Cubic** crystals, for instance, which have many rotational and reflection symmetries, require only 3 independent elastic constants. Ultimately, for homogeneous isotropic materials with full spherical symmetry (amorphous glasses, for instance), the final number comes down to only two elastic constants. It is quite surprising*** that in most applications the assumption of a homogeneous isotropic material seems to work out reasonably well. Even materials such as metals, which are nominally crystalline, can be successfully treated as homogeneous isotropic materials. This stems in large part from the fact that in their final use condition most metals are polycrystalline in nature, which means that they are made up of zillions of very small crystals oriented in random directions. The net effect is that, when viewed over a macroscopically small but microscopically large**** region, the material appears to be homogeneous isotropic. The main types of situations in which one can get into trouble by assuming homogeneous isotropic behavior is when dealing with materials that are large single crystals, composites containing highly oriented fibers, or nonisotropic coatings. The most ubiquitous example of large single crystals is the silicon wafers used in the microelectronics industry. These are near-perfect cubic crystals, and it is important to know how the parent crystal was cut in order to know the mechanical behavior of the product wafer. For example, some laboratories perform wafer-bending experiments to assess the stress state of the wafer. Not knowing which crystal plane the wafer was cut along can lead to very serious errors in such experiments. In particular, it is highly desirable in such experiments to have wafers that have been cut along the (111) plane and thereby have in-plane isotropy; otherwise, one has to deal with a significant level of anisotropy to obtain accurate results. Circuit boards are another example of objects that exhibit a high level of anisotropy because of their composite nature. The common FR4 board material, for example, is made up of a mat of glass fibers embedded in an epoxy matrix. All the fibers lie in the plane of the board, thus giving rise to a large difference between in-plane and out-of-plane mechanical properties. A final example of anisotropy that is of significant concern to the coatings industry is polymer systems made up of stiff chains that tend to orient parallel to the surface on which they are deposited after drying or during the curing process. * The symmetry of the stress tensor arises from the constraint that conservation of angular momentum must hold as well as linear momentum, which is expressed in Equation (3.22). For a detailed derivation, refer to page 20 in the work of Gould.2 Also beware that there are formulations of continuum theory in which the stress and strain tensors are not symmetric. ** A derivation of how this comes about was given by Feynman, Note 8, Chapter 39. *** Or perhaps this is not so surprising given the general human proclivity toward indolence. **** This is what is commonly referred to as the coarse graining approximation.

96

Adhesion Measurement Methods: Theory and Practice

Coatings made from these polymers tend to be highly anisotropic with far different mechanical properties in the plane compared to out-of-plane behavior. This is commonly referred to as orthotropic behavior, and an example is given in Table 3.1. 3.1.5.2 Homogeneous Isotropic Materials It is no accident that the most popular constitutive relation is the one that deals with homogeneous isotropic materials that require only two elastic constants, namely, the Young’s modulus and Poisson’s ratio. It seems that people already regard it as a burden to deal with 2 elastic constants, not to mention 36. If you are working with a newly synthesized polymer, for example, and you browse the manufacturer’s data sheet, you will most likely find only two useful constitutive properties mentioned: the Young’s modulus and the thermal expansion coefficient. In fact, if you inquire about it, the people who made the material, primarily chemists, are most likely unaware of what a Poisson’s ratio is. However, the main reason why it is difficult to find good data on Poisson’s ratio is that it is much more difficult to measure than the Young’s modulus. This problem is discussed in more detail in Section 3.3.1, but now it is important to establish the constitutive relation for homogeneous isotropic materials. This can be done by essentially applying the constraints of spherical symmetry to Equation (3.30). An excellent discussion of the procedure has been given by Gould,2 and the result comes down to the following:

ε11 =

1⎡ σ11 − ν σ 22 + σ 33 ⎤⎦ + αΔT E⎣

ε 22 =

1⎡ σ 22 − ν σ11 + σ 33 ⎤⎦ + αΔT E⎣

(

(

) )

(3.31)

1 ε 33 = ⎡⎣ σ 33 − ν σ11 + σ 22 ⎤⎦ + αΔT E

(

ε12 =

)

σ12 σ σ ; ε 23 = 23 ; ε 31 = 31 2G 2G 2G

Equations (3.31) are the simplest three-dimensional expression of Hooke’s law. In fact, it is easy to see that by collapsing down to one dimension the familiar onedimensional version pops out. Thus, for a simple tensile specimen σ22 = σ33 = σ12 = σ23 = σ31 = 0, and the remaining equation for σ11 becomes σ11 = E ε11, which is the familiar standard form taught in elementary texts. All of this is very satisfying, but yet another essential ingredient is missing. Not only is the real world three dimensional, but also it is governed very strictly by the laws of thermodynamics, which state that everything exists at some finite temperature. Not only that, but also the temperature tends to vary substantially from moment to moment and place to place, giving rise to thermal gradients; these gradients can give rise to strains, which also induce stresses in ordinary objects. In fact, in many

Theoretical Foundations of Quantitative Adhesion Measurement Methods

97

practical situations thermal stresses can entirely dominate the stress distribution in an object. The equation governing the temperature distribution in a body under most conditions is derived from three separate equations, the first of which is in essence a statement of the conservation of energy. Let h be defined as the heat flux vector, which describes the flow of heat (disordered energy) across some small surface area dA in a body per unit time. The quantity h is a vector that will generally vary from point to point in the body. In any particular small volume within the body, heat may be passing through from neighboring volume elements, and there may also be some local heat source within the element generating heat at some rate γ (joules per cubic meter per unit time). Letting q denote the total amount of heat energy per unit volume within the volume at any given time, the conservation of energy requires that

∇·h + γ =

∂q ∂t

(3.32)

Equation (3.32) is commonly referred to as an equation of continuity for the heat flow within a material body. It says in essence that the rate at which heat builds up or drains out of any particular volume is the sum of two terms. The first ∇⋅h accounts for the net flow in from or out to neighboring volume elements. The second term γ accounts for local heat generation, which could be caused by radioactive decay processes or embedded wires. Equation (3.32) states that the time rate of change of heat buildup or loss in any particular volume element is the net sum of energy flow through the bounding surface plus any local contribution from embedded sources. The second equation comes directly from thermodynamics and the definition of the specific heat, that is, (3.33)

dq = ρcv dT or dq dT = ρcv dt dt

In this equation, ρ is the density, and cv is the specific heat (or heat capacity per unit volume) under conditions of constant volume.* Combining Equations (3.32) and (3.33) leads to

∇·h + γ = ρcv

∂T ∂t

* Note that there is also a cp or specific heat under conditions of constant pressure.

(3.34)

98

Adhesion Measurement Methods: Theory and Practice

The final equation is known as Fourier’s law of heat conduction. It is basically the simplest linear constitutive relation for heat flow in solids, relating the heat flux to the gradient of the temperature: h = −κ∇T

(3.35)

Equation (3.35) is simply the statement that when there are spatial variations in the temperature field described by ∇T there will be a concomitant heat flow designated by h, with the constant of proportionality κ known as the thermal conductivity. Combining Equation (3.35) with Equation (3.34) leads to κ∇ 2T + γ = ρcv

∂T ∂t

(3.36)

Using Equation (3.36) along with appropriate initial and boundary conditions, the temperature field in a body can be calculated. If thermal gradients are present or if the body is a composite of materials with different thermal expansion coefficients and is either heated or cooled uniformly, then thermal strains will arise, given by the following formula: ε T = αΔT

(3.37)

with α = (thermal expansion coefficient ΔT = (T – T0) (temperature difference) The parameter α is the thermal expansion coefficient characterizing the tendency of the body to expand or contract on heating. ΔT is the temperature excursion from the reference temperature T0, where the body is in a reference state generally taken to be a condition of zero stress. The thermal strain given by Equation (3.37) must be added to the constitutive relations defined in Equations (3.31) to give the following relations for a thermoelastic solid: ε11 =

1⎡ σ11 − ν σ 22 + σ 33 ⎤⎦ + αΔT E⎣

ε 22 =

1⎡ σ 22 − ν σ11 + σ 33 ⎤⎦ + αΔT E⎣

(

(

) )

(3.38)

1 ε 33 = ⎡⎣ σ 33 − ν σ11 + σ 22 ⎤⎦ + αΔT E

(

ε12 =

)

σ12 σ σ ; ε 23 = 23 ; ε 31 = 31 2G 2G 2G

Equations (3.38) represent the constitutive relations for a homogeneous isotropic material and thereby complete the continuum mechanics program by providing the

Theoretical Foundations of Quantitative Adhesion Measurement Methods

99

essential link between the stresses and the strains in the body. It should be noted that these equations are by no means the most general that can be formulated and are essentially valid in the realm of small strains and temperature excursions. However, they are valid for a wide variety of practical problems, and they form a foundation for considering more elaborate situations in which the assumptions of isotropy, small strains, and the like are not valid. The complete set of field equations for the thermoelastic behavior of a homogeneous isotropic solid are summarized in Table 3.1.

3.2 EXAMPLES Table 3.1 essentially summarizes what was known about the thermoelastic behavior of solids by the end of the 19th century. As such, they represent a cumulative intellectual triumph of that century. However, in addition to representing a purely transcendent accomplishment of the human intellect, the field equations catalogued in Table 3.1 are also amazingly useful tools for analyzing the behavior of solid materials that have found constant application in engineering problems since their derivation. The advent of nearly unlimited computing power represented by the now ubiquitous personal computer workstation has made these equations even more powerful as tools of analysis because previously unusable numerical algorithms can now be fruitfully brought to bear to provide accurate solutions to these equations in support of myriad design and development projects. This section presents a number of “back-of-the-envelope” type calculations designed to give some insight into the utility of the field equations listed in Table 3.1 and provide some feel for how they can be put to work in a number of practical situations. The examples presented, however, only scratch the surface of what can be done with pencil and paper. Indeed, all serious work involving these equations is done on powerful workstations using the exceedingly effective finite element and boundary element analysis schemes.

3.2.1 SIMPLE DEFORMATIONS Some feel for the meaning of the equations for deformation and strain given by Equations (3.29) can be gained by looking at a few simple examples. The simplest possible deformation is a rigid translation. The required deformation mapping comes directly from Equation (3.29a): Consider as a simplest case a rigid translation along the x1 axis, where the displacement vector is simply given by u = b = (b1, 0, 0). Another way to write this is to combine Equations (3.29a) and (3.29b) to obtain the relation x = X + b. Yet another way of looking at it is to write Equation (3.29a) out explicitly; that is, x = K(X) where x = (x1, x2, x3), X = (X1, X2, X3), and K(X) = (X1 + b1, X2, X3). To make things clearer, this can be set out componentwise as follows:

( ) = K (X ) = X = K (X ) = X

x1 = K1 X = X1 + b1 x2 x3

2

2

3

3

(3.39)

100

Adhesion Measurement Methods: Theory and Practice

TABLE 3.1 Collected Field Equations for Homogeneous Isotropic Thermoelastic Material Formula

Variable/Parameter Descriptions

Momentum balance

σ= Stress tensor (N/m2) u = Displacement vector (m) fb = Body force vector (N/m3) ρ = Material density (kg/m3)

Equation (3.22): Newton’s second law generalized for a continuum body

u = Displacement vector (m) I = Identity tensor F, D, J, and ε dimensionless

Equations (3.29): Basic definitions of deformation and strain fields; note that ε is reliable for small strains only

2

fb + ∇ ·σ σ−ρ

d u =0 dt 2

Deformation and strain fields a) Deformation mapping x = K(X) b) Displacement vector u = K(X) – X

Comments

c) Deformation gradient F = ∇K d) Displacement gradient J = ∇u – I e) Finite strain tensor D = 1/2[F FT – I] f) Infinitesimal strain tensor ε = 1/2[∇u + (∇u)T ] g) Equation of compatibility ∇×∇×ε=0 h) Relation between D, ε and u D = ε + 1/2(∇u)(∇u)T εij = Components of strain tensor ε Equations (3.38): Basic equations connecting the σi,j = Components of stress tensor 3) σ stresses to the strains; (N/m Stresses in terms of strains define the solid as a I = Identity matrix ⎞ E ⎛ νI material entity with tr ε = ε11 + ε22 + ε33 σ= ε + tr ε + E α Δ T I ⎟⎠ 1 + ν ⎜⎝ 1 − 2ν recognizable physical tr σ = σ11 + σ22 + σ33 properties; the material is ΔT = (T − T0) thermal excursion Strains in terms of stresses assumed to be (K) 1+ ν ν tr σ homogeneous and E = Young’s modulus (N/m3) ε= σ− I + αΔT I E E G = Shear modulus (N/m3) isotropic v = Poisson’s ratio Componentwise strains in terms of stresses α = Thermal expansion coefficient 1 (K−1) ε11 = ⎡⎣ σ11 − ν σ 22 + σ 33 ⎤⎦ + αΔT E G = E/[2(1 + v)] 1 ε 22 = ⎡⎣ σ 22 − ν σ11 + σ 33 ⎤⎦ + αΔT E Constitutive relations for thermoelastic homogeneous isotropic material

(

)

(

)

ε 33 =

1⎡ σ 33 − ν σ11 + σ 22 ⎤ + αΔT ⎦ E⎣

ε12 =

σ 23 ; σ13 σ12 ; ε 23 = ε13 = 2G 2G 2G

(

)

Theoretical Foundations of Quantitative Adhesion Measurement Methods

101

TABLE 3.1 (continued) Collected Field Equations for Homogeneous Isotropic Thermoelastic Material Formula

Variable/Parameter Descriptions

Comments

εij = Components of strain tensor ε Basic stress-strain relations for a σi,j = Components of stress tensor 3) σ nonisotropic coating for (N/m Componentwise strains in terms of stresses which the elastic ΔT = (T − T0) thermal excursion 1 behavior is dependent on (K) ⎡⎣ σ11 − ν12 σ 22 − ν13σ 33 ⎤⎦ + α1ΔT ε11 = E 11 direction; these relations E1, E1, E1 = Nonisotropic Young’s 3) form the next level of moduli (N/m 1 ⎡⎣ σ 22 − ν21σ11 − ν23σ 33 ⎤⎦ + α 2ΔT ε 22 = i, j = 1, 2, 3 = Nonisotropic complexity above v ij, E 22 Poisson’s ratios Equations (3.38); for the 1 ⎡⎣ σ 33 − ν31σ11 − ν32 σ 22 ⎤⎦ + α 3ΔT G12, G13, G23 = Nonisotropic shear case of in-plane isotropy, ε 33 = E 33 moduli (N/m3) the following constraints α , α , α = Nonisotropic thermal hold: 1 2 3 ν12 = ν 21 expansion coefficients (K−1) E 11 E 22 E11 = E22 = E; E33 = Ez Constitutive relations for thermoelastic homogeneous orthotropic material

ε12 =

σ12 σ σ ; ε13 = 13 ; ε 23 = 23 2G12 2G13 2G23

ν12 = ν21 = ν ν31 = ν13 = ν23 = ν32 = ν z G12 =

E 2(1 + ν)

G13 = G23 =

EEz ( E + Ez + 2 E ν z )

ν2 < 1 and ν2z

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close